#------------------------------------------------------------------------------
#$Date: 2025-07-01 14:21:32 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1233 $
#$URL: svn://crystallography.net/testcod/cif/1/00/00/1000021.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1000021
loop_
_publ_author_name
'Hunger, Jens'
'Beta, Ilir A.'
'Böhlig, Heinz'
'Ling, Chris'
'Jobic, Herve'
'Hunger, Bernd'
_publ_section_title
;
 Adsorption Structures of Water in NaX Studied by DRIFT Spectroscopy and
 Neutron Powder Diffraction
;
_journal_issue                   1
_journal_name_full               'The Journal of Physical Chemistry B'
_journal_page_first              342
_journal_page_last               353
_journal_paper_doi               10.1021/jp054636u
_journal_volume                  110
_journal_year                    2006
_chemical_formula_analytical     'Na88.1[Al88.1Si103.9O384] *66H2O'
_chemical_formula_sum            'Al2.75 D4.1 Na2.92 O14.05 Si3.25'
_chemical_formula_weight         465.62
_chemical_name_common            NaX
_space_group_IT_number           203
_space_group_name_Hall           '-F 2uv 2vw 3'
_space_group_name_H-M_alt        'F d -3 :2'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 2uv 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 :2'
_audit_creation_date             2005-08-01T20:05
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2005-08-01T20:05  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            32
_cell_length_a                   25.05049(15)
_cell_length_b                   25.05049
_cell_length_c                   25.05049
_cell_measurement_temperature    5
_cell_volume                     15719.86(9)
_computing_data_collection       D2B
_computing_data_reduction        D2B
_computing_molecular_graphics    'Diamond 3'
_computing_publication_material  EXPGUI
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      5
_diffrn_detector                 D2B
_diffrn_detector_type            D2B
_diffrn_measurement_device_type  D2B
_diffrn_radiation_monochromator  Ge
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     2.4
_exptl_absorpt_correction_T_max  0.98183
_exptl_absorpt_correction_T_min  0.98177
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 Debye-Scherrer absorption correction
Term (= MU.r/wave) =     0.45173E-02
Correction is not refined.
;
_pd_block_id                     2005-08-01T20:05|NAX72
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               Grenoble
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        151.2
_pd_meas_2theta_range_min        0.05
_pd_meas_number_of_points        3024
_pd_meas_scan_method             step
_pd_phase_name                   NaX-72
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        151.1297
_pd_proc_2theta_range_min        -0.0203
_pd_proc_info_datetime           2005-08-01T20:05:32
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 20 terms.
 Shifted Chebyshev function of 1st kind
      1:    215.498     2:   -48.0005     3:    34.1116     4:   -3.84184    
      5:    3.98441     6:   -5.84984     7:    6.09365     8:   -1.98605    
      9:   0.536063    10:  -0.292147    11:   0.675845    12:    2.65773    
     13:   -1.56939    14:   -4.07720    15:    4.47366    16:   -2.49782    
     17:   0.957255    18:   0.431821    19:   -1.33596    20:  -3.895620E-02
;
_pd_proc_ls_peak_cutoff          0.00000
_pd_proc_ls_profile_function
;
 CW Profile function number 2 with  18 terms
 Profile coefficients for Simpson's rule integration of pseudovoigt function
 C.J. Howard (1982). J. Appl. Cryst.,15,615-620.
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 #1(GU)   =   85.897 #2(GV)   = -150.017 #3(GW)   =  157.967
 #4(LX)   =    8.472 #5(LY)   =    7.960 #6(trns) =    0.000
 #7(asym) =   7.3810 #8(shft) =   0.0000 #9(GP)   =    0.000
 #10(stec)=     0.00 #11(ptec)=     0.00 #12(sfec)=     0.00
 #13(L11) =    0.000 #14(L22) =    0.000 #15(L33) =    0.000
 #16(L12) =    0.000 #17(L13) =    0.000 #18(L23) =    0.000
 Peak tails are ignored  where the intensity is below 0.0000 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0225
_pd_proc_ls_prof_wR_expected     0.0201
_pd_proc_ls_prof_wR_factor       0.0293
_pd_proc_number_of_points        3024
_pd_spec_mounting                ' ?'
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_pd_spec_size_axial              50
_pd_spec_size_equat              14
_refine_ls_goodness_of_fit_all   1.49
_refine_ls_matrix_type           full
_refine_ls_number_parameters     99
_refine_ls_number_restraints     1
_refine_ls_R_Fsqd_factor         0.01940
_refine_ls_shift/su_max          0.05
_refine_ls_shift/su_mean         0.00
_reflns_d_resolution_high        1.246
_reflns_d_resolution_low         8.857
_reflns_limit_h_max              20
_reflns_limit_h_min              1
_reflns_limit_k_max              14
_reflns_limit_k_min              0
_reflns_limit_l_max              13
_reflns_limit_l_min              0
_reflns_number_total             367
_cod_data_source_file            jp054636usi20050825_095740.cif
_cod_data_source_block           NAX72_publ
_cod_original_cell_volume        15719.85(27)
_cod_original_sg_symbol_Hall     'F d -3'
_cod_original_sg_symbol_H-M      'F d -3'
_cod_original_formula_sum        'Al2.75 D4.10 Na2.92 O14.05 Si3.25'
_cod_database_code               1000021
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 +z,+x,+y
3 +y,+z,+x
4 +x+1/4,+y+1/4,-z
5 -z,+x+1/4,+y+1/4
6 +y+1/4,-z,+x+1/4
7 -z+1/4,+x+1/2,-y+3/4
8 -y+3/4,-z+1/4,+x+1/2
9 +y+1/2,-z+1/4,-x+3/4
10 -x+3/4,+y+1/2,-z+1/4
11 -z+1/4,-x+3/4,+y+1/2
12 +x+1/2,-y+3/4,-z+1/4
-1 -x,-y,-z
-2 -z,-x,-y
-3 -y,-z,-x
-4 -x+3/4,-y+3/4,+z
-5 +z,-x+3/4,-y+3/4
-6 -y+3/4,+z,-x+3/4
-7 +z+3/4,-x+1/2,+y+1/4
-8 +y+1/4,+z+3/4,-x+1/2
-9 -y+1/2,+z+3/4,+x+1/4
-10 +x+1/4,-y+1/2,+z+3/4
-11 +z+3/4,+x+1/4,-y+1/2
-12 -x+1/2,+y+1/4,+z+3/4
101 +x,+y+1/2,+z+1/2
102 +z,+x+1/2,+y+1/2
103 +y,+z+1/2,+x+1/2
104 +x+1/4,+y+3/4,-z+1/2
105 -z,+x+3/4,+y+3/4
106 +y+1/4,-z+1/2,+x+3/4
107 -z+1/4,+x,-y+1/4
108 -y+3/4,-z+3/4,+x
109 +y+1/2,-z+3/4,-x+1/4
110 -x+3/4,+y,-z+3/4
111 -z+1/4,-x+1/4,+y
112 +x+1/2,-y+1/4,-z+3/4
-101 -x,-y+1/2,-z+1/2
-102 -z,-x+1/2,-y+1/2
-103 -y,-z+1/2,-x+1/2
-104 -x+3/4,-y+1/4,+z+1/2
-105 +z,-x+1/4,-y+1/4
-106 -y+3/4,+z+1/2,-x+1/4
-107 +z+3/4,-x,+y+3/4
-108 +y+1/4,+z+1/4,-x
-109 -y+1/2,+z+1/4,+x+3/4
-110 +x+1/4,-y,+z+1/4
-111 +z+3/4,+x+3/4,-y
-112 -x+1/2,+y+3/4,+z+1/4
201 +x+1/2,+y,+z+1/2
202 +z+1/2,+x,+y+1/2
203 +y+1/2,+z,+x+1/2
204 +x+3/4,+y+1/4,-z+1/2
205 -z+1/2,+x+1/4,+y+3/4
206 +y+3/4,-z,+x+3/4
207 -z+3/4,+x+1/2,-y+1/4
208 -y+1/4,-z+1/4,+x
209 +y,-z+1/4,-x+1/4
210 -x+1/4,+y+1/2,-z+3/4
211 -z+3/4,-x+3/4,+y
212 +x,-y+3/4,-z+3/4
-201 -x+1/2,-y,-z+1/2
-202 -z+1/2,-x,-y+1/2
-203 -y+1/2,-z,-x+1/2
-204 -x+1/4,-y+3/4,+z+1/2
-205 +z+1/2,-x+3/4,-y+1/4
-206 -y+1/4,+z,-x+1/4
-207 +z+1/4,-x+1/2,+y+3/4
-208 +y+3/4,+z+3/4,-x
-209 -y,+z+3/4,+x+3/4
-210 +x+3/4,-y+1/2,+z+1/4
-211 +z+1/4,+x+1/4,-y
-212 -x,+y+1/4,+z+1/4
301 +x+1/2,+y+1/2,+z
302 +z+1/2,+x+1/2,+y
303 +y+1/2,+z+1/2,+x
304 +x+3/4,+y+3/4,-z
305 -z+1/2,+x+3/4,+y+1/4
306 +y+3/4,-z+1/2,+x+1/4
307 -z+3/4,+x,-y+3/4
308 -y+1/4,-z+3/4,+x+1/2
309 +y,-z+3/4,-x+3/4
310 -x+1/4,+y,-z+1/4
311 -z+3/4,-x+1/4,+y+1/2
312 +x,-y+1/4,-z+1/4
-301 -x+1/2,-y+1/2,-z
-302 -z+1/2,-x+1/2,-y
-303 -y+1/2,-z+1/2,-x
-304 -x+1/4,-y+1/4,+z
-305 +z+1/2,-x+1/4,-y+3/4
-306 -y+1/4,+z+1/2,-x+3/4
-307 +z+1/4,-x,+y+1/4
-308 +y+3/4,+z+1/4,-x+1/2
-309 -y,+z+1/4,+x+1/4
-310 +x+3/4,-y,+z+3/4
-311 +z+1/4,+x+3/4,-y+1/2
-312 -x,+y+3/4,+z+3/4
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Si Si1 0.12358(28) -0.05544(25) 0.03769(25) 1.0 Uiso 0.0082(6) 96
Si Si2 -0.05195(32) 0.12623(28) 0.03514(31) 0.0826 Uiso 0.0082(6) 96
Al Al1 -0.05195(32) 0.12623(28) 0.03514(31) 0.9174 Uiso 0.0082(6) 96
O O1 0.10782(17) -0.10318(18) 0.0001(4) 1.0 Uiso 0.02247(30) 96
O O2 0.17927(20) 0.17468(20) -0.03309(12) 1.0 Uiso 0.02247(30) 96
O O3 -0.00113(19) -0.00292(20) 0.14452(11) 1.0 Uiso 0.02247(30) 96
O O4 0.17920(20) 0.17772(20) 0.31987(13) 1.0 Uiso 0.02247(30) 96
Na SI 0.0 0.0 0.0 0.083(19) Uiso 0.0241(18) 16
Na SI' 0.05534(22) 0.05534(22) 0.05534(22) 0.810(15) Uiso 0.0241(18) 32
Na SII 0.23383(20) 0.23383(20) 0.23383(20) 1.0 Uiso 0.0241(18) 32
Na SJ 0.2022(8) 0.0338(8) -0.1439(7) 0.317(9) Uiso 0.0241(18) 96
O Og 0.1902(5) -0.0188(6) -0.1697(5) 0.2134(31) Uiso 0.0745(35) 96
D Dg1 0.2038(7) 0.0143(7) -0.1836(8) 0.2134(31) Uiso 0.0745(35) 96
D Dg2 0.1607(5) -0.0084(8) -0.1475(6) 0.2134(31) Uiso 0.0745(35) 96
O Oh 0.2511(9) 0.0084(10) -0.1166(8) 0.1256(27) Uiso 0.0745(35) 96
D Dh1 0.2329(12) -0.0109(13) -0.1442(11) 0.1256(27) Uiso 0.0745(35) 96
D Dh2 0.2244(12) 0.0318(12) -0.1020(12) 0.1256(27) Uiso 0.0745(35) 96
O OII' 0.1631(4) 0.1631(4) 0.1631(4) 0.2550(31) Uiso 0.0745(35) 32
D DII'1 0.1856(11) 0.1321(8) 0.1645(18) 0.0850(10) Uiso 0.0745(35) 96
D DII'2 0.1312(6) 0.1510(15) 0.1455(14) 0.0850(10) Uiso 0.0745(35) 96
O OII* 0.2852(8) 0.2852(8) 0.2852(8) 0.172(4) Uiso 0.0745(35) 32
D DII*1 0.2631(21) 0.3163(13) 0.2892(28) 0.0572(15) Uiso 0.0745(35) 96
D DII*2 0.3191(7) 0.2989(22) 0.2738(24) 0.0572(15) Uiso 0.0745(35) 96
O Oi 0.1543(10) 0.1623(9) -0.2093(10) 0.1069(24) Uiso 0.0745(35) 96
D Di1 0.1498(11) 0.1966(12) -0.2258(15) 0.1069(24) Uiso 0.0745(35) 96
D Di2 0.1224(11) 0.1572(13) -0.1887(13) 0.1069(24) Uiso 0.0745(35) 96
O Ok 0.2984(10) 0.0861(11) -0.1555(15) 0.0952(28) Uiso 0.0745(35) 96
D Dk1 0.3327(13) 0.0752(16) -0.1686(16) 0.0952(28) Uiso 0.0745(35) 96
D Dk2 0.3035(16) 0.0903(20) -0.1177(14) 0.0952(28) Uiso 0.0745(35) 96
Na SIII 0.375 0.375 0.1318(33) 0.078(10) Uiso 0.0241(18) 48
loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_length_neutron
_atom_type_scat_source
Si 103.93 0.4149 International_Tables_Vol_C
Al 88.07 0.3449 International_Tables_Vol_C
O 449.594 0.5803 International_Tables_Vol_C
Na 93.405 0.3630 International_Tables_Vol_C
D 131.185 0.6671 International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Si1 O2 113.2(5) 1_555 . -206_444 N
O1 Si1 O3 108.3(5) 1_555 . 2_555 N
O1 Si1 O4 110.2(4) 1_555 . 209_343 N
O2 Si1 O3 104.8(4) -206_444 . 2_555 N
O2 Si1 O4 116.9(4) -206_444 . 209_343 N
O3 Si1 O4 102.4(4) 2_555 . 209_343 N
O1 Si2 O2 103.9(4) -1_555 . -105_444 N
O1 Si2 O3 115.0(5) -1_555 . 3_555 N
O1 Si2 O4 109.0(5) -1_555 . 107_433 N
O2 Si2 O3 110.0(5) -105_444 . 3_555 N
O2 Si2 O4 112.0(5) -105_444 . 107_433 N
O3 Si2 O4 107.1(4) 3_555 . 107_433 N
O1 Al1 O2 103.9(4) -1_555 . -105_444 N
O1 Al1 O3 115.0(5) -1_555 . 3_555 N
O1 Al1 O4 109.0(5) -1_555 . 107_433 N
O2 Al1 O3 110.0(5) -105_444 . 3_555 N
O2 Al1 O4 112.0(5) -105_444 . 107_433 N
O3 Al1 O4 107.1(4) 3_555 . 107_433 N
Si1 O1 Si2 138.82(34) 1_555 . -1_555 N
Si1 O1 Al1 138.82(34) 1_555 . -1_555 N
Si1 O1 O1 78.0(4) 1_555 . -2_555 N
Si1 O1 O1 85.15(32) 1_555 . -3_555 N
Si1 O1 O2 110.69(29) 1_555 . 105_544 N
Si1 O1 O2 33.35(30) 1_555 . -206_444 N
Si1 O1 O2 91.21(33) 1_555 . 304_445 N
Si1 O1 O2 54.89(29) 1_555 . -304_444 N
Si1 O1 O3 38.40(29) 1_555 . 2_555 N
Si1 O1 O3 120.5(4) 1_555 . -3_555 N
Si1 O1 O4 172.6(4) 1_555 . -107_444 N
Si1 O1 O4 119.7(4) 1_555 . -111_444 N
Si1 O1 O4 48.2(4) 1_555 . 208_343 N
Si1 O1 O4 35.64(28) 1_555 . 209_343 N
Si1 O1 Og 111.4(5) 1_555 . -2_555 N
Si1 O1 Og 136.5(4) 1_555 . 212_445 N
Si1 O1 Og 82.0(4) 1_555 . -206_556 N
Si1 O1 Dg1 121.4(5) 1_555 . -2_555 N
Si1 O1 Dg1 90.5(4) 1_555 . -206_565 N
Si1 O1 Dg2 114.2(8) 1_555 . -2_555 N
Si1 O1 Oh 141.1(6) 1_555 . -2_555 N
Si1 O1 Oh 80.3(5) 1_555 . -206_565 N
Si1 O1 Dh1 127.9(6) 1_555 . -2_555 N
Si1 O1 Dh1 83.7(5) 1_555 . -206_544 N
Si2 O1 Al1 0.0 -1_555 . -1_555 N
Si2 O1 O1 76.14(32) -1_555 . -2_555 N
Si2 O1 O1 80.7(4) -1_555 . -3_555 N
Si2 O1 O2 38.41(29) -1_555 . 105_544 N
Si2 O1 O2 108.21(32) -1_555 . -206_444 N
Si2 O1 O2 50.53(29) -1_555 . 304_445 N
Si2 O1 O2 93.85(29) -1_555 . -304_444 N
Si2 O1 O3 124.5(4) -1_555 . 2_555 N
Si2 O1 O3 30.79(30) -1_555 . -3_555 N
Si2 O1 O4 34.66(29) -1_555 . -107_444 N
Si2 O1 O4 53.7(4) -1_555 . -111_444 N
Si2 O1 O4 113.1(4) -1_555 . 208_343 N
Si2 O1 O4 167.6(5) -1_555 . 209_343 N
Si2 O1 Og 106.1(4) -1_555 . -2_555 N
Si2 O1 Og 84.4(4) -1_555 . 212_445 N
Si2 O1 Og 137.95(34) -1_555 . -206_556 N
Si2 O1 Dg1 99.1(5) -1_555 . -2_555 N
Si2 O1 Dg1 128.7(4) -1_555 . -206_565 N
Si2 O1 Dg2 104.0(7) -1_555 . -2_555 N
Si2 O1 Oh 71.9(5) -1_555 . -2_555 N
Si2 O1 Oh 139.2(5) -1_555 . -206_565 N
Si2 O1 Dh1 86.5(5) -1_555 . -2_555 N
Si2 O1 Dh1 137.4(5) -1_555 . -206_544 N
Al1 O1 O1 76.14(32) -1_555 . -2_555 N
Al1 O1 O1 80.7(4) -1_555 . -3_555 N
Al1 O1 O2 38.41(29) -1_555 . 105_544 N
Al1 O1 O2 108.21(32) -1_555 . -206_444 N
Al1 O1 O2 50.53(29) -1_555 . 304_445 N
Al1 O1 O2 93.85(29) -1_555 . -304_444 N
Al1 O1 O3 124.5(4) -1_555 . 2_555 N
Al1 O1 O3 30.79(30) -1_555 . -3_555 N
Al1 O1 O4 34.66(29) -1_555 . -107_444 N
Al1 O1 O4 53.7(4) -1_555 . -111_444 N
Al1 O1 O4 113.1(4) -1_555 . 208_343 N
Al1 O1 O4 167.6(5) -1_555 . 209_343 N
Al1 O1 Og 106.1(4) -1_555 . -2_555 N
Al1 O1 Og 84.4(4) -1_555 . 212_445 N
Al1 O1 Og 137.95(34) -1_555 . -206_556 N
Al1 O1 Dg1 99.1(5) -1_555 . -2_555 N
Al1 O1 Dg1 128.7(4) -1_555 . -206_565 N
Al1 O1 Dg2 104.0(7) -1_555 . -2_555 N
Al1 O1 Oh 71.9(5) -1_555 . -2_555 N
Al1 O1 Oh 139.2(5) -1_555 . -206_565 N
Al1 O1 Dh1 86.5(5) -1_555 . -2_555 N
Al1 O1 Dh1 137.4(5) -1_555 . -206_544 N
O1 O1 O1 119.866(28) -2_555 . -3_555 N
O1 O1 O2 89.51(16) -2_555 . 105_544 N
O1 O1 O2 47.98(17) -2_555 . -206_444 N
O1 O1 O2 34.73(11) -2_555 . 304_445 N
O1 O1 O2 90.51(9) -2_555 . -304_444 N
O1 O1 O3 107.04(23) -2_555 . 2_555 N
O1 O1 O3 46.36(15) -2_555 . -3_555 N
O1 O1 O4 100.42(23) -2_555 . -107_444 N
O1 O1 O4 121.44(21) -2_555 . -111_444 N
O1 O1 O4 36.97(19) -2_555 . 208_343 N
O1 O1 O4 91.5(4) -2_555 . 209_343 N
O1 O1 Og 105.6(4) -2_555 . -2_555 N
O1 O1 Og 130.18(24) -2_555 . 212_445 N
O1 O1 Og 113.40(31) -2_555 . -206_556 N
O1 O1 Dg1 119.1(4) -2_555 . -2_555 N
O1 O1 Dg1 111.6(4) -2_555 . -206_565 N
O1 O1 Dg2 107.5(7) -2_555 . -2_555 N
O1 O1 Oh 92.95(35) -2_555 . -2_555 N
O1 O1 Oh 136.2(5) -2_555 . -206_565 N
O1 O1 Dh1 96.3(6) -2_555 . -2_555 N
O1 O1 Dh1 127.8(6) -2_555 . -206_544 N
O1 O1 O2 44.46(17) -3_555 . 105_544 N
O1 O1 O2 90.90(15) -3_555 . -206_444 N
O1 O1 O2 89.71(9) -3_555 . 304_445 N
O1 O1 O2 36.81(10) -3_555 . -304_444 N
O1 O1 O3 48.78(15) -3_555 . 2_555 N
O1 O1 O3 103.34(25) -3_555 . -3_555 N
O1 O1 O4 89.47(34) -3_555 . -107_444 N
O1 O1 O4 34.57(20) -3_555 . -111_444 N
O1 O1 O4 124.59(20) -3_555 . 208_343 N
O1 O1 O4 106.79(24) -3_555 . 209_343 N
O1 O1 Og 134.1(4) -3_555 . -2_555 N
O1 O1 Og 100.98(32) -3_555 . 212_445 N
O1 O1 Og 120.72(22) -3_555 . -206_556 N
O1 O1 Dg1 119.0(5) -3_555 . -2_555 N
O1 O1 Dg1 126.0(4) -3_555 . -206_565 N
O1 O1 Dg2 131.8(8) -3_555 . -2_555 N
O1 O1 Oh 130.4(5) -3_555 . -2_555 N
O1 O1 Oh 95.4(4) -3_555 . -206_565 N
O1 O1 Dh1 136.8(7) -3_555 . -2_555 N
O1 O1 Dh1 106.5(5) -3_555 . -206_544 N
O2 O1 O2 93.07(18) 105_544 . -206_444 N
O2 O1 O2 54.79(15) 105_544 . 304_445 N
O2 O1 O2 57.46(14) 105_544 . -304_444 N
O2 O1 O3 86.20(20) 105_544 . 2_555 N
O2 O1 O3 59.14(18) 105_544 . -3_555 N
O2 O1 O4 61.94(20) 105_544 . -107_444 N
O2 O1 O4 32.47(14) 105_544 . -111_444 N
O2 O1 O4 118.31(17) 105_544 . 208_343 N
O2 O1 O4 144.48(21) 105_544 . 209_343 N
O2 O1 Og 137.4(4) 105_544 . -2_555 N
O2 O1 Og 102.83(31) 105_544 . 212_445 N
O2 O1 Og 156.10(29) 105_544 . -206_556 N
O2 O1 Dg1 123.9(5) 105_544 . -2_555 N
O2 O1 Dg1 153.1(4) 105_544 . -206_565 N
O2 O1 Dg2 134.3(7) 105_544 . -2_555 N
O2 O1 Oh 107.0(4) 105_544 . -2_555 N
O2 O1 Oh 133.9(5) 105_544 . -206_565 N
O2 O1 Dh1 121.1(5) 105_544 . -2_555 N
O2 O1 Dh1 142.6(5) 105_544 . -206_544 N
O2 O1 O2 58.36(16) -206_444 . 304_445 N
O2 O1 O2 54.10(15) -206_444 . -304_444 N
O2 O1 O3 59.60(18) -206_444 . 2_555 N
O2 O1 O3 87.16(21) -206_444 . -3_555 N
O2 O1 O4 142.00(21) -206_444 . -107_444 N
O2 O1 O4 117.93(17) -206_444 . -111_444 N
O2 O1 O4 33.83(15) -206_444 . 208_343 N
O2 O1 O4 62.57(23) -206_444 . 209_343 N
O2 O1 Og 126.8(4) -206_556 . -2_555 N
O2 O1 Og 164.07(30) -206_556 . 212_445 N
O2 O1 Og 107.14(29) -206_556 . -206_556 N
O2 O1 Dg1 142.5(5) -206_565 . -2_555 N
O2 O1 Dg1 113.3(4) -206_565 . -206_565 N
O2 O1 Dg2 130.0(8) -206_566 . -2_555 N
O2 O1 Oh 136.4(4) -206_565 . -2_555 N
O2 O1 Oh 112.4(4) -206_565 . -206_565 N
O2 O1 Dh1 132.3(6) -206_544 . -2_555 N
O2 O1 Dh1 113.5(5) -206_544 . -206_544 N
O2 O1 O2 72.03(9) 304_445 . -304_444 N
O2 O1 O3 101.02(12) 304_445 . 2_555 N
O2 O1 O3 31.76(10) 304_445 . -3_555 N
O2 O1 O4 83.64(14) 304_445 . -107_444 N
O2 O1 O4 86.93(12) 304_445 . -111_444 N
O2 O1 O4 67.26(12) 304_445 . 208_343 N
O2 O1 O4 118.60(25) 304_445 . 209_343 N
O2 O1 Og 130.20(33) 304_445 . -2_555 N
O2 O1 Og 131.43(22) 304_445 . 212_445 N
O2 O1 Og 147.83(24) 304_445 . -206_556 N
O2 O1 Dg1 136.2(4) 304_445 . -2_555 N
O2 O1 Dg1 144.3(4) 304_445 . -206_565 N
O2 O1 Dg2 130.6(6) 304_445 . -2_555 N
O2 O1 Oh 102.65(33) 304_445 . -2_555 N
O2 O1 Oh 169.7(5) 304_445 . -206_565 N
O2 O1 Dh1 113.1(6) 304_445 . -2_555 N
O2 O1 Dh1 162.4(5) 304_445 . -206_544 N
O2 O1 O3 32.50(11) -304_444 . 2_555 N
O2 O1 O3 99.70(11) -304_444 . -3_555 N
O2 O1 O4 118.15(22) -304_444 . -107_444 N
O2 O1 O4 67.51(12) -304_444 . -111_444 N
O2 O1 O4 87.80(12) -304_444 . 208_343 N
O2 O1 O4 87.03(15) -304_444 . 209_343 N
O2 O1 Og 156.72(31) -304_556 . -2_555 N
O2 O1 Og 136.75(27) -304_556 . 212_445 N
O2 O1 Og 125.52(21) -304_556 . -206_556 N
O2 O1 Dg1 149.7(4) -304_565 . -2_555 N
O2 O1 Dg1 134.82(30) -304_565 . -206_565 N
O2 O1 Dg2 157.1(6) -304_566 . -2_555 N
O2 O1 Oh 164.0(5) -304_565 . -2_555 N
O2 O1 Oh 107.1(4) -304_565 . -206_565 N
O2 O1 Dh1 173.1(6) -304_544 . -2_555 N
O2 O1 Dh1 117.3(5) -304_544 . -206_544 N
O3 O1 O3 131.28(16) 2_555 . -3_555 N
O3 O1 O4 137.5(4) 2_555 . -107_444 N
O3 O1 O4 82.98(22) 2_555 . -111_444 N
O3 O1 O4 85.57(22) 2_555 . 208_343 N
O3 O1 O4 59.63(18) 2_555 . 209_343 N
O3 O1 Og 124.56(31) 2_555 . -2_555 N
O3 O1 Og 121.64(24) 2_555 . 212_445 N
O3 O1 Og 93.04(24) 2_555 . -206_556 N
O3 O1 Dg1 122.8(4) 2_555 . -2_555 N
O3 O1 Dg1 102.31(32) 2_555 . -206_565 N
O3 O1 Dg2 125.5(6) 2_555 . -2_555 N
O3 O1 Oh 156.33(34) 2_555 . -2_555 N
O3 O1 Oh 75.9(4) 2_555 . -206_565 N
O3 O1 Dh1 144.5(5) 2_555 . -2_555 N
O3 O1 Dh1 85.4(5) 2_555 . -206_544 N
O3 O1 O4 55.94(17) -3_555 . -107_444 N
O3 O1 O4 83.21(21) -3_555 . -111_444 N
O3 O1 O4 83.05(22) -3_555 . 208_343 N
O3 O1 O4 136.9(4) -3_555 . 209_343 N
O3 O1 Og 103.58(32) -3_555 . -2_555 N
O3 O1 Og 100.19(24) -3_555 . 212_445 N
O3 O1 Og 132.70(23) -3_555 . -206_556 N
O3 O1 Dg1 105.5(4) -3_555 . -2_555 N
O3 O1 Dg1 124.33(33) -3_555 . -206_565 N
O3 O1 Dg2 103.0(6) -3_555 . -2_555 N
O3 O1 Oh 71.95(34) -3_555 . -2_555 N
O3 O1 Oh 152.8(4) -3_555 . -206_565 N
O3 O1 Dh1 84.1(5) -3_555 . -2_555 N
O3 O1 Dh1 143.0(5) -3_555 . -206_544 N
O4 O1 O4 54.90(19) -107_444 . -111_444 N
O4 O1 O4 133.08(21) -107_444 . 208_343 N
O4 O1 O4 151.68(19) -107_444 . 209_343 N
O4 O1 Og 76.03(32) -107_556 . -2_555 N
O4 O1 Og 49.72(20) -107_556 . 212_445 N
O4 O1 Og 105.16(20) -107_556 . -206_556 N
O4 O1 Dg1 65.8(4) -107_565 . -2_555 N
O4 O1 Dg1 96.76(26) -107_565 . -206_565 N
O4 O1 Dg2 73.3(6) -107_566 . -2_555 N
O4 O1 Oh 45.9(4) -107_565 . -2_555 N
O4 O1 Oh 105.3(4) -107_565 . -206_565 N
O4 O1 Dh1 59.3(4) -107_544 . -2_555 N
O4 O1 Dh1 102.7(4) -107_544 . -206_544 N
O4 O1 O4 149.12(8) -111_444 . 208_343 N
O4 O1 O4 136.93(22) -111_444 . 209_343 N
O4 O1 Og 115.1(4) -111_556 . -2_555 N
O4 O1 Og 77.23(24) -111_556 . 212_445 N
O4 O1 Og 123.71(20) -111_556 . -206_556 N
O4 O1 Dg1 98.8(4) -111_565 . -2_555 N
O4 O1 Dg1 122.45(32) -111_565 . -206_565 N
O4 O1 Dg2 111.9(7) -111_566 . -2_555 N
O4 O1 Oh 97.5(4) -111_565 . -2_555 N
O4 O1 Oh 102.3(4) -111_565 . -206_565 N
O4 O1 Dh1 107.5(6) -111_544 . -2_555 N
O4 O1 Dh1 110.2(5) -111_544 . -206_544 N
O4 O1 O4 54.55(21) 208_343 . 209_343 N
O4 O1 Og 95.0(4) 208_455 . -2_555 N
O4 O1 Og 132.51(23) 208_455 . 212_445 N
O4 O1 Og 85.39(21) 208_455 . -206_556 N
O4 O1 Dg1 111.5(4) 208_464 . -2_555 N
O4 O1 Dg1 87.99(31) 208_464 . -206_565 N
O4 O1 Dg2 98.1(7) 208_465 . -2_555 N
O4 O1 Oh 104.2(4) 208_464 . -2_555 N
O4 O1 Oh 102.5(4) 208_464 . -206_565 N
O4 O1 Dh1 98.4(6) 208_443 . -2_555 N
O4 O1 Dh1 97.3(5) 208_443 . -206_544 N
O4 O1 Og 76.05(32) 209_455 . -2_555 N
O4 O1 Og 103.42(20) 209_455 . 212_445 N
O4 O1 Og 46.64(20) 209_455 . -206_556 N
O4 O1 Dg1 86.0(4) 209_464 . -2_555 N
O4 O1 Dg1 54.92(27) 209_464 . -206_565 N
O4 O1 Dg2 78.7(6) 209_465 . -2_555 N
O4 O1 Oh 108.4(4) 209_464 . -2_555 N
O4 O1 Oh 51.3(4) 209_464 . -206_565 N
O4 O1 Dh1 94.1(4) 209_443 . -2_555 N
O4 O1 Dh1 50.9(4) 209_443 . -206_544 N
Og O1 Og 37.8(4) -2_555 . 212_445 N
Og O1 Og 32.4(4) -2_555 . -206_556 N
Og O1 Dg1 16.49(19) -2_555 . -2_555 N
Og O1 Dg1 22.92(34) -2_555 . -206_565 N
Og O1 Dg2 3.2(6) -2_555 . -2_555 N
Og O1 Oh 34.5(4) -2_555 . -2_555 N
Og O1 Oh 49.7(4) -2_555 . -206_565 N
Og O1 Dh1 20.3(5) -2_555 . -2_555 N
Og O1 Dh1 39.4(5) -2_555 . -206_544 N
Og O1 Og 57.61(33) 212_445 . -206_556 N
Og O1 Dg1 21.7(5) 212_454 . -2_555 N
Og O1 Dg1 51.0(4) 212_454 . -206_565 N
Og O1 Dg2 34.7(7) 212_455 . -2_555 N
Og O1 Oh 37.23(34) 212_454 . -2_555 N
Og O1 Oh 56.3(4) 212_454 . -206_565 N
Og O1 Dh1 36.4(6) 212_433 . -2_555 N
Og O1 Dh1 53.1(4) 212_433 . -206_544 N
Og O1 Dg1 39.4(4) -206_565 . -2_555 N
Og O1 Dg1 9.45(22) -206_565 . -206_565 N
Og O1 Dg2 34.2(6) -206_566 . -2_555 N
Og O1 Oh 66.9(4) -206_565 . -2_555 N
Og O1 Oh 25.4(4) -206_565 . -206_565 N
Og O1 Dh1 52.6(5) -206_544 . -2_555 N
Og O1 Dh1 14.7(5) -206_544 . -206_544 N
Dg1 O1 Dg1 31.2(5) -2_555 . -206_565 N
Dg1 O1 Dg2 13.5(8) -2_555 . -2_555 N
Dg1 O1 Oh 33.6(5) -2_555 . -2_555 N
Dg1 O1 Oh 47.5(5) -2_555 . -206_565 N
Dg1 O1 Dh1 24.0(7) -2_555 . -2_555 N
Dg1 O1 Dh1 40.0(6) -2_555 . -206_544 N
Dg1 O1 Dg2 24.8(5) -206_566 . -2_555 N
Dg1 O1 Oh 57.4(4) -206_565 . -2_555 N
Dg1 O1 Oh 31.4(4) -206_565 . -206_565 N
Dg1 O1 Dh1 43.1(5) -206_544 . -2_555 N
Dg1 O1 Dh1 20.0(5) -206_544 . -206_544 N
Dg2 O1 Oh 32.8(6) -2_555 . -2_555 N
Dg2 O1 Oh 50.1(7) -2_555 . -206_565 N
Dg2 O1 Dh1 19.0(7) -2_555 . -2_555 N
Dg2 O1 Dh1 40.1(7) -2_555 . -206_544 N
Oh O1 Oh 80.9(7) -2_555 . -206_565 N
Oh O1 Dh1 14.58(15) -2_555 . -2_555 N
Oh O1 Dh1 72.1(7) -2_555 . -206_544 N
Oh O1 Dh1 68.7(8) -206_544 . -2_555 N
Oh O1 Dh1 11.4(4) -206_544 . -206_544 N
Dh1 O1 Dh1 59.1(9) -2_555 . -206_544 N
Si1 O2 Si2 138.86(32) 111_533 . 208_443 N
Si1 O2 Al1 138.86(32) 111_443 . 208_353 N
Si1 O2 O1 55.54(30) 111_433 . 4_555 N
Si1 O2 O1 33.44(28) 111_433 . 111_433 N
Si1 O2 O1 115.95(32) 111_433 . -108_544 N
Si1 O2 O1 155.78(32) 111_433 . -304_444 N
Si1 O2 O2 85.2(4) 111_433 . 107_433 N
Si1 O2 O2 68.28(30) 111_433 . -109_544 N
Si1 O2 O2 145.0(4) 111_433 . 209_343 N
Si1 O2 O2 119.71(31) 111_433 . -207_454 N
Si1 O2 O2 82.46(31) 111_433 . -304_444 N
Si1 O2 O3 54.16(28) 111_433 . 2_555 N
Si1 O2 O3 116.73(29) 111_433 . 3_555 N
Si1 O2 O3 82.06(28) 111_433 . 4_555 N
Si1 O2 O3 169.59(35) 111_433 . 111_433 N
Si1 O2 O3 40.34(29) 111_433 . 208_343 N
Si1 O2 O4 113.91(30) 111_433 . 310_334 N
Si1 O2 O4 32.25(26) 111_433 . 312_334 N
Si1 O2 SI' 114.99(35) 111_433 . 111_433 N
Si1 O2 Og 34.90(29) 111_545 . -108_656 N
Si1 O2 Dg2 32.7(4) 111_555 . -108_666 N
Si1 O2 Dg2 115.1(4) 111_555 . -304_566 N
Si1 O2 Oh 10.9(4) 111_554 . 1_555 N
Si1 O2 Dh2 16.0(5) 111_533 . 1_555 N
Si2 O2 Al1 0.0 208_353 . 208_353 N
Si2 O2 O1 153.19(31) 208_343 . 4_555 N
Si2 O2 O1 121.64(33) 208_343 . 111_433 N
Si2 O2 O1 37.72(29) 208_343 . -108_544 N
Si2 O2 O1 49.21(28) 208_343 . -304_444 N
Si2 O2 O2 135.59(34) 208_343 . 107_433 N
Si2 O2 O2 120.80(30) 208_343 . -109_544 N
Si2 O2 O2 75.62(34) 208_343 . 209_343 N
Si2 O2 O2 65.73(28) 208_343 . -207_454 N
Si2 O2 O2 78.80(31) 208_343 . -304_444 N
Si2 O2 O3 116.21(29) 208_343 . 2_555 N
Si2 O2 O3 51.47(27) 208_343 . 3_555 N
Si2 O2 O3 83.81(29) 208_343 . 4_555 N
Si2 O2 O3 32.81(29) 208_343 . 111_433 N
Si2 O2 O3 172.66(32) 208_343 . 208_343 N
Si2 O2 O4 32.91(27) 208_343 . 310_334 N
Si2 O2 O4 116.22(30) 208_343 . 312_334 N
Si2 O2 SI' 105.26(33) 208_343 . 111_433 N
Si2 O2 Og 105.90(31) 208_455 . -108_656 N
Si2 O2 Dg2 110.4(4) 208_465 . -108_666 N
Si2 O2 Dg2 28.2(4) 208_465 . -304_566 N
Si2 O2 Oh 129.9(4) 208_464 . 1_555 N
Si2 O2 Dh2 126.3(6) 208_443 . 1_555 N
Al1 O2 O1 153.19(31) 208_343 . 4_555 N
Al1 O2 O1 121.64(33) 208_343 . 111_433 N
Al1 O2 O1 37.72(29) 208_343 . -108_544 N
Al1 O2 O1 49.21(28) 208_343 . -304_444 N
Al1 O2 O2 135.59(34) 208_343 . 107_433 N
Al1 O2 O2 120.80(30) 208_343 . -109_544 N
Al1 O2 O2 75.62(34) 208_343 . 209_343 N
Al1 O2 O2 65.73(28) 208_343 . -207_454 N
Al1 O2 O2 78.80(31) 208_343 . -304_444 N
Al1 O2 O3 116.21(29) 208_343 . 2_555 N
Al1 O2 O3 51.47(27) 208_343 . 3_555 N
Al1 O2 O3 83.81(29) 208_343 . 4_555 N
Al1 O2 O3 32.81(29) 208_343 . 111_433 N
Al1 O2 O3 172.66(32) 208_343 . 208_343 N
Al1 O2 O4 32.91(27) 208_343 . 310_334 N
Al1 O2 O4 116.22(30) 208_343 . 312_334 N
Al1 O2 SI' 105.26(33) 208_343 . 111_433 N
Al1 O2 Og 105.90(31) 208_455 . -108_656 N
Al1 O2 Dg2 110.4(4) 208_465 . -108_666 N
Al1 O2 Dg2 28.2(4) 208_465 . -304_566 N
Al1 O2 Oh 129.9(4) 208_464 . 1_555 N
Al1 O2 Dh2 126.3(6) 208_443 . 1_555 N
O1 O2 O1 54.36(11) 4_555 . 111_433 N
O1 O2 O1 120.53(22) 4_555 . -108_544 N
O1 O2 O1 107.97(9) 4_555 . -304_444 N
O1 O2 O2 37.16(15) 4_555 . 107_433 N
O1 O2 O2 34.68(10) 4_555 . -109_544 N
O1 O2 O2 90.86(14) 4_555 . 209_343 N
O1 O2 O2 87.49(10) 4_555 . -207_454 N
O1 O2 O2 127.91(23) 4_555 . -304_444 N
O1 O2 O3 90.53(12) 4_555 . 2_555 N
O1 O2 O3 152.86(13) 4_555 . 3_555 N
O1 O2 O3 75.85(16) 4_555 . 4_555 N
O1 O2 O3 134.85(16) 4_555 . 111_433 N
O1 O2 O3 34.05(11) 4_555 . 208_343 N
O1 O2 O4 169.06(19) 4_555 . 310_334 N
O1 O2 O4 85.33(18) 4_555 . 312_334 N
O1 O2 SI' 72.40(19) 4_555 . 111_433 N
O1 O2 Og 78.92(21) 4_555 . -108_656 N
O1 O2 Dg2 72.23(31) 4_555 . -108_666 N
O1 O2 Dg2 135.94(26) 4_555 . -304_566 N
O1 O2 Oh 66.34(29) 4_555 . 1_555 N
O1 O2 Dh2 71.2(5) 4_555 . 1_555 N
O1 O2 O1 87.56(9) 111_433 . -108_544 N
O1 O2 O1 123.65(23) 111_433 . -304_444 N
O1 O2 O2 91.52(25) 111_433 . 107_433 N
O1 O2 O2 45.06(18) 111_433 . -109_544 N
O1 O2 O2 135.05(17) 111_433 . 209_343 N
O1 O2 O2 86.95(17) 111_433 . -207_454 N
O1 O2 O2 106.73(23) 111_433 . -304_444 N
O1 O2 O3 86.55(18) 111_433 . 2_555 N
O1 O2 O3 136.06(19) 111_433 . 3_555 N
O1 O2 O3 48.66(14) 111_433 . 4_555 N
O1 O2 O3 148.06(22) 111_433 . 111_433 N
O1 O2 O3 61.99(21) 111_433 . 208_343 N
O1 O2 O4 115.59(20) 111_433 . 310_334 N
O1 O2 O4 58.79(20) 111_433 . 312_334 N
O1 O2 SI' 126.76(28) 111_433 . 111_433 N
O1 O2 Og 27.11(22) 111_545 . -108_656 N
O1 O2 Dg2 19.78(30) 111_555 . -108_666 N
O1 O2 Dg2 93.43(29) 111_555 . -304_566 N
O1 O2 Oh 38.53(29) 111_554 . 1_555 N
O1 O2 Dh2 42.8(4) 111_533 . 1_555 N
O1 O2 O1 53.68(11) -108_544 . -304_444 N
O1 O2 O2 131.85(18) -108_544 . 107_433 N
O1 O2 O2 85.85(16) -108_544 . -109_544 N
O1 O2 O2 88.05(25) -108_544 . 209_343 N
O1 O2 O2 41.87(18) -108_544 . -207_454 N
O1 O2 O2 104.07(23) -108_544 . -304_444 N
O1 O2 O3 135.49(20) -108_544 . 2_555 N
O1 O2 O3 86.56(18) -108_544 . 3_555 N
O1 O2 O3 46.19(14) -108_544 . 4_555 N
O1 O2 O3 61.21(19) -108_544 . 111_433 N
O1 O2 O3 148.17(21) -108_544 . 208_343 N
O1 O2 O4 59.28(18) -108_544 . 310_334 N
O1 O2 O4 114.31(20) -108_544 . 312_334 N
O1 O2 SI' 123.27(29) -108_544 . 111_433 N
O1 O2 Og 82.01(22) -108_656 . -108_656 N
O1 O2 Dg2 83.30(29) -108_666 . -108_666 N
O1 O2 Dg2 17.44(28) -108_666 . -304_566 N
O1 O2 Oh 112.94(29) -108_665 . 1_555 N
O1 O2 Dh2 112.8(5) -108_644 . 1_555 N
O1 O2 O2 88.83(15) -304_444 . 107_433 N
O1 O2 O2 88.28(10) -304_444 . -109_544 N
O1 O2 O2 34.38(16) -304_444 . 209_343 N
O1 O2 O2 36.70(10) -304_444 . -207_454 N
O1 O2 O2 120.19(23) -304_444 . -304_444 N
O1 O2 O3 149.75(13) -304_444 . 2_555 N
O1 O2 O3 85.98(12) -304_444 . 3_555 N
O1 O2 O3 76.17(16) -304_444 . 4_555 N
O1 O2 O3 31.86(10) -304_444 . 111_433 N
O1 O2 O3 135.56(18) -304_444 . 208_343 N
O1 O2 O4 80.94(17) -304_444 . 310_334 N
O1 O2 O4 165.23(19) -304_444 . 312_334 N
O1 O2 SI' 69.63(20) -304_444 . 111_433 N
O1 O2 Og 132.79(21) -304_556 . -108_656 N
O1 O2 Dg2 131.18(29) -304_566 . -108_666 N
O1 O2 Dg2 62.27(31) -304_566 . -304_566 N
O1 O2 Oh 161.82(28) -304_565 . 1_555 N
O1 O2 Dh2 164.6(5) -304_544 . 1_555 N
O2 O2 O2 61.35(5) 107_433 . -109_544 N
O2 O2 O2 60.00000(30) 107_433 . 209_343 N
O2 O2 O2 90.00000(20) 107_433 . -207_454 N
O2 O2 O2 122.04(14) 107_433 . -304_444 N
O2 O2 O3 92.40(16) 107_433 . 2_555 N
O2 O2 O3 123.63(9) 107_433 . 3_555 N
O2 O2 O3 101.58(10) 107_433 . 4_555 N
O2 O2 O3 104.09(17) 107_433 . 111_433 N
O2 O2 O3 47.30(18) 107_433 . 208_343 N
O2 O2 O4 152.31(17) 107_433 . 310_334 N
O2 O2 O4 105.86(25) 107_433 . 312_334 N
O2 O2 SI' 35.26(12) 107_433 . 111_433 N
O2 O2 Og 114.96(26) 107_545 . -108_656 N
O2 O2 Dg2 108.8(4) 107_555 . -108_666 N
O2 O2 Dg2 147.90(32) 107_555 . -304_566 N
O2 O2 Oh 94.52(32) 107_554 . 1_555 N
O2 O2 Dh2 98.0(5) 107_533 . 1_555 N
O2 O2 O2 90.00000(20) -109_544 . 209_343 N
O2 O2 O2 57.29(10) -109_544 . -207_454 N
O2 O2 O2 150.44(25) -109_544 . -304_444 N
O2 O2 O3 118.62(13) -109_544 . 2_555 N
O2 O2 O3 172.25(12) -109_544 . 3_555 N
O2 O2 O3 42.16(13) -109_544 . 4_555 N
O2 O2 O3 120.13(14) -109_544 . 111_433 N
O2 O2 O3 66.46(9) -109_544 . 208_343 N
O2 O2 O4 142.98(15) -109_544 . 310_334 N
O2 O2 O4 99.97(20) -109_544 . 312_334 N
O2 O2 SI' 90.94(20) -109_544 . 111_433 N
O2 O2 Og 71.39(20) -109_656 . -108_656 N
O2 O2 Dg2 64.21(30) -109_666 . -108_666 N
O2 O2 Dg2 101.61(24) -109_666 . -304_566 N
O2 O2 Oh 77.78(29) -109_665 . 1_555 N
O2 O2 Dh2 83.0(5) -109_644 . 1_555 N
O2 O2 O2 61.35(5) 209_343 . -207_454 N
O2 O2 O2 117.71(18) 209_343 . -304_444 N
O2 O2 O3 125.29(8) 209_343 . 2_555 N
O2 O2 O3 88.20(16) 209_343 . 3_555 N
O2 O2 O3 100.33(10) 209_343 . 4_555 N
O2 O2 O3 44.85(17) 209_343 . 111_433 N
O2 O2 O3 106.50(17) 209_343 . 208_343 N
O2 O2 O4 100.02(25) 209_343 . 310_334 N
O2 O2 O4 155.93(14) 209_343 . 312_334 N
O2 O2 SI' 35.26(12) 209_343 . 111_433 N
O2 O2 Og 159.40(16) 209_455 . -108_656 N
O2 O2 Dg2 153.24(27) 209_465 . -108_666 N
O2 O2 Dg2 95.4(4) 209_465 . -304_566 N
O2 O2 Oh 154.46(31) 209_464 . 1_555 N
O2 O2 Dh2 157.3(5) 209_443 . 1_555 N
O2 O2 O2 143.80(25) -207_454 . -304_444 N
O2 O2 O3 173.13(10) -207_454 . 2_555 N
O2 O2 O3 115.45(13) -207_454 . 3_555 N
O2 O2 O3 40.37(13) -207_454 . 4_555 N
O2 O2 O3 65.72(9) -207_454 . 111_433 N
O2 O2 O3 121.54(14) -207_454 . 208_343 N
O2 O2 O4 96.68(18) -207_454 . 310_334 N
O2 O2 O4 141.87(15) -207_454 . 312_334 N
O2 O2 SI' 90.94(20) -207_454 . 111_433 N
O2 O2 Og 100.01(18) -207_566 . -108_656 N
O2 O2 Dg2 96.48(27) -207_576 . -108_666 N
O2 O2 Dg2 58.67(29) -207_576 . -304_566 N
O2 O2 Oh 125.30(27) -207_575 . 1_555 N
O2 O2 Dh2 129.0(4) -207_554 . 1_555 N
O2 O2 O3 37.41(13) -304_444 . 2_555 N
O2 O2 O3 34.34(13) -304_444 . 3_555 N
O2 O2 O3 131.92(8) -304_444 . 4_555 N
O2 O2 O3 88.55(22) -304_444 . 111_433 N
O2 O2 O3 94.11(22) -304_444 . 208_343 N
O2 O2 O4 47.13(16) -304_444 . 310_334 N
O2 O2 O4 50.51(16) -304_444 . 312_334 N
O2 O2 SI' 105.68(24) -304_444 . 111_433 N
O2 O2 Og 82.35(19) -304_556 . -108_656 N
O2 O2 Dg2 88.99(29) -304_566 . -108_666 N
O2 O2 Dg2 86.65(28) -304_566 . -304_566 N
O2 O2 Oh 72.70(32) -304_565 . 1_555 N
O2 O2 Dh2 67.5(5) -304_544 . 1_555 N
O3 O2 O3 68.29(8) 2_555 . 3_555 N
O3 O2 O3 132.76(16) 2_555 . 4_555 N
O3 O2 O3 119.77(13) 2_555 . 111_433 N
O3 O2 O3 56.71(14) 2_555 . 208_343 N
O3 O2 O4 84.14(14) 2_555 . 310_334 N
O3 O2 O4 31.30(12) 2_555 . 312_334 N
O3 O2 SI' 94.73(22) 2_555 . 111_433 N
O3 O2 Og 73.14(17) 2_555 . -108_656 N
O3 O2 Dg2 76.65(26) 2_555 . -108_666 N
O3 O2 Dg2 119.54(28) 2_555 . -304_566 N
O3 O2 Oh 48.08(26) 2_555 . 1_555 N
O3 O2 Dh2 44.2(4) 2_555 . 1_555 N
O3 O2 O3 130.95(17) 3_555 . 4_555 N
O3 O2 O3 54.22(14) 3_555 . 111_433 N
O3 O2 O3 121.26(13) 3_555 . 208_343 N
O3 O2 O4 30.54(11) 3_555 . 310_334 N
O3 O2 O4 84.58(15) 3_555 . 312_334 N
O3 O2 SI' 91.93(22) 3_555 . 111_433 N
O3 O2 Og 109.04(19) 3_555 . -108_656 N
O3 O2 Dg2 116.36(29) 3_555 . -108_666 N
O3 O2 Dg2 71.08(24) 3_555 . -304_566 N
O3 O2 Oh 106.70(29) 3_555 . 1_555 N
O3 O2 Dh2 101.4(4) 3_555 . 1_555 N
O3 O2 O3 100.30(17) 4_555 . 111_433 N
O3 O2 O3 102.51(17) 4_555 . 208_343 N
O3 O2 O4 100.83(15) 4_555 . 310_334 N
O3 O2 O4 101.74(15) 4_555 . 312_334 N
O3 O2 SI' 122.13(27) 4_555 . 111_433 N
O3 O2 Og 59.98(17) 4_555 . -108_656 N
O3 O2 Dg2 56.11(25) 4_555 . -108_666 N
O3 O2 Dg2 60.10(24) 4_555 . -304_566 N
O3 O2 Oh 85.65(27) 4_555 . 1_555 N
O3 O2 Dh2 88.9(5) 4_555 . 1_555 N
O3 O2 O3 146.48(17) 111_433 . 208_343 N
O3 O2 O4 55.73(18) 111_433 . 310_334 N
O3 O2 O4 138.01(21) 111_433 . 312_334 N
O3 O2 SI' 72.47(16) 111_433 . 111_433 N
O3 O2 Og 138.62(21) 111_545 . -108_656 N
O3 O2 Dg2 142.56(31) 111_555 . -108_666 N
O3 O2 Dg2 58.89(28) 111_555 . -304_566 N
O3 O2 Oh 158.75(31) 111_554 . 1_555 N
O3 O2 Dh2 153.7(5) 111_533 . 1_555 N
O3 O2 O4 140.53(20) 208_343 . 310_334 N
O3 O2 O4 59.20(17) 208_343 . 312_334 N
O3 O2 SI' 74.67(16) 208_343 . 111_433 N
O3 O2 Og 74.68(20) 208_455 . -108_656 N
O3 O2 Dg2 70.95(31) 208_465 . -108_666 N
O3 O2 Dg2 154.58(31) 208_465 . -304_566 N
O3 O2 Oh 48.07(28) 208_464 . 1_555 N
O3 O2 Dh2 51.0(5) 208_443 . 1_555 N
O4 O2 O4 85.17(15) 310_334 . 312_334 N
O4 O2 SI' 117.48(25) 310_334 . 111_433 N
O4 O2 Og 90.38(19) 310_446 . -108_656 N
O4 O2 Dg2 97.20(30) 310_456 . -108_666 N
O4 O2 Dg2 42.35(25) 310_456 . -304_566 N
O4 O2 Oh 103.21(30) 310_455 . 1_555 N
O4 O2 Dh2 98.5(5) 310_434 . 1_555 N
O4 O2 SI' 121.98(24) 312_334 . 111_433 N
O4 O2 Og 41.87(18) 312_446 . -108_656 N
O4 O2 Dg2 45.80(26) 312_456 . -108_666 N
O4 O2 Dg2 103.79(29) 312_456 . -304_566 N
O4 O2 Oh 22.20(31) 312_455 . 1_555 N
O4 O2 Dh2 17.0(4) 312_434 . 1_555 N
SI' O2 Og 148.77(26) 111_545 . -108_656 N
SI' O2 Dg2 143.4(4) 111_555 . -108_666 N
SI' O2 Dg2 129.6(4) 111_555 . -304_566 N
SI' O2 Oh 121.57(30) 111_554 . 1_555 N
SI' O2 Dh2 123.0(5) 111_533 . 1_555 N
Og O2 Dg2 7.33(21) -108_666 . -108_666 N
Og O2 Dg2 80.26(23) -108_666 . -304_566 N
Og O2 Oh 31.08(27) -108_665 . 1_555 N
Og O2 Dh2 32.0(5) -108_644 . 1_555 N
Dg2 O2 Dg2 83.67(7) -108_666 . -304_566 N
Dg2 O2 Oh 31.33(33) -108_665 . 1_555 N
Dg2 O2 Dh2 33.5(5) -108_644 . 1_555 N
Dg2 O2 Oh 108.9(4) -304_565 . 1_555 N
Dg2 O2 Dh2 107.1(5) -304_544 . 1_555 N
Oh O2 Dh2 5.31(31) 1_555 . 1_555 N
Si1 O3 Si2 142.35(31) 3_555 . 2_555 N
Si1 O3 Al1 142.35(31) 3_555 . 2_555 N
Si1 O3 O1 33.32(30) 3_555 . 3_555 N
Si1 O3 O1 115.53(30) 3_555 . -2_555 N
Si1 O3 O2 50.27(25) 3_555 . 2_555 N
Si1 O3 O2 153.09(26) 3_555 . 3_555 N
Si1 O3 O2 34.82(23) 3_555 . -105_444 N
Si1 O3 O2 119.26(26) 3_555 . -206_444 N
Si1 O3 O2 72.66(25) 3_555 . 304_445 N
Si1 O3 O3 137.75(33) 3_555 . 107_433 N
Si1 O3 O3 77.88(34) 3_555 . 209_343 N
Si1 O3 O4 36.79(26) 3_555 . 111_433 N
Si1 O3 O4 174.30(30) 3_555 . 208_343 N
Si1 O3 SII 107.97(33) 3_555 . 111_555 N
Si1 O3 Og 123.30(32) 3_555 . 3_555 N
Si1 O3 Og 38.77(29) 3_555 . -1_555 N
Si1 O3 Dg2 124.2(4) 3_555 . 3_555 N
Si1 O3 Dg2 37.1(4) 3_555 . -1_555 N
Si1 O3 Oh 131.7(4) 3_555 . 3_555 N
Si1 O3 Oh 66.2(4) 3_555 . -105_565 N
Si1 O3 Dh1 126.6(5) 3_555 . 3_555 N
Si1 O3 Dh2 143.3(5) 3_555 . 3_555 N
Si1 O3 Dh2 55.9(7) 3_555 . -105_544 N
Si1 O3 OII' 76.89(31) 3_555 . 107_533 N
Si2 O3 Al1 0.0 2_555 . 2_555 N
Si2 O3 O1 117.4(4) 2_555 . 3_555 N
Si2 O3 O1 34.22(34) 2_555 . -2_555 N
Si2 O3 O2 153.12(34) 2_555 . 2_555 N
Si2 O3 O2 51.39(31) 2_555 . 3_555 N
Si2 O3 O2 121.28(30) 2_555 . -105_444 N
Si2 O3 O2 37.20(28) 2_555 . -206_444 N
Si2 O3 O2 71.29(31) 2_555 . 304_445 N
Si2 O3 O3 79.3(4) 2_555 . 107_433 N
Si2 O3 O3 139.2(4) 2_555 . 209_343 N
Si2 O3 O4 173.6(4) 2_555 . 111_433 N
Si2 O3 O4 37.57(30) 2_555 . 208_343 N
Si2 O3 SII 109.2(4) 2_555 . 111_555 N
Si2 O3 Og 52.73(34) 2_555 . 3_555 N
Si2 O3 Og 133.3(4) 2_555 . -1_555 N
Si2 O3 Dg2 45.2(4) 2_555 . 3_555 N
Si2 O3 Dg2 128.9(4) 2_555 . -1_555 N
Si2 O3 Oh 66.4(4) 2_555 . 3_555 N
Si2 O3 Oh 129.1(5) 2_555 . -105_565 N
Si2 O3 Dh1 62.2(6) 2_555 . 3_555 N
Si2 O3 Dh2 56.7(6) 2_555 . 3_555 N
Si2 O3 Dh2 141.7(6) 2_555 . -105_544 N
Si2 O3 OII' 108.12(34) 2_555 . 107_533 N
Al1 O3 O1 117.4(4) 2_555 . 3_555 N
Al1 O3 O1 34.22(34) 2_555 . -2_555 N
Al1 O3 O2 153.12(34) 2_555 . 2_555 N
Al1 O3 O2 51.39(31) 2_555 . 3_555 N
Al1 O3 O2 121.28(30) 2_555 . -105_444 N
Al1 O3 O2 37.20(28) 2_555 . -206_444 N
Al1 O3 O2 71.29(31) 2_555 . 304_445 N
Al1 O3 O3 79.3(4) 2_555 . 107_433 N
Al1 O3 O3 139.2(4) 2_555 . 209_343 N
Al1 O3 O4 173.6(4) 2_555 . 111_433 N
Al1 O3 O4 37.57(30) 2_555 . 208_343 N
Al1 O3 SII 109.2(4) 2_555 . 111_555 N
Al1 O3 Og 52.73(34) 2_555 . 3_555 N
Al1 O3 Og 133.3(4) 2_555 . -1_555 N
Al1 O3 Dg2 45.2(4) 2_555 . 3_555 N
Al1 O3 Dg2 128.9(4) 2_555 . -1_555 N
Al1 O3 Oh 66.4(4) 2_555 . 3_555 N
Al1 O3 Oh 129.1(5) 2_555 . -105_565 N
Al1 O3 Dh1 62.2(6) 2_555 . 3_555 N
Al1 O3 Dh2 56.7(6) 2_555 . 3_555 N
Al1 O3 Dh2 141.7(6) 2_555 . -105_544 N
Al1 O3 OII' 108.12(34) 2_555 . 107_533 N
O1 O3 O1 84.86(10) 3_555 . -2_555 N
O1 O3 O2 82.35(25) 3_555 . 2_555 N
O1 O3 O2 168.32(21) 3_555 . 3_555 N
O1 O3 O2 58.41(22) 3_555 . -105_444 N
O1 O3 O2 115.64(15) 3_555 . -206_444 N
O1 O3 O2 47.60(17) 3_555 . 304_445 N
O1 O3 O3 154.20(17) 3_555 . 107_433 N
O1 O3 O3 101.90(29) 3_555 . 209_343 N
O1 O3 O4 58.47(24) 3_555 . 111_433 N
O1 O3 O4 141.75(26) 3_555 . 208_343 N
O1 O3 SII 119.63(25) 3_555 . 111_555 N
O1 O3 Og 91.17(28) 3_555 . 3_555 N
O1 O3 Og 27.71(17) 3_555 . -1_555 N
O1 O3 Dg2 91.0(4) 3_555 . 3_555 N
O1 O3 Dg2 20.98(23) 3_555 . -1_555 N
O1 O3 Oh 108.0(4) 3_555 . 3_555 N
O1 O3 Oh 59.81(34) 3_555 . -105_565 N
O1 O3 Dh1 98.5(4) 3_555 . 3_555 N
O1 O3 Dh2 117.5(5) 3_555 . 3_555 N
O1 O3 Dh2 56.5(6) 3_555 . -105_544 N
O1 O3 OII' 107.38(31) 3_555 . 107_533 N
O1 O3 O2 164.78(21) -2_555 . 2_555 N
O1 O3 O2 84.66(24) -2_555 . 3_555 N
O1 O3 O2 114.19(15) -2_555 . -105_444 N
O1 O3 O2 59.65(20) -2_555 . -206_444 N
O1 O3 O2 44.18(17) -2_555 . 304_445 N
O1 O3 O3 105.42(29) -2_555 . 107_433 N
O1 O3 O3 156.98(15) -2_555 . 209_343 N
O1 O3 O4 140.07(29) -2_555 . 111_433 N
O1 O3 O4 61.48(23) -2_555 . 208_343 N
O1 O3 SII 122.79(24) -2_555 . 111_555 N
O1 O3 Og 37.32(18) -2_555 . 3_555 N
O1 O3 Og 99.32(26) -2_555 . -1_555 N
O1 O3 Dg2 28.07(24) -2_555 . 3_555 N
O1 O3 Dg2 94.69(34) -2_555 . -1_555 N
O1 O3 Oh 64.67(35) -2_555 . 3_555 N
O1 O3 Oh 104.7(4) -2_555 . -105_565 N
O1 O3 Dh1 53.6(4) -2_555 . 3_555 N
O1 O3 Dh2 61.3(6) -2_555 . 3_555 N
O1 O3 Dh2 115.2(5) -2_555 . -105_544 N
O1 O3 OII' 132.40(18) -2_555 . 107_533 N
O2 O3 O2 107.19(11) 2_555 . 3_555 N
O2 O3 O2 51.55(15) 2_555 . -105_444 N
O2 O3 O2 119.41(16) 2_555 . -206_444 N
O2 O3 O2 120.64(13) 2_555 . 304_445 N
O2 O3 O3 89.62(12) 2_555 . 107_433 N
O2 O3 O3 36.11(12) 2_555 . 209_343 N
O2 O3 O4 33.27(12) 2_555 . 111_433 N
O2 O3 O4 133.19(15) 2_555 . 208_343 N
O2 O3 SII 71.19(18) 2_555 . 111_555 N
O2 O3 Og 150.82(18) 2_555 . 3_555 N
O2 O3 Og 72.62(19) 2_555 . -1_555 N
O2 O3 Dg2 159.81(29) 2_555 . 3_555 N
O2 O3 Dg2 76.00(32) 2_555 . -1_555 N
O2 O3 Oh 127.48(33) 2_555 . 3_555 N
O2 O3 Oh 75.8(4) 2_555 . -105_565 N
O2 O3 Dh1 136.7(5) 2_555 . 3_555 N
O2 O3 Dh2 132.7(6) 2_555 . 3_555 N
O2 O3 Dh2 63.7(5) 2_555 . -105_544 N
O2 O3 OII' 45.77(12) 2_555 . 107_533 N
O2 O3 O2 122.13(16) 3_555 . -105_444 N
O2 O3 O2 54.04(15) 3_555 . -206_444 N
O2 O3 O2 120.71(13) 3_555 . 304_445 N
O2 O3 O3 35.64(12) 3_555 . 107_433 N
O2 O3 O3 89.75(13) 3_555 . 209_343 N
O2 O3 O4 133.01(16) 3_555 . 111_433 N
O2 O3 O4 32.49(12) 3_555 . 208_343 N
O2 O3 SII 70.75(17) 3_555 . 111_555 N
O2 O3 Og 83.60(21) 3_555 . 3_555 N
O2 O3 Og 161.18(18) 3_555 . -1_555 N
O2 O3 Dg2 82.09(35) 3_555 . 3_555 N
O2 O3 Dg2 166.64(25) 3_555 . -1_555 N
O2 O3 Oh 71.9(4) 3_555 . 3_555 N
O2 O3 Oh 128.28(33) 3_555 . -105_565 N
O2 O3 Dh1 79.3(5) 3_555 . 3_555 N
O2 O3 Dh2 61.1(5) 3_555 . 3_555 N
O2 O3 Dh2 133.5(6) 3_555 . -105_544 N
O2 O3 OII' 76.28(22) 3_555 . 107_533 N
O2 O3 O2 87.84(16) -105_444 . -206_444 N
O2 O3 O2 73.17(13) -105_444 . 304_445 N
O2 O3 O3 131.97(13) -105_444 . 107_433 N
O2 O3 O3 87.64(21) -105_444 . 209_343 N
O2 O3 O4 61.72(17) -105_444 . 111_433 N
O2 O3 O4 150.18(20) -105_444 . 208_343 N
O2 O3 SII 122.74(25) -105_566 . 111_555 N
O2 O3 Og 143.89(23) -105_556 . 3_555 N
O2 O3 Og 73.15(22) -105_556 . -1_555 N
O2 O3 Dg2 138.33(30) -105_566 . 3_555 N
O2 O3 Dg2 70.27(32) -105_566 . -1_555 N
O2 O3 Oh 166.0(4) -105_565 . 3_555 N
O2 O3 Oh 100.4(4) -105_565 . -105_565 N
O2 O3 Dh1 156.4(4) -105_544 . 3_555 N
O2 O3 Dh2 174.8(6) -105_544 . 3_555 N
O2 O3 Dh2 89.1(6) -105_544 . -105_544 N
O2 O3 OII' 49.98(22) -105_544 . 107_533 N
O2 O3 O2 72.12(13) -206_444 . 304_445 N
O2 O3 O3 89.67(20) -206_444 . 107_433 N
O2 O3 O3 132.17(12) -206_444 . 209_343 N
O2 O3 O4 147.90(19) -206_444 . 111_433 N
O2 O3 O4 64.12(17) -206_444 . 208_343 N
O2 O3 SII 124.69(25) -206_566 . 111_555 N
O2 O3 Og 89.07(21) -206_556 . 3_555 N
O2 O3 Og 143.14(19) -206_556 . -1_555 N
O2 O3 Dg2 80.65(31) -206_566 . 3_555 N
O2 O3 Dg2 136.24(25) -206_566 . -1_555 N
O2 O3 Oh 102.40(34) -206_565 . 3_555 N
O2 O3 Oh 164.4(4) -206_565 . -105_565 N
O2 O3 Dh1 99.4(5) -206_544 . 3_555 N
O2 O3 Dh2 91.5(6) -206_544 . 3_555 N
O2 O3 Dh2 171.9(6) -206_544 . -105_544 N
O2 O3 OII' 74.03(12) -206_544 . 107_533 N
O2 O3 O3 149.38(25) 304_445 . 107_433 N
O2 O3 O3 149.26(25) 304_445 . 209_343 N
O2 O3 O4 105.49(20) 304_445 . 111_433 N
O2 O3 O4 105.15(19) 304_445 . 208_343 N
O2 O3 SII 154.05(26) 304_445 . 111_555 N
O2 O3 Og 71.66(21) 304_445 . 3_555 N
O2 O3 Og 72.23(19) 304_445 . -1_555 N
O2 O3 Dg2 65.17(29) 304_445 . 3_555 N
O2 O3 Dg2 65.51(26) 304_445 . -1_555 N
O2 O3 Oh 100.6(4) 304_445 . 3_555 N
O2 O3 Oh 97.4(4) 304_445 . -105_565 N
O2 O3 Dh1 87.6(4) 304_445 . 3_555 N
O2 O3 Dh2 101.8(6) 304_445 . 3_555 N
O2 O3 Dh2 99.8(6) 304_445 . -105_544 N
O2 O3 OII' 113.44(16) 304_445 . 107_533 N
O3 O3 O3 60.00000(30) 107_433 . 209_343 N
O3 O3 O4 102.89(16) 107_433 . 111_433 N
O3 O3 O4 44.23(16) 107_433 . 208_343 N
O3 O3 SII 35.13(11) 107_555 . 111_555 N
O3 O3 Og 83.96(23) 107_545 . 3_555 N
O3 O3 Og 126.58(19) 107_545 . -1_555 N
O3 O3 Dg2 88.15(34) 107_555 . 3_555 N
O3 O3 Dg2 133.23(24) 107_555 . -1_555 N
O3 O3 Oh 58.6(4) 107_554 . 3_555 N
O3 O3 Oh 94.47(32) 107_554 . -105_565 N
O3 O3 Dh1 71.0(4) 107_533 . 3_555 N
O3 O3 Dh2 53.1(5) 107_533 . 3_555 N
O3 O3 Dh2 98.0(6) 107_533 . -105_544 N
O3 O3 OII' 83.39(20) 107_533 . 107_533 N
O3 O3 O4 43.77(17) 209_343 . 111_433 N
O3 O3 O4 103.34(16) 209_343 . 208_343 N
O3 O3 SII 35.13(11) 209_465 . 111_555 N
O3 O3 Og 119.89(17) 209_455 . 3_555 N
O3 O3 Og 79.41(22) 209_455 . -1_555 N
O3 O3 Dg2 129.00(23) 209_465 . 3_555 N
O3 O3 Dg2 85.67(30) 209_465 . -1_555 N
O3 O3 Oh 92.36(33) 209_464 . 3_555 N
O3 O3 Oh 62.0(4) 209_464 . -105_565 N
O3 O3 Dh1 103.4(4) 209_443 . 3_555 N
O3 O3 Dh2 96.6(6) 209_443 . 3_555 N
O3 O3 Dh2 55.2(6) 209_443 . -105_544 N
O3 O3 OII' 66.96(6) 209_443 . 107_533 N
O4 O3 O4 142.26(14) 111_433 . 208_343 N
O4 O3 SII 71.18(15) 111_555 . 111_555 N
O4 O3 Og 121.23(22) 111_545 . 3_555 N
O4 O3 Og 40.77(21) 111_545 . -1_555 N
O4 O3 Dg2 128.5(4) 111_555 . 3_555 N
O4 O3 Dg2 45.49(31) 111_555 . -1_555 N
O4 O3 Oh 109.39(31) 111_554 . 3_555 N
O4 O3 Oh 45.13(34) 111_554 . -105_565 N
O4 O3 Dh1 112.6(5) 111_533 . 3_555 N
O4 O3 Dh2 119.7(6) 111_533 . 3_555 N
O4 O3 Dh2 32.4(5) 111_533 . -105_544 N
O4 O3 OII' 78.18(18) 111_533 . 107_533 N
O4 O3 SII 71.59(14) 208_465 . 111_555 N
O4 O3 Og 51.22(22) 208_455 . 3_555 N
O4 O3 Og 135.70(20) 208_455 . -1_555 N
O4 O3 Dg2 50.71(34) 208_465 . 3_555 N
O4 O3 Dg2 137.27(31) 208_465 . -1_555 N
O4 O3 Oh 43.03(34) 208_464 . 3_555 N
O4 O3 Oh 109.25(32) 208_464 . -105_565 N
O4 O3 Dh1 47.8(5) 208_443 . 3_555 N
O4 O3 Dh2 31.3(5) 208_443 . 3_555 N
O4 O3 Dh2 120.1(6) 208_443 . -105_544 N
O4 O3 OII' 108.75(24) 208_443 . 107_533 N
SII O3 Og 87.89(25) 111_545 . 3_555 N
SII O3 Og 91.97(24) 111_545 . -1_555 N
SII O3 Dg2 96.12(30) 111_555 . 3_555 N
SII O3 Dg2 98.80(29) 111_555 . -1_555 N
SII O3 Oh 58.8(4) 111_554 . 3_555 N
SII O3 Oh 61.4(4) 111_554 . -105_565 N
SII O3 Dh1 71.1(4) 111_533 . 3_555 N
SII O3 Dh2 61.6(6) 111_533 . 3_555 N
SII O3 Dh2 63.1(6) 111_533 . -105_544 N
SII O3 OII' 91.42(27) 111_533 . 107_533 N
Og O3 Og 88.51(7) 3_555 . -1_555 N
Og O3 Dg2 9.41(15) 3_555 . 3_555 N
Og O3 Dg2 87.81(27) 3_555 . -1_555 N
Og O3 Oh 29.3(4) 3_555 . 3_555 N
Og O3 Oh 76.4(4) 3_555 . -105_565 N
Og O3 Dh1 16.8(4) 3_555 . 3_555 N
Og O3 Dh2 30.9(6) 3_555 . 3_555 N
Og O3 Dh2 89.0(5) 3_555 . -105_544 N
Og O3 OII' 158.89(28) 3_555 . 107_533 N
Og O3 Dg2 92.77(31) -1_555 . 3_555 N
Og O3 Dg2 6.90(12) -1_555 . -1_555 N
Og O3 Oh 93.0(4) -1_555 . 3_555 N
Og O3 Oh 32.90(34) -1_555 . -105_565 N
Og O3 Dh1 88.2(5) -1_555 . 3_555 N
Og O3 Dh2 104.6(5) -1_555 . 3_555 N
Og O3 Dh2 28.9(6) -1_555 . -105_544 N
Og O3 OII' 112.61(27) -1_555 . 107_533 N
Dg2 O3 Dg2 91.05(8) 3_555 . -1_555 N
Dg2 O3 Oh 37.3(4) 3_555 . 3_555 N
Dg2 O3 Oh 84.4(4) 3_555 . -105_565 N
Dg2 O3 Dh1 25.6(4) 3_555 . 3_555 N
Dg2 O3 Dh2 36.6(6) 3_555 . 3_555 N
Dg2 O3 Dh2 96.8(6) 3_555 . -105_544 N
Dg2 O3 OII' 153.3(4) 3_555 . 107_533 N
Dg2 O3 Oh 95.7(4) -1_555 . 3_555 N
Dg2 O3 Oh 39.1(4) -1_555 . -105_565 N
Dg2 O3 Dh1 89.5(6) -1_555 . 3_555 N
Dg2 O3 Dh2 107.0(5) -1_555 . 3_555 N
Dg2 O3 Dh2 35.7(6) -1_555 . -105_544 N
Dg2 O3 OII' 113.1(4) -1_555 . 107_533 N
Oh O3 Oh 67.5(6) 3_555 . -105_565 N
Oh O3 Dh1 13.08(14) 3_555 . 3_555 N
Oh O3 Dh2 11.77(34) 3_555 . 3_555 N
Oh O3 Dh2 79.5(8) 3_555 . -105_544 N
Oh O3 OII' 142.0(4) 3_555 . 107_533 N
Oh O3 Dh1 68.0(6) -105_544 . 3_555 N
Oh O3 Dh2 79.0(7) -105_544 . 3_555 N
Oh O3 Dh2 12.77(32) -105_544 . -105_544 N
Oh O3 OII' 121.4(4) -105_544 . 107_533 N
Dh1 O3 Dh2 19.1(4) 3_555 . 3_555 N
Dh1 O3 Dh2 80.7(6) 3_555 . -105_544 N
Dh1 O3 OII' 153.7(5) 3_555 . 107_533 N
Dh2 O3 Dh2 90.9(11) 3_555 . -105_544 N
Dh2 O3 OII' 134.6(5) 3_555 . 107_533 N
Dh2 O3 OII' 109.5(5) -105_544 . 107_533 N
Si1 O4 Si2 143.37(35) 107_533 . 209_443 N
Si1 O4 Al1 143.37(35) 107_443 . 209_353 N
Si1 O4 O1 48.23(26) 107_433 . 6_555 N
Si1 O4 O1 34.19(26) 107_433 . 107_433 N
Si1 O4 O1 111.81(27) 107_433 . -105_444 N
Si1 O4 O1 164.03(35) 107_433 . -309_445 N
Si1 O4 O2 112.86(28) 107_433 . 310_334 N
Si1 O4 O2 30.89(23) 107_433 . 312_334 N
Si1 O4 O3 127.36(30) 107_433 . -105_444 N
Si1 O4 O3 40.78(27) 107_433 . -206_444 N
Si1 O4 O4 77.57(27) 107_433 . -304_444 N
Si1 O4 SJ 115.1(6) 107_545 . 312_446 N
Si1 O4 Og 87.2(4) 107_545 . 6_555 N
Si1 O4 Og 132.9(4) 107_545 . 312_446 N
Si1 O4 Dg1 86.9(4) 107_554 . 6_555 N
Si1 O4 Dg1 118.0(4) 107_554 . 312_455 N
Si1 O4 Dg2 71.3(4) 107_555 . 6_555 N
Si1 O4 Dg2 145.7(5) 107_555 . 312_456 N
Si1 O4 Oh 131.2(4) 107_554 . -102_565 N
Si1 O4 Oh 104.6(6) 107_554 . 312_455 N
Si1 O4 Dh1 82.8(4) 107_533 . 6_555 N
Si1 O4 Dh1 118.1(6) 107_533 . 312_434 N
Si1 O4 Dh2 105.1(12) 107_533 . 312_434 N
Si1 O4 OII' 75.83(26) 107_533 . 1_555 N
Si2 O4 Al1 0.0 209_353 . 209_353 N
Si2 O4 O1 116.69(32) 209_343 . 6_555 N
Si2 O4 O1 170.3(4) 209_343 . 107_433 N
Si2 O4 O1 52.59(29) 209_343 . -105_444 N
Si2 O4 O1 36.35(30) 209_343 . -309_445 N
Si2 O4 O2 35.11(28) 209_343 . 310_334 N
Si2 O4 O2 115.53(33) 209_343 . 312_334 N
Si2 O4 O3 35.34(29) 209_343 . -105_444 N
Si2 O4 O3 123.25(32) 209_343 . -206_444 N
Si2 O4 O4 79.64(32) 209_343 . -304_444 N
Si2 O4 SJ 101.1(6) 209_455 . 312_446 N
Si2 O4 Og 126.2(4) 209_455 . 6_555 N
Si2 O4 Og 83.6(4) 209_455 . 312_446 N
Si2 O4 Dg1 128.9(5) 209_464 . 6_555 N
Si2 O4 Dg1 97.8(4) 209_464 . 312_455 N
Si2 O4 Dg2 142.1(5) 209_465 . 6_555 N
Si2 O4 Dg2 70.2(4) 209_465 . 312_456 N
Si2 O4 Oh 77.3(4) 209_464 . -102_565 N
Si2 O4 Oh 108.5(7) 209_464 . 312_455 N
Si2 O4 Dh1 128.2(5) 209_443 . 6_555 N
Si2 O4 Dh1 97.5(7) 209_443 . 312_434 N
Si2 O4 Dh2 108.5(12) 209_443 . 312_434 N
Si2 O4 OII' 72.93(29) 209_443 . 1_555 N
Al1 O4 O1 116.69(32) 209_343 . 6_555 N
Al1 O4 O1 170.3(4) 209_343 . 107_433 N
Al1 O4 O1 52.59(29) 209_343 . -105_444 N
Al1 O4 O1 36.35(30) 209_343 . -309_445 N
Al1 O4 O2 35.11(28) 209_343 . 310_334 N
Al1 O4 O2 115.53(33) 209_343 . 312_334 N
Al1 O4 O3 35.34(29) 209_343 . -105_444 N
Al1 O4 O3 123.25(32) 209_343 . -206_444 N
Al1 O4 O4 79.64(32) 209_343 . -304_444 N
Al1 O4 SJ 101.1(6) 209_455 . 312_446 N
Al1 O4 Og 126.2(4) 209_455 . 6_555 N
Al1 O4 Og 83.6(4) 209_455 . 312_446 N
Al1 O4 Dg1 128.9(5) 209_464 . 6_555 N
Al1 O4 Dg1 97.8(4) 209_464 . 312_455 N
Al1 O4 Dg2 142.1(5) 209_465 . 6_555 N
Al1 O4 Dg2 70.2(4) 209_465 . 312_456 N
Al1 O4 Oh 77.3(4) 209_464 . -102_565 N
Al1 O4 Oh 108.5(7) 209_464 . 312_455 N
Al1 O4 Dh1 128.2(5) 209_443 . 6_555 N
Al1 O4 Dh1 97.5(7) 209_443 . 312_434 N
Al1 O4 Dh2 108.5(12) 209_443 . 312_434 N
Al1 O4 OII' 72.93(29) 209_443 . 1_555 N
O1 O4 O1 53.92(19) 6_555 . 107_433 N
O1 O4 O1 67.02(7) 6_555 . -105_444 N
O1 O4 O1 115.80(20) 6_555 . -309_445 N
O1 O4 O2 82.79(15) 6_555 . 310_334 N
O1 O4 O2 33.22(11) 6_555 . 312_334 N
O1 O4 O3 138.13(16) 6_555 . -105_444 N
O1 O4 O3 87.35(16) 6_555 . -206_444 N
O1 O4 O4 37.15(13) 6_555 . -304_444 N
O1 O4 SJ 107.4(5) 6_555 . 312_446 N
O1 O4 Og 79.76(25) 6_555 . 6_555 N
O1 O4 Og 120.64(26) 6_555 . 312_446 N
O1 O4 Dg1 87.51(32) 6_555 . 6_555 N
O1 O4 Dg1 106.44(35) 6_555 . 312_455 N
O1 O4 Dg2 71.2(4) 6_555 . 6_555 N
O1 O4 Dg2 121.0(4) 6_555 . 312_456 N
O1 O4 Oh 96.53(25) 6_555 . -102_565 N
O1 O4 Oh 127.1(5) 6_555 . 312_455 N
O1 O4 Dh1 71.8(4) 6_555 . 6_555 N
O1 O4 Dh1 126.8(7) 6_555 . 312_434 N
O1 O4 Dh2 126.0(12) 6_555 . 312_434 N
O1 O4 OII' 95.54(20) 6_555 . 1_555 N
O1 O4 O1 117.77(21) 107_433 . -105_444 N
O1 O4 O1 141.58(15) 107_433 . -309_445 N
O1 O4 O2 136.28(25) 107_433 . 310_334 N
O1 O4 O2 58.64(19) 107_433 . 312_334 N
O1 O4 O3 152.79(22) 107_433 . -105_444 N
O1 O4 O3 61.89(20) 107_433 . -206_444 N
O1 O4 O4 91.06(25) 107_433 . -304_444 N
O1 O4 SJ 81.1(5) 107_545 . 312_446 N
O1 O4 Og 53.20(23) 107_545 . 6_555 N
O1 O4 Og 99.14(29) 107_545 . 312_446 N
O1 O4 Dg1 52.81(32) 107_554 . 6_555 N
O1 O4 Dg1 83.80(29) 107_554 . 312_455 N
O1 O4 Dg2 37.16(28) 107_555 . 6_555 N
O1 O4 Dg2 111.5(4) 107_555 . 312_456 N
O1 O4 Oh 100.32(28) 107_554 . -102_565 N
O1 O4 Oh 78.8(6) 107_554 . 312_455 N
O1 O4 Dh1 49.64(33) 107_533 . 6_555 N
O1 O4 Dh1 88.0(6) 107_533 . 312_434 N
O1 O4 Dh2 78.5(11) 107_533 . 312_434 N
O1 O4 OII' 108.77(17) 107_533 . 1_555 N
O1 O4 O1 53.56(18) -105_444 . -309_445 N
O1 O4 O2 30.58(11) -105_444 . 310_334 N
O1 O4 O2 83.17(15) -105_444 . 312_334 N
O1 O4 O3 85.98(15) -105_444 . -105_444 N
O1 O4 O3 136.61(16) -105_444 . -206_444 N
O1 O4 O4 34.39(13) -105_444 . -304_444 N
O1 O4 SJ 100.8(5) -105_556 . 312_446 N
O1 O4 Og 101.90(24) -105_556 . 6_555 N
O1 O4 Og 94.31(22) -105_556 . 312_446 N
O1 O4 Dg1 111.89(30) -105_565 . 6_555 N
O1 O4 Dg1 96.4(4) -105_565 . 312_455 N
O1 O4 Dg2 109.5(4) -105_566 . 6_555 N
O1 O4 Dg2 81.71(31) -105_566 . 312_456 N
O1 O4 Oh 66.69(28) -105_565 . -102_565 N
O1 O4 Oh 133.2(5) -105_565 . 312_455 N
O1 O4 Dh1 97.2(5) -105_544 . 6_555 N
O1 O4 Dh1 116.1(6) -105_544 . 312_434 N
O1 O4 Dh2 131.6(12) -105_544 . 312_434 N
O1 O4 OII' 93.54(21) -105_544 . 1_555 N
O1 O4 O2 58.78(17) -309_445 . 310_334 N
O1 O4 O2 136.53(23) -309_445 . 312_334 N
O1 O4 O3 62.58(18) -309_445 . -105_444 N
O1 O4 O3 153.66(22) -309_445 . -206_444 N
O1 O4 O4 87.94(23) -309_445 . -304_444 N
O1 O4 SJ 66.5(6) -309_557 . 312_446 N
O1 O4 Og 89.89(25) -309_557 . 6_555 N
O1 O4 Og 50.91(25) -309_557 . 312_446 N
O1 O4 Dg1 93.09(33) -309_566 . 6_555 N
O1 O4 Dg1 62.74(28) -309_566 . 312_455 N
O1 O4 Dg2 105.85(31) -309_567 . 6_555 N
O1 O4 Dg2 36.41(28) -309_567 . 312_456 N
O1 O4 Oh 41.37(28) -309_566 . -102_565 N
O1 O4 Oh 85.5(6) -309_566 . 312_455 N
O1 O4 Dh1 92.31(34) -309_545 . 6_555 N
O1 O4 Dh1 69.8(6) -309_545 . 312_434 N
O1 O4 Dh2 84.6(11) -309_545 . 312_434 N
O1 O4 OII' 109.11(16) -309_545 . 1_555 N
O2 O4 O2 82.37(16) 310_334 . 312_334 N
O2 O4 O3 60.15(16) 310_334 . -105_444 N
O2 O4 O3 116.19(17) 310_334 . -206_444 N
O2 O4 O4 45.81(15) 310_334 . -304_444 N
O2 O4 SJ 122.5(6) 310_446 . 312_446 N
O2 O4 Og 131.88(26) 310_446 . 6_555 N
O2 O4 Og 109.35(27) 310_446 . 312_446 N
O2 O4 Dg1 141.18(33) 310_455 . 6_555 N
O2 O4 Dg1 118.15(35) 310_455 . 312_455 N
O2 O4 Dg2 139.9(4) 310_456 . 6_555 N
O2 O4 Dg2 94.82(30) 310_456 . 312_456 N
O2 O4 Oh 89.34(30) 310_455 . -102_565 N
O2 O4 Oh 142.5(6) 310_455 . 312_455 N
O2 O4 Dh1 127.7(5) 310_434 . 6_555 N
O2 O4 Dh1 128.4(6) 310_434 . 312_434 N
O2 O4 Dh2 142.1(12) 310_434 . 312_434 N
O2 O4 OII' 65.36(18) 310_434 . 1_555 N
O2 O4 O3 116.21(18) 312_334 . -105_444 N
O2 O4 O3 59.08(16) 312_334 . -206_444 N
O2 O4 O4 49.02(15) 312_334 . -304_444 N
O2 O4 SJ 135.0(5) 312_446 . 312_446 N
O2 O4 Og 104.58(28) 312_446 . 6_555 N
O2 O4 Og 151.77(30) 312_446 . 312_446 N
O2 O4 Dg1 108.7(4) 312_455 . 6_555 N
O2 O4 Dg1 135.68(34) 312_455 . 312_455 N
O2 O4 Dg2 91.13(34) 312_456 . 6_555 N
O2 O4 Dg2 154.2(4) 312_456 . 312_456 N
O2 O4 Oh 129.63(27) 312_455 . -102_565 N
O2 O4 Oh 135.2(6) 312_455 . 312_455 N
O2 O4 Dh1 97.6(4) 312_434 . 6_555 N
O2 O4 Dh1 146.6(6) 312_434 . 312_434 N
O2 O4 Dh2 135.5(12) 312_434 . 312_434 N
O2 O4 OII' 65.05(17) 312_434 . 1_555 N
O3 O4 O3 92.00(16) -105_444 . -206_444 N
O3 O4 O4 104.49(19) -105_444 . -304_444 N
O3 O4 SJ 108.8(5) -105_556 . 312_446 N
O3 O4 Og 139.13(29) -105_556 . 6_555 N
O3 O4 Og 91.54(29) -105_556 . 312_446 N
O3 O4 Dg1 133.41(35) -105_565 . 6_555 N
O3 O4 Dg1 107.92(32) -105_565 . 312_455 N
O3 O4 Dg2 150.5(4) -105_566 . 6_555 N
O3 O4 Dg2 83.4(4) -105_566 . 312_456 N
O3 O4 Oh 101.45(30) -105_565 . -102_565 N
O3 O4 Oh 94.8(5) -105_565 . 312_455 N
O3 O4 Dh1 146.1(4) -105_544 . 6_555 N
O3 O4 Dh1 93.2(7) -105_544 . 312_434 N
O3 O4 Dh2 95.9(12) -105_544 . 312_434 N
O3 O4 OII' 53.19(14) -105_544 . 1_555 N
O3 O4 O4 106.25(19) -206_444 . -304_444 N
O3 O4 SJ 120.6(6) -206_556 . 312_446 N
O3 O4 Og 107.40(30) -206_556 . 6_555 N
O3 O4 Og 129.08(24) -206_556 . 312_446 N
O3 O4 Dg1 100.7(4) -206_565 . 6_555 N
O3 O4 Dg1 125.1(4) -206_565 . 312_455 N
O3 O4 Dg2 93.0(4) -206_566 . 6_555 N
O3 O4 Dg2 141.16(33) -206_566 . 312_456 N
O3 O4 Oh 154.47(31) -206_565 . -102_565 N
O3 O4 Oh 90.2(5) -206_565 . 312_455 N
O3 O4 Dh1 107.6(4) -206_544 . 6_555 N
O3 O4 Dh1 107.3(6) -206_544 . 312_434 N
O3 O4 Dh2 91.7(12) -206_544 . 312_434 N
O3 O4 OII' 53.14(14) -206_544 . 1_555 N
O4 O4 SJ 120.0(5) -304_556 . 312_446 N
O4 O4 Og 103.96(25) -304_556 . 6_555 N
O4 O4 Og 121.79(22) -304_556 . 312_446 N
O4 O4 Dg1 114.21(31) -304_565 . 6_555 N
O4 O4 Dg1 116.5(4) -304_565 . 312_455 N
O4 O4 Dg2 102.0(4) -304_566 . 6_555 N
O4 O4 Dg2 112.3(4) -304_566 . 312_456 N
O4 O4 Oh 91.39(27) -304_565 . -102_565 N
O4 O4 Oh 154.0(4) -304_565 . 312_455 N
O4 O4 Dh1 96.4(5) -304_544 . 6_555 N
O4 O4 Dh1 141.2(6) -304_544 . 312_434 N
O4 O4 Dh2 152.0(12) -304_544 . 312_434 N
O4 O4 OII' 82.10(21) -304_544 . 1_555 N
SJ O4 Og 30.5(5) 312_446 . 6_555 N
SJ O4 Og 18.1(6) 312_446 . 312_446 N
SJ O4 Dg1 28.3(6) 312_455 . 6_555 N
SJ O4 Dg1 4.5(6) 312_455 . 312_455 N
SJ O4 Dg2 45.0(6) 312_456 . 6_555 N
SJ O4 Dg2 30.9(6) 312_456 . 312_456 N
SJ O4 Oh 34.4(6) 312_455 . -102_565 N
SJ O4 Oh 35.1(6) 312_455 . 312_455 N
SJ O4 Dh1 37.4(6) 312_434 . 6_555 N
SJ O4 Dh1 21.9(8) 312_434 . 312_434 N
SJ O4 Dh2 33.2(12) 312_434 . 312_434 N
SJ O4 OII' 156.3(5) 312_434 . 1_555 N
Og O4 Og 48.3(4) 6_555 . 312_446 N
Og O4 Dg1 10.65(22) 6_555 . 6_555 N
Og O4 Dg1 31.9(4) 6_555 . 312_455 N
Og O4 Dg2 16.09(11) 6_555 . 6_555 N
Og O4 Dg2 58.8(4) 6_555 . 312_456 N
Og O4 Oh 49.21(34) 6_555 . -102_565 N
Og O4 Oh 50.9(5) 6_555 . 312_455 N
Og O4 Dh1 8.1(5) 6_555 . 6_555 N
Og O4 Dh1 47.1(7) 6_555 . 312_434 N
Og O4 Dh2 49.2(12) 6_555 . 312_434 N
Og O4 OII' 160.41(29) 6_555 . 1_555 N
Og O4 Dg1 46.4(4) 312_455 . 6_555 N
Og O4 Dg1 16.42(7) 312_455 . 312_455 N
Og O4 Dg2 63.1(5) 312_456 . 6_555 N
Og O4 Dg2 14.55(12) 312_456 . 312_456 N
Og O4 Oh 30.41(34) 312_455 . -102_565 N
Og O4 Oh 38.9(5) 312_455 . 312_455 N
Og O4 Dh1 54.6(4) 312_434 . 6_555 N
Og O4 Dh1 21.7(5) 312_434 . 312_434 N
Og O4 Dh2 37.4(12) 312_434 . 312_434 N
Og O4 OII' 143.11(32) 312_434 . 1_555 N
Dg1 O4 Dg1 31.2(4) 6_555 . 312_455 N
Dg1 O4 Dg2 17.6(4) 6_555 . 6_555 N
Dg1 O4 Dg2 58.9(6) 6_555 . 312_456 N
Dg1 O4 Oh 54.5(4) 6_555 . -102_565 N
Dg1 O4 Oh 41.3(5) 6_555 . 312_455 N
Dg1 O4 Dh1 17.9(6) 6_555 . 6_555 N
Dg1 O4 Dh1 40.2(7) 6_555 . 312_434 N
Dg1 O4 Dh2 39.7(12) 6_555 . 312_434 N
Dg1 O4 OII' 153.3(4) 6_555 . 1_555 N
Dg1 O4 Dg2 47.1(4) 312_456 . 6_555 N
Dg1 O4 Dg2 27.78(22) 312_456 . 312_456 N
Dg1 O4 Oh 29.8(5) 312_455 . -102_565 N
Dg1 O4 Oh 39.1(5) 312_455 . 312_455 N
Dg1 O4 Dh1 38.2(4) 312_434 . 6_555 N
Dg1 O4 Dh1 24.9(7) 312_434 . 312_434 N
Dg1 O4 Dh2 37.2(12) 312_434 . 312_434 N
Dg1 O4 OII' 158.0(4) 312_434 . 1_555 N
Dg2 O4 Dg2 74.5(5) 6_555 . 312_456 N
Dg2 O4 Oh 64.8(4) 6_555 . -102_565 N
Dg2 O4 Oh 56.1(6) 6_555 . 312_455 N
Dg2 O4 Dh1 14.6(5) 6_555 . 6_555 N
Dg2 O4 Dh1 57.5(7) 6_555 . 312_434 N
Dg2 O4 Dh2 54.9(12) 6_555 . 312_434 N
Dg2 O4 OII' 144.94(35) 6_555 . 1_555 N
Dg2 O4 Oh 24.6(5) 312_455 . -102_565 N
Dg2 O4 Oh 52.1(6) 312_455 . 312_455 N
Dg2 O4 Dh1 63.9(5) 312_434 . 6_555 N
Dg2 O4 Dh1 35.1(6) 312_434 . 312_434 N
Dg2 O4 Dh2 50.8(12) 312_434 . 312_434 N
Dg2 O4 OII' 136.6(4) 312_434 . 1_555 N
Oh O4 Oh 67.4(8) -102_565 . 312_455 N
Oh O4 Dh1 51.0(5) -102_544 . 6_555 N
Oh O4 Dh1 50.9(8) -102_544 . 312_434 N
Oh O4 Dh2 65.6(13) -102_544 . 312_434 N
Oh O4 OII' 150.24(30) -102_544 . 1_555 N
Oh O4 Dh1 58.8(7) 312_434 . 6_555 N
Oh O4 Dh1 17.20(28) 312_434 . 312_434 N
Oh O4 Dh2 2.0(11) 312_434 . 312_434 N
Oh O4 OII' 123.8(5) 312_434 . 1_555 N
Dh1 O4 Dh1 55.0(11) 6_555 . 312_434 N
Dh1 O4 Dh2 57.2(11) 6_555 . 312_434 N
Dh1 O4 OII' 158.41(35) 6_555 . 1_555 N
Dh1 O4 Dh2 15.7(12) 312_434 . 312_434 N
Dh1 O4 OII' 134.5(7) 312_434 . 1_555 N
Dh2 O4 OII' 125.8(12) 312_434 . 1_555 N
O2 SI' O2 109.48(24) -105_444 . -206_444 N
O2 SI' O2 109.48(24) -105_444 . -304_444 N
O2 SI' O2 109.48(24) -206_444 . -304_444 N
O3 SII O3 109.75(23) -105_444 . -206_444 N
O3 SII O3 109.75(23) -105_444 . -304_444 N
O3 SII OII* 109.19(23) -105_444 . 1_555 N
O3 SII O3 109.75(23) -206_444 . -304_444 N
O3 SII OII* 109.19(23) -206_444 . 1_555 N
O3 SII OII* 109.19(23) -304_444 . 1_555 N
O4 SJ Og 135.0(12) 312_446 . 1_555 N
O4 SJ Og 111.8(11) 312_446 . -108_656 N
O4 SJ Dg1 166.7(18) 312_455 . 1_555 N
O4 SJ Dg2 100.6(11) 312_456 . 1_555 N
O4 SJ Oh 90.9(12) 312_455 . 1_555 N
O4 SJ Dh1 121.5(16) 312_434 . 1_555 N
O4 SJ Dh2 52.3(13) 312_434 . 1_555 N
O4 SJ Ok 88.1(15) 312_324 . 105_544 N
O4 SJ Dk1 86.4(16) 312_446 . 105_544 N
Og SJ Og 111.8(13) 1_555 . -108_656 N
Og SJ Dg1 39.9(8) 1_555 . 1_555 N
Og SJ Dg2 37.6(6) 1_555 . 1_555 N
Og SJ Oh 89.3(15) 1_555 . 1_555 N
Og SJ Dh1 52.1(14) 1_555 . 1_555 N
Og SJ Dh2 115.9(20) 1_555 . 1_555 N
Og SJ Ok 84.4(17) 1_555 . 105_544 N
Og SJ Dk1 110.1(18) 1_555 . 105_544 N
Og SJ Dg1 72.1(13) -108_665 . 1_555 N
Og SJ Dg2 134.8(14) -108_666 . 1_555 N
Og SJ Oh 103.4(14) -108_665 . 1_555 N
Og SJ Dh1 107.5(18) -108_644 . 1_555 N
Og SJ Dh2 114.1(22) -108_644 . 1_555 N
Og SJ Ok 86.2(17) -108_534 . 105_544 N
Og SJ Dk1 55.3(14) -108_656 . 105_544 N
Dg1 SJ Dg2 69.9(13) 1_555 . 1_555 N
Dg1 SJ Oh 100.8(19) 1_555 . 1_555 N
Dg1 SJ Dh1 67.1(19) 1_555 . 1_555 N
Dg1 SJ Dh2 139.1(23) 1_555 . 1_555 N
Dg1 SJ Ok 79.3(19) 1_555 . 105_544 N
Dg1 SJ Dk1 85.7(19) 1_555 . 105_544 N
Dg2 SJ Oh 106.9(16) 1_555 . 1_555 N
Dg2 SJ Dh1 79.0(18) 1_555 . 1_555 N
Dg2 SJ Dh2 110.6(20) 1_555 . 1_555 N
Dg2 SJ Ok 63.6(18) 1_555 . 105_544 N
Dg2 SJ Dk1 98.1(18) 1_555 . 105_544 N
Oh SJ Dh1 38.0(7) 1_555 . 1_555 N
Oh SJ Dh2 38.6(8) 1_555 . 1_555 N
Oh SJ Ok 170.0(23) 1_555 . 105_544 N
Oh SJ Dk1 154.9(22) 1_555 . 105_544 N
Dh1 SJ Dh2 72.8(14) 1_555 . 1_555 N
Dh1 SJ Ok 136.5(25) 1_555 . 105_544 N
Dh1 SJ Dk1 152.1(22) 1_555 . 105_544 N
Dh2 SJ Ok 139.5(22) 1_555 . 105_544 N
Dh2 SJ Dk1 132.4(26) 1_555 . 105_544 N
Ok SJ Dk1 34.9(10) 105_544 . 105_544 N
O1 Og O1 84.48(31) -3_555 . 111_433 N
O1 Og O1 90.57(35) -3_555 . 212_333 N
O1 Og O2 26.10(25) -3_555 . 105_544 N
O1 Og O3 39.10(21) -3_555 . 2_555 N
O1 Og O3 27.73(18) -3_555 . -1_555 N
O1 Og O4 50.75(28) -3_555 . -111_444 N
O1 Og O4 53.05(28) -3_555 . 312_334 N
O1 Og SJ 76.3(9) -3_555 . 1_555 N
O1 Og SJ 85.5(8) -3_555 . 105_544 N
O1 Og Og 115.5(6) -3_555 . 105_544 N
O1 Og Og 104.7(7) -3_555 . -108_656 N
O1 Og Og 153.2(5) -3_555 . 308_445 N
O1 Og Og 141.3(6) -3_555 . -305_556 N
O1 Og Dg1 110.1(11) -3_555 . 1_555 N
O1 Og Dg1 121.1(9) -3_555 . 105_544 N
O1 Og Dg1 123.1(7) -3_555 . -108_665 N
O1 Og Dg1 145.0(6) -3_555 . 308_454 N
O1 Og Dg1 147.7(5) -3_555 . -305_565 N
O1 Og Dg2 5.9(10) -3_555 . 1_555 N
O1 Og Dg2 103.6(6) -3_555 . 105_544 N
O1 Og Dg2 96.6(6) -3_555 . -108_666 N
O1 Og Oh 99.4(7) -3_555 . 1_555 N
O1 Og Oh 78.1(7) -3_555 . 105_544 N
O1 Og Oh 113.9(5) -3_555 . -108_665 N
O1 Og O1 166.89(33) 111_433 . 212_333 N
O1 Og O2 109.09(27) 111_433 . 105_544 N
O1 Og O3 69.51(21) 111_433 . 2_555 N
O1 Og O3 99.97(25) 111_433 . -1_555 N
O1 Og O4 131.7(4) 111_433 . -111_444 N
O1 Og O4 34.22(19) 111_433 . 312_334 N
O1 Og SJ 8.2(8) 111_545 . 1_555 N
O1 Og SJ 142.9(8) 111_545 . 105_544 N
O1 Og Og 135.8(5) 111_545 . 105_544 N
O1 Og Og 32.11(32) 111_545 . -108_656 N
O1 Og Og 117.3(4) 111_545 . 308_445 N
O1 Og Og 57.7(4) 111_545 . -305_556 N
O1 Og Dg1 42.6(14) 111_554 . 1_555 N
O1 Og Dg1 134.1(10) 111_554 . 105_544 N
O1 Og Dg1 43.1(4) 111_554 . -108_665 N
O1 Og Dg1 120.6(5) 111_554 . 308_454 N
O1 Og Dg1 68.1(4) 111_554 . -305_565 N
O1 Og Dg2 78.8(9) 111_555 . 1_555 N
O1 Og Dg2 152.6(5) 111_555 . 105_544 N
O1 Og Dg2 17.45(29) 111_555 . -108_666 N
O1 Og Oh 42.6(7) 111_554 . 1_555 N
O1 Og Oh 108.1(7) 111_554 . 105_544 N
O1 Og Oh 47.34(31) 111_554 . -108_665 N
O1 Og O2 68.51(23) 212_333 . 105_544 N
O1 Og O3 113.43(35) 212_333 . 2_555 N
O1 Og O3 70.96(21) 212_333 . -1_555 N
O1 Og O4 40.40(20) 212_333 . -111_444 N
O1 Og O4 143.5(4) 212_333 . 312_334 N
O1 Og SJ 162.0(9) 212_445 . 1_555 N
O1 Og SJ 24.2(6) 212_445 . 105_544 N
O1 Og Og 37.51(33) 212_445 . 105_544 N
O1 Og Og 140.0(5) 212_445 . -108_656 N
O1 Og Og 64.6(4) 212_445 . 308_445 N
O1 Og Og 124.2(4) 212_445 . -305_556 N
O1 Og Dg1 129.8(15) 212_454 . 1_555 N
O1 Og Dg1 40.7(8) 212_454 . 105_544 N
O1 Og Dg1 134.6(5) 212_454 . -108_665 N
O1 Og Dg1 59.3(5) 212_454 . 308_454 N
O1 Og Dg1 112.22(31) 212_454 . -305_565 N
O1 Og Dg2 95.8(8) 212_455 . 1_555 N
O1 Og Dg2 19.29(33) 212_455 . 105_544 N
O1 Og Dg2 154.3(5) 212_455 . -108_666 N
O1 Og Oh 150.5(8) 212_454 . 1_555 N
O1 Og Oh 58.9(6) 212_454 . 105_544 N
O1 Og Oh 125.5(4) 212_454 . -108_665 N
O2 Og O3 48.36(16) 105_544 . 2_555 N
O2 Og O3 32.17(11) 105_544 . -1_555 N
O2 Og O4 33.55(17) 105_544 . -111_444 N
O2 Og O4 75.60(26) 105_544 . 312_334 N
O2 Og SJ 101.0(9) 105_544 . 1_555 N
O2 Og SJ 71.2(7) 105_544 . 105_544 N
O2 Og Og 101.0(4) 105_544 . 105_544 N
O2 Og Og 130.6(5) 105_544 . -108_656 N
O2 Og Og 133.0(5) 105_544 . 308_445 N
O2 Og Og 166.8(5) 105_544 . -305_556 N
O2 Og Dg1 135.0(11) 105_544 . 1_555 N
O2 Og Dg1 106.0(8) 105_544 . 105_544 N
O2 Og Dg1 149.1(5) 105_544 . -108_665 N
O2 Og Dg1 127.7(6) 105_544 . 308_454 N
O2 Og Dg1 171.40(32) 105_544 . -305_565 N
O2 Og Dg2 32.0(11) 105_544 . 1_555 N
O2 Og Dg2 85.0(4) 105_544 . 105_544 N
O2 Og Dg2 122.5(5) 105_544 . -108_666 N
O2 Og Oh 111.6(7) 105_544 . 1_555 N
O2 Og Oh 79.1(6) 105_544 . 105_544 N
O2 Og Oh 138.1(4) 105_544 . -108_665 N
O3 Og O3 66.66(19) 2_555 . -1_555 N
O3 Og O4 81.83(30) 2_555 . -111_444 N
O3 Og O4 37.25(17) 2_555 . 312_334 N
O3 Og SJ 63.2(8) 2_555 . 1_555 N
O3 Og SJ 119.5(8) 2_555 . 105_544 N
O3 Og Og 149.2(5) 2_555 . 105_544 N
O3 Og Og 100.8(5) 2_555 . -108_656 N
O3 Og Og 159.70(19) 2_555 . 308_445 N
O3 Og Og 120.8(5) 2_555 . -305_556 N
O3 Og Dg1 110.8(14) 2_555 . 1_555 N
O3 Og Dg1 153.7(9) 2_555 . 105_544 N
O3 Og Dg1 111.7(5) 2_555 . -108_665 N
O3 Og Dg1 165.7(4) 2_555 . 308_454 N
O3 Og Dg1 133.5(5) 2_555 . -305_565 N
O3 Og Dg2 38.4(8) 2_555 . 1_555 N
O3 Og Dg2 132.0(5) 2_555 . 105_544 N
O3 Og Dg2 86.8(4) 2_555 . -108_666 N
O3 Og Oh 63.8(7) 2_555 . 1_555 N
O3 Og Oh 117.0(7) 2_555 . 105_544 N
O3 Og Oh 115.8(4) 2_555 . -108_665 N
O3 Og O4 31.83(16) -1_555 . -111_444 N
O3 Og O4 75.37(23) -1_555 . 312_334 N
O3 Og SJ 92.3(9) -1_555 . 1_555 N
O3 Og SJ 59.7(7) -1_555 . 105_544 N
O3 Og Og 88.6(5) -1_555 . 105_544 N
O3 Og Og 107.0(6) -1_555 . -108_656 N
O3 Og Og 126.6(4) -1_555 . 308_445 N
O3 Og Og 142.91(27) -1_555 . -305_556 N
O3 Og Dg1 107.4(11) -1_555 . 1_555 N
O3 Og Dg1 94.2(8) -1_555 . 105_544 N
O3 Og Dg1 125.1(6) -1_555 . -108_665 N
O3 Og Dg1 117.9(5) -1_555 . 308_454 N
O3 Og Dg1 139.31(30) -1_555 . -305_565 N
O3 Og Dg2 30.1(6) -1_555 . 1_555 N
O3 Og Dg2 79.3(5) -1_555 . 105_544 N
O3 Og Dg2 105.7(5) -1_555 . -108_666 N
O3 Og Oh 125.9(7) -1_555 . 1_555 N
O3 Og Oh 51.4(6) -1_555 . 105_544 N
O3 Og Oh 109.1(4) -1_555 . -108_665 N
O4 Og O4 103.68(34) -111_444 . 312_334 N
O4 Og SJ 123.9(10) -111_556 . 1_555 N
O4 Og SJ 37.7(7) -111_556 . 105_544 N
O4 Og Og 67.9(5) -111_556 . 105_544 N
O4 Og Og 133.8(7) -111_556 . -108_656 N
O4 Og Og 103.1(5) -111_556 . 308_445 N
O4 Og Og 154.84(32) -111_556 . -305_556 N
O4 Og Dg1 130.0(12) -111_565 . 1_555 N
O4 Og Dg1 73.0(8) -111_565 . 105_544 N
O4 Og Dg1 147.5(7) -111_565 . -108_665 N
O4 Og Dg1 96.1(5) -111_565 . 308_454 N
O4 Og Dg1 142.6(4) -111_565 . -305_565 N
O4 Og Dg2 55.7(8) -111_566 . 1_555 N
O4 Og Dg2 53.2(4) -111_566 . 105_544 N
O4 Og Dg2 136.4(6) -111_566 . -108_666 N
O4 Og Oh 145.0(8) -111_565 . 1_555 N
O4 Og Oh 52.4(5) -111_565 . 105_544 N
O4 Og Oh 129.4(4) -111_565 . -108_665 N
O4 Og SJ 26.8(7) 312_446 . 1_555 N
O4 Og SJ 134.1(8) 312_446 . 105_544 N
O4 Og Og 154.8(6) 312_446 . 105_544 N
O4 Og Og 63.9(5) 312_446 . -108_656 N
O4 Og Og 151.3(5) 312_446 . 308_445 N
O4 Og Og 91.3(5) 312_446 . -305_556 N
O4 Og Dg1 73.6(13) 312_455 . 1_555 N
O4 Og Dg1 157.9(11) 312_455 . 105_544 N
O4 Og Dg1 77.2(5) 312_455 . -108_665 N
O4 Og Dg1 154.6(6) 312_455 . 308_454 N
O4 Og Dg1 102.3(5) 312_455 . -305_565 N
O4 Og Dg2 48.0(7) 312_456 . 1_555 N
O4 Og Dg2 154.4(5) 312_456 . 105_544 N
O4 Og Dg2 50.5(4) 312_456 . -108_666 N
O4 Og Oh 52.1(6) 312_455 . 1_555 N
O4 Og Oh 108.7(7) 312_455 . 105_544 N
O4 Og Oh 78.6(4) 312_455 . -108_665 N
SJ Og SJ 139.9(8) 1_555 . 105_544 N
SJ Og Og 139.4(10) 1_555 . 105_544 N
SJ Og Og 37.6(9) 1_555 . -108_656 N
SJ Og Og 125.1(9) 1_555 . 308_445 N
SJ Og Og 65.8(9) 1_555 . -305_556 N
SJ Og Dg1 47.8(13) 1_555 . 1_555 N
SJ Og Dg1 138.7(14) 1_555 . 105_544 N
SJ Og Dg1 50.5(9) 1_555 . -108_665 N
SJ Og Dg1 127.8(11) 1_555 . 308_454 N
SJ Og Dg1 75.9(10) 1_555 . -305_565 N
SJ Og Dg2 70.6(10) 1_555 . 1_555 N
SJ Og Dg2 154.0(11) 1_555 . 105_544 N
SJ Og Dg2 23.8(8) 1_555 . -108_666 N
SJ Og Oh 46.2(9) 1_555 . 1_555 N
SJ Og Oh 105.6(11) 1_555 . 105_544 N
SJ Og Oh 52.7(8) 1_555 . -108_665 N
SJ Og Og 30.5(8) 105_544 . 105_544 N
SJ Og Og 119.2(9) 105_544 . -108_656 N
SJ Og Og 67.8(8) 105_544 . 308_445 N
SJ Og Og 118.6(7) 105_544 . -305_556 N
SJ Og Dg1 109.9(16) 105_544 . 1_555 N
SJ Og Dg1 35.9(9) 105_544 . 105_544 N
SJ Og Dg1 120.7(10) 105_544 . -108_665 N
SJ Og Dg1 59.7(8) 105_544 . 308_454 N
SJ Og Dg1 105.8(7) 105_544 . -305_565 N
SJ Og Dg2 89.2(10) 105_544 . 1_555 N
SJ Og Dg2 20.3(8) 105_544 . 105_544 N
SJ Og Dg2 131.9(9) 105_544 . -108_666 N
SJ Og Oh 173.5(11) 105_544 . 1_555 N
SJ Og Oh 34.8(8) 105_544 . 105_544 N
SJ Og Oh 106.6(8) 105_544 . -108_665 N
Og Og Og 103.9(5) 105_544 . -108_656 N
Og Og Og 38.04(26) 105_544 . 308_445 N
Og Og Og 90.00000(30) 105_544 . -305_556 N
Og Og Dg1 93.4(15) 105_544 . 1_555 N
Og Og Dg1 5.6(7) 105_544 . 105_544 N
Og Og Dg1 97.3(5) 105_544 . -108_665 N
Og Og Dg1 29.5(4) 105_544 . 308_454 N
Og Og Dg1 77.23(7) 105_544 . -305_565 N
Og Og Dg2 118.7(6) 105_544 . 1_555 N
Og Og Dg2 18.23(15) 105_544 . 105_544 N
Og Og Dg2 118.7(5) 105_544 . -108_666 N
Og Og Oh 145.1(8) 105_544 . 1_555 N
Og Og Oh 46.9(7) 105_544 . 105_544 N
Og Og Oh 88.8(4) 105_544 . -108_665 N
Og Og Og 90.00000(20) -108_656 . 308_445 N
Og Og Og 38.04(26) -108_656 . -305_556 N
Og Og Dg1 10.5(14) -108_665 . 1_555 N
Og Og Dg1 102.0(9) -108_665 . 105_544 N
Og Og Dg1 18.94(17) -108_665 . -108_665 N
Og Og Dg1 90.9(4) -108_665 . 308_454 N
Og Og Dg1 43.28(27) -108_665 . -305_565 N
Og Og Dg2 98.8(12) -108_666 . 1_555 N
Og Og Dg2 121.5(6) -108_666 . 105_544 N
Og Og Dg2 14.78(14) -108_666 . -108_666 N
Og Og Oh 63.9(7) -108_665 . 1_555 N
Og Og Oh 87.9(8) -108_665 . 105_544 N
Og Og Oh 15.24(35) -108_665 . -108_665 N
Og Og Og 60.00000(10) 308_445 . -305_556 N
Og Og Dg1 81.4(13) 308_454 . 1_555 N
Og Og Dg1 32.5(7) 308_454 . 105_544 N
Og Og Dg1 74.70(24) 308_454 . -108_665 N
Og Og Dg1 9.03(24) 308_454 . 308_454 N
Og Og Dg1 49.22(17) 308_454 . -305_565 N
Og Og Dg2 156.7(6) 308_455 . 1_555 N
Og Og Dg2 49.89(19) 308_455 . 105_544 N
Og Og Dg2 101.93(26) 308_455 . -108_666 N
Og Og Oh 107.2(7) 308_454 . 1_555 N
Og Og Oh 80.2(7) 308_454 . 105_544 N
Og Og Oh 76.61(34) 308_454 . -108_665 N
Og Og Dg1 35.7(12) -305_565 . 1_555 N
Og Og Dg1 85.4(6) -305_565 . 105_544 N
Og Og Dg1 19.10(31) -305_565 . -108_665 N
Og Og Dg1 64.85(34) -305_565 . 308_454 N
Og Og Dg1 12.84(6) -305_565 . -305_565 N
Og Og Dg2 135.4(11) -305_566 . 1_555 N
Og Og Dg2 106.90(14) -305_566 . 105_544 N
Og Og Dg2 44.61(32) -305_566 . -108_666 N
Og Og Oh 59.7(8) -305_565 . 1_555 N
Og Og Oh 103.9(6) -305_565 . 105_544 N
Og Og Oh 33.82(32) -305_565 . -108_665 N
Dg1 Og Dg1 91.5(18) 1_555 . 105_544 N
Dg1 Og Dg1 18.2(15) 1_555 . -108_665 N
Dg1 Og Dg1 81.5(17) 1_555 . 308_454 N
Dg1 Og Dg1 37.6(11) 1_555 . -305_565 N
Dg1 Og Dg2 104.49450(30) 1_555 . 1_555 N
Dg1 Og Dg2 111.1(14) 1_555 . 105_544 N
Dg1 Og Dg2 25.3(13) 1_555 . -108_666 N
Dg1 Og Oh 72.5(16) 1_555 . 1_555 N
Dg1 Og Oh 80.5(14) 1_555 . 105_544 N
Dg1 Og Oh 5.0(13) 1_555 . -108_665 N
Dg1 Og Dg1 93.9(10) 105_544 . -108_665 N
Dg1 Og Dg1 24.0(6) 105_544 . 308_454 N
Dg1 Og Dg1 72.8(6) 105_544 . -305_565 N
Dg1 Og Dg2 124.2(11) 105_544 . 1_555 N
Dg1 Og Dg2 21.8(7) 105_544 . 105_544 N
Dg1 Og Dg2 116.7(9) 105_544 . -108_666 N
Dg1 Og Oh 139.5(11) 105_544 . 1_555 N
Dg1 Og Oh 51.5(9) 105_544 . 105_544 N
Dg1 Og Oh 86.8(9) 105_544 . -108_665 N
Dg1 Og Dg1 77.5(6) -108_665 . 308_454 N
Dg1 Og Dg1 25.80(26) -108_665 . -305_565 N
Dg1 Og Dg2 117.2(10) -108_666 . 1_555 N
Dg1 Og Dg2 115.5(4) -108_666 . 105_544 N
Dg1 Og Dg2 27.35(15) -108_666 . -108_666 N
Dg1 Og Oh 60.1(7) -108_665 . 1_555 N
Dg1 Og Oh 96.1(9) -108_665 . 105_544 N
Dg1 Og Oh 18.2(6) -108_665 . -108_665 N
Dg1 Og Dg1 53.07(31) 308_454 . -305_565 N
Dg1 Og Dg2 148.0(6) 308_455 . 1_555 N
Dg1 Og Dg2 43.0(4) 308_455 . 105_544 N
Dg1 Og Dg2 104.1(6) 308_455 . -108_666 N
Dg1 Og Oh 115.6(8) 308_454 . 1_555 N
Dg1 Og Oh 71.3(7) 308_454 . 105_544 N
Dg1 Og Oh 76.5(5) 308_454 . -108_665 N
Dg1 Og Dg2 142.0(11) -305_566 . 1_555 N
Dg1 Og Dg2 94.38(14) -305_566 . 105_544 N
Dg1 Og Dg2 53.13(33) -305_566 . -108_666 N
Dg1 Og Oh 72.3(8) -305_565 . 1_555 N
Dg1 Og Oh 93.9(6) -305_565 . 105_544 N
Dg1 Og Oh 34.1(4) -305_565 . -108_665 N
Dg2 Og Dg2 107.9(6) 1_555 . 105_544 N
Dg2 Og Dg2 90.7(8) 1_555 . -108_666 N
Dg2 Og Oh 96.0(9) 1_555 . 1_555 N
Dg2 Og Oh 78.6(10) 1_555 . 105_544 N
Dg2 Og Oh 108.4(12) 1_555 . -108_665 N
Dg2 Og Dg2 136.2(6) 105_544 . -108_666 N
Dg2 Og Oh 153.4(9) 105_544 . 1_555 N
Dg2 Og Oh 50.2(7) 105_544 . 105_544 N
Dg2 Og Oh 106.6(5) 105_544 . -108_665 N
Dg2 Og Oh 52.1(7) -108_665 . 1_555 N
Dg2 Og Oh 98.4(8) -108_665 . 105_544 N
Dg2 Og Oh 29.96(35) -108_665 . -108_665 N
Oh Og Oh 150.3(11) 1_555 . 105_544 N
Oh Og Oh 75.5(8) 1_555 . -108_665 N
Oh Og Oh 78.6(8) 105_544 . -108_665 N
O1 Dg1 O1 91.1(5) -3_555 . 111_433 N
O1 Dg1 O4 41.21(24) -3_555 . -111_444 N
O1 Dg1 O4 51.50(35) -3_555 . 312_334 N
O1 Dg1 SJ 59.0(12) -3_555 . 1_555 N
O1 Dg1 Og 53.4(9) -3_555 . 1_555 N
O1 Dg1 Og 97.5(5) -3_555 . 105_544 N
O1 Dg1 Og 117.6(12) -3_555 . -108_656 N
O1 Dg1 Og 133.0(6) -3_555 . 308_445 N
O1 Dg1 Og 160.0(8) -3_555 . -305_556 N
O1 Dg1 Dg1 95.8(9) -3_555 . 105_544 N
O1 Dg1 Dg1 143.2(8) -3_555 . -108_665 N
O1 Dg1 Dg1 126.0(8) -3_555 . 308_454 N
O1 Dg1 Dg1 173.4(8) -3_555 . -305_565 N
O1 Dg1 Dg2 15.7(9) -3_555 . 1_555 N
O1 Dg1 Dg2 85.2(5) -3_555 . 105_544 N
O1 Dg1 Dg2 105.4(6) -3_555 . -108_666 N
O1 Dg1 Oh 87.8(9) -3_555 . 1_555 N
O1 Dg1 Oh 70.0(7) -3_555 . 105_544 N
O1 Dg1 Oh 131.3(7) -3_555 . -108_665 N
O1 Dg1 Oh 108.4(6) -3_555 . 308_454 N
O1 Dg1 Dh1 86.5(14) -3_555 . 1_555 N
O1 Dg1 Dh1 87.4(7) -3_555 . 105_544 N
O1 Dg1 Dh1 128.2(10) -3_555 . -108_644 N
O1 Dg1 Dh1 121.3(6) -3_555 . 308_433 N
O1 Dg1 O4 131.4(5) 111_433 . -111_444 N
O1 Dg1 O4 41.28(28) 111_433 . 312_334 N
O1 Dg1 SJ 36.6(12) 111_545 . 1_555 N
O1 Dg1 Og 128.0(16) 111_545 . 1_555 N
O1 Dg1 Og 163.9(7) 111_545 . 105_544 N
O1 Dg1 Og 36.0(6) 111_545 . -108_656 N
O1 Dg1 Og 135.6(4) 111_545 . 308_445 N
O1 Dg1 Og 69.7(5) 111_545 . -305_556 N
O1 Dg1 Dg1 171.3(9) 111_554 . 105_544 N
O1 Dg1 Dg1 53.0(5) 111_554 . -108_665 N
O1 Dg1 Dg1 142.9(5) 111_554 . 308_454 N
O1 Dg1 Dg1 82.9(5) 111_554 . -305_565 N
O1 Dg1 Dg2 102.0(13) 111_555 . 1_555 N
O1 Dg1 Dg2 172.4(6) 111_555 . 105_544 N
O1 Dg1 Dg2 17.44(34) 111_555 . -108_666 N
O1 Dg1 Oh 58.3(8) 111_554 . 1_555 N
O1 Dg1 Oh 128.5(9) 111_554 . 105_544 N
O1 Dg1 Oh 58.0(4) 111_554 . -108_665 N
O1 Dg1 Oh 148.8(6) 111_554 . 308_454 N
O1 Dg1 Dh1 81.4(14) 111_533 . 1_555 N
O1 Dg1 Dh1 143.3(10) 111_533 . 105_544 N
O1 Dg1 Dh1 57.3(7) 111_533 . -108_644 N
O1 Dg1 Dh1 141.6(6) 111_533 . 308_433 N
O4 Dg1 O4 92.7(4) -111_444 . 312_334 N
O4 Dg1 SJ 99.9(13) -111_556 . 1_555 N
O4 Dg1 Og 39.3(10) -111_556 . 1_555 N
O4 Dg1 Og 56.4(4) -111_556 . 105_544 N
O4 Dg1 Og 144.9(12) -111_556 . -108_656 N
O4 Dg1 Og 93.0(5) -111_556 . 308_445 N
O4 Dg1 Og 158.7(7) -111_556 . -305_556 N
O4 Dg1 Dg1 54.8(8) -111_565 . 105_544 N
O4 Dg1 Dg1 165.4(14) -111_565 . -108_665 N
O4 Dg1 Dg1 85.1(7) -111_565 . 308_454 N
O4 Dg1 Dg1 144.1(7) -111_565 . -305_565 N
O4 Dg1 Dg2 34.7(9) -111_566 . 1_555 N
O4 Dg1 Dg2 44.15(32) -111_566 . 105_544 N
O4 Dg1 Dg2 142.5(6) -111_566 . -108_666 N
O4 Dg1 Oh 114.6(9) -111_565 . 1_555 N
O4 Dg1 Oh 42.0(5) -111_565 . 105_544 N
O4 Dg1 Oh 139.7(7) -111_565 . -108_665 N
O4 Dg1 Oh 74.3(5) -111_565 . 308_454 N
O4 Dg1 Dh1 100.0(15) -111_544 . 1_555 N
O4 Dg1 Dh1 51.2(6) -111_544 . 105_544 N
O4 Dg1 Dh1 137.3(10) -111_544 . -108_644 N
O4 Dg1 Dh1 85.2(5) -111_544 . 308_433 N
O4 Dg1 SJ 8.8(12) 312_446 . 1_555 N
O4 Dg1 Og 89.9(13) 312_446 . 1_555 N
O4 Dg1 Og 149.0(5) 312_446 . 105_544 N
O4 Dg1 Og 75.1(9) 312_446 . -108_656 N
O4 Dg1 Og 165.1(6) 312_446 . 308_445 N
O4 Dg1 Og 108.5(7) 312_446 . -305_556 N
O4 Dg1 Dg1 146.6(7) 312_455 . 105_544 N
O4 Dg1 Dg1 94.1(7) 312_455 . -108_665 N
O4 Dg1 Dg1 171.3(4) 312_455 . 308_454 N
O4 Dg1 Dg1 123.1(7) 312_455 . -305_565 N
O4 Dg1 Dg2 60.8(11) 312_456 . 1_555 N
O4 Dg1 Dg2 136.3(6) 312_456 . 105_544 N
O4 Dg1 Dg2 58.0(5) 312_456 . -108_666 N
O4 Dg1 Oh 55.1(8) 312_455 . 1_555 N
O4 Dg1 Oh 112.3(9) 312_455 . 105_544 N
O4 Dg1 Oh 96.3(6) 312_455 . -108_665 N
O4 Dg1 Oh 141.7(6) 312_455 . 308_454 N
O4 Dg1 Dh1 71.2(13) 312_434 . 1_555 N
O4 Dg1 Dh1 133.3(10) 312_434 . 105_544 N
O4 Dg1 Dh1 94.7(8) 312_434 . -108_644 N
O4 Dg1 Dh1 151.1(8) 312_434 . 308_433 N
SJ Dg1 Og 92.3(17) 1_555 . 1_555 N
SJ Dg1 Og 156.1(13) 1_555 . 105_544 N
SJ Dg1 Og 72.0(15) 1_555 . -108_656 N
SJ Dg1 Og 157.2(16) 1_555 . 308_445 N
SJ Dg1 Og 101.0(15) 1_555 . -305_556 N
SJ Dg1 Dg1 151.9(15) 1_555 . 105_544 N
SJ Dg1 Dg1 88.1(15) 1_555 . -108_665 N
SJ Dg1 Dg1 165.7(15) 1_555 . 308_454 N
SJ Dg1 Dg1 116.0(15) 1_555 . -305_565 N
SJ Dg1 Dg2 66.7(15) 1_555 . 1_555 N
SJ Dg1 Dg2 142.4(13) 1_555 . 105_544 N
SJ Dg1 Dg2 53.9(13) 1_555 . -108_666 N
SJ Dg1 Oh 47.3(14) 1_555 . 1_555 N
SJ Dg1 Oh 121.1(18) 1_555 . 105_544 N
SJ Dg1 Oh 93.9(13) 1_555 . -108_665 N
SJ Dg1 Oh 138.9(15) 1_555 . 308_454 N
SJ Dg1 Dh1 65.1(18) 1_555 . 1_555 N
SJ Dg1 Dh1 142.2(18) 1_555 . 105_544 N
SJ Dg1 Dh1 92.7(15) 1_555 . -108_644 N
SJ Dg1 Dh1 145.9(17) 1_555 . 308_433 N
Og Dg1 Og 67.6(13) 1_555 . 105_544 N
Og Dg1 Og 163.9(20) 1_555 . -108_656 N
Og Dg1 Og 85.8(13) 1_555 . 308_445 N
Og Dg1 Og 135.2(14) 1_555 . -305_556 N
Og Dg1 Dg1 60.7(16) 1_555 . 105_544 N
Og Dg1 Dg1 153.4(22) 1_555 . -108_665 N
Og Dg1 Dg1 83.1(16) 1_555 . 308_454 N
Og Dg1 Dg1 132.9(13) 1_555 . -305_565 N
Og Dg1 Dg2 37.77090(10) 1_555 . 1_555 N
Og Dg1 Dg2 54.1(12) 1_555 . 105_544 N
Og Dg1 Dg2 145.2(17) 1_555 . -108_666 N
Og Dg1 Oh 81.1(16) 1_555 . 1_555 N
Og Dg1 Oh 78.5(13) 1_555 . 105_544 N
Og Dg1 Oh 173.8(17) 1_555 . -108_665 N
Og Dg1 Oh 57.1(12) 1_555 . 308_454 N
Og Dg1 Dh1 62.1(18) 1_555 . 1_555 N
Og Dg1 Dh1 78.8(15) 1_555 . 105_544 N
Og Dg1 Dh1 174.6(19) 1_555 . -108_644 N
Og Dg1 Dh1 70.3(13) 1_555 . 308_433 N
Og Dg1 Og 128.4(10) 105_544 . -108_656 N
Og Dg1 Og 39.4(4) 105_544 . 308_445 N
Og Dg1 Og 102.5(6) 105_544 . -305_556 N
Og Dg1 Dg1 8.4(7) 105_544 . 105_544 N
Og Dg1 Dg1 115.7(7) 105_544 . -108_665 N
Og Dg1 Dg1 30.3(5) 105_544 . 308_454 N
Og Dg1 Dg1 87.7(5) 105_544 . -305_565 N
Og Dg1 Dg2 89.4(10) 105_544 . 1_555 N
Og Dg1 Dg2 14.15(22) 105_544 . 105_544 N
Og Dg1 Dg2 147.2(8) 105_544 . -108_666 N
Og Dg1 Oh 135.3(12) 105_544 . 1_555 N
Og Dg1 Oh 44.4(6) 105_544 . 105_544 N
Og Dg1 Oh 106.5(7) 105_544 . -108_665 N
Og Dg1 Oh 38.9(5) 105_544 . 308_454 N
Og Dg1 Dh1 112.5(16) 105_544 . 1_555 N
Og Dg1 Dh1 25.2(7) 105_544 . 105_544 N
Og Dg1 Dh1 107.0(9) 105_544 . -108_644 N
Og Dg1 Dh1 40.6(6) 105_544 . 308_433 N
Og Dg1 Og 107.2(6) -108_656 . 308_445 N
Og Dg1 Og 48.5(5) -108_656 . -305_556 N
Og Dg1 Dg1 135.3(10) -108_665 . 105_544 N
Og Dg1 Dg1 27.73(31) -108_665 . -108_665 N
Og Dg1 Dg1 111.3(4) -108_665 . 308_454 N
Og Dg1 Dg1 55.8(6) -108_665 . -305_565 N
Og Dg1 Dg2 132.1(18) -108_666 . 1_555 N
Og Dg1 Dg2 141.9(12) -108_666 . 105_544 N
Og Dg1 Dg2 18.7(4) -108_666 . -108_666 N
Og Dg1 Oh 85.4(11) -108_665 . 1_555 N
Og Dg1 Oh 112.3(13) -108_665 . 105_544 N
Og Dg1 Oh 22.0(6) -108_665 . -108_665 N
Og Dg1 Oh 134.1(9) -108_665 . 308_454 N
Og Dg1 Dh1 106.5(17) -108_644 . 1_555 N
Og Dg1 Dh1 115.8(13) -108_644 . 105_544 N
Og Dg1 Dh1 21.4(7) -108_644 . -108_644 N
Og Dg1 Dh1 121.0(9) -108_644 . 308_433 N
Og Dg1 Og 65.92(31) 308_445 . -305_556 N
Og Dg1 Dg1 38.5(4) 308_454 . 105_544 N
Og Dg1 Dg1 83.69(30) 308_454 . -108_665 N
Og Dg1 Dg1 9.48(18) 308_454 . 308_454 N
Og Dg1 Dg1 53.36(31) 308_454 . -305_565 N
Og Dg1 Dg2 120.2(12) 308_455 . 1_555 N
Og Dg1 Dg2 49.1(4) 308_455 . 105_544 N
Og Dg1 Dg2 121.47(21) 308_455 . -108_666 N
Og Dg1 Oh 110.2(9) 308_454 . 1_555 N
Og Dg1 Oh 80.8(8) 308_454 . 105_544 N
Og Dg1 Oh 88.2(5) 308_454 . -108_665 N
Og Dg1 Oh 29.3(4) 308_454 . 308_454 N
Og Dg1 Dh1 94.3(14) 308_433 . 1_555 N
Og Dg1 Dh1 59.6(8) 308_433 . 105_544 N
Og Dg1 Dh1 90.5(8) 308_433 . -108_644 N
Og Dg1 Dh1 17.0(5) 308_433 . 308_433 N
Og Dg1 Dg1 103.90(31) -305_565 . 105_544 N
Og Dg1 Dg1 20.8(5) -305_565 . -108_665 N
Og Dg1 Dg1 73.57(19) -305_565 . 308_454 N
Og Dg1 Dg1 15.47(11) -305_565 . -305_565 N
Og Dg1 Dg2 161.6(14) -305_566 . 1_555 N
Og Dg1 Dg2 114.5(7) -305_566 . 105_544 N
Og Dg1 Dg2 56.8(4) -305_566 . -108_666 N
Og Dg1 Oh 77.6(8) -305_565 . 1_555 N
Og Dg1 Oh 126.1(8) -305_565 . 105_544 N
Og Dg1 Oh 42.3(4) -305_565 . -108_665 N
Og Dg1 Oh 87.2(6) -305_565 . 308_454 N
Og Dg1 Dh1 85.2(14) -305_544 . 1_555 N
Og Dg1 Dh1 111.2(8) -305_544 . 105_544 N
Og Dg1 Dh1 45.5(9) -305_544 . -108_644 N
Og Dg1 Dh1 75.1(6) -305_544 . 308_433 N
Dg1 Dg1 Dg1 119.32(33) 105_544 . -108_665 N
Dg1 Dg1 Dg1 30.34(17) 105_544 . 308_454 N
Dg1 Dg1 Dg1 90.00000(30) 105_544 . -305_565 N
Dg1 Dg1 Dg2 85.9(15) 105_544 . 1_555 N
Dg1 Dg1 Dg2 10.7(7) 105_544 . 105_544 N
Dg1 Dg1 Dg2 153.9(8) 105_544 . -108_666 N
Dg1 Dg1 Oh 127.2(17) 105_544 . 1_555 N
Dg1 Dg1 Oh 50.1(11) 105_544 . 105_544 N
Dg1 Dg1 Oh 113.3(9) 105_544 . -108_665 N
Dg1 Dg1 Oh 32.1(9) 105_544 . 308_454 N
Dg1 Dg1 Dh1 104.3(19) 105_544 . 1_555 N
Dg1 Dg1 Dh1 32.4(11) 105_544 . 105_544 N
Dg1 Dg1 Dh1 114.0(11) 105_544 . -108_644 N
Dg1 Dg1 Dh1 36.0(8) 105_544 . 308_433 N
Dg1 Dg1 Dg1 90.00000(20) -108_665 . 308_454 N
Dg1 Dg1 Dg1 30.34(17) -108_665 . -305_565 N
Dg1 Dg1 Dg2 154.8(16) -108_666 . 1_555 N
Dg1 Dg1 Dg2 129.4(8) -108_666 . 105_544 N
Dg1 Dg1 Dg2 37.8(4) -108_666 . -108_666 N
Dg1 Dg1 Oh 79.7(12) -108_665 . 1_555 N
Dg1 Dg1 Oh 123.5(14) -108_665 . 105_544 N
Dg1 Dg1 Oh 26.4(9) -108_665 . -108_665 N
Dg1 Dg1 Oh 107.5(7) -108_665 . 308_454 N
Dg1 Dg1 Dh1 94.4(18) -108_644 . 1_555 N
Dg1 Dg1 Dh1 115.9(12) -108_644 . 105_544 N
Dg1 Dg1 Dh1 29.1(11) -108_644 . -108_644 N
Dg1 Dg1 Dh1 95.0(6) -108_644 . 308_433 N
Dg1 Dg1 Dg1 60.00000(20) 308_454 . -305_565 N
Dg1 Dg1 Dg2 114.8(15) 308_455 . 1_555 N
Dg1 Dg1 Dg2 41.0(7) 308_455 . 105_544 N
Dg1 Dg1 Dg2 127.3(4) 308_455 . -108_666 N
Dg1 Dg1 Oh 118.4(8) 308_454 . 1_555 N
Dg1 Dg1 Oh 71.3(9) 308_454 . 105_544 N
Dg1 Dg1 Oh 90.7(4) 308_454 . -108_665 N
Dg1 Dg1 Oh 29.7(5) 308_454 . 308_454 N
Dg1 Dg1 Dh1 100.9(14) 308_433 . 1_555 N
Dg1 Dg1 Dh1 50.2(9) 308_433 . 105_544 N
Dg1 Dg1 Dh1 92.6(7) 308_433 . -108_644 N
Dg1 Dg1 Dh1 20.4(6) 308_433 . 308_433 N
Dg1 Dg1 Dg2 170.1(12) -305_566 . 1_555 N
Dg1 Dg1 Dg2 100.5(7) -305_566 . 105_544 N
Dg1 Dg1 Dg2 68.1(4) -305_566 . -108_666 N
Dg1 Dg1 Oh 91.3(8) -305_565 . 1_555 N
Dg1 Dg1 Oh 111.8(8) -305_565 . 105_544 N
Dg1 Dg1 Oh 42.7(5) -305_565 . -108_665 N
Dg1 Dg1 Oh 78.3(5) -305_565 . 308_454 N
Dg1 Dg1 Dh1 95.2(14) -305_544 . 1_555 N
Dg1 Dg1 Dh1 95.8(7) -305_544 . 105_544 N
Dg1 Dg1 Dh1 45.8(9) -305_544 . -108_644 N
Dg1 Dg1 Dh1 65.3(5) -305_544 . 308_433 N
Dg2 Dg1 Dg2 75.8(8) 1_555 . 105_544 N
Dg2 Dg1 Dg2 117.9(12) 1_555 . -108_666 N
Dg2 Dg1 Oh 84.1(13) 1_555 . 1_555 N
Dg2 Dg1 Oh 72.1(12) 1_555 . 105_544 N
Dg2 Dg1 Oh 147.0(14) 1_555 . -108_665 N
Dg2 Dg1 Oh 93.6(11) 1_555 . 308_454 N
Dg2 Dg1 Dh1 77.2(16) 1_555 . 1_555 N
Dg2 Dg1 Dh1 85.5(12) 1_555 . 105_544 N
Dg2 Dg1 Dh1 143.9(17) 1_555 . -108_644 N
Dg2 Dg1 Dh1 106.8(12) 1_555 . 308_433 N
Dg2 Dg1 Dg2 160.5(9) 105_544 . -108_666 N
Dg2 Dg1 Oh 128.0(11) 105_544 . 1_555 N
Dg2 Dg1 Oh 44.0(6) 105_544 . 105_544 N
Dg2 Dg1 Oh 120.3(8) 105_544 . -108_665 N
Dg2 Dg1 Oh 38.7(4) 105_544 . 308_454 N
Dg2 Dg1 Dh1 104.9(15) 105_544 . 1_555 N
Dg2 Dg1 Dh1 30.1(8) 105_544 . 105_544 N
Dg2 Dg1 Dh1 120.5(10) 105_544 . -108_644 N
Dg2 Dg1 Dh1 45.1(6) 105_544 . 308_433 N
Dg2 Dg1 Oh 69.7(10) -108_665 . 1_555 N
Dg2 Dg1 Oh 123.8(10) -108_665 . 105_544 N
Dg2 Dg1 Oh 40.7(4) -108_665 . -108_665 N
Dg2 Dg1 Oh 143.2(7) -108_665 . 308_454 N
Dg2 Dg1 Dh1 92.3(15) -108_644 . 1_555 N
Dg2 Dg1 Dh1 132.2(11) -108_644 . 105_544 N
Dg2 Dg1 Dh1 40.2(6) -108_644 . -108_644 N
Dg2 Dg1 Dh1 131.9(6) -108_644 . 308_433 N
Oh Dg1 Oh 156.0(11) 1_555 . 105_544 N
Oh Dg1 Oh 102.5(10) 1_555 . -108_665 N
Oh Dg1 Oh 97.3(11) 1_555 . 308_454 N
Oh Dg1 Dh1 23.2(10) 1_555 . 1_555 N
Oh Dg1 Dh1 158.0(14) 1_555 . 105_544 N
Oh Dg1 Dh1 103.9(11) 1_555 . -108_644 N
Oh Dg1 Dh1 99.8(11) 1_555 . 308_433 N
Oh Dg1 Oh 99.0(10) 105_544 . -108_665 N
Oh Dg1 Oh 82.0(8) 105_544 . 308_454 N
Oh Dg1 Dh1 140.6(17) 105_544 . 1_555 N
Oh Dg1 Dh1 21.17(23) 105_544 . 105_544 N
Oh Dg1 Dh1 97.1(11) 105_544 . -108_644 N
Oh Dg1 Dh1 85.0(9) 105_544 . 308_433 N
Oh Dg1 Oh 117.1(6) -108_665 . 308_454 N
Oh Dg1 Dh1 120.1(15) -108_644 . 1_555 N
Oh Dg1 Dh1 96.8(10) -108_644 . 105_544 N
Oh Dg1 Dh1 3.2(8) -108_644 . -108_644 N
Oh Dg1 Dh1 103.9(6) -108_644 . 308_433 N
Oh Dg1 Dh1 75.8(14) 308_433 . 1_555 N
Oh Dg1 Dh1 64.1(9) 308_433 . 105_544 N
Oh Dg1 Dh1 119.5(9) 308_433 . -108_644 N
Oh Dg1 Dh1 13.27(13) 308_433 . 308_433 N
Dh1 Dg1 Dh1 135.0(18) 1_555 . 105_544 N
Dh1 Dg1 Dh1 122.1(19) 1_555 . -108_644 N
Dh1 Dg1 Dh1 80.8(16) 1_555 . 308_433 N
Dh1 Dg1 Dh1 96.0(14) 105_544 . -108_644 N
Dh1 Dg1 Dh1 64.9(11) 105_544 . 308_433 N
Dh1 Dg1 Dh1 106.4(9) -108_644 . 308_433 N
O1 Dg2 O2 30.2(5) -3_555 . 105_544 N
O1 Dg2 O2 28.2(5) -3_555 . -304_444 N
O1 Dg2 O3 48.9(4) -3_555 . 2_555 N
O1 Dg2 O3 33.5(4) -3_555 . -1_555 N
O1 Dg2 O4 64.2(5) -3_555 . -111_444 N
O1 Dg2 O4 70.3(6) -3_555 . 312_334 N
O1 Dg2 SJ 116.9(13) -3_555 . 1_555 N
O1 Dg2 Og 170.9(16) -3_555 . 1_555 N
O1 Dg2 Og 128.3(9) -3_555 . 105_544 N
O1 Dg2 Og 126.1(10) -3_555 . -108_656 N
O1 Dg2 Dg1 150.8(17) -3_555 . 1_555 N
O1 Dg2 Dg1 137.7(8) -3_555 . 105_544 N
O1 Dg2 Dg1 140.4(12) -3_555 . -108_665 N
O1 Dg2 Dg2 116.4(9) -3_555 . 105_544 N
O1 Dg2 Dg2 116.0(11) -3_555 . -108_666 N
O1 Dg2 Oh 124.1(10) -3_555 . 1_555 N
O1 Dg2 Oh 98.8(9) -3_555 . 105_544 N
O1 Dg2 Dh1 142.5(13) -3_555 . 1_555 N
O1 Dg2 Dh1 116.7(9) -3_555 . 105_544 N
O1 Dg2 Dh2 104.2(9) -3_555 . 1_555 N
O1 Dg2 Dh2 86.3(9) -3_555 . 105_544 N
O1 Dg2 OII* 104.1(8) -3_555 . -105_444 N
O1 Dg2 DII*1 113.1(11) -3_555 . -105_443 N
O1 Dg2 DII*1 83.6(10) -3_555 . -208_443 N
O2 Dg2 O2 57.12(20) 105_544 . -304_444 N
O2 Dg2 O3 58.72(23) 105_544 . 2_555 N
O2 Dg2 O3 38.78(15) 105_544 . -1_555 N
O2 Dg2 O4 43.07(24) 105_544 . -111_444 N
O2 Dg2 O4 95.7(4) 105_544 . 312_334 N
O2 Dg2 SJ 144.2(10) 105_544 . 1_555 N
O2 Dg2 Og 140.7(13) 105_544 . 1_555 N
O2 Dg2 Og 108.6(6) 105_544 . 105_544 N
O2 Dg2 Og 155.9(6) 105_544 . -108_656 N
O2 Dg2 Dg1 170.3(13) 105_544 . 1_555 N
O2 Dg2 Dg1 116.2(5) 105_544 . 105_544 N
O2 Dg2 Dg1 170.6(7) 105_544 . -108_665 N
O2 Dg2 Dg2 93.4(6) 105_544 . 105_544 N
O2 Dg2 Dg2 145.9(6) 105_544 . -108_666 N
O2 Dg2 Oh 132.0(8) 105_544 . 1_555 N
O2 Dg2 Oh 96.1(7) 105_544 . 105_544 N
O2 Dg2 Dh1 139.9(15) 105_544 . 1_555 N
O2 Dg2 Dh1 107.6(7) 105_544 . 105_544 N
O2 Dg2 Dh2 121.6(9) 105_544 . 1_555 N
O2 Dg2 Dh2 76.6(7) 105_544 . 105_544 N
O2 Dg2 OII* 103.0(5) 105_544 . -105_444 N
O2 Dg2 DII*1 115.0(6) 105_544 . -105_443 N
O2 Dg2 DII*1 88.3(10) 105_544 . -208_443 N
O2 Dg2 O3 40.47(17) -304_444 . 2_555 N
O2 Dg2 O3 54.39(18) -304_444 . -1_555 N
O2 Dg2 O4 91.53(33) -304_444 . -111_444 N
O2 Dg2 O4 42.83(21) -304_444 . 312_334 N
O2 Dg2 SJ 88.7(10) -304_556 . 1_555 N
O2 Dg2 Og 160.2(9) -304_556 . 1_555 N
O2 Dg2 Og 148.9(6) -304_556 . 105_544 N
O2 Dg2 Og 100.8(6) -304_556 . -108_656 N
O2 Dg2 Dg1 126.9(14) -304_565 . 1_555 N
O2 Dg2 Dg1 157.7(7) -304_565 . 105_544 N
O2 Dg2 Dg1 113.9(7) -304_565 . -108_665 N
O2 Dg2 Dg2 142.2(6) -304_566 . 105_544 N
O2 Dg2 Dg2 88.8(6) -304_566 . -108_666 N
O2 Dg2 Oh 101.2(7) -304_565 . 1_555 N
O2 Dg2 Oh 110.0(7) -304_565 . 105_544 N
O2 Dg2 Dh1 121.4(10) -304_544 . 1_555 N
O2 Dg2 Dh1 129.3(8) -304_544 . 105_544 N
O2 Dg2 Dh2 78.9(7) -304_544 . 1_555 N
O2 Dg2 Dh2 105.7(9) -304_544 . 105_544 N
O2 Dg2 OII* 91.2(6) -304_444 . -105_444 N
O2 Dg2 DII*1 96.0(11) -304_443 . -105_443 N
O2 Dg2 DII*1 91.6(7) -304_443 . -208_443 N
O3 Dg2 O3 82.37(25) 2_555 . -1_555 N
O3 Dg2 O4 101.6(4) 2_555 . -111_444 N
O3 Dg2 O4 45.85(24) 2_555 . 312_334 N
O3 Dg2 SJ 88.9(9) 2_555 . 1_555 N
O3 Dg2 Og 132.2(9) 2_555 . 1_555 N
O3 Dg2 Og 159.9(8) 2_555 . 105_544 N
O3 Dg2 Og 112.2(6) 2_555 . -108_656 N
O3 Dg2 Dg1 130.6(13) 2_555 . 1_555 N
O3 Dg2 Dg1 158.8(8) 2_555 . 105_544 N
O3 Dg2 Dg1 117.1(6) 2_555 . -108_665 N
O3 Dg2 Dg2 144.8(8) 2_555 . 105_544 N
O3 Dg2 Dg2 96.9(6) 2_555 . -108_666 N
O3 Dg2 Oh 77.2(6) 2_555 . 1_555 N
O3 Dg2 Oh 147.5(8) 2_555 . 105_544 N
O3 Dg2 Dh1 93.8(11) 2_555 . 1_555 N
O3 Dg2 Dh1 165.3(8) 2_555 . 105_544 N
O3 Dg2 Dh2 62.9(8) 2_555 . 1_555 N
O3 Dg2 Dh2 133.6(8) 2_555 . 105_544 N
O3 Dg2 OII* 55.4(5) 2_555 . -105_444 N
O3 Dg2 DII*1 64.2(9) 2_555 . -105_443 N
O3 Dg2 DII*1 130.6(8) 2_555 . -208_443 N
O3 Dg2 O4 41.49(22) -1_555 . -111_444 N
O3 Dg2 O4 95.7(4) -1_555 . 312_334 N
O3 Dg2 SJ 130.3(12) -1_555 . 1_555 N
O3 Dg2 Og 143.0(7) -1_555 . 1_555 N
O3 Dg2 Og 96.5(5) -1_555 . 105_544 N
O3 Dg2 Og 122.4(7) -1_555 . -108_656 N
O3 Dg2 Dg1 134.0(13) -1_555 . 1_555 N
O3 Dg2 Dg1 106.0(6) -1_555 . 105_544 N
O3 Dg2 Dg1 135.2(7) -1_555 . -108_665 N
O3 Dg2 Dg2 87.8(6) -1_555 . 105_544 N
O3 Dg2 Dg2 122.0(8) -1_555 . -108_666 N
O3 Dg2 Oh 155.6(8) -1_555 . 1_555 N
O3 Dg2 Oh 65.7(6) -1_555 . 105_544 N
O3 Dg2 Dh1 175.7(10) -1_555 . 1_555 N
O3 Dg2 Dh1 83.2(7) -1_555 . 105_544 N
O3 Dg2 Dh2 132.8(8) -1_555 . 1_555 N
O3 Dg2 Dh2 53.2(7) -1_555 . 105_544 N
O3 Dg2 OII* 136.9(6) -1_555 . -105_444 N
O3 Dg2 DII*1 146.6(9) -1_555 . -105_443 N
O3 Dg2 DII*1 52.5(9) -1_555 . -208_443 N
O4 Dg2 O4 134.3(5) -111_444 . 312_334 N
O4 Dg2 SJ 164.0(12) -111_556 . 1_555 N
O4 Dg2 Og 108.2(9) -111_556 . 1_555 N
O4 Dg2 Og 66.4(5) -111_556 . 105_544 N
O4 Dg2 Og 140.4(7) -111_556 . -108_656 N
O4 Dg2 Dg1 127.8(13) -111_565 . 1_555 N
O4 Dg2 Dg1 74.9(5) -111_565 . 105_544 N
O4 Dg2 Dg1 140.9(5) -111_565 . -108_665 N
O4 Dg2 Dg2 52.5(5) -111_566 . 105_544 N
O4 Dg2 Dg2 151.7(9) -111_566 . -108_666 N
O4 Dg2 Oh 156.9(10) -111_565 . 1_555 N
O4 Dg2 Oh 58.4(6) -111_565 . 105_544 N
O4 Dg2 Dh1 141.9(13) -111_544 . 1_555 N
O4 Dg2 Dh1 65.4(6) -111_544 . 105_544 N
O4 Dg2 Dh2 164.0(11) -111_544 . 1_555 N
O4 Dg2 Dh2 36.9(6) -111_544 . 105_544 N
O4 Dg2 OII* 132.2(6) -111_444 . -105_444 N
O4 Dg2 DII*1 142.7(9) -111_443 . -105_443 N
O4 Dg2 DII*1 59.5(11) -111_443 . -208_443 N
O4 Dg2 SJ 48.5(9) 312_446 . 1_555 N
O4 Dg2 Og 117.4(8) 312_446 . 1_555 N
O4 Dg2 Og 153.4(7) 312_446 . 105_544 N
O4 Dg2 Og 68.0(5) 312_446 . -108_656 N
O4 Dg2 Dg1 91.5(13) 312_455 . 1_555 N
O4 Dg2 Dg1 147.8(5) 312_455 . 105_544 N
O4 Dg2 Dg1 76.9(7) 312_455 . -108_665 N
O4 Dg2 Dg2 169.4(8) 312_456 . 105_544 N
O4 Dg2 Dg2 53.0(5) 312_456 . -108_666 N
O4 Dg2 Oh 60.4(7) 312_455 . 1_555 N
O4 Dg2 Oh 128.4(9) 312_455 . 105_544 N
O4 Dg2 Dh1 80.2(10) 312_434 . 1_555 N
O4 Dg2 Dh1 138.8(10) 312_434 . 105_544 N
O4 Dg2 Dh2 37.2(6) 312_434 . 1_555 N
O4 Dg2 Dh2 138.7(11) 312_434 . 105_544 N
O4 Dg2 OII* 62.6(5) 312_334 . -105_444 N
O4 Dg2 DII*1 61.2(11) 312_333 . -105_443 N
O4 Dg2 DII*1 112.8(9) 312_333 . -208_443 N
SJ Dg2 Og 71.8(10) 1_555 . 1_555 N
SJ Dg2 Og 106.6(8) 1_555 . 105_544 N
SJ Dg2 Og 24.9(8) 1_555 . -108_656 N
SJ Dg2 Dg1 43.4(11) 1_555 . 1_555 N
SJ Dg2 Dg1 99.5(8) 1_555 . 105_544 N
SJ Dg2 Dg1 28.9(9) 1_555 . -108_665 N
SJ Dg2 Dg2 122.3(8) 1_555 . 105_544 N
SJ Dg2 Dg2 12.3(7) 1_555 . -108_666 N
SJ Dg2 Oh 37.3(9) 1_555 . 1_555 N
SJ Dg2 Oh 106.7(12) 1_555 . 105_544 N
SJ Dg2 Dh1 47.4(13) 1_555 . 1_555 N
SJ Dg2 Dh1 102.4(11) 1_555 . 105_544 N
SJ Dg2 Dh2 30.3(10) 1_555 . 1_555 N
SJ Dg2 Dh2 128.1(13) 1_555 . 105_544 N
SJ Dg2 OII* 63.8(9) 1_555 . -105_444 N
SJ Dg2 DII*1 53.0(10) 1_555 . -105_443 N
SJ Dg2 DII*1 104.5(14) 1_555 . -208_443 N
Og Dg2 Og 46.6(5) 1_555 . 105_544 N
Og Dg2 Og 62.9(11) 1_555 . -108_656 N
Og Dg2 Dg1 37.73460(10) 1_555 . 1_555 N
Og Dg2 Dg1 37.0(7) 1_555 . 105_544 N
Og Dg2 Dg1 48.7(8) 1_555 . -108_665 N
Og Dg2 Dg2 56.7(5) 1_555 . 105_544 N
Og Dg2 Dg2 73.1(7) 1_555 . -108_666 N
Og Dg2 Oh 60.8(7) 1_555 . 1_555 N
Og Dg2 Oh 80.2(9) 1_555 . 105_544 N
Og Dg2 Dh1 41.2(9) 1_555 . 1_555 N
Og Dg2 Dh1 61.4(9) 1_555 . 105_544 N
Og Dg2 Dh2 82.2(8) 1_555 . 1_555 N
Og Dg2 Dh2 89.9(10) 1_555 . 105_544 N
Og Dg2 OII* 76.9(9) 1_555 . -105_444 N
Og Dg2 DII*1 69.4(11) 1_555 . -105_443 N
Og Dg2 DII*1 96.9(12) 1_555 . -208_443 N
Og Dg2 Og 85.5(4) 105_544 . -108_656 N
Og Dg2 Dg1 63.3(9) 105_544 . 1_555 N
Og Dg2 Dg1 9.5(4) 105_544 . 105_544 N
Og Dg2 Dg1 77.75(20) 105_544 . -108_665 N
Og Dg2 Dg2 16.15(7) 105_544 . 105_544 N
Og Dg2 Dg2 100.69(33) 105_544 . -108_666 N
Og Dg2 Oh 107.3(6) 105_544 . 1_555 N
Og Dg2 Oh 40.2(6) 105_544 . 105_544 N
Og Dg2 Dh1 87.8(8) 105_544 . 1_555 N
Og Dg2 Dh1 22.1(6) 105_544 . 105_544 N
Og Dg2 Dh2 127.1(7) 105_544 . 1_555 N
Og Dg2 Dh2 43.7(9) 105_544 . 105_544 N
Og Dg2 OII* 119.8(6) 105_544 . -105_444 N
Og Dg2 DII*1 114.9(11) 105_544 . -105_443 N
Og Dg2 DII*1 58.8(8) 105_544 . -208_443 N
Og Dg2 Dg1 26.1(11) -108_665 . 1_555 N
Og Dg2 Dg1 80.22(26) -108_665 . 105_544 N
Og Dg2 Dg1 14.84(25) -108_665 . -108_665 N
Og Dg2 Dg2 101.7(4) -108_666 . 105_544 N
Og Dg2 Dg2 15.35(8) -108_666 . -108_666 N
Og Dg2 Oh 56.1(6) -108_665 . 1_555 N
Og Dg2 Oh 82.1(7) -108_665 . 105_544 N
Og Dg2 Dh1 57.3(13) -108_644 . 1_555 N
Og Dg2 Dh1 78.0(7) -108_644 . 105_544 N
Og Dg2 Dh2 55.0(9) -108_644 . 1_555 N
Og Dg2 Dh2 103.5(8) -108_644 . 105_544 N
Og Dg2 OII* 85.5(5) -108_544 . -105_444 N
Og Dg2 DII*1 73.7(5) -108_543 . -105_443 N
Og Dg2 DII*1 82.4(11) -108_543 . -208_443 N
Dg1 Dg2 Dg1 56.3(12) 1_555 . 105_544 N
Dg1 Dg2 Dg1 14.5(9) 1_555 . -108_665 N
Dg1 Dg2 Dg2 79.0(9) 1_555 . 105_544 N
Dg1 Dg2 Dg2 39.2(9) 1_555 . -108_666 N
Dg1 Dg2 Oh 57.5(12) 1_555 . 1_555 N
Dg1 Dg2 Oh 74.3(12) 1_555 . 105_544 N
Dg1 Dg2 Dh1 47.9(15) 1_555 . 1_555 N
Dg1 Dg2 Dh1 62.8(11) 1_555 . 105_544 N
Dg1 Dg2 Dh2 67.8(13) 1_555 . 1_555 N
Dg1 Dg2 Dh2 93.7(13) 1_555 . 105_544 N
Dg1 Dg2 OII* 86.1(11) 1_555 . -105_444 N
Dg1 Dg2 DII*1 74.3(12) 1_555 . -105_443 N
Dg1 Dg2 DII*1 82.9(15) 1_555 . -208_443 N
Dg1 Dg2 Dg1 70.9(5) 105_544 . -108_665 N
Dg1 Dg2 Dg2 22.86(32) 105_544 . 105_544 N
Dg1 Dg2 Dg2 94.96(27) 105_544 . -108_666 N
Dg1 Dg2 Oh 97.8(8) 105_544 . 1_555 N
Dg1 Dg2 Oh 47.7(7) 105_544 . 105_544 N
Dg1 Dg2 Dh1 78.2(10) 105_544 . 1_555 N
Dg1 Dg2 Dh1 28.6(7) 105_544 . 105_544 N
Dg1 Dg2 Dh2 118.0(7) 105_544 . 1_555 N
Dg1 Dg2 Dh2 53.1(9) 105_544 . 105_544 N
Dg1 Dg2 OII* 111.1(8) 105_544 . -105_444 N
Dg1 Dg2 DII*1 105.6(12) 105_544 . -105_443 N
Dg1 Dg2 DII*1 66.2(9) 105_544 . -208_443 N
Dg1 Dg2 Dg2 93.50(17) -108_666 . 105_544 N
Dg1 Dg2 Dg2 25.23(14) -108_666 . -108_666 N
Dg1 Dg2 Oh 49.0(7) -108_665 . 1_555 N
Dg1 Dg2 Oh 84.4(6) -108_665 . 105_544 N
Dg1 Dg2 Dh1 45.3(13) -108_644 . 1_555 N
Dg1 Dg2 Dh1 75.5(6) -108_644 . 105_544 N
Dg1 Dg2 Dh2 55.0(9) -108_644 . 1_555 N
Dg1 Dg2 Dh2 105.1(7) -108_644 . 105_544 N
Dg1 Dg2 OII* 78.9(4) -108_544 . -105_444 N
Dg1 Dg2 DII*1 66.7(5) -108_543 . -105_443 N
Dg1 Dg2 DII*1 89.3(11) -108_543 . -208_443 N
Dg2 Dg2 Dg2 116.82(35) 105_544 . -108_666 N
Dg2 Dg2 Oh 116.6(7) 105_544 . 1_555 N
Dg2 Dg2 Oh 44.6(7) 105_544 . 105_544 N
Dg2 Dg2 Dh1 96.4(9) 105_544 . 1_555 N
Dg2 Dg2 Dh1 31.6(6) 105_544 . 105_544 N
Dg2 Dg2 Dh2 138.8(7) 105_544 . 1_555 N
Dg2 Dg2 Dh2 39.1(10) 105_544 . 105_544 N
Dg2 Dg2 OII* 120.6(8) 105_544 . -105_444 N
Dg2 Dg2 DII*1 119.5(12) 105_544 . -105_443 N
Dg2 Dg2 DII*1 61.8(9) 105_544 . -208_443 N
Dg2 Dg2 Oh 49.0(6) -108_665 . 1_555 N
Dg2 Dg2 Oh 95.1(8) -108_665 . 105_544 N
Dg2 Dg2 Dh1 56.4(12) -108_644 . 1_555 N
Dg2 Dg2 Dh1 92.9(8) -108_644 . 105_544 N
Dg2 Dg2 Dh2 42.1(9) -108_644 . 1_555 N
Dg2 Dg2 Dh2 116.4(10) -108_644 . 105_544 N
Dg2 Dg2 OII* 76.1(5) -108_544 . -105_444 N
Dg2 Dg2 DII*1 65.2(7) -108_543 . -105_443 N
Dg2 Dg2 DII*1 92.2(12) -108_543 . -208_443 N
Oh Dg2 Oh 131.7(11) 1_555 . 105_544 N
Oh Dg2 Dh1 20.1(5) 1_555 . 1_555 N
Oh Dg2 Dh1 117.5(11) 1_555 . 105_544 N
Oh Dg2 Dh2 23.27(28) 1_555 . 1_555 N
Oh Dg2 Dh2 149.1(11) 1_555 . 105_544 N
Oh Dg2 OII* 29.9(6) 1_555 . -105_444 N
Oh Dg2 DII*1 17.8(6) 1_555 . -105_443 N
Oh Dg2 DII*1 138.1(12) 1_555 . -208_443 N
Oh Dg2 Dh1 117.8(15) 105_544 . 1_555 N
Oh Dg2 Dh1 19.37(33) 105_544 . 105_544 N
Oh Dg2 Dh2 137.0(13) 105_544 . 1_555 N
Oh Dg2 Dh2 21.48(25) 105_544 . 105_544 N
Oh Dg2 OII* 157.0(8) 105_544 . -105_444 N
Oh Dg2 DII*1 147.3(9) 105_544 . -105_443 N
Oh Dg2 DII*1 18.6(9) 105_544 . -208_443 N
Dh1 Dg2 Dh1 100.7(15) 1_555 . 105_544 N
Dh1 Dg2 Dh2 43.1(7) 1_555 . 1_555 N
Dh1 Dg2 Dh2 130.9(15) 1_555 . 105_544 N
Dh1 Dg2 OII* 39.9(11) 1_555 . -105_444 N
Dh1 Dg2 DII*1 29.7(13) 1_555 . -105_443 N
Dh1 Dg2 DII*1 130.2(15) 1_555 . -208_443 N
Dh1 Dg2 Dh2 130.5(11) 105_544 . 1_555 N
Dh1 Dg2 Dh2 31.8(5) 105_544 . 105_544 N
Dh1 Dg2 OII* 138.2(9) 105_544 . -105_444 N
Dh1 Dg2 DII*1 130.2(10) 105_544 . -105_443 N
Dh1 Dg2 DII*1 37.7(9) 105_544 . -208_443 N
Dh2 Dg2 Dh2 158.4(13) 1_555 . 105_544 N
Dh2 Dg2 OII* 36.8(10) 1_555 . -105_444 N
Dh2 Dg2 DII*1 29.1(13) 1_555 . -105_443 N
Dh2 Dg2 DII*1 132.8(15) 1_555 . -208_443 N
Dh2 Dg2 OII* 158.7(12) 105_544 . -105_444 N
Dh2 Dg2 DII*1 158.2(15) 105_544 . -105_443 N
Dh2 Dg2 DII*1 28.3(12) 105_544 . -208_443 N
OII* Dg2 DII*1 12.1(4) -105_443 . -105_443 N
OII* Dg2 DII*1 167.9(11) -105_443 . -208_443 N
DII*1 Dg2 DII*1 155.9(12) -105_443 . -208_443 N
O1 Oh O1 92.4(5) -3_555 . 111_433 N
O1 Oh O2 70.4(4) -3_555 . 1_555 N
O1 Oh O3 43.38(26) -3_555 . 2_555 N
O1 Oh O3 90.2(5) -3_555 . 208_343 N
O1 Oh O4 48.6(4) -3_555 . 312_334 N
O1 Oh O4 115.5(5) -3_555 . -303_444 N
O1 Oh SJ 42.0(10) -3_555 . 1_555 N
O1 Oh Og 46.1(5) -3_555 . 1_555 N
O1 Oh Og 65.8(4) -3_555 . 105_544 N
O1 Oh Og 83.8(6) -3_555 . -108_656 N
O1 Oh Og 126.7(6) -3_555 . -305_556 N
O1 Oh Dg1 58.6(7) -3_555 . 1_555 N
O1 Oh Dg1 64.6(5) -3_555 . 105_544 N
O1 Oh Dg1 101.8(7) -3_555 . -108_665 N
O1 Oh Dg1 117.3(6) -3_555 . -305_565 N
O1 Oh Dg2 23.1(4) -3_555 . 1_555 N
O1 Oh Dg2 89.2(7) -3_555 . -108_666 N
O1 Oh Oh 46.2(5) -3_555 . 105_544 N
O1 Oh Oh 129.0(5) -3_555 . 111_554 N
O1 Oh Oh 97.0(6) -3_555 . -108_665 N
O1 Oh Oh 82.1(7) -3_555 . -206_565 N
O1 Oh Oh 87.1(7) -3_555 . 308_454 N
O1 Oh Oh 136.0(5) -3_555 . -305_565 N
O1 Oh Dh1 62.6(15) -3_555 . 1_555 N
O1 Oh O2 29.02(25) 111_433 . 1_555 N
O1 Oh O3 89.0(5) 111_433 . 2_555 N
O1 Oh O3 44.25(34) 111_433 . 208_343 N
O1 Oh O4 49.9(5) 111_433 . 312_334 N
O1 Oh O4 33.29(25) 111_433 . -303_444 N
O1 Oh SJ 68.1(12) 111_545 . 1_555 N
O1 Oh Og 111.9(8) 111_545 . 1_555 N
O1 Oh Og 116.3(5) 111_545 . 105_544 N
O1 Oh Og 52.1(5) 111_545 . -108_656 N
O1 Oh Og 74.8(5) 111_545 . -305_556 N
O1 Oh Dg1 90.3(9) 111_554 . 1_555 N
O1 Oh Dg1 116.5(7) 111_554 . 105_544 N
O1 Oh Dg1 62.4(6) 111_554 . -108_665 N
O1 Oh Dg1 82.3(5) 111_554 . -305_565 N
O1 Oh Dg2 101.3(8) 111_555 . 1_555 N
O1 Oh Dg2 31.2(4) 111_555 . -108_666 N
O1 Oh Oh 95.8(7) 111_554 . 105_544 N
O1 Oh Oh 89.3(8) 111_554 . 111_554 N
O1 Oh Oh 52.9(5) 111_554 . -108_665 N
O1 Oh Oh 131.4(5) 111_554 . -206_565 N
O1 Oh Oh 142.6(4) 111_554 . 308_454 N
O1 Oh Oh 97.3(7) 111_554 . -305_565 N
O1 Oh Dh1 124.7(23) 111_533 . 1_555 N
O2 Oh O3 60.02(31) 1_555 . 2_555 N
O2 Oh O3 31.52(21) 1_555 . 208_343 N
O2 Oh O4 22.62(34) 1_555 . 312_334 N
O2 Oh O4 62.27(30) 1_555 . -303_444 N
O2 Oh SJ 63.6(12) 1_555 . 1_555 N
O2 Oh Og 105.7(7) 1_555 . 1_555 N
O2 Oh Og 119.5(4) 1_555 . 105_544 N
O2 Oh Og 69.8(6) 1_555 . -108_656 N
O2 Oh Og 103.1(6) 1_555 . -305_556 N
O2 Oh Dg1 94.3(9) 1_555 . 1_555 N
O2 Oh Dg1 118.9(6) 1_555 . 105_544 N
O2 Oh Dg1 86.2(7) 1_555 . -108_665 N
O2 Oh Dg1 109.0(5) 1_555 . -305_565 N
O2 Oh Dg2 86.7(7) 1_555 . 1_555 N
O2 Oh Dg2 52.6(6) 1_555 . -108_666 N
O2 Oh Oh 93.1(5) 1_555 . 105_544 N
O2 Oh Oh 89.1(4) 1_555 . 111_554 N
O2 Oh Oh 75.8(5) 1_555 . -108_665 N
O2 Oh Oh 107.91(21) 1_555 . -206_565 N
O2 Oh Oh 151.2(4) 1_555 . 308_454 N
O2 Oh Oh 126.3(7) 1_555 . -305_565 N
O2 Oh Dh1 123.4(19) 1_555 . 1_555 N
O3 Oh O3 59.36(33) 2_555 . 208_343 N
O3 Oh O4 42.21(33) 2_555 . 312_334 N
O3 Oh O4 122.3(6) 2_555 . -303_444 N
O3 Oh SJ 78.8(10) 2_555 . 1_555 N
O3 Oh Og 86.9(8) 2_555 . 1_555 N
O3 Oh Og 106.0(5) 2_555 . 105_544 N
O3 Oh Og 115.1(7) 2_555 . -108_656 N
O3 Oh Og 161.4(7) 2_555 . -305_556 N
O3 Oh Dg1 101.8(9) 2_555 . 1_555 N
O3 Oh Dg1 104.7(7) 2_555 . 105_544 N
O3 Oh Dg1 136.1(8) 2_555 . -108_665 N
O3 Oh Dg1 158.6(6) 2_555 . -305_565 N
O3 Oh Dg2 65.5(6) 2_555 . 1_555 N
O3 Oh Dg2 107.5(8) 2_555 . -108_666 N
O3 Oh Oh 89.6(6) 2_555 . 105_544 N
O3 Oh Oh 85.70(29) 2_555 . 111_554 N
O3 Oh Oh 127.0(7) 2_555 . -108_665 N
O3 Oh Oh 54.8(4) 2_555 . -206_565 N
O3 Oh Oh 114.7(9) 2_555 . 308_454 N
O3 Oh Oh 173.7(7) 2_555 . -305_565 N
O3 Oh Dh1 99.8(17) 2_555 . 1_555 N
O3 Oh O4 44.7(4) 208_343 . 312_334 N
O3 Oh O4 71.1(4) 208_343 . -303_444 N
O3 Oh SJ 94.8(13) 208_455 . 1_555 N
O3 Oh Og 133.7(9) 208_455 . 1_555 N
O3 Oh Og 150.4(6) 208_455 . 105_544 N
O3 Oh Og 95.7(8) 208_455 . -108_656 N
O3 Oh Og 111.2(7) 208_455 . -305_556 N
O3 Oh Dg1 125.8(10) 208_464 . 1_555 N
O3 Oh Dg1 149.6(7) 208_464 . 105_544 N
O3 Oh Dg1 106.1(9) 208_464 . -108_665 N
O3 Oh Dg1 122.0(7) 208_464 . -305_565 N
O3 Oh Dg2 111.5(8) 208_465 . 1_555 N
O3 Oh Dg2 75.2(7) 208_465 . -108_666 N
O3 Oh Oh 123.7(6) 208_464 . 105_544 N
O3 Oh Oh 57.7(4) 208_464 . 111_554 N
O3 Oh Oh 97.0(6) 208_464 . -108_665 N
O3 Oh Oh 87.36(30) 208_464 . -206_565 N
O3 Oh Oh 172.7(7) 208_464 . 308_454 N
O3 Oh Oh 125.6(8) 208_464 . -305_565 N
O3 Oh Dh1 151.9(17) 208_443 . 1_555 N
O4 Oh O4 82.0(6) 312_334 . -303_444 N
O4 Oh SJ 54.0(10) 312_446 . 1_555 N
O4 Oh Og 89.0(8) 312_446 . 1_555 N
O4 Oh Og 106.4(6) 312_446 . 105_544 N
O4 Oh Og 76.7(7) 312_446 . -108_656 N
O4 Oh Og 119.3(7) 312_446 . -305_556 N
O4 Oh Dg1 85.8(9) 312_455 . 1_555 N
O4 Oh Dg1 105.5(8) 312_455 . 105_544 N
O4 Oh Dg1 96.7(8) 312_455 . -108_665 N
O4 Oh Dg1 121.2(7) 312_455 . -305_565 N
O4 Oh Dg2 67.5(7) 312_456 . 1_555 N
O4 Oh Dg2 65.5(7) 312_456 . -108_666 N
O4 Oh Oh 80.1(7) 312_455 . 105_544 N
O4 Oh Oh 99.7(5) 312_455 . 111_554 N
O4 Oh Oh 86.6(7) 312_455 . -108_665 N
O4 Oh Oh 96.0(5) 312_455 . -206_565 N
O4 Oh Oh 134.5(9) 312_455 . 308_454 N
O4 Oh Oh 143.8(7) 312_455 . -305_565 N
O4 Oh Dh1 107.3(17) 312_434 . 1_555 N
O4 Oh SJ 77.7(12) -303_556 . 1_555 N
O4 Oh Og 109.9(8) -303_556 . 1_555 N
O4 Oh Og 102.7(4) -303_556 . 105_544 N
O4 Oh Og 40.9(5) -303_556 . -108_656 N
O4 Oh Og 42.05(33) -303_556 . -305_556 N
O4 Oh Dg1 83.5(8) -303_565 . 1_555 N
O4 Oh Dg1 103.5(5) -303_565 . 105_544 N
O4 Oh Dg1 37.8(6) -303_565 . -108_665 N
O4 Oh Dg1 51.20(35) -303_565 . -305_565 N
O4 Oh Dg2 112.9(8) -303_566 . 1_555 N
O4 Oh Dg2 27.0(5) -303_566 . -108_666 N
O4 Oh Oh 94.8(5) -303_565 . 105_544 N
O4 Oh Oh 92.1(8) -303_565 . 111_554 N
O4 Oh Oh 32.48(29) -303_565 . -108_665 N
O4 Oh Oh 151.5(8) -303_565 . -206_565 N
O4 Oh Oh 116.1(4) -303_565 . 308_454 N
O4 Oh Oh 64.1(5) -303_565 . -305_565 N
O4 Oh Dh1 112.6(23) -303_544 . 1_555 N
SJ Oh Og 44.5(11) 1_555 . 1_555 N
SJ Oh Og 55.8(12) 1_555 . 105_544 N
SJ Oh Og 41.8(9) 1_555 . -108_656 N
SJ Oh Og 86.5(10) 1_555 . -305_556 N
SJ Oh Dg1 32.0(10) 1_555 . 1_555 N
SJ Oh Dg1 55.3(12) 1_555 . 105_544 N
SJ Oh Dg1 60.4(10) 1_555 . -108_665 N
SJ Oh Dg1 79.9(10) 1_555 . -305_565 N
SJ Oh Dg2 35.8(11) 1_555 . 1_555 N
SJ Oh Dg2 50.8(11) 1_555 . -108_666 N
SJ Oh Oh 29.8(13) 1_555 . 105_544 N
SJ Oh Oh 152.6(13) 1_555 . 111_554 N
SJ Oh Oh 55.0(11) 1_555 . -108_665 N
SJ Oh Oh 124.0(15) 1_555 . -206_565 N
SJ Oh Oh 87.7(14) 1_555 . 308_454 N
SJ Oh Oh 103.8(10) 1_555 . -305_565 N
SJ Oh Dh1 60.6(21) 1_555 . 1_555 N
Og Oh Og 19.7(5) 1_555 . 105_544 N
Og Oh Og 69.3(7) 1_555 . -108_656 N
Og Oh Og 90.6(9) 1_555 . -305_556 N
Og Oh Dg1 26.38(30) 1_555 . 1_555 N
Og Oh Dg1 18.4(6) 1_555 . 105_544 N
Og Oh Dg1 75.5(8) 1_555 . -108_665 N
Og Oh Dg1 78.4(8) 1_555 . -305_565 N
Og Oh Dg2 23.15(29) 1_555 . 1_555 N
Og Oh Dg2 87.7(8) 1_555 . -108_666 N
Og Oh Oh 16.4(5) 1_555 . 105_544 N
Og Oh Oh 157.4(11) 1_555 . 111_554 N
Og Oh Oh 77.9(7) 1_555 . -108_665 N
Og Oh Oh 98.5(12) 1_555 . -206_565 N
Og Oh Oh 46.2(8) 1_555 . 308_454 N
Og Oh Oh 90.9(7) 1_555 . -305_565 N
Og Oh Dh1 18.3(16) 1_555 . 1_555 N
Og Oh Og 66.0(6) 105_544 . -108_656 N
Og Oh Og 74.2(5) 105_544 . -305_556 N
Og Oh Dg1 26.5(8) 105_544 . 1_555 N
Og Oh Dg1 1.29(35) 105_544 . 105_544 N
Og Oh Dg1 65.1(7) 105_544 . -108_665 N
Og Oh Dg1 61.7(4) 105_544 . -305_565 N
Og Oh Dg2 42.8(5) 105_544 . 1_555 N
Og Oh Dg2 86.8(7) 105_544 . -108_666 N
Og Oh Oh 26.67(23) 105_544 . 105_544 N
Og Oh Oh 151.4(4) 105_544 . 111_554 N
Og Oh Oh 70.57(34) 105_544 . -108_665 N
Og Oh Oh 105.2(8) 105_544 . -206_565 N
Og Oh Oh 31.94(33) 105_544 . 308_454 N
Og Oh Oh 71.46(35) 105_544 . -305_565 N
Og Oh Dh1 9.9(22) 105_544 . 1_555 N
Og Oh Og 47.3(5) -108_656 . -305_556 N
Og Oh Dg1 43.1(6) -108_665 . 1_555 N
Og Oh Dg1 66.4(7) -108_665 . 105_544 N
Og Oh Dg1 20.99(19) -108_665 . -108_665 N
Og Oh Dg1 45.0(6) -108_665 . -305_565 N
Og Oh Dg2 73.7(7) -108_666 . 1_555 N
Og Oh Dg2 21.14(19) -108_666 . -108_666 N
Og Oh Oh 53.9(6) -108_665 . 105_544 N
Og Oh Oh 133.0(12) -108_665 . 111_554 N
Og Oh Oh 13.3(6) -108_665 . -108_665 N
Og Oh Oh 165.6(11) -108_665 . -206_565 N
Og Oh Oh 90.7(5) -108_665 . 308_454 N
Og Oh Oh 69.5(6) -108_665 . -305_565 N
Og Oh Dh1 75.5(23) -108_644 . 1_555 N
Og Oh Dg1 69.7(8) -305_565 . 1_555 N
Og Oh Dg1 75.4(6) -305_565 . 105_544 N
Og Oh Dg1 26.6(5) -305_565 . -108_665 N
Og Oh Dg1 12.51(18) -305_565 . -305_565 N
Og Oh Dg2 108.1(9) -305_566 . 1_555 N
Og Oh Dg2 53.9(5) -305_566 . -108_666 N
Og Oh Oh 83.1(4) -305_565 . 105_544 N
Og Oh Oh 102.9(8) -305_565 . 111_554 N
Og Oh Oh 34.77(22) -305_565 . -108_665 N
Og Oh Oh 143.7(4) -305_565 . -206_565 N
Og Oh Oh 75.7(4) -305_565 . 308_454 N
Og Oh Oh 24.4(4) -305_565 . -305_565 N
Og Oh Dh1 82.6(20) -305_544 . 1_555 N
Dg1 Oh Dg1 26.4(9) 1_555 . 105_544 N
Dg1 Oh Dg1 50.2(7) 1_555 . -108_665 N
Dg1 Oh Dg1 59.0(8) 1_555 . -305_565 N
Dg1 Oh Dg2 38.4(4) 1_555 . 1_555 N
Dg1 Oh Dg2 62.6(8) 1_555 . -108_666 N
Dg1 Oh Oh 13.5(6) 1_555 . 105_544 N
Dg1 Oh Oh 172.4(10) 1_555 . 111_554 N
Dg1 Oh Oh 51.6(7) 1_555 . -108_665 N
Dg1 Oh Oh 124.9(13) 1_555 . -206_565 N
Dg1 Oh Oh 57.9(9) 1_555 . 308_454 N
Dg1 Oh Oh 78.5(7) 1_555 . -305_565 N
Dg1 Oh Dh1 34.4(22) 1_555 . 1_555 N
Dg1 Oh Dg1 66.0(9) 105_544 . -108_665 N
Dg1 Oh Dg1 62.9(6) 105_544 . -305_565 N
Dg1 Oh Dg2 41.5(6) 105_544 . 1_555 N
Dg1 Oh Dg2 87.2(8) 105_544 . -108_666 N
Dg1 Oh Oh 25.9(4) 105_544 . 105_544 N
Dg1 Oh Oh 151.9(6) 105_544 . 111_554 N
Dg1 Oh Oh 71.3(5) 105_544 . -108_665 N
Dg1 Oh Oh 104.5(9) 105_544 . -206_565 N
Dg1 Oh Oh 32.5(5) 105_544 . 308_454 N
Dg1 Oh Oh 72.7(5) 105_544 . -305_565 N
Dg1 Oh Dh1 9.2(23) 105_544 . 1_555 N
Dg1 Oh Dg1 24.5(6) -108_665 . -305_565 N
Dg1 Oh Dg2 87.0(10) -108_666 . 1_555 N
Dg1 Oh Dg2 33.59(30) -108_666 . -108_666 N
Dg1 Oh Oh 63.3(7) -108_665 . 105_544 N
Dg1 Oh Oh 123.5(12) -108_665 . 111_554 N
Dg1 Oh Oh 10.5(5) -108_665 . -108_665 N
Dg1 Oh Oh 165.8(8) -108_665 . -206_565 N
Dg1 Oh Oh 81.0(6) -108_665 . 308_454 N
Dg1 Oh Oh 48.6(6) -108_665 . -305_565 N
Dg1 Oh Dh1 75.0(22) -108_644 . 1_555 N
Dg1 Oh Dg2 97.0(8) -305_566 . 1_555 N
Dg1 Oh Dg2 56.9(6) -305_566 . -108_666 N
Dg1 Oh Oh 72.0(4) -305_565 . 105_544 N
Dg1 Oh Oh 113.5(8) -305_565 . 111_554 N
Dg1 Oh Oh 34.66(30) -305_565 . -108_665 N
Dg1 Oh Oh 142.4(4) -305_565 . -206_565 N
Dg1 Oh Oh 65.10(32) -305_565 . 308_454 N
Dg1 Oh Oh 24.8(4) -305_565 . -305_565 N
Dg1 Oh Dh1 70.1(19) -305_544 . 1_555 N
Dg2 Oh Dg2 86.4(7) 1_555 . -108_666 N
Dg2 Oh Oh 25.1(6) 1_555 . 105_544 N
Dg2 Oh Oh 148.8(9) 1_555 . 111_554 N
Dg2 Oh Oh 85.5(8) 1_555 . -108_665 N
Dg2 Oh Oh 92.1(11) 1_555 . -206_565 N
Dg2 Oh Oh 67.1(9) 1_555 . 308_454 N
Dg2 Oh Oh 113.2(7) 1_555 . -305_565 N
Dg2 Oh Dh1 40.5(15) 1_555 . 1_555 N
Dg2 Oh Oh 71.5(7) -108_665 . 105_544 N
Dg2 Oh Oh 115.0(11) -108_665 . 111_554 N
Dg2 Oh Oh 23.2(6) -108_665 . -108_665 N
Dg2 Oh Oh 160.5(6) -108_665 . -206_565 N
Dg2 Oh Oh 111.5(6) -108_665 . 308_454 N
Dg2 Oh Oh 78.3(7) -108_665 . -305_565 N
Dg2 Oh Dh1 96.1(23) -108_644 . 1_555 N
Oh Oh Oh 173.0(9) 105_544 . 111_554 N
Oh Oh Oh 63.8(6) 105_544 . -108_665 N
Oh Oh Oh 113.0(9) 105_544 . -206_565 N
Oh Oh Oh 58.09(31) 105_544 . 308_454 N
Oh Oh Oh 90.0000(5) 105_544 . -305_565 N
Oh Oh Dh1 30.9(20) 105_544 . 1_555 N
Oh Oh Oh 123.2(8) 111_554 . -108_665 N
Oh Oh Oh 60.00000(30) 111_554 . -206_565 N
Oh Oh Oh 119.48(14) 111_554 . 308_454 N
Oh Oh Oh 94.1(6) 111_554 . -305_565 N
Oh Oh Dh1 145.3(23) 111_533 . 1_555 N
Oh Oh Oh 175.5(7) -108_665 . -206_565 N
Oh Oh Oh 90.0000(5) -108_665 . 308_454 N
Oh Oh Oh 58.09(31) -108_665 . -305_565 N
Oh Oh Dh1 80.5(23) -108_644 . 1_555 N
Oh Oh Oh 85.6(7) -206_565 . 308_454 N
Oh Oh Oh 119.80(8) -206_565 . -305_565 N
Oh Oh Dh1 95.3(25) -206_544 . 1_555 N
Oh Oh Oh 60.00000(30) 308_454 . -305_565 N
Oh Oh Dh1 28.0(19) 308_433 . 1_555 N
Oh Oh Dh1 76.9(16) -305_544 . 1_555 N
O1 Dh1 O1 87.5(6) -3_555 . 111_433 N
O1 Dh1 O3 42.22(32) -3_555 . 2_555 N
O1 Dh1 O4 36.25(31) -3_555 . -111_444 N
O1 Dh1 O4 50.8(5) -3_555 . 312_334 N
O1 Dh1 SJ 52.3(14) -3_555 . 1_555 N
O1 Dh1 Og 48.3(11) -3_555 . 1_555 N
O1 Dh1 Og 81.0(7) -3_555 . 105_544 N
O1 Dh1 Og 92.0(10) -3_555 . -108_656 N
O1 Dh1 Og 138.6(11) -3_555 . -305_556 N
O1 Dh1 Dg1 69.5(13) -3_555 . 1_555 N
O1 Dh1 Dg1 79.6(9) -3_555 . 105_544 N
O1 Dh1 Dg1 113.0(12) -3_555 . -108_665 N
O1 Dh1 Dg1 133.4(11) -3_555 . -305_565 N
O1 Dh1 Dg2 18.5(6) -3_555 . 1_555 N
O1 Dh1 Dg2 91.9(9) -3_555 . -108_666 N
O1 Dh1 Oh 102.8(16) -3_555 . 1_555 N
O1 Dh1 Oh 55.4(7) -3_555 . 105_544 N
O1 Dh1 Oh 83.0(7) -3_555 . -206_565 N
O1 Dh1 Oh 106.7(10) -3_555 . 308_454 N
O1 Dh1 Dh1 68.7(8) -3_555 . 105_544 N
O1 Dh1 Dh1 98.1(13) -3_555 . -108_644 N
O1 Dh1 Dh1 115.4(10) -3_555 . 308_433 N
O1 Dh1 Dh1 153.6(6) -3_555 . -305_544 N
O1 Dh1 Dh2 67.8(15) -3_555 . 1_555 N
O1 Dh1 O3 77.4(4) 111_433 . 2_555 N
O1 Dh1 O4 118.2(8) 111_433 . -111_444 N
O1 Dh1 O4 41.1(4) 111_433 . 312_334 N
O1 Dh1 SJ 42.9(14) 111_545 . 1_555 N
O1 Dh1 Og 111.8(19) 111_545 . 1_555 N
O1 Dh1 Og 125.4(10) 111_545 . 105_544 N
O1 Dh1 Og 42.3(5) 111_545 . -108_656 N
O1 Dh1 Og 67.9(6) 111_545 . -305_556 N
O1 Dh1 Dg1 78.6(15) 111_554 . 1_555 N
O1 Dh1 Dg1 124.9(13) 111_554 . 105_544 N
O1 Dh1 Dg1 52.6(6) 111_554 . -108_665 N
O1 Dh1 Dg1 77.9(6) 111_554 . -305_565 N
O1 Dh1 Dg2 94.9(13) 111_555 . 1_555 N
O1 Dh1 Dg2 23.24(34) 111_555 . -108_666 N
O1 Dh1 Oh 43.9(20) 111_554 . 1_555 N
O1 Dh1 Oh 99.8(9) 111_554 . 105_544 N
O1 Dh1 Oh 111.0(6) 111_554 . -206_565 N
O1 Dh1 Oh 152.9(9) 111_554 . 308_454 N
O1 Dh1 Dh1 108.1(12) 111_533 . 105_544 N
O1 Dh1 Dh1 52.2(7) 111_533 . -108_644 N
O1 Dh1 Dh1 139.4(9) 111_533 . 308_433 N
O1 Dh1 Dh1 84.3(10) 111_533 . -305_544 N
O1 Dh1 Dh2 32.8(16) 111_533 . 1_555 N
O3 Dh1 O4 72.1(5) 2_555 . -111_444 N
O3 Dh1 O4 39.01(32) 2_555 . 312_334 N
O3 Dh1 SJ 69.3(13) 2_555 . 1_555 N
O3 Dh1 Og 89.4(14) 2_555 . 1_555 N
O3 Dh1 Og 120.4(8) 2_555 . 105_544 N
O3 Dh1 Og 108.7(8) 2_555 . -108_656 N
O3 Dh1 Og 144.6(8) 2_555 . -305_556 N
O3 Dh1 Dg1 107.4(15) 2_555 . 1_555 N
O3 Dh1 Dg1 119.2(10) 2_555 . 105_544 N
O3 Dh1 Dg1 127.6(9) 2_555 . -108_665 N
O3 Dh1 Dg1 155.2(9) 2_555 . -305_565 N
O3 Dh1 Dg2 60.6(9) 2_555 . 1_555 N
O3 Dh1 Dg2 96.0(7) 2_555 . -108_666 N
O3 Dh1 Oh 67.2(16) 2_555 . 1_555 N
O3 Dh1 Oh 97.6(8) 2_555 . 105_544 N
O3 Dh1 Oh 51.7(4) 2_555 . -206_565 N
O3 Dh1 Oh 128.5(10) 2_555 . 308_454 N
O3 Dh1 Dh1 110.9(8) 2_555 . 105_544 N
O3 Dh1 Dh1 119.2(10) 2_555 . -108_644 N
O3 Dh1 Dh1 142.0(11) 2_555 . 308_433 N
O3 Dh1 Dh1 155.6(10) 2_555 . -305_544 N
O3 Dh1 Dh2 45.2(15) 2_555 . 1_555 N
O4 Dh1 O4 86.7(6) -111_444 . 312_334 N
O4 Dh1 SJ 76.0(16) -111_556 . 1_555 N
O4 Dh1 Og 21.5(13) -111_556 . 1_555 N
O4 Dh1 Og 48.3(4) -111_556 . 105_544 N
O4 Dh1 Og 101.7(10) -111_556 . -108_656 N
O4 Dh1 Og 130.9(8) -111_556 . -305_556 N
O4 Dh1 Dg1 62.1(12) -111_565 . 1_555 N
O4 Dh1 Dg1 47.1(6) -111_565 . 105_544 N
O4 Dh1 Dg1 115.3(11) -111_565 . -108_665 N
O4 Dh1 Dg1 117.9(8) -111_565 . -305_565 N
O4 Dh1 Dg2 23.5(8) -111_566 . 1_555 N
O4 Dh1 Dg2 112.2(10) -111_566 . -108_666 N
O4 Dh1 Oh 138.2(18) -111_565 . 1_555 N
O4 Dh1 Oh 37.0(4) -111_565 . 105_544 N
O4 Dh1 Oh 89.8(7) -111_565 . -206_565 N
O4 Dh1 Oh 70.7(7) -111_565 . 308_454 N
O4 Dh1 Dh1 43.8(4) -111_544 . 105_544 N
O4 Dh1 Dh1 101.2(11) -111_544 . -108_644 N
O4 Dh1 Dh1 79.2(8) -111_544 . 308_433 N
O4 Dh1 Dh1 131.6(6) -111_544 . -305_544 N
O4 Dh1 Dh2 104.0(17) -111_544 . 1_555 N
O4 Dh1 SJ 36.6(10) 312_446 . 1_555 N
O4 Dh1 Og 92.4(15) 312_446 . 1_555 N
O4 Dh1 Og 122.8(10) 312_446 . 105_544 N
O4 Dh1 Og 70.4(8) 312_446 . -108_656 N
O4 Dh1 Og 108.5(9) 312_446 . -305_556 N
O4 Dh1 Dg1 83.9(15) 312_455 . 1_555 N
O4 Dh1 Dg1 121.5(12) 312_455 . 105_544 N
O4 Dh1 Dg1 88.6(9) 312_455 . -108_665 N
O4 Dh1 Dg1 116.5(10) 312_455 . -305_565 N
O4 Dh1 Dg2 64.6(9) 312_456 . 1_555 N
O4 Dh1 Dg2 57.0(6) 312_456 . -108_666 N
O4 Dh1 Oh 55.6(14) 312_455 . 1_555 N
O4 Dh1 Oh 90.0(10) 312_455 . 105_544 N
O4 Dh1 Oh 86.4(6) 312_455 . -206_565 N
O4 Dh1 Oh 157.4(11) 312_455 . 308_454 N
O4 Dh1 Dh1 104.1(12) 312_434 . 105_544 N
O4 Dh1 Dh1 81.2(11) 312_434 . -108_644 N
O4 Dh1 Dh1 161.6(7) 312_434 . 308_433 N
O4 Dh1 Dh1 125.4(12) 312_434 . -305_544 N
O4 Dh1 Dh2 17.9(14) 312_434 . 1_555 N
SJ Dh1 Og 69.6(20) 1_555 . 1_555 N
SJ Dh1 Og 92.0(17) 1_555 . 105_544 N
SJ Dh1 Og 42.1(13) 1_555 . -108_656 N
SJ Dh1 Og 89.0(18) 1_555 . -305_556 N
SJ Dh1 Dg1 47.8(16) 1_555 . 1_555 N
SJ Dh1 Dg1 90.9(18) 1_555 . 105_544 N
SJ Dh1 Dg1 63.6(16) 1_555 . -108_665 N
SJ Dh1 Dg1 90.4(18) 1_555 . -305_565 N
SJ Dh1 Dg2 53.6(15) 1_555 . 1_555 N
SJ Dh1 Dg2 39.7(14) 1_555 . -108_666 N
SJ Dh1 Oh 81.3(20) 1_555 . 1_555 N
SJ Dh1 Oh 60.4(17) 1_555 . 105_544 N
SJ Dh1 Oh 120.8(14) 1_555 . -206_565 N
SJ Dh1 Oh 131.3(18) 1_555 . 308_454 N
SJ Dh1 Dh1 72.4(19) 1_555 . 105_544 N
SJ Dh1 Dh1 51.1(19) 1_555 . -108_644 N
SJ Dh1 Dh1 126.9(14) 1_555 . 308_433 N
SJ Dh1 Dh1 107.4(19) 1_555 . -305_544 N
SJ Dh1 Dh2 48.4(18) 1_555 . 1_555 N
Og Dh1 Og 32.8(9) 1_555 . 105_544 N
Og Dh1 Og 84.2(19) 1_555 . -108_656 N
Og Dh1 Og 109.5(20) 1_555 . -305_556 N
Og Dh1 Dg1 42.4(11) 1_555 . 1_555 N
Og Dh1 Dg1 31.5(10) 1_555 . 105_544 N
Og Dh1 Dg1 94.8(21) 1_555 . -108_665 N
Og Dh1 Dg1 96.9(18) 1_555 . -305_565 N
Og Dh1 Dg2 30.2(8) 1_555 . 1_555 N
Og Dh1 Dg2 98.4(20) 1_555 . -108_666 N
Og Dh1 Oh 147.9(26) 1_555 . 1_555 N
Og Dh1 Oh 16.3(14) 1_555 . 105_544 N
Og Dh1 Oh 110.8(20) 1_555 . -206_565 N
Og Dh1 Oh 66.3(14) 1_555 . 308_454 N
Og Dh1 Dh1 22.8(14) 1_555 . 105_544 N
Og Dh1 Dh1 81.6(22) 1_555 . -108_644 N
Og Dh1 Dh1 70.2(14) 1_555 . 308_433 N
Og Dh1 Dh1 112.6(13) 1_555 . -305_544 N
Og Dh1 Dh2 110.1(26) 1_555 . 1_555 N
Og Dh1 Og 84.8(10) 105_544 . -108_656 N
Og Dh1 Og 86.8(7) 105_544 . -305_556 N
Og Dh1 Dg1 47.4(12) 105_544 . 1_555 N
Og Dh1 Dg1 1.4(5) 105_544 . 105_544 N
Og Dh1 Dg1 83.7(10) 105_544 . -108_665 N
Og Dh1 Dg1 72.8(6) 105_544 . -305_565 N
Og Dh1 Dg2 63.0(8) 105_544 . 1_555 N
Og Dh1 Dg2 103.8(11) 105_544 . -108_666 N
Og Dh1 Oh 167.5(28) 105_544 . 1_555 N
Og Dh1 Oh 32.95(29) 105_544 . 105_544 N
Og Dh1 Oh 120.1(9) 105_544 . -206_565 N
Og Dh1 Oh 39.3(4) 105_544 . 308_454 N
Og Dh1 Dh1 19.64(35) 105_544 . 105_544 N
Og Dh1 Dh1 76.8(8) 105_544 . -108_644 N
Og Dh1 Dh1 38.9(6) 105_544 . 308_433 N
Og Dh1 Dh1 83.4(5) 105_544 . -305_544 N
Og Dh1 Dh2 139.4(24) 105_544 . 1_555 N
Og Dh1 Og 47.3(6) -108_656 . -305_556 N
Og Dh1 Dg1 42.4(12) -108_665 . 1_555 N
Og Dh1 Dg1 84.5(12) -108_665 . 105_544 N
Og Dh1 Dg1 21.58(32) -108_665 . -108_665 N
Og Dh1 Dg1 48.6(7) -108_665 . -305_565 N
Og Dh1 Dg2 86.2(15) -108_666 . 1_555 N
Og Dh1 Dg2 19.23(28) -108_666 . -108_666 N
Og Dh1 Oh 83.2(22) -108_665 . 1_555 N
Og Dh1 Oh 68.2(9) -108_665 . 105_544 N
Og Dh1 Oh 153.2(8) -108_665 . -206_565 N
Og Dh1 Oh 112.7(9) -108_665 . 308_454 N
Og Dh1 Dh1 70.7(11) -108_644 . 105_544 N
Og Dh1 Dh1 11.0(7) -108_644 . -108_644 N
Og Dh1 Dh1 100.9(7) -108_644 . 308_433 N
Og Dh1 Dh1 65.4(9) -108_644 . -305_544 N
Og Dh1 Dh2 71.5(20) -108_644 . 1_555 N
Og Dh1 Dg1 73.1(15) -305_565 . 1_555 N
Og Dh1 Dg1 87.6(9) -305_565 . 105_544 N
Og Dh1 Dg1 25.8(5) -305_565 . -108_665 N
Og Dh1 Dg1 14.06(15) -305_565 . -305_565 N
Og Dh1 Dg2 127.7(17) -305_566 . 1_555 N
Og Dh1 Dg2 52.9(7) -305_566 . -108_666 N
Og Dh1 Oh 82.6(19) -305_565 . 1_555 N
Og Dh1 Oh 95.1(8) -305_565 . 105_544 N
Og Dh1 Oh 136.1(9) -305_565 . -206_565 N
Og Dh1 Oh 86.9(6) -305_565 . 308_454 N
Og Dh1 Dh1 87.2(7) -305_544 . 105_544 N
Og Dh1 Dh1 40.50(29) -305_544 . -108_644 N
Og Dh1 Dh1 73.3(6) -305_544 . 308_433 N
Og Dh1 Dh1 18.6(5) -305_544 . -305_544 N
Og Dh1 Dh2 99.5(17) -305_544 . 1_555 N
Dg1 Dh1 Dg1 46.6(13) 1_555 . 105_544 N
Dg1 Dh1 Dg1 53.2(14) 1_555 . -108_665 N
Dg1 Dh1 Dg1 64.4(14) 1_555 . -305_565 N
Dg1 Dh1 Dg2 54.8(11) 1_555 . 1_555 N
Dg1 Dh1 Dg2 59.1(15) 1_555 . -108_666 N
Dg1 Dh1 Oh 122.5(31) 1_555 . 1_555 N
Dg1 Dh1 Oh 26.1(11) 1_555 . 105_544 N
Dg1 Dh1 Oh 150.7(18) 1_555 . -206_565 N
Dg1 Dh1 Oh 84.9(14) 1_555 . 308_454 N
Dg1 Dh1 Dh1 29.6(13) 1_555 . 105_544 N
Dg1 Dh1 Dh1 39.3(15) 1_555 . -108_644 N
Dg1 Dh1 Dh1 79.1(14) 1_555 . 308_433 N
Dg1 Dh1 Dh1 84.2(13) 1_555 . -305_544 N
Dg1 Dh1 Dh2 95.9(28) 1_555 . 1_555 N
Dg1 Dh1 Dg1 84.0(14) 105_544 . -108_665 N
Dg1 Dh1 Dg1 73.6(9) 105_544 . -305_565 N
Dg1 Dh1 Dg2 61.6(11) 105_544 . 1_555 N
Dg1 Dh1 Dg2 103.4(13) 105_544 . -108_666 N
Dg1 Dh1 Oh 167.6(30) 105_544 . 1_555 N
Dg1 Dh1 Oh 31.7(5) 105_544 . 105_544 N
Dg1 Dh1 Oh 120.1(11) 105_544 . -206_565 N
Dg1 Dh1 Oh 40.4(7) 105_544 . 308_454 N
Dg1 Dh1 Dh1 18.5(5) 105_544 . 105_544 N
Dg1 Dh1 Dh1 76.8(11) 105_544 . -108_644 N
Dg1 Dh1 Dh1 40.2(8) 105_544 . 308_433 N
Dg1 Dh1 Dh1 84.6(6) 105_544 . -305_544 N
Dg1 Dh1 Dh2 138.1(25) 105_544 . 1_555 N
Dg1 Dh1 Dg1 28.2(5) -108_665 . -305_565 N
Dg1 Dh1 Dg2 104.7(18) -108_666 . 1_555 N
Dg1 Dh1 Dg2 31.7(4) -108_666 . -108_666 N
Dg1 Dh1 Oh 83.9(22) -108_665 . 1_555 N
Dg1 Dh1 Oh 78.6(10) -108_665 . 105_544 N
Dg1 Dh1 Oh 154.1(13) -108_665 . -206_565 N
Dg1 Dh1 Oh 100.3(8) -108_665 . 308_454 N
Dg1 Dh1 Dh1 75.8(11) -108_644 . 105_544 N
Dg1 Dh1 Dh1 15.4(6) -108_644 . -108_644 N
Dg1 Dh1 Dh1 86.9(7) -108_644 . 308_433 N
Dg1 Dh1 Dh1 43.8(8) -108_644 . -305_544 N
Dg1 Dh1 Dh2 85.3(19) -108_644 . 1_555 N
Dg1 Dh1 Dg2 118.9(16) -305_566 . 1_555 N
Dg1 Dh1 Dg2 59.4(7) -305_566 . -108_666 N
Dg1 Dh1 Oh 96.6(20) -305_565 . 1_555 N
Dg1 Dh1 Oh 83.6(7) -305_565 . 105_544 N
Dg1 Dh1 Oh 143.5(9) -305_565 . -206_565 N
Dg1 Dh1 Oh 75.6(5) -305_565 . 308_454 N
Dg1 Dh1 Dh1 74.3(6) -305_544 . 105_544 N
Dg1 Dh1 Dh1 39.3(4) -305_544 . -108_644 N
Dg1 Dh1 Dh1 61.9(5) -305_544 . 308_433 N
Dg1 Dh1 Dh1 20.1(6) -305_544 . -305_544 N
Dg1 Dh1 Dh2 110.6(19) -305_544 . 1_555 N
Dg2 Dh1 Dg2 92.0(14) 1_555 . -108_666 N
Dg2 Dh1 Oh 119.4(20) 1_555 . 1_555 N
Dg2 Dh1 Oh 37.3(11) 1_555 . 105_544 N
Dg2 Dh1 Oh 96.1(14) 1_555 . -206_565 N
Dg2 Dh1 Oh 92.9(13) 1_555 . 308_454 N
Dg2 Dh1 Dh1 50.3(11) 1_555 . 105_544 N
Dg2 Dh1 Dh1 89.3(19) 1_555 . -108_644 N
Dg2 Dh1 Dh1 99.3(12) 1_555 . 308_433 N
Dg2 Dh1 Dh1 138.1(11) 1_555 . -305_544 N
Dg2 Dh1 Dh2 82.4(20) 1_555 . 1_555 N
Dg2 Dh1 Oh 64.5(20) -108_665 . 1_555 N
Dg2 Dh1 Oh 83.6(10) -108_665 . 105_544 N
Dg2 Dh1 Oh 134.2(8) -108_665 . -206_565 N
Dg2 Dh1 Oh 130.7(10) -108_665 . 308_454 N
Dg2 Dh1 Dh1 88.5(13) -108_644 . 105_544 N
Dg2 Dh1 Dh1 29.0(7) -108_644 . -108_644 N
Dg2 Dh1 Dh1 117.9(8) -108_644 . 308_433 N
Dg2 Dh1 Dh1 71.3(10) -108_644 . -305_544 N
Dg2 Dh1 Dh2 54.3(17) -108_644 . 1_555 N
Oh Dh1 Oh 141.7(24) 1_555 . 105_544 N
Oh Dh1 Oh 72.4(24) 1_555 . -206_565 N
Oh Dh1 Oh 145.6(23) 1_555 . 308_454 N
Oh Dh1 Dh1 151.9(29) 1_555 . 105_544 N
Oh Dh1 Dh1 90.8(23) 1_555 . -108_644 N
Oh Dh1 Dh1 141.3(18) 1_555 . 308_433 N
Oh Dh1 Dh1 88.5(21) 1_555 . -305_544 N
Oh Dh1 Dh2 37.77100(20) 1_555 . 1_555 N
Oh Dh1 Oh 126.7(10) 105_544 . -206_565 N
Oh Dh1 Oh 71.7(4) 105_544 . 308_454 N
Oh Dh1 Dh1 14.59(16) 105_544 . 105_544 N
Oh Dh1 Dh1 65.4(11) 105_544 . -108_644 N
Oh Dh1 Dh1 71.6(4) 105_544 . 308_433 N
Oh Dh1 Dh1 101.34(24) 105_544 . -305_544 N
Oh Dh1 Dh2 106.5(23) 105_544 . 1_555 N
Oh Dh1 Oh 93.9(8) -206_565 . 308_454 N
Oh Dh1 Dh1 130.0(9) -206_544 . 105_544 N
Oh Dh1 Dh1 162.9(8) -206_544 . -108_644 N
Oh Dh1 Dh1 105.1(6) -206_544 . 308_433 N
Oh Dh1 Dh1 123.4(5) -206_544 . -305_544 N
Oh Dh1 Dh2 82.2(20) -206_544 . 1_555 N
Oh Dh1 Dh1 58.9(5) 308_433 . 105_544 N
Oh Dh1 Dh1 102.09(32) 308_433 . -108_644 N
Oh Dh1 Dh1 13.73(12) 308_433 . 308_433 N
Oh Dh1 Dh1 72.71(23) 308_433 . -305_544 N
Oh Dh1 Dh2 173.5(19) 308_433 . 1_555 N
Dh1 Dh1 Dh1 65.1(12) 105_544 . -108_644 N
Dh1 Dh1 Dh1 57.5(6) 105_544 . 308_433 N
Dh1 Dh1 Dh1 90.0000(5) 105_544 . -305_544 N
Dh1 Dh1 Dh2 120.0(26) 105_544 . 1_555 N
Dh1 Dh1 Dh1 90.0000(5) -108_644 . 308_433 N
Dh1 Dh1 Dh1 57.5(6) -108_644 . -305_544 N
Dh1 Dh1 Dh2 82.4(23) -108_644 . 1_555 N
Dh1 Dh1 Dh1 60.00000(20) 308_433 . -305_544 N
Dh1 Dh1 Dh2 172.2(22) 308_433 . 1_555 N
Dh1 Dh1 Dh2 113.8(19) -305_544 . 1_555 N
O1 Dh2 O1 117.7(9) -3_555 . 111_433 N
O1 Dh2 O2 88.6(5) -3_555 . 1_555 N
O1 Dh2 O2 39.53(30) -3_555 . -304_444 N
O1 Dh2 O3 52.0(5) -3_555 . 2_555 N
O1 Dh2 O3 113.5(7) -3_555 . 208_343 N
O1 Dh2 O4 62.4(10) -3_555 . 312_334 N
O1 Dh2 SJ 61.2(16) -3_555 . 1_555 N
O1 Dh2 Og 57.5(8) -3_555 . 1_555 N
O1 Dh2 Og 98.5(11) -3_555 . -108_656 N
O1 Dh2 Og 127.6(9) -3_555 . -305_556 N
O1 Dh2 Dg1 70.9(10) -3_555 . 1_555 N
O1 Dh2 Dg1 111.8(12) -3_555 . -108_665 N
O1 Dh2 Dg2 32.9(5) -3_555 . 1_555 N
O1 Dh2 Dg2 109.9(13) -3_555 . -108_666 N
O1 Dh2 Oh 120.0(16) -3_555 . 1_555 N
O1 Dh2 Oh 48.6(6) -3_555 . 105_544 N
O1 Dh2 Dh1 85.6(16) -3_555 . 1_555 N
O1 Dh2 Dh1 100.3(8) -3_555 . -108_644 N
O1 Dh2 OII* 113.5(11) -3_555 . -105_444 N
O1 Dh2 DII*1 127.6(17) -3_555 . -105_443 N
O1 Dh2 DII*1 120.8(12) -3_555 . 209_342 N
O1 Dh2 DII*1 97.2(12) -3_555 . 312_333 N
O1 Dh2 DII*2 101.4(14) -3_555 . -105_444 N
O1 Dh2 DII*2 127.1(14) -3_555 . 209_343 N
O1 Dh2 O2 38.91(34) 111_433 . 1_555 N
O1 Dh2 O2 87.7(6) 111_433 . -304_444 N
O1 Dh2 O3 112.9(7) 111_433 . 2_555 N
O1 Dh2 O3 53.0(5) 111_433 . 208_343 N
O1 Dh2 O4 65.1(10) 111_433 . 312_334 N
O1 Dh2 SJ 93.1(21) 111_545 . 1_555 N
O1 Dh2 Og 128.1(15) 111_545 . 1_555 N
O1 Dh2 Og 60.5(8) 111_545 . -108_656 N
O1 Dh2 Og 72.0(7) 111_545 . -305_556 N
O1 Dh2 Dg1 104.0(13) 111_554 . 1_555 N
O1 Dh2 Dg1 67.6(9) 111_554 . -108_665 N
O1 Dh2 Dg2 127.0(16) 111_555 . 1_555 N
O1 Dh2 Dg2 38.3(6) 111_555 . -108_666 N
O1 Dh2 Oh 115.6(18) 111_554 . 1_555 N
O1 Dh2 Oh 107.1(11) 111_554 . 105_544 N
O1 Dh2 Dh1 130.3(22) 111_533 . 1_555 N
O1 Dh2 Dh1 59.4(7) 111_533 . -108_644 N
O1 Dh2 OII* 117.7(12) 111_433 . -105_444 N
O1 Dh2 DII*1 109.9(16) 111_432 . -105_443 N
O1 Dh2 DII*1 109.8(14) 111_432 . 209_342 N
O1 Dh2 DII*1 135.5(14) 111_432 . 312_333 N
O1 Dh2 DII*2 134.9(13) 111_433 . -105_444 N
O1 Dh2 DII*2 112.5(15) 111_433 . 209_343 N
O2 Dh2 O2 51.39(26) 1_555 . -304_444 N
O2 Dh2 O3 74.7(4) 1_555 . 2_555 N
O2 Dh2 O3 39.98(30) 1_555 . 208_343 N
O2 Dh2 O4 27.6(7) 1_555 . 312_334 N
O2 Dh2 SJ 101.8(18) 1_555 . 1_555 N
O2 Dh2 Og 133.5(12) 1_555 . 1_555 N
O2 Dh2 Og 88.1(9) 1_555 . -108_656 N
O2 Dh2 Og 110.3(8) 1_555 . -305_556 N
O2 Dh2 Dg1 120.5(13) 1_555 . 1_555 N
O2 Dh2 Dg1 101.8(10) 1_555 . -108_665 N
O2 Dh2 Dg2 114.4(10) 1_555 . 1_555 N
O2 Dh2 Dg2 70.0(8) 1_555 . -108_666 N
O2 Dh2 Oh 151.2(18) 1_555 . 1_555 N
O2 Dh2 Oh 108.0(8) 1_555 . 105_544 N
O2 Dh2 Dh1 159.9(26) 1_555 . 1_555 N
O2 Dh2 Dh1 87.9(7) 1_555 . -108_644 N
O2 Dh2 OII* 114.6(10) 1_555 . -105_444 N
O2 Dh2 DII*1 118.8(18) 1_555 . -105_443 N
O2 Dh2 DII*1 109.8(14) 1_555 . 209_342 N
O2 Dh2 DII*1 124.4(16) 1_555 . 312_333 N
O2 Dh2 DII*2 129.3(13) 1_555 . -105_444 N
O2 Dh2 DII*2 123.8(14) 1_555 . 209_343 N
O2 Dh2 O3 39.41(28) -304_444 . 2_555 N
O2 Dh2 O3 75.0(4) -304_444 . 208_343 N
O2 Dh2 O4 23.9(8) -304_444 . 312_334 N
O2 Dh2 SJ 85.7(15) -304_556 . 1_555 N
O2 Dh2 Og 95.9(10) -304_556 . 1_555 N
O2 Dh2 Og 106.6(10) -304_556 . -108_656 N
O2 Dh2 Og 144.4(9) -304_556 . -305_556 N
O2 Dh2 Dg1 102.5(11) -304_565 . 1_555 N
O2 Dh2 Dg1 125.7(11) -304_565 . -108_665 N
O2 Dh2 Dg2 71.3(7) -304_566 . 1_555 N
O2 Dh2 Dg2 102.8(10) -304_566 . -108_666 N
O2 Dh2 Oh 156.7(18) -304_565 . 1_555 N
O2 Dh2 Oh 79.6(7) -304_565 . 105_544 N
O2 Dh2 Dh1 125.2(17) -304_544 . 1_555 N
O2 Dh2 Dh1 107.9(8) -304_544 . -108_644 N
O2 Dh2 OII* 113.0(10) -304_444 . -105_444 N
O2 Dh2 DII*1 128.9(17) -304_443 . -105_443 N
O2 Dh2 DII*1 115.8(12) -304_443 . 209_342 N
O2 Dh2 DII*1 106.0(16) -304_443 . 312_333 N
O2 Dh2 DII*2 112.7(16) -304_444 . -105_444 N
O2 Dh2 DII*2 132.6(11) -304_444 . 209_343 N
O3 Dh2 O3 71.7(5) 2_555 . 208_343 N
O3 Dh2 O4 52.8(8) 2_555 . 312_334 N
O3 Dh2 SJ 113.1(19) 2_555 . 1_555 N
O3 Dh2 Og 101.2(11) 2_555 . 1_555 N
O3 Dh2 Og 145.2(12) 2_555 . -108_656 N
O3 Dh2 Og 175.0(9) 2_555 . -305_556 N
O3 Dh2 Dg1 121.3(13) 2_555 . 1_555 N
O3 Dh2 Dg1 162.9(13) 2_555 . -108_665 N
O3 Dh2 Dg2 80.6(9) 2_555 . 1_555 N
O3 Dh2 Dg2 140.8(11) 2_555 . -108_666 N
O3 Dh2 Oh 123.9(22) 2_555 . 1_555 N
O3 Dh2 Oh 100.3(8) 2_555 . 105_544 N
O3 Dh2 Dh1 115.7(19) 2_555 . 1_555 N
O3 Dh2 Dh1 146.6(9) 2_555 . -108_644 N
O3 Dh2 OII* 74.4(9) 2_555 . -105_444 N
O3 Dh2 DII*1 90.8(16) 2_555 . -105_443 N
O3 Dh2 DII*1 78.6(11) 2_555 . 209_342 N
O3 Dh2 DII*1 66.8(15) 2_555 . 312_333 N
O3 Dh2 DII*2 73.5(16) 2_555 . -105_444 N
O3 Dh2 DII*2 93.8(11) 2_555 . 209_343 N
O3 Dh2 O4 55.9(8) 208_343 . 312_334 N
O3 Dh2 SJ 140.8(21) 208_455 . 1_555 N
O3 Dh2 Og 170.8(11) 208_455 . 1_555 N
O3 Dh2 Og 113.3(12) 208_455 . -108_656 N
O3 Dh2 Og 111.5(9) 208_455 . -305_556 N
O3 Dh2 Dg1 156.6(15) 208_464 . 1_555 N
O3 Dh2 Dg1 116.6(12) 208_464 . -108_665 N
O3 Dh2 Dg2 146.2(10) 208_465 . 1_555 N
O3 Dh2 Dg2 91.0(10) 208_465 . -108_666 N
O3 Dh2 Oh 119.6(21) 208_464 . 1_555 N
O3 Dh2 Oh 147.8(9) 208_464 . 105_544 N
O3 Dh2 Dh1 157.2(22) 208_443 . 1_555 N
O3 Dh2 Dh1 112.2(8) 208_443 . -108_644 N
O3 Dh2 OII* 75.8(10) 208_343 . -105_444 N
O3 Dh2 DII*1 78.9(17) 208_342 . -105_443 N
O3 Dh2 DII*1 70.2(14) 208_342 . 209_342 N
O3 Dh2 DII*1 89.2(13) 208_342 . 312_333 N
O3 Dh2 DII*2 92.4(11) 208_343 . -105_444 N
O3 Dh2 DII*2 83.9(14) 208_343 . 209_343 N
O4 Dh2 SJ 94.6(20) 312_446 . 1_555 N
O4 Dh2 Og 115.4(17) 312_446 . 1_555 N
O4 Dh2 Og 99.8(15) 312_446 . -108_656 N
O4 Dh2 Og 132.1(15) 312_446 . -305_556 N
O4 Dh2 Dg1 114.0(18) 312_455 . 1_555 N
O4 Dh2 Dg1 117.8(17) 312_455 . -108_665 N
O4 Dh2 Dg2 92.0(14) 312_456 . 1_555 N
O4 Dh2 Dg2 88.2(14) 312_456 . -108_666 N
O4 Dh2 Oh 174.5(31) 312_455 . 1_555 N
O4 Dh2 Oh 94.0(14) 312_455 . 105_544 N
O4 Dh2 Dh1 146.4(26) 312_434 . 1_555 N
O4 Dh2 Dh1 100.4(13) 312_434 . -108_644 N
O4 Dh2 OII* 115.4(16) 312_334 . -105_444 N
O4 Dh2 DII*1 127.3(22) 312_333 . -105_443 N
O4 Dh2 DII*1 114.6(17) 312_333 . 209_342 N
O4 Dh2 DII*1 116.1(20) 312_333 . 312_333 N
O4 Dh2 DII*2 122.7(20) 312_334 . -105_444 N
O4 Dh2 DII*2 132.4(18) 312_334 . 209_343 N
SJ Dh2 Og 36.2(14) 1_555 . 1_555 N
SJ Dh2 Og 40.5(15) 1_555 . -108_656 N
SJ Dh2 Og 67.2(15) 1_555 . -305_556 N
SJ Dh2 Dg1 19.7(12) 1_555 . 1_555 N
SJ Dh2 Dg1 50.7(15) 1_555 . -108_665 N
SJ Dh2 Dg2 39.1(15) 1_555 . 1_555 N
SJ Dh2 Dg2 60.0(17) 1_555 . -108_666 N
SJ Dh2 Oh 90.9(21) 1_555 . 1_555 N
SJ Dh2 Oh 15.7(16) 1_555 . 105_544 N
SJ Dh2 Dh1 58.7(22) 1_555 . 1_555 N
SJ Dh2 Dh1 42.3(17) 1_555 . -108_644 N
SJ Dh2 OII* 143.4(21) 1_555 . -105_444 N
SJ Dh2 DII*1 137.5(24) 1_555 . -105_443 N
SJ Dh2 DII*1 148.4(22) 1_555 . 209_342 N
SJ Dh2 DII*1 129.3(23) 1_555 . 312_333 N
SJ Dh2 DII*2 126.7(21) 1_555 . -105_444 N
SJ Dh2 DII*2 132.2(19) 1_555 . 209_343 N
Og Dh2 Og 69.1(10) 1_555 . -108_656 N
Og Dh2 Og 76.1(8) 1_555 . -305_556 N
Og Dh2 Dg1 24.8(4) 1_555 . 1_555 N
Og Dh2 Dg1 68.8(9) 1_555 . -108_665 N
Og Dh2 Dg2 24.7(4) 1_555 . 1_555 N
Og Dh2 Dg2 91.3(12) 1_555 . -108_666 N
Og Dh2 Oh 68.9(14) 1_555 . 1_555 N
Og Dh2 Oh 25.8(6) 1_555 . 105_544 N
Og Dh2 Dh1 31.2(14) 1_555 . 1_555 N
Og Dh2 Dh1 70.4(8) 1_555 . -108_644 N
Og Dh2 OII* 108.3(13) 1_555 . -105_444 N
Og Dh2 DII*1 107.4(19) 1_555 . -105_443 N
Og Dh2 DII*1 114.7(16) 1_555 . 209_342 N
Og Dh2 DII*1 93.2(14) 1_555 . 312_333 N
Og Dh2 DII*2 90.9(11) 1_555 . -105_444 N
Og Dh2 DII*2 102.6(14) 1_555 . 209_343 N
Og Dh2 Og 37.9(6) -108_656 . -305_556 N
Og Dh2 Dg1 44.3(8) -108_665 . 1_555 N
Og Dh2 Dg1 19.14(29) -108_665 . -108_665 N
Og Dh2 Dg2 79.4(12) -108_666 . 1_555 N
Og Dh2 Dg2 22.32(31) -108_666 . -108_666 N
Og Dh2 Oh 85.0(19) -108_665 . 1_555 N
Og Dh2 Oh 56.1(8) -108_665 . 105_544 N
Og Dh2 Dh1 73.7(20) -108_644 . 1_555 N
Og Dh2 Dh1 1.8(7) -108_644 . -108_644 N
Og Dh2 OII* 140.3(12) -108_544 . -105_444 N
Og Dh2 DII*1 124.0(17) -108_543 . -105_443 N
Og Dh2 DII*1 136.2(14) -108_543 . 209_342 N
Og Dh2 DII*1 144.1(18) -108_543 . 312_333 N
Og Dh2 DII*2 137.5(15) -108_544 . -105_444 N
Og Dh2 DII*2 120.7(10) -108_544 . 209_343 N
Og Dh2 Dg1 57.3(8) -305_565 . 1_555 N
Og Dh2 Dg1 19.2(6) -305_565 . -108_665 N
Og Dh2 Dg2 97.6(9) -305_566 . 1_555 N
Og Dh2 Dg2 44.0(6) -305_566 . -108_666 N
Og Dh2 Oh 51.3(16) -305_565 . 1_555 N
Og Dh2 Oh 79.0(6) -305_565 . 105_544 N
Og Dh2 Dh1 59.8(15) -305_544 . 1_555 N
Og Dh2 Dh1 36.6(7) -305_544 . -108_644 N
Og Dh2 OII* 102.3(9) -305_444 . -105_444 N
Og Dh2 DII*1 86.1(14) -305_443 . -105_443 N
Og Dh2 DII*1 98.7(11) -305_443 . 209_342 N
Og Dh2 DII*1 108.9(16) -305_443 . 312_333 N
Og Dh2 DII*2 102.2(14) -305_444 . -105_444 N
Og Dh2 DII*2 82.8(7) -305_444 . 209_343 N
Dg1 Dh2 Dg1 45.7(8) 1_555 . -108_665 N
Dg1 Dh2 Dg2 40.8(6) 1_555 . 1_555 N
Dg1 Dh2 Dg2 66.5(10) 1_555 . -108_666 N
Dg1 Dh2 Oh 71.4(17) 1_555 . 1_555 N
Dg1 Dh2 Oh 23.2(8) 1_555 . 105_544 N
Dg1 Dh2 Dh1 39.6(18) 1_555 . 1_555 N
Dg1 Dh2 Dh1 45.6(8) 1_555 . -108_644 N
Dg1 Dh2 OII* 124.9(13) 1_555 . -105_444 N
Dg1 Dh2 DII*1 117.7(20) 1_555 . -105_443 N
Dg1 Dh2 DII*1 128.9(17) 1_555 . 209_342 N
Dg1 Dh2 DII*1 113.5(17) 1_555 . 312_333 N
Dg1 Dh2 DII*2 109.6(13) 1_555 . -105_444 N
Dg1 Dh2 DII*2 112.5(13) 1_555 . 209_343 N
Dg1 Dh2 Dg2 86.0(12) -108_666 . 1_555 N
Dg1 Dh2 Dg2 31.8(5) -108_666 . -108_666 N
Dg1 Dh2 Oh 66.6(17) -108_665 . 1_555 N
Dg1 Dh2 Oh 64.5(8) -108_665 . 105_544 N
Dg1 Dh2 Dh1 62.9(18) -108_644 . 1_555 N
Dg1 Dh2 Dh1 18.1(8) -108_644 . -108_644 N
Dg1 Dh2 OII* 121.3(11) -108_544 . -105_444 N
Dg1 Dh2 DII*1 105.2(16) -108_543 . -105_443 N
Dg1 Dh2 DII*1 117.9(14) -108_543 . 209_342 N
Dg1 Dh2 DII*1 125.8(18) -108_543 . 312_333 N
Dg1 Dh2 DII*2 119.1(15) -108_544 . -105_444 N
Dg1 Dh2 DII*2 101.7(9) -108_544 . 209_343 N
Dg2 Dh2 Dg2 98.8(14) 1_555 . -108_666 N
Dg2 Dh2 Oh 91.7(15) 1_555 . 1_555 N
Dg2 Dh2 Oh 23.4(7) 1_555 . 105_544 N
Dg2 Dh2 Dh1 54.5(15) 1_555 . 1_555 N
Dg2 Dh2 Dh1 81.1(10) 1_555 . -108_644 N
Dg2 Dh2 OII* 115.3(14) 1_555 . -105_444 N
Dg2 Dh2 DII*1 121.2(20) 1_555 . -105_443 N
Dg2 Dh2 DII*1 123.2(16) 1_555 . 209_342 N
Dg2 Dh2 DII*1 97.4(13) 1_555 . 312_333 N
Dg2 Dh2 DII*2 97.9(13) 1_555 . -105_444 N
Dg2 Dh2 DII*2 117.5(16) 1_555 . 209_343 N
Dg2 Dh2 Oh 95.3(19) -108_665 . 1_555 N
Dg2 Dh2 Oh 75.6(10) -108_665 . 105_544 N
Dg2 Dh2 Dh1 94.0(21) -108_644 . 1_555 N
Dg2 Dh2 Dh1 21.2(7) -108_644 . -108_644 N
Dg2 Dh2 OII* 136.4(14) -108_544 . -105_444 N
Dg2 Dh2 DII*1 120.9(17) -108_543 . -105_443 N
Dg2 Dh2 DII*1 129.3(15) -108_543 . 209_342 N
Dg2 Dh2 DII*1 150.1(18) -108_543 . 312_333 N
Dg2 Dh2 DII*2 144.0(17) -108_544 . -105_444 N
Dg2 Dh2 DII*2 119.7(13) -108_544 . 209_343 N
Oh Dh2 Oh 91.0(19) 1_555 . 105_544 N
Oh Dh2 Dh1 37.73570(30) 1_555 . 1_555 N
Oh Dh2 Dh1 84.3(21) 1_555 . -108_644 N
Oh Dh2 OII* 59.2(21) 1_555 . -105_444 N
Oh Dh2 DII*1 47.2(25) 1_555 . -105_443 N
Oh Dh2 DII*1 59.9(24) 1_555 . 209_342 N
Oh Dh2 DII*1 59.3(25) 1_555 . 312_333 N
Oh Dh2 DII*2 52.5(21) 1_555 . -105_444 N
Oh Dh2 DII*2 42.1(18) 1_555 . 209_343 N
Oh Dh2 Dh1 54.6(19) 105_544 . 1_555 N
Oh Dh2 Dh1 57.8(6) 105_544 . -108_644 N
Oh Dh2 OII* 133.4(10) 105_544 . -105_444 N
Oh Dh2 DII*1 133.1(17) 105_544 . -105_443 N
Oh Dh2 DII*1 140.3(14) 105_544 . 209_342 N
Oh Dh2 DII*1 116.9(10) 105_544 . 312_333 N
Oh Dh2 DII*2 115.7(8) 105_544 . -105_444 N
Oh Dh2 DII*2 128.2(12) 105_544 . 209_343 N
Dh1 Dh2 Dh1 74.2(23) 1_555 . -108_644 N
Dh1 Dh2 OII* 85.4(22) 1_555 . -105_444 N
Dh1 Dh2 DII*1 79.5(26) 1_555 . -105_443 N
Dh1 Dh2 DII*1 89.6(25) 1_555 . 209_342 N
Dh1 Dh2 DII*1 75.5(25) 1_555 . 312_333 N
Dh1 Dh2 DII*2 70.8(21) 1_555 . -105_444 N
Dh1 Dh2 DII*2 74.3(19) 1_555 . 209_343 N
Dh1 Dh2 OII* 138.9(11) -108_544 . -105_444 N
Dh1 Dh2 DII*1 122.6(16) -108_543 . -105_443 N
Dh1 Dh2 DII*1 134.7(12) -108_543 . 209_342 N
Dh1 Dh2 DII*1 143.5(17) -108_543 . 312_333 N
Dh1 Dh2 DII*2 136.8(16) -108_544 . -105_444 N
Dh1 Dh2 DII*2 119.4(11) -108_544 . 209_343 N
OII* Dh2 DII*1 16.5(13) -105_443 . -105_443 N
OII* Dh2 DII*1 8.1(9) -105_443 . 209_342 N
OII* Dh2 DII*1 18.1(5) -105_443 . 312_333 N
OII* Dh2 DII*2 17.8(4) -105_444 . -105_444 N
OII* Dh2 DII*2 19.6(6) -105_444 . 209_343 N
DII*1 Dh2 DII*1 13.3(6) -105_443 . 209_342 N
DII*1 Dh2 DII*1 30.5(13) -105_443 . 312_333 N
DII*1 Dh2 DII*2 26.5(11) -105_444 . -105_444 N
DII*1 Dh2 DII*2 5.2(21) -105_444 . 209_343 N
DII*1 Dh2 DII*1 26.2(8) 209_342 . 312_333 N
DII*1 Dh2 DII*2 25.3(10) 209_343 . -105_444 N
DII*1 Dh2 DII*2 18.0(16) 209_343 . 209_343 N
DII*1 Dh2 DII*2 6.8(26) 312_334 . -105_444 N
DII*1 Dh2 DII*2 30.7(12) 312_334 . 209_343 N
DII*2 Dh2 DII*2 25.8(15) -105_444 . 209_343 N
O2 OII' O2 97.78(26) 1_555 . 2_555 N
O2 OII' O2 97.78(26) 1_555 . 3_555 N
O2 OII' O2 49.00(12) 1_555 . 107_433 N
O2 OII' O2 92.69(18) 1_555 . 111_433 N
O2 OII' O2 96.24(17) 1_555 . 208_343 N
O2 OII' O2 48.87(11) 1_555 . 209_343 N
O2 OII' O2 146.27(30) 1_555 . 310_334 N
O2 OII' O2 145.49(27) 1_555 . 312_334 N
O2 OII' O3 122.0(4) 1_555 . 107_433 N
O2 OII' O3 32.58(10) 1_555 . 111_433 N
O2 OII' O3 132.39(18) 1_555 . -105_444 N
O2 OII' O3 31.29(11) 1_555 . 208_343 N
O2 OII' O3 122.2(4) 1_555 . 209_343 N
O2 OII' O3 129.76(16) 1_555 . -206_444 N
O2 OII' O3 73.82(17) 1_555 . 310_334 N
O2 OII' O3 75.48(17) 1_555 . 312_334 N
O2 OII' O3 75.90(8) 1_555 . -304_444 N
O2 OII' O4 166.3(4) 1_555 . 1_555 N
O2 OII' O4 90.27(9) 1_555 . 2_555 N
O2 OII' O4 92.03(10) 1_555 . 3_555 N
O2 OII' OII' 49.80(15) 1_555 . 107_533 N
O2 OII' OII' 95.72(20) 1_555 . 111_533 N
O2 OII' OII' 48.56(16) 1_555 . -105_544 N
O2 OII' DII'1 92.0(29) 1_555 . 1_555 N
O2 OII' O2 97.78(26) 2_555 . 3_555 N
O2 OII' O2 145.49(27) 2_555 . 107_433 N
O2 OII' O2 146.27(30) 2_555 . 111_433 N
O2 OII' O2 49.00(12) 2_555 . 208_343 N
O2 OII' O2 92.69(18) 2_555 . 209_343 N
O2 OII' O2 48.87(11) 2_555 . 310_334 N
O2 OII' O2 96.24(17) 2_555 . 312_334 N
O2 OII' O3 75.48(17) 2_555 . 107_433 N
O2 OII' O3 73.82(17) 2_555 . 111_433 N
O2 OII' O3 75.90(8) 2_555 . -105_444 N
O2 OII' O3 122.0(4) 2_555 . 208_343 N
O2 OII' O3 32.58(10) 2_555 . 209_343 N
O2 OII' O3 132.39(18) 2_555 . -206_444 N
O2 OII' O3 122.2(4) 2_555 . 310_334 N
O2 OII' O3 31.29(11) 2_555 . 312_334 N
O2 OII' O3 129.75(16) 2_555 . -304_444 N
O2 OII' O4 92.03(10) 2_555 . 1_555 N
O2 OII' O4 166.3(4) 2_555 . 2_555 N
O2 OII' O4 90.27(9) 2_555 . 3_555 N
O2 OII' OII' 48.56(16) 2_555 . 107_533 N
O2 OII' OII' 49.80(15) 2_555 . 111_533 N
O2 OII' OII' 95.72(20) 2_555 . -105_544 N
O2 OII' DII'1 130.4(25) 2_555 . 1_555 N
O2 OII' O2 96.24(17) 3_555 . 107_433 N
O2 OII' O2 48.87(11) 3_555 . 111_433 N
O2 OII' O2 145.49(27) 3_555 . 208_343 N
O2 OII' O2 146.27(30) 3_555 . 209_343 N
O2 OII' O2 92.69(18) 3_555 . 310_334 N
O2 OII' O2 49.00(12) 3_555 . 312_334 N
O2 OII' O3 31.29(11) 3_555 . 107_433 N
O2 OII' O3 122.2(4) 3_555 . 111_433 N
O2 OII' O3 129.75(16) 3_555 . -105_444 N
O2 OII' O3 75.48(17) 3_555 . 208_343 N
O2 OII' O3 73.82(17) 3_555 . 209_343 N
O2 OII' O3 75.90(8) 3_555 . -206_444 N
O2 OII' O3 32.58(10) 3_555 . 310_334 N
O2 OII' O3 122.0(4) 3_555 . 312_334 N
O2 OII' O3 132.39(18) 3_555 . -304_444 N
O2 OII' O4 90.27(9) 3_555 . 1_555 N
O2 OII' O4 92.03(10) 3_555 . 2_555 N
O2 OII' O4 166.3(4) 3_555 . 3_555 N
O2 OII' OII' 95.72(20) 3_555 . 107_533 N
O2 OII' OII' 48.56(16) 3_555 . 111_533 N
O2 OII' OII' 49.80(15) 3_555 . -105_544 N
O2 OII' DII'1 32.6(23) 3_555 . 1_555 N
O2 OII' O2 58.44(12) 107_433 . 111_433 N
O2 OII' O2 116.59(18) 107_433 . 208_343 N
O2 OII' O2 59.76(12) 107_433 . 209_343 N
O2 OII' O2 160.6(6) 107_433 . 310_334 N
O2 OII' O2 116.59(18) 107_433 . 312_334 N
O2 OII' O3 126.58(14) 107_433 . 107_433 N
O2 OII' O3 72.00(10) 107_433 . 111_433 N
O2 OII' O3 117.2(5) 107_433 . -105_444 N
O2 OII' O3 34.07(13) 107_433 . 208_343 N
O2 OII' O3 166.5(5) 107_433 . 209_343 N
O2 OII' O3 81.67(27) 107_433 . -206_444 N
O2 OII' O3 63.89(12) 107_433 . 310_334 N
O2 OII' O3 116.78(12) 107_433 . 312_334 N
O2 OII' O3 44.13(14) 107_433 . -304_444 N
O2 OII' O4 119.3(4) 107_433 . 1_555 N
O2 OII' O4 41.27(14) 107_433 . 2_555 N
O2 OII' O4 83.01(25) 107_433 . 3_555 N
O2 OII' OII' 98.77(24) 107_533 . 107_533 N
O2 OII' OII' 130.09(28) 107_533 . 111_533 N
O2 OII' OII' 70.22(29) 107_533 . -105_544 N
O2 OII' DII'1 68.8(28) 107_433 . 1_555 N
O2 OII' O2 160.6(6) 111_433 . 208_343 N
O2 OII' O2 117.81(15) 111_433 . 209_343 N
O2 OII' O2 117.81(15) 111_433 . 310_334 N
O2 OII' O2 59.76(12) 111_433 . 312_334 N
O2 OII' O3 71.79(10) 111_433 . 107_433 N
O2 OII' O3 124.65(16) 111_433 . 111_433 N
O2 OII' O3 118.8(5) 111_433 . -105_444 N
O2 OII' O3 61.49(12) 111_433 . 208_343 N
O2 OII' O3 117.07(14) 111_433 . 209_343 N
O2 OII' O3 45.58(14) 111_433 . -206_444 N
O2 OII' O3 32.31(13) 111_433 . 310_334 N
O2 OII' O3 164.6(5) 111_433 . 312_334 N
O2 OII' O3 83.89(27) 111_433 . -304_444 N
O2 OII' O4 84.26(25) 111_433 . 1_555 N
O2 OII' O4 43.29(14) 111_433 . 2_555 N
O2 OII' O4 121.4(4) 111_433 . 3_555 N
O2 OII' OII' 127.79(29) 111_533 . 107_533 N
O2 OII' OII' 97.40(25) 111_533 . 111_533 N
O2 OII' OII' 67.92(30) 111_533 . -105_544 N
O2 OII' DII'1 16.6(21) 111_433 . 1_555 N
O2 OII' O2 58.44(12) 208_343 . 209_343 N
O2 OII' O2 59.76(12) 208_343 . 310_334 N
O2 OII' O2 116.59(18) 208_343 . 312_334 N
O2 OII' O3 116.78(12) 208_343 . 107_433 N
O2 OII' O3 63.89(12) 208_343 . 111_433 N
O2 OII' O3 44.13(14) 208_343 . -105_444 N
O2 OII' O3 126.58(14) 208_343 . 208_343 N
O2 OII' O3 72.00(10) 208_343 . 209_343 N
O2 OII' O3 117.2(5) 208_343 . -206_444 N
O2 OII' O3 166.5(5) 208_343 . 310_334 N
O2 OII' O3 34.07(13) 208_343 . 312_334 N
O2 OII' O3 81.67(27) 208_343 . -304_444 N
O2 OII' O4 83.01(25) 208_343 . 1_555 N
O2 OII' O4 119.3(4) 208_343 . 2_555 N
O2 OII' O4 41.27(14) 208_343 . 3_555 N
O2 OII' OII' 70.22(29) 208_443 . 107_533 N
O2 OII' OII' 98.77(24) 208_443 . 111_533 N
O2 OII' OII' 130.09(28) 208_443 . -105_544 N
O2 OII' DII'1 171.7(29) 208_343 . 1_555 N
O2 OII' O2 117.81(15) 209_343 . 310_334 N
O2 OII' O2 160.6(6) 209_343 . 312_334 N
O2 OII' O3 164.6(5) 209_343 . 107_433 N
O2 OII' O3 32.31(13) 209_343 . 111_433 N
O2 OII' O3 83.89(27) 209_343 . -105_444 N
O2 OII' O3 71.79(10) 209_343 . 208_343 N
O2 OII' O3 124.65(16) 209_343 . 209_343 N
O2 OII' O3 118.8(5) 209_343 . -206_444 N
O2 OII' O3 117.07(14) 209_343 . 310_334 N
O2 OII' O3 61.49(12) 209_343 . 312_334 N
O2 OII' O3 45.58(14) 209_343 . -304_444 N
O2 OII' O4 121.4(4) 209_343 . 1_555 N
O2 OII' O4 84.26(25) 209_343 . 2_555 N
O2 OII' O4 43.29(14) 209_343 . 3_555 N
O2 OII' OII' 67.92(30) 209_443 . 107_533 N
O2 OII' OII' 127.79(29) 209_443 . 111_533 N
O2 OII' OII' 97.40(25) 209_443 . -105_544 N
O2 OII' DII'1 128.0(29) 209_343 . 1_555 N
O2 OII' O2 58.44(12) 310_334 . 312_334 N
O2 OII' O3 61.49(12) 310_334 . 107_433 N
O2 OII' O3 117.07(14) 310_334 . 111_433 N
O2 OII' O3 45.58(14) 310_334 . -105_444 N
O2 OII' O3 164.6(5) 310_334 . 208_343 N
O2 OII' O3 32.31(13) 310_334 . 209_343 N
O2 OII' O3 83.89(27) 310_334 . -206_444 N
O2 OII' O3 124.65(16) 310_334 . 310_334 N
O2 OII' O3 71.79(10) 310_334 . 312_334 N
O2 OII' O3 118.8(5) 310_334 . -304_444 N
O2 OII' O4 43.29(14) 310_334 . 1_555 N
O2 OII' O4 121.4(4) 310_334 . 2_555 N
O2 OII' O4 84.26(25) 310_334 . 3_555 N
O2 OII' OII' 97.40(25) 310_434 . 107_533 N
O2 OII' OII' 67.92(30) 310_434 . 111_533 N
O2 OII' OII' 127.79(29) 310_434 . -105_544 N
O2 OII' DII'1 113.0(29) 310_334 . 1_555 N
O2 OII' O3 34.07(13) 312_334 . 107_433 N
O2 OII' O3 166.5(5) 312_334 . 111_433 N
O2 OII' O3 81.67(27) 312_334 . -105_444 N
O2 OII' O3 116.78(12) 312_334 . 208_343 N
O2 OII' O3 63.89(12) 312_334 . 209_343 N
O2 OII' O3 44.13(14) 312_334 . -206_444 N
O2 OII' O3 72.00(10) 312_334 . 310_334 N
O2 OII' O3 126.58(14) 312_334 . 312_334 N
O2 OII' O3 117.2(5) 312_334 . -304_444 N
O2 OII' O4 41.27(14) 312_334 . 1_555 N
O2 OII' O4 83.01(25) 312_334 . 2_555 N
O2 OII' O4 119.3(4) 312_334 . 3_555 N
O2 OII' OII' 130.09(28) 312_434 . 107_533 N
O2 OII' OII' 70.22(29) 312_434 . 111_533 N
O2 OII' OII' 98.77(24) 312_434 . -105_544 N
O2 OII' DII'1 55.5(29) 312_334 . 1_555 N
O3 OII' O3 132.6(4) 107_433 . 111_433 N
O3 OII' O3 102.33(18) 107_433 . -105_444 N
O3 OII' O3 105.84(24) 107_433 . 208_343 N
O3 OII' O3 45.60(9) 107_433 . 209_343 N
O3 OII' O3 76.57(7) 107_433 . -206_444 N
O3 OII' O3 63.77(12) 107_433 . 310_334 N
O3 OII' O3 105.84(24) 107_433 . 312_334 N
O3 OII' O3 149.66(34) 107_433 . -304_444 N
O3 OII' O4 69.70(9) 107_433 . 1_555 N
O3 OII' O4 109.53(12) 107_433 . 2_555 N
O3 OII' O4 144.19(25) 107_433 . 3_555 N
O3 OII' OII' 96.69(20) 107_533 . 107_533 N
O3 OII' OII' 36.79(20) 107_533 . 111_533 N
O3 OII' OII' 74.42(18) 107_533 . -105_544 N
O3 OII' DII'1 58.5(27) 107_433 . 1_555 N
O3 OII' O3 104.11(18) 111_433 . -105_444 N
O3 OII' O3 63.77(12) 111_433 . 208_343 N
O3 OII' O3 105.20(24) 111_433 . 209_343 N
O3 OII' O3 149.02(33) 111_433 . -206_444 N
O3 OII' O3 105.20(24) 111_433 . 310_334 N
O3 OII' O3 45.60(9) 111_433 . 312_334 N
O3 OII' O3 76.30(7) 111_433 . -304_444 N
O3 OII' O4 145.59(25) 111_433 . 1_555 N
O3 OII' O4 108.83(12) 111_433 . 2_555 N
O3 OII' O4 70.69(9) 111_433 . 3_555 N
O3 OII' OII' 36.44(19) 111_533 . 107_533 N
O3 OII' OII' 96.29(20) 111_533 . 111_533 N
O3 OII' OII' 73.72(18) 111_533 . -105_544 N
O3 OII' DII'1 124.4(28) 111_433 . 1_555 N
O3 OII' O3 149.66(34) -105_444 . 208_343 N
O3 OII' O3 76.30(7) -105_444 . 209_343 N
O3 OII' O3 73.4(4) -105_444 . -206_444 N
O3 OII' O3 149.02(33) -105_444 . 310_334 N
O3 OII' O3 76.57(7) -105_444 . 312_334 N
O3 OII' O3 73.4(4) -105_444 . -304_444 N
O3 OII' O4 41.50(21) -105_444 . 1_555 N
O3 OII' O4 90.5(5) -105_444 . 2_555 N
O3 OII' O4 41.90(21) -105_444 . 3_555 N
O3 OII' OII' 113.35(22) -105_544 . 107_533 N
O3 OII' OII' 112.74(22) -105_544 . 111_533 N
O3 OII' OII' 171.59(25) -105_544 . -105_544 N
O3 OII' DII'1 128.3(26) -105_444 . 1_555 N
O3 OII' O3 132.6(4) 208_343 . 209_343 N
O3 OII' O3 102.33(18) 208_343 . -206_444 N
O3 OII' O3 45.60(9) 208_343 . 310_334 N
O3 OII' O3 105.84(24) 208_343 . 312_334 N
O3 OII' O3 76.57(7) 208_343 . -304_444 N
O3 OII' O4 144.19(25) 208_343 . 1_555 N
O3 OII' O4 69.70(9) 208_343 . 2_555 N
O3 OII' O4 109.53(12) 208_343 . 3_555 N
O3 OII' OII' 74.42(18) 208_443 . 107_533 N
O3 OII' OII' 96.69(20) 208_443 . 111_533 N
O3 OII' OII' 36.79(20) 208_443 . -105_544 N
O3 OII' DII'1 61.5(29) 208_343 . 1_555 N
O3 OII' O3 104.11(18) 209_343 . -206_444 N
O3 OII' O3 105.20(24) 209_343 . 310_334 N
O3 OII' O3 63.77(12) 209_343 . 312_334 N
O3 OII' O3 149.02(33) 209_343 . -304_444 N
O3 OII' O4 70.69(9) 209_343 . 1_555 N
O3 OII' O4 145.59(25) 209_343 . 2_555 N
O3 OII' O4 108.83(12) 209_343 . 3_555 N
O3 OII' OII' 73.72(18) 209_443 . 107_533 N
O3 OII' OII' 36.44(19) 209_443 . 111_533 N
O3 OII' OII' 96.29(20) 209_443 . -105_544 N
O3 OII' DII'1 104.0(27) 209_343 . 1_555 N
O3 OII' O3 76.30(7) -206_444 . 310_334 N
O3 OII' O3 149.66(34) -206_444 . 312_334 N
O3 OII' O3 73.4(4) -206_444 . -304_444 N
O3 OII' O4 41.90(21) -206_444 . 1_555 N
O3 OII' O4 41.50(21) -206_444 . 2_555 N
O3 OII' O4 90.5(5) -206_444 . 3_555 N
O3 OII' OII' 171.59(25) -206_544 . 107_533 N
O3 OII' OII' 113.35(22) -206_544 . 111_533 N
O3 OII' OII' 112.74(22) -206_544 . -105_544 N
O3 OII' DII'1 56.1(23) -206_444 . 1_555 N
O3 OII' O3 132.6(4) 310_334 . 312_334 N
O3 OII' O3 104.11(18) 310_334 . -304_444 N
O3 OII' O4 108.83(12) 310_334 . 1_555 N
O3 OII' O4 70.69(9) 310_334 . 2_555 N
O3 OII' O4 145.59(25) 310_334 . 3_555 N
O3 OII' OII' 96.29(20) 310_434 . 107_533 N
O3 OII' OII' 73.72(18) 310_434 . 111_533 N
O3 OII' OII' 36.44(19) 310_434 . -105_544 N
O3 OII' DII'1 20.7(25) 310_334 . 1_555 N
O3 OII' O3 102.33(18) 312_334 . -304_444 N
O3 OII' O4 109.53(12) 312_334 . 1_555 N
O3 OII' O4 144.19(25) 312_334 . 2_555 N
O3 OII' O4 69.70(9) 312_334 . 3_555 N
O3 OII' OII' 36.79(20) 312_434 . 107_533 N
O3 OII' OII' 74.42(18) 312_434 . 111_533 N
O3 OII' OII' 96.69(20) 312_434 . -105_544 N
O3 OII' DII'1 150.9(23) 312_334 . 1_555 N
O3 OII' O4 90.5(5) -304_444 . 1_555 N
O3 OII' O4 41.90(21) -304_444 . 2_555 N
O3 OII' O4 41.50(21) -304_444 . 3_555 N
O3 OII' OII' 112.74(22) -304_544 . 107_533 N
O3 OII' OII' 171.59(25) -304_544 . 111_533 N
O3 OII' OII' 113.35(22) -304_544 . -105_544 N
O3 OII' DII'1 99.8(24) -304_444 . 1_555 N
O4 OII' O4 78.35(33) 1_555 . 2_555 N
O4 OII' O4 78.35(33) 1_555 . 3_555 N
O4 OII' OII' 140.57(15) 1_555 . 107_533 N
O4 OII' OII' 97.90(21) 1_555 . 111_533 N
O4 OII' OII' 139.98(15) 1_555 . -105_544 N
O4 OII' DII'1 88.8(27) 1_555 . 1_555 N
O4 OII' O4 78.35(33) 2_555 . 3_555 N
O4 OII' OII' 139.98(15) 2_555 . 107_533 N
O4 OII' OII' 140.57(15) 2_555 . 111_533 N
O4 OII' OII' 97.90(21) 2_555 . -105_544 N
O4 OII' DII'1 59.8(22) 2_555 . 1_555 N
O4 OII' OII' 97.90(21) 3_555 . 107_533 N
O4 OII' OII' 139.98(15) 3_555 . 111_533 N
O4 OII' OII' 140.57(15) 3_555 . -105_544 N
O4 OII' DII'1 138.0(23) 3_555 . 1_555 N
OII' OII' OII' 60.00000(10) 107_533 . 111_533 N
OII' OII' OII' 60.00000(30) 107_533 . -105_544 N
OII' OII' DII'1 116.1(24) 107_433 . 1_555 N
OII' OII' OII' 60.00000(10) 111_533 . -105_544 N
OII' OII' DII'1 81.0(23) 111_433 . 1_555 N
OII' OII' DII'1 56.9(25) -105_444 . 1_555 N
O2 DII'1 O2 115.9(7) 3_555 . 107_433 N
O2 DII'1 O2 61.33(31) 3_555 . 111_433 N
O2 DII'1 O2 152.3(10) 3_555 . 209_343 N
O2 DII'1 O2 98.2(9) 3_555 . 310_334 N
O2 DII'1 O2 59.2(5) 3_555 . 312_334 N
O2 DII'1 O3 35.54(31) 3_555 . 107_433 N
O2 DII'1 O3 134.4(13) 3_555 . -105_444 N
O2 DII'1 O3 94.7(7) 3_555 . -206_444 N
O2 DII'1 O3 39.39(18) 3_555 . 310_334 N
O2 DII'1 O3 155.3(7) 3_555 . -304_444 N
O2 DII'1 O4 101.1(10) 3_555 . 1_555 N
O2 DII'1 O4 112.39(24) 3_555 . 2_555 N
O2 DII'1 O4 75.39(25) 3_555 . -105_444 N
O2 DII'1 OII' 140.2(28) 3_555 . 1_555 N
O2 DII'1 OII' 104.0(8) 3_555 . 107_533 N
O2 DII'1 OII' 61.8(6) 3_555 . 111_533 N
O2 DII'1 OII' 64.8(5) 3_555 . -105_544 N
O2 DII'1 DII'1 145.9(4) 3_555 . 2_555 N
O2 DII'1 DII'1 113.9(28) 3_555 . 3_555 N
O2 DII'1 DII'1 114.5(7) 3_555 . 107_433 N
O2 DII'1 DII'1 55.4(12) 3_555 . 111_433 N
O2 DII'1 DII'1 40.5(4) 3_555 . -105_444 N
O2 DII'1 DII'1 51.7(10) 3_555 . 208_343 N
O2 DII'1 DII'1 70.5(10) 3_555 . 209_343 N
O2 DII'1 O2 69.4(8) 107_433 . 111_433 N
O2 DII'1 O2 54.7(6) 107_433 . 209_343 N
O2 DII'1 O2 145.7(6) 107_433 . 310_334 N
O2 DII'1 O2 138.7(7) 107_433 . 312_334 N
O2 DII'1 O3 151.2(4) 107_433 . 107_433 N
O2 DII'1 O3 106.9(7) 107_433 . -105_444 N
O2 DII'1 O3 92.1(9) 107_433 . -206_444 N
O2 DII'1 O3 76.5(7) 107_433 . 310_334 N
O2 DII'1 O3 44.6(5) 107_433 . -304_444 N
O2 DII'1 O4 122.8(8) 107_433 . 1_555 N
O2 DII'1 O4 45.2(5) 107_433 . 2_555 N
O2 DII'1 O4 41.0(4) 107_433 . -105_444 N
O2 DII'1 OII' 96.5(29) 107_533 . 1_555 N
O2 DII'1 OII' 93.9(11) 107_533 . 107_533 N
O2 DII'1 OII' 139.8(15) 107_533 . 111_533 N
O2 DII'1 OII' 78.5(13) 107_533 . -105_544 N
O2 DII'1 DII'1 68.8(30) 107_433 . 2_555 N
O2 DII'1 DII'1 127.0(29) 107_433 . 3_555 N
O2 DII'1 DII'1 100.3(5) 107_433 . 107_433 N
O2 DII'1 DII'1 125.0(12) 107_433 . 111_433 N
O2 DII'1 DII'1 95.3(23) 107_433 . -105_444 N
O2 DII'1 DII'1 153.8(22) 107_433 . 208_343 N
O2 DII'1 DII'1 85.0(7) 107_433 . 209_343 N
O2 DII'1 O2 123.2(13) 111_433 . 209_343 N
O2 DII'1 O2 129.7(13) 111_433 . 310_334 N
O2 DII'1 O2 74.5(7) 111_433 . 312_334 N
O2 DII'1 O3 86.5(7) 111_433 . 107_433 N
O2 DII'1 O3 125.8(11) 111_433 . -105_444 N
O2 DII'1 O3 58.4(5) 111_433 . -206_444 N
O2 DII'1 O3 41.02(28) 111_433 . 310_334 N
O2 DII'1 O3 94.4(9) 111_433 . -304_444 N
O2 DII'1 O4 95.6(9) 111_433 . 1_555 N
O2 DII'1 O4 51.3(5) 111_433 . 2_555 N
O2 DII'1 O4 37.8(5) 111_433 . -105_444 N
O2 DII'1 OII' 158.0(28) 111_533 . 1_555 N
O2 DII'1 OII' 145.5(14) 111_533 . 107_533 N
O2 DII'1 OII' 123.2(8) 111_533 . 111_533 N
O2 DII'1 OII' 91.2(9) 111_533 . -105_544 N
O2 DII'1 DII'1 138(4) 111_433 . 2_555 N
O2 DII'1 DII'1 156.2(33) 111_433 . 3_555 N
O2 DII'1 DII'1 162.3(15) 111_433 . 107_433 N
O2 DII'1 DII'1 114.2(11) 111_433 . 111_433 N
O2 DII'1 DII'1 80.5(14) 111_433 . -105_444 N
O2 DII'1 DII'1 111.1(5) 111_433 . 208_343 N
O2 DII'1 DII'1 103.8(14) 111_433 . 209_343 N
O2 DII'1 O2 96.50(14) 209_343 . 310_334 N
O2 DII'1 O2 146.8(8) 209_343 . 312_334 N
O2 DII'1 O3 149.8(6) 209_343 . 107_433 N
O2 DII'1 O3 68.30(27) 209_343 . -105_444 N
O2 DII'1 O3 110.8(8) 209_343 . -206_444 N
O2 DII'1 O3 122.8(11) 209_343 . 310_334 N
O2 DII'1 O3 38.34(34) 209_343 . -304_444 N
O2 DII'1 O4 105.3(4) 209_343 . 1_555 N
O2 DII'1 O4 80.0(7) 209_343 . 2_555 N
O2 DII'1 O4 93.8(9) 209_343 . -105_444 N
O2 DII'1 OII' 42.2(24) 209_443 . 1_555 N
O2 DII'1 OII' 55.5(5) 209_443 . 107_533 N
O2 DII'1 OII' 106.9(6) 209_443 . 111_533 N
O2 DII'1 OII' 87.6(11) 209_443 . -105_544 N
O2 DII'1 DII'1 15.2(21) 209_343 . 2_555 N
O2 DII'1 DII'1 72.7(24) 209_343 . 3_555 N
O2 DII'1 DII'1 51.7(4) 209_343 . 107_433 N
O2 DII'1 DII'1 105.9(12) 209_343 . 111_433 N
O2 DII'1 DII'1 111.9(13) 209_343 . -105_444 N
O2 DII'1 DII'1 123.2(6) 209_343 . 208_343 N
O2 DII'1 DII'1 82.29(18) 209_343 . 209_343 N
O2 DII'1 O2 56.5(7) 310_334 . 312_334 N
O2 DII'1 O3 62.6(6) 310_334 . 107_433 N
O2 DII'1 O3 39.4(4) 310_334 . -105_444 N
O2 DII'1 O3 80.6(10) 310_334 . -206_444 N
O2 DII'1 O3 137.5(10) 310_334 . 310_334 N
O2 DII'1 O3 101.6(5) 310_334 . -304_444 N
O2 DII'1 O4 40.2(4) 310_334 . 1_555 N
O2 DII'1 O4 119.1(9) 310_334 . 2_555 N
O2 DII'1 O4 167.5(9) 310_334 . -105_444 N
O2 DII'1 OII' 55.1(25) 310_434 . 1_555 N
O2 DII'1 OII' 81.0(5) 310_434 . 107_533 N
O2 DII'1 OII' 60.0(7) 310_434 . 111_533 N
O2 DII'1 OII' 122.8(11) 310_434 . -105_544 N
O2 DII'1 DII'1 85.6(25) 310_334 . 2_555 N
O2 DII'1 DII'1 27.0(24) 310_334 . 3_555 N
O2 DII'1 DII'1 66.77(8) 310_334 . 107_433 N
O2 DII'1 DII'1 77.1(6) 310_334 . 111_433 N
O2 DII'1 DII'1 114.4(21) 310_334 . -105_444 N
O2 DII'1 DII'1 55.0(21) 310_334 . 208_343 N
O2 DII'1 DII'1 111.63(31) 310_334 . 209_343 N
O2 DII'1 O3 38.0(4) 312_334 . 107_433 N
O2 DII'1 O3 78.6(9) 312_334 . -105_444 N
O2 DII'1 O3 51.0(7) 312_334 . -206_444 N
O2 DII'1 O3 89.3(4) 312_334 . 310_334 N
O2 DII'1 O3 121.8(10) 312_334 . -304_444 N
O2 DII'1 O4 41.9(5) 312_334 . 1_555 N
O2 DII'1 O4 95.9(8) 312_334 . 2_555 N
O2 DII'1 O4 111.24(25) 312_334 . -105_444 N
O2 DII'1 OII' 110.7(32) 312_434 . 1_555 N
O2 DII'1 OII' 127.4(12) 312_434 . 107_533 N
O2 DII'1 OII' 77.8(11) 312_434 . 111_533 N
O2 DII'1 OII' 122.2(11) 312_434 . -105_544 N
O2 DII'1 DII'1 140.9(30) 312_334 . 2_555 N
O2 DII'1 DII'1 83.4(31) 312_334 . 3_555 N
O2 DII'1 DII'1 119.4(6) 312_334 . 107_433 N
O2 DII'1 DII'1 87.8(15) 312_334 . 111_433 N
O2 DII'1 DII'1 98.0(13) 312_334 . -105_444 N
O2 DII'1 DII'1 60.0(13) 312_334 . 208_343 N
O2 DII'1 DII'1 123.4(6) 312_334 . 209_343 N
O3 DII'1 O3 99.9(10) 107_433 . -105_444 N
O3 DII'1 O3 88.2(10) 107_433 . -206_444 N
O3 DII'1 O3 74.9(4) 107_433 . 310_334 N
O3 DII'1 O3 158.5(12) 107_433 . -304_444 N
O3 DII'1 O4 73.6(8) 107_433 . 1_555 N
O3 DII'1 O4 128.3(8) 107_433 . 2_555 N
O3 DII'1 O4 110.20(26) 107_433 . -105_444 N
O3 DII'1 OII' 110.9(29) 107_533 . 1_555 N
O3 DII'1 OII' 97.7(8) 107_533 . 107_533 N
O3 DII'1 OII' 44.7(7) 107_533 . 111_533 N
O3 DII'1 OII' 86.7(9) 107_533 . -105_544 N
O3 DII'1 DII'1 134.7(25) 107_433 . 2_555 N
O3 DII'1 DII'1 81.0(29) 107_433 . 3_555 N
O3 DII'1 DII'1 98.47(32) 107_433 . 107_433 N
O3 DII'1 DII'1 50.7(12) 107_433 . 111_433 N
O3 DII'1 DII'1 64.3(13) 107_433 . -105_444 N
O3 DII'1 DII'1 27.21(26) 107_433 . 208_343 N
O3 DII'1 DII'1 85.7(6) 107_433 . 209_343 N
O3 DII'1 O3 67.9(7) -105_444 . -206_444 N
O3 DII'1 O3 165.1(10) -105_444 . 310_334 N
O3 DII'1 O3 62.3(4) -105_444 . -304_444 N
O3 DII'1 O4 38.8(4) -105_444 . 1_555 N
O3 DII'1 O4 86.7(6) -105_444 . 2_555 N
O3 DII'1 O4 141.5(9) -105_444 . -105_444 N
O3 DII'1 OII' 40.4(22) -105_544 . 1_555 N
O3 DII'1 OII' 87.46(18) -105_544 . 107_533 N
O3 DII'1 OII' 95.0(8) -105_544 . 111_533 N
O3 DII'1 OII' 142.6(7) -105_544 . -105_544 N
O3 DII'1 DII'1 64.5(16) -105_444 . 2_555 N
O3 DII'1 DII'1 38.8(4) -105_444 . 3_555 N
O3 DII'1 DII'1 70.31(34) -105_444 . 107_433 N
O3 DII'1 DII'1 110.7(4) -105_444 . 111_433 N
O3 DII'1 DII'1 150.0(19) -105_444 . -105_444 N
O3 DII'1 DII'1 93.9(24) -105_444 . 208_343 N
O3 DII'1 DII'1 130.3(4) -105_444 . 209_343 N
O3 DII'1 O3 97.66(23) -206_444 . 310_334 N
O3 DII'1 O3 74.2(7) -206_444 . -304_444 N
O3 DII'1 O4 40.5(6) -206_444 . 1_555 N
O3 DII'1 O4 46.9(5) -206_444 . 2_555 N
O3 DII'1 O4 89.1(6) -206_444 . -105_444 N
O3 DII'1 OII' 107.2(26) -206_544 . 1_555 N
O3 DII'1 OII' 155.4(7) -206_544 . 107_533 N
O3 DII'1 OII' 127.7(18) -206_544 . 111_533 N
O3 DII'1 OII' 149.4(6) -206_544 . -105_544 N
O3 DII'1 DII'1 119.26(30) -206_444 . 2_555 N
O3 DII'1 DII'1 100.8(19) -206_444 . 3_555 N
O3 DII'1 DII'1 138.2(10) -206_444 . 107_433 N
O3 DII'1 DII'1 138.8(21) -206_444 . 111_433 N
O3 DII'1 DII'1 132.25(27) -206_444 . -105_444 N
O3 DII'1 DII'1 110.7(21) -206_444 . 208_343 N
O3 DII'1 DII'1 161.6(9) -206_444 . 209_343 N
O3 DII'1 O3 118.9(11) 310_334 . -304_444 N
O3 DII'1 O4 127.0(8) 310_334 . 1_555 N
O3 DII'1 O4 85.9(5) 310_334 . 2_555 N
O3 DII'1 O4 36.66(27) 310_334 . -105_444 N
O3 DII'1 OII' 154.5(30) 310_434 . 1_555 N
O3 DII'1 OII' 107.0(9) 310_434 . 107_533 N
O3 DII'1 OII' 91.0(6) 310_434 . 111_533 N
O3 DII'1 OII' 51.9(5) 310_434 . -105_544 N
O3 DII'1 DII'1 129.0(30) 310_334 . 2_555 N
O3 DII'1 DII'1 149.0(17) 310_334 . 3_555 N
O3 DII'1 DII'1 123.9(11) 310_334 . 107_433 N
O3 DII'1 DII'1 77.1(8) 310_334 . 111_433 N
O3 DII'1 DII'1 39.9(13) 310_334 . -105_444 N
O3 DII'1 DII'1 87.5(13) 310_334 . 208_343 N
O3 DII'1 DII'1 64.0(11) 310_334 . 209_343 N
O3 DII'1 O4 84.9(6) -304_444 . 1_555 N
O3 DII'1 O4 44.2(4) -304_444 . 2_555 N
O3 DII'1 O4 82.3(8) -304_444 . -105_444 N
O3 DII'1 OII' 64.4(22) -304_544 . 1_555 N
O3 DII'1 OII' 93.8(8) -304_544 . 107_533 N
O3 DII'1 OII' 142.1(4) -304_544 . 111_533 N
O3 DII'1 OII' 114.8(17) -304_544 . -105_544 N
O3 DII'1 DII'1 51.4(16) -304_444 . 2_555 N
O3 DII'1 DII'1 90.1(17) -304_444 . 3_555 N
O3 DII'1 DII'1 87.19(23) -304_444 . 107_433 N
O3 DII'1 DII'1 144.2(15) -304_444 . 111_433 N
O3 DII'1 DII'1 137.1(25) -304_444 . -105_444 N
O3 DII'1 DII'1 152.8(18) -304_444 . 208_343 N
O3 DII'1 DII'1 114.8(5) -304_444 . 209_343 N
O4 DII'1 O4 81.7(7) 1_555 . 2_555 N
O4 DII'1 O4 129.6(6) 1_555 . -105_444 N
O4 DII'1 OII' 77.5(26) 1_555 . 1_555 N
O4 DII'1 OII' 118.5(7) 1_555 . 107_533 N
O4 DII'1 OII' 95.4(12) 1_555 . 111_533 N
O4 DII'1 OII' 158.7(16) 1_555 . -105_544 N
O4 DII'1 DII'1 103.3(18) 1_555 . 2_555 N
O4 DII'1 DII'1 61.5(19) 1_555 . 3_555 N
O4 DII'1 DII'1 102.1(6) 1_555 . 107_433 N
O4 DII'1 DII'1 111.7(12) 1_555 . 111_433 N
O4 DII'1 DII'1 137.8(21) 1_555 . -105_444 N
O4 DII'1 DII'1 83.4(22) 1_555 . 208_343 N
O4 DII'1 DII'1 150.7(6) 1_555 . 209_343 N
O4 DII'1 O4 56.0(5) 2_555 . -105_444 N
O4 DII'1 OII' 106.8(24) 2_555 . 1_555 N
O4 DII'1 OII' 133.9(13) 2_555 . 107_533 N
O4 DII'1 OII' 173.0(12) 2_555 . 111_533 N
O4 DII'1 OII' 117.9(15) 2_555 . -105_544 N
O4 DII'1 DII'1 94.5(22) 2_555 . 2_555 N
O4 DII'1 DII'1 124.8(6) 2_555 . 3_555 N
O4 DII'1 DII'1 131.14(26) 2_555 . 107_433 N
O4 DII'1 DII'1 162.6(4) 2_555 . 111_433 N
O4 DII'1 DII'1 123.2(21) 2_555 . -105_444 N
O4 DII'1 DII'1 155.2(11) 2_555 . 208_343 N
O4 DII'1 DII'1 127.6(10) 2_555 . 209_343 N
O4 DII'1 OII' 136.0(33) -105_544 . 1_555 N
O4 DII'1 OII' 110.8(12) -105_544 . 107_533 N
O4 DII'1 OII' 123.3(9) -105_544 . 111_533 N
O4 DII'1 OII' 64.7(9) -105_544 . -105_544 N
O4 DII'1 DII'1 105.8(34) -105_444 . 2_555 N
O4 DII'1 DII'1 165.4(33) -105_444 . 3_555 N
O4 DII'1 DII'1 125.6(10) -105_444 . 107_433 N
O4 DII'1 DII'1 106.8(4) -105_444 . 111_433 N
O4 DII'1 DII'1 67.7(19) -105_444 . -105_444 N
O4 DII'1 DII'1 123.7(17) -105_444 . 208_343 N
O4 DII'1 DII'1 76.8(10) -105_444 . 209_343 N
OII' DII'1 OII' 48.4(20) 1_555 . 107_533 N
OII' DII'1 OII' 78.6(23) 1_555 . 111_533 N
OII' DII'1 OII' 102.8(28) 1_555 . -105_544 N
OII' DII'1 DII'1 30.6(4) 1_555 . 2_555 N
OII' DII'1 DII'1 30.6(4) 1_555 . 3_555 N
OII' DII'1 DII'1 32.3(19) 1_555 . 107_433 N
OII' DII'1 DII'1 87.6(19) 1_555 . 111_433 N
OII' DII'1 DII'1 118.6(21) 1_555 . -105_444 N
OII' DII'1 DII'1 89.1(34) 1_555 . 208_343 N
OII' DII'1 DII'1 91.2(19) 1_555 . 209_343 N
OII' DII'1 OII' 53.0(6) 107_533 . 111_533 N
OII' DII'1 OII' 55.2(8) 107_533 . -105_544 N
OII' DII'1 DII'1 42.9(6) 107_433 . 2_555 N
OII' DII'1 DII'1 57.0(12) 107_433 . 3_555 N
OII' DII'1 DII'1 17.25(15) 107_433 . 107_433 N
OII' DII'1 DII'1 50.5(7) 107_433 . 111_433 N
OII' DII'1 DII'1 70.9(5) 107_433 . -105_444 N
OII' DII'1 DII'1 70.9(5) 107_433 . 208_343 N
OII' DII'1 DII'1 43.00(25) 107_433 . 209_343 N
OII' DII'1 OII' 64.2(9) 111_533 . -105_544 N
OII' DII'1 DII'1 92.3(14) 111_433 . 2_555 N
OII' DII'1 DII'1 58.1(15) 111_433 . 3_555 N
OII' DII'1 DII'1 55.6(7) 111_433 . 107_433 N
OII' DII'1 DII'1 17.1(6) 111_433 . 111_433 N
OII' DII'1 DII'1 55.6(13) 111_433 . -105_444 N
OII' DII'1 DII'1 18.06(34) 111_433 . 208_343 N
OII' DII'1 DII'1 55.6(7) 111_433 . 209_343 N
OII' DII'1 DII'1 84.6(18) -105_444 . 2_555 N
OII' DII'1 DII'1 108.1(7) -105_444 . 3_555 N
OII' DII'1 DII'1 72.3(8) -105_444 . 107_433 N
OII' DII'1 DII'1 47.5(5) -105_444 . 111_433 N
OII' DII'1 DII'1 24.5(4) -105_444 . -105_444 N
OII' DII'1 DII'1 75.3(10) -105_444 . 208_343 N
OII' DII'1 DII'1 12.8(8) -105_444 . 209_343 N
DII'1 DII'1 DII'1 60.0000(4) 2_555 . 3_555 N
DII'1 DII'1 DII'1 36.8(22) 2_555 . 107_433 N
DII'1 DII'1 DII'1 93.18(23) 2_555 . 111_433 N
DII'1 DII'1 DII'1 107.3(11) 2_555 . -105_444 N
DII'1 DII'1 DII'1 108.2(25) 2_555 . 208_343 N
DII'1 DII'1 DII'1 76.6(5) 2_555 . 209_343 N
DII'1 DII'1 DII'1 41.1(18) 3_555 . 107_433 N
DII'1 DII'1 DII'1 72.5(5) 3_555 . 111_433 N
DII'1 DII'1 DII'1 111.4(20) 3_555 . -105_444 N
DII'1 DII'1 DII'1 63(4) 3_555 . 208_343 N
DII'1 DII'1 DII'1 95.4(6) 3_555 . 209_343 N
DII'1 DII'1 DII'1 59.0(13) 107_433 . 111_433 N
DII'1 DII'1 DII'1 86.37(33) 107_433 . -105_444 N
DII'1 DII'1 DII'1 71.52(12) 107_433 . 208_343 N
DII'1 DII'1 DII'1 60.00000(10) 107_433 . 209_343 N
DII'1 DII'1 DII'1 39.4(18) 111_433 . -105_444 N
DII'1 DII'1 DII'1 29.4(7) 111_433 . 208_343 N
DII'1 DII'1 DII'1 40.0(8) 111_433 . 209_343 N
DII'1 DII'1 DII'1 60.0 -105_444 . 208_343 N
DII'1 DII'1 DII'1 30.8(9) -105_444 . 209_343 N
DII'1 DII'1 DII'1 69.3(16) 208_343 . 209_343 N
O2 DII'2 O2 155.8(12) 2_555 . 107_433 N
O2 DII'2 O2 153.4(12) 2_555 . 111_433 N
O2 DII'2 O2 56.13(29) 2_555 . 208_343 N
O2 DII'2 O2 102.1(8) 2_555 . 209_343 N
O2 DII'2 O2 55.42(35) 2_555 . 310_334 N
O2 DII'2 O2 102.5(9) 2_555 . 312_334 N
O2 DII'2 O3 81.3(4) 2_555 . -105_444 N
O2 DII'2 O3 37.17(26) 2_555 . 209_343 N
O2 DII'2 O3 128.8(8) 2_555 . -206_444 N
O2 DII'2 O3 36.21(19) 2_555 . 312_334 N
O2 DII'2 O3 129.3(8) 2_555 . -304_444 N
O2 DII'2 O4 93.6(5) 2_555 . 3_555 N
O2 DII'2 OII' 132.5(17) 2_555 . 1_555 N
O2 DII'2 OII' 62.0(5) 2_555 . 107_533 N
O2 DII'2 OII' 63.8(5) 2_555 . 111_533 N
O2 DII'2 OII' 124.02(28) 2_555 . -105_544 N
O2 DII'2 DII'1 150.4(30) 2_555 . 1_555 N
O2 DII'2 DII'1 125.4(28) 2_555 . 2_555 N
O2 DII'2 DII'1 78.7(16) 2_555 . 3_555 N
O2 DII'2 DII'1 44.5(20) 2_555 . 107_433 N
O2 DII'2 DII'1 73.8(12) 2_555 . 111_433 N
O2 DII'2 DII'1 122.2(14) 2_555 . -105_444 N
O2 DII'2 DII'1 83.5(10) 2_555 . 208_343 N
O2 DII'2 DII'1 104.3(5) 2_555 . 209_343 N
O2 DII'2 O2 50.63(21) 107_433 . 111_433 N
O2 DII'2 O2 106.6(9) 107_433 . 208_343 N
O2 DII'2 O2 54.4(5) 107_433 . 209_343 N
O2 DII'2 O2 134.74(23) 107_433 . 310_334 N
O2 DII'2 O2 99.27(34) 107_433 . 312_334 N
O2 DII'2 O3 96.2(5) 107_433 . -105_444 N
O2 DII'2 O3 165.8(9) 107_433 . 209_343 N
O2 DII'2 O3 66.55(21) 107_433 . -206_444 N
O2 DII'2 O3 119.6(11) 107_433 . 312_334 N
O2 DII'2 O3 37.58(29) 107_433 . -304_444 N
O2 DII'2 O4 71.8(5) 107_433 . 3_555 N
O2 DII'2 OII' 52.6(19) 107_533 . 1_555 N
O2 DII'2 OII' 100.4(15) 107_533 . 107_533 N
O2 DII'2 OII' 136.1(10) 107_533 . 111_533 N
O2 DII'2 OII' 62.9(6) 107_533 . -105_544 N
O2 DII'2 DII'1 51.5(24) 107_433 . 1_555 N
O2 DII'2 DII'1 34.4(22) 107_433 . 2_555 N
O2 DII'2 DII'1 108.7(16) 107_433 . 3_555 N
O2 DII'2 DII'1 111.9(29) 107_433 . 107_433 N
O2 DII'2 DII'1 120.2(13) 107_433 . 111_433 N
O2 DII'2 DII'1 73.9(10) 107_433 . -105_444 N
O2 DII'2 DII'1 120.3(15) 107_433 . 208_343 N
O2 DII'2 DII'1 77.0(11) 107_433 . 209_343 N
O2 DII'2 O2 134.84(29) 111_433 . 208_343 N
O2 DII'2 O2 103.0(6) 111_433 . 209_343 N
O2 DII'2 O2 105.5(8) 111_433 . 310_334 N
O2 DII'2 O2 52.6(4) 111_433 . 312_334 N
O2 DII'2 O3 96.43(30) 111_433 . -105_444 N
O2 DII'2 O3 116.3(10) 111_433 . 209_343 N
O2 DII'2 O3 38.19(21) 111_433 . -206_444 N
O2 DII'2 O3 169.7(11) 111_433 . 312_334 N
O2 DII'2 O3 68.59(22) 111_433 . -304_444 N
O2 DII'2 O4 100.20(25) 111_433 . 3_555 N
O2 DII'2 OII' 49.0(15) 111_533 . 1_555 N
O2 DII'2 OII' 136.5(11) 111_533 . 107_533 N
O2 DII'2 OII' 94.4(11) 111_533 . 111_533 N
O2 DII'2 OII' 59.1(5) 111_533 . -105_544 N
O2 DII'2 DII'1 12.0(15) 111_433 . 1_555 N
O2 DII'2 DII'1 77.4(20) 111_433 . 2_555 N
O2 DII'2 DII'1 88.2(19) 111_433 . 3_555 N
O2 DII'2 DII'1 161.6(27) 111_433 . 107_433 N
O2 DII'2 DII'1 91.2(14) 111_433 . 111_433 N
O2 DII'2 DII'1 48.4(11) 111_433 . -105_444 N
O2 DII'2 DII'1 71.0(12) 111_433 . 208_343 N
O2 DII'2 DII'1 80.4(4) 111_433 . 209_343 N
O2 DII'2 O2 57.5(6) 208_343 . 209_343 N
O2 DII'2 O2 60.2(4) 208_343 . 310_334 N
O2 DII'2 O2 109.4(6) 208_343 . 312_334 N
O2 DII'2 O3 42.15(29) 208_343 . -105_444 N
O2 DII'2 O3 78.8(5) 208_343 . 209_343 N
O2 DII'2 O3 99.9(4) 208_343 . -206_444 N
O2 DII'2 O3 39.58(31) 208_343 . 312_334 N
O2 DII'2 O3 73.1(6) 208_343 . -304_444 N
O2 DII'2 O4 37.53(32) 208_343 . 3_555 N
O2 DII'2 OII' 85.9(17) 208_443 . 1_555 N
O2 DII'2 OII' 79.0(10) 208_443 . 107_533 N
O2 DII'2 OII' 117.3(9) 208_443 . 111_533 N
O2 DII'2 OII' 153.8(17) 208_443 . -105_544 N
O2 DII'2 DII'1 123.3(17) 208_343 . 1_555 N
O2 DII'2 DII'1 72.1(27) 208_343 . 2_555 N
O2 DII'2 DII'1 60.4(30) 208_343 . 3_555 N
O2 DII'2 DII'1 48.7(9) 208_343 . 107_433 N
O2 DII'2 DII'1 129.9(13) 208_343 . 111_433 N
O2 DII'2 DII'1 176.2(14) 208_343 . -105_444 N
O2 DII'2 DII'1 124.8(15) 208_343 . 208_343 N
O2 DII'2 DII'1 138.1(14) 208_343 . 209_343 N
O2 DII'2 O2 114.1(7) 209_343 . 310_334 N
O2 DII'2 O2 134.56(25) 209_343 . 312_334 N
O2 DII'2 O3 75.6(6) 209_343 . -105_444 N
O2 DII'2 O3 135.1(7) 209_343 . 209_343 N
O2 DII'2 O3 97.8(5) 209_343 . -206_444 N
O2 DII'2 O3 66.8(6) 209_343 . 312_334 N
O2 DII'2 O3 41.0(4) 209_343 . -304_444 N
O2 DII'2 O4 39.25(35) 209_343 . 3_555 N
O2 DII'2 OII' 74.0(26) 209_443 . 1_555 N
O2 DII'2 OII' 69.8(13) 209_443 . 107_533 N
O2 DII'2 OII' 158.2(10) 209_443 . 111_533 N
O2 DII'2 OII' 100.6(13) 209_443 . -105_544 N
O2 DII'2 DII'1 99.3(26) 209_343 . 1_555 N
O2 DII'2 DII'1 26.9(19) 209_343 . 2_555 N
O2 DII'2 DII'1 100.2(35) 209_343 . 3_555 N
O2 DII'2 DII'1 62.4(25) 209_343 . 107_433 N
O2 DII'2 DII'1 142.8(10) 209_343 . 111_433 N
O2 DII'2 DII'1 121.2(13) 209_343 . -105_444 N
O2 DII'2 DII'1 173.5(7) 209_343 . 208_343 N
O2 DII'2 DII'1 98.9(18) 209_343 . 209_343 N
O2 DII'2 O2 55.3(6) 310_334 . 312_334 N
O2 DII'2 O3 43.24(31) 310_334 . -105_444 N
O2 DII'2 O3 36.66(35) 310_334 . 209_343 N
O2 DII'2 O3 73.4(5) 310_334 . -206_444 N
O2 DII'2 O3 79.2(4) 310_334 . 312_334 N
O2 DII'2 O3 102.0(4) 310_334 . -304_444 N
O2 DII'2 O4 77.6(4) 310_334 . 3_555 N
O2 DII'2 OII' 82.4(20) 310_434 . 1_555 N
O2 DII'2 OII' 116.8(8) 310_434 . 107_533 N
O2 DII'2 OII' 72.9(11) 310_434 . 111_533 N
O2 DII'2 OII' 144.8(18) 310_434 . -105_544 N
O2 DII'2 DII'1 97.0(24) 310_334 . 1_555 N
O2 DII'2 DII'1 113.7(20) 310_334 . 2_555 N
O2 DII'2 DII'1 26.1(17) 310_334 . 3_555 N
O2 DII'2 DII'1 91.3(15) 310_334 . 107_433 N
O2 DII'2 DII'1 94.3(11) 310_334 . 111_433 N
O2 DII'2 DII'1 122.3(18) 310_334 . -105_444 N
O2 DII'2 DII'1 66.3(14) 310_334 . 208_343 N
O2 DII'2 DII'1 143.6(19) 310_334 . 209_343 N
O2 DII'2 O3 71.1(5) 312_334 . -105_444 N
O2 DII'2 O3 66.6(7) 312_334 . 209_343 N
O2 DII'2 O3 37.99(31) 312_334 . -206_444 N
O2 DII'2 O3 134.0(8) 312_334 . 312_334 N
O2 DII'2 O3 94.62(27) 312_334 . -304_444 N
O2 DII'2 O4 101.64(32) 312_334 . 3_555 N
O2 DII'2 OII' 61.2(25) 312_434 . 1_555 N
O2 DII'2 OII' 155.3(15) 312_434 . 107_533 N
O2 DII'2 OII' 66.9(12) 312_434 . 111_533 N
O2 DII'2 OII' 96.3(12) 312_434 . -105_544 N
O2 DII'2 DII'1 48.1(25) 312_334 . 1_555 N
O2 DII'2 DII'1 110.5(12) 312_334 . 2_555 N
O2 DII'2 DII'1 49.2(32) 312_334 . 3_555 N
O2 DII'2 DII'1 145.6(22) 312_334 . 107_433 N
O2 DII'2 DII'1 81.1(11) 312_334 . 111_433 N
O2 DII'2 DII'1 74.1(13) 312_334 . -105_444 N
O2 DII'2 DII'1 39.8(7) 312_334 . 208_343 N
O2 DII'2 DII'1 111.1(15) 312_334 . 209_343 N
O3 DII'2 O3 78.9(6) -105_444 . 209_343 N
O3 DII'2 O3 58.81(23) -105_444 . -206_444 N
O3 DII'2 O3 80.6(5) -105_444 . 312_334 N
O3 DII'2 O3 59.74(31) -105_444 . -304_444 N
O3 DII'2 O4 36.48(30) -105_444 . 3_555 N
O3 DII'2 OII' 51.5(12) -105_544 . 1_555 N
O3 DII'2 OII' 121.2(12) -105_544 . 107_533 N
O3 DII'2 OII' 115.8(14) -105_544 . 111_533 N
O3 DII'2 OII' 154.2(4) -105_544 . -105_544 N
O3 DII'2 DII'1 84.5(15) -105_444 . 1_555 N
O3 DII'2 DII'1 70.4(19) -105_444 . 2_555 N
O3 DII'2 DII'1 24.7(31) -105_444 . 3_555 N
O3 DII'2 DII'1 90.7(10) -105_444 . 107_433 N
O3 DII'2 DII'1 137.4(13) -105_444 . 111_433 N
O3 DII'2 DII'1 141.6(14) -105_444 . -105_444 N
O3 DII'2 DII'1 102.2(14) -105_444 . 208_343 N
O3 DII'2 DII'1 173.0(18) -105_444 . 209_343 N
O3 DII'2 O3 99.8(9) 209_343 . -206_444 N
O3 DII'2 O3 72.99(31) 209_343 . 312_334 N
O3 DII'2 O3 138.5(5) 209_343 . -304_444 N
O3 DII'2 O4 109.2(5) 209_343 . 3_555 N
O3 DII'2 OII' 116.0(26) 209_443 . 1_555 N
O3 DII'2 OII' 93.5(8) 209_443 . 107_533 N
O3 DII'2 OII' 40.6(7) 209_443 . 111_533 N
O3 DII'2 OII' 117.5(12) 209_443 . -105_544 N
O3 DII'2 DII'1 114.4(30) 209_343 . 1_555 N
O3 DII'2 DII'1 147.9(24) 209_343 . 2_555 N
O3 DII'2 DII'1 62.1(23) 209_343 . 3_555 N
O3 DII'2 DII'1 81.6(21) 209_343 . 107_433 N
O3 DII'2 DII'1 60.3(9) 209_343 . 111_433 N
O3 DII'2 DII'1 101.6(16) 209_343 . -105_444 N
O3 DII'2 DII'1 49.2(11) 209_343 . 208_343 N
O3 DII'2 DII'1 108.0(14) 209_343 . 209_343 N
O3 DII'2 O3 139.3(6) -206_444 . 312_334 N
O3 DII'2 O3 56.98(12) -206_444 . -304_444 N
O3 DII'2 O4 73.59(23) -206_444 . 3_555 N
O3 DII'2 OII' 23.8(21) -206_544 . 1_555 N
O3 DII'2 OII' 166.2(18) -206_544 . 107_533 N
O3 DII'2 OII' 104.0(15) -206_544 . 111_533 N
O3 DII'2 OII' 97.3(7) -206_544 . -105_544 N
O3 DII'2 DII'1 26.6(16) -206_444 . 1_555 N
O3 DII'2 DII'1 72.6(11) -206_444 . 2_555 N
O3 DII'2 DII'1 51.4(14) -206_444 . 3_555 N
O3 DII'2 DII'1 148.0(15) -206_444 . 107_433 N
O3 DII'2 DII'1 113.7(14) -206_444 . 111_433 N
O3 DII'2 DII'1 83.8(12) -206_444 . -105_444 N
O3 DII'2 DII'1 76.0(9) -206_444 . 208_343 N
O3 DII'2 DII'1 118.5(5) -206_444 . 209_343 N
O3 DII'2 O3 101.6(9) 312_334 . -304_444 N
O3 DII'2 O4 71.5(6) 312_334 . 3_555 N
O3 DII'2 OII' 124.1(22) 312_434 . 1_555 N
O3 DII'2 OII' 42.4(6) 312_434 . 107_533 N
O3 DII'2 OII' 95.8(5) 312_434 . 111_533 N
O3 DII'2 OII' 121.9(9) 312_434 . -105_544 N
O3 DII'2 DII'1 161.7(24) 312_334 . 1_555 N
O3 DII'2 DII'1 92.3(26) 312_334 . 2_555 N
O3 DII'2 DII'1 92.8(24) 312_334 . 3_555 N
O3 DII'2 DII'1 12.3(11) 312_334 . 107_433 N
O3 DII'2 DII'1 97.6(12) 312_334 . 111_433 N
O3 DII'2 DII'1 136.8(11) 312_334 . -105_444 N
O3 DII'2 DII'1 119.2(9) 312_334 . 208_343 N
O3 DII'2 DII'1 101.4(7) 312_334 . 209_343 N
O3 DII'2 O4 35.85(29) -304_444 . 3_555 N
O3 DII'2 OII' 33.4(23) -304_544 . 1_555 N
O3 DII'2 OII' 110.1(17) -304_544 . 107_533 N
O3 DII'2 OII' 160.7(13) -304_544 . 111_533 N
O3 DII'2 OII' 100.5(9) -304_544 . -105_544 N
O3 DII'2 DII'1 61.3(20) -304_444 . 1_555 N
O3 DII'2 DII'1 16.3(9) -304_444 . 2_555 N
O3 DII'2 DII'1 77.5(24) -304_444 . 3_555 N
O3 DII'2 DII'1 101.1(26) -304_444 . 107_433 N
O3 DII'2 DII'1 156.7(15) -304_444 . 111_433 N
O3 DII'2 DII'1 108.4(11) -304_444 . -105_444 N
O3 DII'2 DII'1 132.6(9) -304_444 . 208_343 N
O3 DII'2 DII'1 113.3(15) -304_444 . 209_343 N
O4 DII'2 OII' 53.1(19) 3_555 . 1_555 N
O4 DII'2 OII' 98.7(14) 3_555 . 107_533 N
O4 DII'2 OII' 149.7(11) 3_555 . 111_533 N
O4 DII'2 OII' 133.3(13) 3_555 . -105_544 N
O4 DII'2 DII'1 90.2(18) 3_555 . 1_555 N
O4 DII'2 DII'1 38.7(23) 3_555 . 2_555 N
O4 DII'2 DII'1 61.0(33) 3_555 . 3_555 N
O4 DII'2 DII'1 75.8(18) 3_555 . 107_433 N
O4 DII'2 DII'1 167.4(14) 3_555 . 111_433 N
O4 DII'2 DII'1 144.2(12) 3_555 . -105_444 N
O4 DII'2 DII'1 138.0(12) 3_555 . 208_343 N
O4 DII'2 DII'1 137.7(20) 3_555 . 209_343 N
OII' DII'2 OII' 144(4) 1_555 . 107_533 N
OII' DII'2 OII' 128(4) 1_555 . 111_533 N
OII' DII'2 OII' 102.8(15) 1_555 . -105_544 N
OII' DII'2 DII'1 37.73(27) 1_555 . 1_555 N
OII' DII'2 DII'1 49.5(22) 1_555 . 2_555 N
OII' DII'2 DII'1 56.5(11) 1_555 . 3_555 N
OII' DII'2 DII'1 129(4) 1_555 . 107_433 N
OII' DII'2 DII'1 136.2(31) 1_555 . 111_433 N
OII' DII'2 DII'1 97.2(19) 1_555 . -105_444 N
OII' DII'2 DII'1 99.8(31) 1_555 . 208_343 N
OII' DII'2 DII'1 123.1(17) 1_555 . 209_343 N
OII' DII'2 OII' 88.49(33) 107_533 . 111_533 N
OII' DII'2 OII' 79.6(9) 107_533 . -105_544 N
OII' DII'2 DII'1 146.1(29) 107_433 . 1_555 N
OII' DII'2 DII'1 94.2(23) 107_433 . 2_555 N
OII' DII'2 DII'1 135.0(26) 107_433 . 3_555 N
OII' DII'2 DII'1 31.0(5) 107_433 . 107_433 N
OII' DII'2 DII'1 76.1(11) 107_433 . 111_433 N
OII' DII'2 DII'1 97.2(12) 107_433 . -105_444 N
OII' DII'2 DII'1 116.1(10) 107_433 . 208_343 N
OII' DII'2 DII'1 59.6(9) 107_433 . 209_343 N
OII' DII'2 OII' 77.0(9) 111_533 . -105_544 N
OII' DII'2 DII'1 100.2(32) 111_433 . 1_555 N
OII' DII'2 DII'1 170.5(28) 111_433 . 2_555 N
OII' DII'2 DII'1 93(4) 111_433 . 3_555 N
OII' DII'2 DII'1 97.7(19) 111_433 . 107_433 N
OII' DII'2 DII'1 21.62(27) 111_433 . 111_433 N
OII' DII'2 DII'1 62.3(14) 111_433 . -105_444 N
OII' DII'2 DII'1 28.1(6) 111_433 . 208_343 N
OII' DII'2 DII'1 70.8(12) 111_433 . 209_343 N
OII' DII'2 DII'1 70.9(20) -105_444 . 1_555 N
OII' DII'2 DII'1 94.6(21) -105_444 . 2_555 N
OII' DII'2 DII'1 144.4(33) -105_444 . 3_555 N
OII' DII'2 DII'1 110.4(13) -105_444 . 107_433 N
OII' DII'2 DII'1 57.7(11) -105_444 . 111_433 N
OII' DII'2 DII'1 23.22(13) -105_444 . -105_444 N
OII' DII'2 DII'1 78.6(20) -105_444 . 208_343 N
OII' DII'2 DII'1 21.42(33) -105_444 . 209_343 N
DII'1 DII'2 DII'1 72.6(11) 1_555 . 2_555 N
DII'1 DII'2 DII'1 77.5(7) 1_555 . 3_555 N
DII'1 DII'2 DII'1 162(5) 1_555 . 107_433 N
DII'1 DII'2 DII'1 100.5(27) 1_555 . 111_433 N
DII'1 DII'2 DII'1 60.1(19) 1_555 . -105_444 N
DII'1 DII'2 DII'1 74.3(32) 1_555 . 208_343 N
DII'1 DII'2 DII'1 92.2(17) 1_555 . 209_343 N
DII'1 DII'2 DII'1 91.2(33) 2_555 . 3_555 N
DII'1 DII'2 DII'1 89(4) 2_555 . 107_433 N
DII'1 DII'2 DII'1 151.6(23) 2_555 . 111_433 N
DII'1 DII'2 DII'1 108.3(30) 2_555 . -105_444 N
DII'1 DII'2 DII'1 146.7(23) 2_555 . 208_343 N
DII'1 DII'2 DII'1 102.7(17) 2_555 . 209_343 N
DII'1 DII'2 DII'1 104.7(30) 3_555 . 107_433 N
DII'1 DII'2 DII'1 115(4) 3_555 . 111_433 N
DII'1 DII'2 DII'1 123(4) 3_555 . -105_444 N
DII'1 DII'2 DII'1 77(4) 3_555 . 208_343 N
DII'1 DII'2 DII'1 160(4) 3_555 . 209_343 N
DII'1 DII'2 DII'1 94.9(26) 107_433 . 111_433 N
DII'1 DII'2 DII'1 127.6(11) 107_433 . -105_444 N
DII'1 DII'2 DII'1 123.9(21) 107_433 . 208_343 N
DII'1 DII'2 DII'1 90.6(10) 107_433 . 209_343 N
DII'1 DII'2 DII'1 48.4(23) 111_433 . -105_444 N
DII'1 DII'2 DII'1 41.8(4) 111_433 . 208_343 N
DII'1 DII'2 DII'1 49.3(13) 111_433 . 209_343 N
DII'1 DII'2 DII'1 56.8(18) -105_444 . 208_343 N
DII'1 DII'2 DII'1 38.11(25) -105_444 . 209_343 N
DII'1 DII'2 DII'1 82.7(26) 208_343 . 209_343 N
O1 OII* O1 44.72(16) 107_433 . -110_544 N
O1 OII* O1 102.7(5) 107_433 . 208_343 N
O1 OII* O1 128.7(8) 107_433 . -211_454 N
O1 OII* O1 102.7(5) 107_433 . 312_334 N
O1 OII* O1 62.80(22) 107_433 . -309_445 N
O1 OII* O3 72.1(4) 107_433 . -105_444 N
O1 OII* O3 33.93(14) 107_433 . -206_444 N
O1 OII* O3 95.3(7) 107_433 . -304_444 N
O1 OII* O4 32.77(18) 107_433 . 1_555 N
O1 OII* O4 69.9(4) 107_433 . 2_555 N
O1 OII* O4 108.7(7) 107_433 . 3_555 N
O1 OII* SII 64.4(4) 107_555 . 1_555 N
O1 OII* Og 69.92(27) 107_545 . 107_545 N
O1 OII* Og 158.5(9) 107_545 . 208_455 N
O1 OII* Og 61.18(24) 107_545 . 312_446 N
O1 OII* Dg1 80.14(27) 107_554 . 107_554 N
O1 OII* Dg1 152.1(7) 107_554 . 208_464 N
O1 OII* Dg1 50.36(27) 107_554 . 312_455 N
O1 OII* Dg2 60.22(30) 107_555 . 107_555 N
O1 OII* Dg2 146.8(9) 107_555 . 208_465 N
O1 OII* Dg2 59.24(32) 107_555 . 312_456 N
O1 OII* Oh 89.4(7) 107_554 . 107_554 N
O1 OII* Oh 143.1(10) 107_554 . 208_464 N
O1 OII* Oh 40.4(7) 107_554 . 312_455 N
O1 OII* O1 62.80(22) -110_544 . 208_343 N
O1 OII* O1 103.7(5) -110_544 . -211_454 N
O1 OII* O1 128.7(8) -110_544 . 312_334 N
O1 OII* O1 103.7(5) -110_544 . -309_445 N
O1 OII* O3 95.6(6) -110_544 . -105_444 N
O1 OII* O3 34.07(13) -110_544 . -206_444 N
O1 OII* O3 73.6(4) -110_544 . -304_444 N
O1 OII* O4 69.8(4) -110_544 . 1_555 N
O1 OII* O4 33.94(17) -110_544 . 2_555 N
O1 OII* O4 109.7(7) -110_544 . 3_555 N
O1 OII* SII 65.2(4) -110_666 . 1_555 N
O1 OII* Og 32.99(21) -110_656 . 107_545 N
O1 OII* Og 132.7(4) -110_656 . 208_455 N
O1 OII* Og 105.18(30) -110_656 . 312_446 N
O1 OII* Dg1 38.88(24) -110_665 . 107_554 N
O1 OII* Dg1 142.2(5) -110_665 . 208_464 N
O1 OII* Dg1 93.46(29) -110_665 . 312_455 N
O1 OII* Dg2 20.05(20) -110_666 . 107_555 N
O1 OII* Dg2 122.2(5) -110_666 . 208_465 N
O1 OII* Dg2 103.9(4) -110_666 . 312_456 N
O1 OII* Oh 45.9(6) -110_665 . 107_554 N
O1 OII* Oh 148.9(11) -110_665 . 208_464 N
O1 OII* Oh 82.4(7) -110_665 . 312_455 N
O1 OII* O1 44.72(16) 208_343 . -211_454 N
O1 OII* O1 102.7(5) 208_343 . 312_334 N
O1 OII* O1 128.7(8) 208_343 . -309_445 N
O1 OII* O3 95.3(7) 208_343 . -105_444 N
O1 OII* O3 72.1(4) 208_343 . -206_444 N
O1 OII* O3 33.93(14) 208_343 . -304_444 N
O1 OII* O4 108.7(7) 208_343 . 1_555 N
O1 OII* O4 32.77(18) 208_343 . 2_555 N
O1 OII* O4 69.9(4) 208_343 . 3_555 N
O1 OII* SII 64.4(4) 208_465 . 1_555 N
O1 OII* Og 61.18(24) 208_455 . 107_545 N
O1 OII* Og 69.92(27) 208_455 . 208_455 N
O1 OII* Og 158.5(9) 208_455 . 312_446 N
O1 OII* Dg1 50.36(27) 208_464 . 107_554 N
O1 OII* Dg1 80.14(27) 208_464 . 208_464 N
O1 OII* Dg1 152.1(7) 208_464 . 312_455 N
O1 OII* Dg2 59.24(32) 208_465 . 107_555 N
O1 OII* Dg2 60.22(30) 208_465 . 208_465 N
O1 OII* Dg2 146.8(9) 208_465 . 312_456 N
O1 OII* Oh 40.4(7) 208_464 . 107_554 N
O1 OII* Oh 89.4(7) 208_464 . 208_464 N
O1 OII* Oh 143.1(10) 208_464 . 312_455 N
O1 OII* O1 62.80(22) -211_454 . 312_334 N
O1 OII* O1 103.7(5) -211_454 . -309_445 N
O1 OII* O3 73.6(4) -211_454 . -105_444 N
O1 OII* O3 95.6(6) -211_454 . -206_444 N
O1 OII* O3 34.07(13) -211_454 . -304_444 N
O1 OII* O4 109.7(7) -211_454 . 1_555 N
O1 OII* O4 69.8(4) -211_454 . 2_555 N
O1 OII* O4 33.94(17) -211_454 . 3_555 N
O1 OII* SII 65.2(4) -211_576 . 1_555 N
O1 OII* Og 105.18(30) -211_566 . 107_545 N
O1 OII* Og 32.99(21) -211_566 . 208_455 N
O1 OII* Og 132.7(4) -211_566 . 312_446 N
O1 OII* Dg1 93.46(29) -211_575 . 107_554 N
O1 OII* Dg1 38.88(24) -211_575 . 208_464 N
O1 OII* Dg1 142.2(5) -211_575 . 312_455 N
O1 OII* Dg2 103.9(4) -211_576 . 107_555 N
O1 OII* Dg2 20.05(20) -211_576 . 208_465 N
O1 OII* Dg2 122.2(5) -211_576 . 312_456 N
O1 OII* Oh 82.4(7) -211_575 . 107_554 N
O1 OII* Oh 45.9(6) -211_575 . 208_464 N
O1 OII* Oh 148.9(11) -211_575 . 312_455 N
O1 OII* O1 44.72(16) 312_334 . -309_445 N
O1 OII* O3 33.93(14) 312_334 . -105_444 N
O1 OII* O3 95.3(7) 312_334 . -206_444 N
O1 OII* O3 72.1(4) 312_334 . -304_444 N
O1 OII* O4 69.9(4) 312_334 . 1_555 N
O1 OII* O4 108.7(7) 312_334 . 2_555 N
O1 OII* O4 32.77(18) 312_334 . 3_555 N
O1 OII* SII 64.4(4) 312_456 . 1_555 N
O1 OII* Og 158.5(9) 312_446 . 107_545 N
O1 OII* Og 61.18(24) 312_446 . 208_455 N
O1 OII* Og 69.92(27) 312_446 . 312_446 N
O1 OII* Dg1 152.1(7) 312_455 . 107_554 N
O1 OII* Dg1 50.36(27) 312_455 . 208_464 N
O1 OII* Dg1 80.14(27) 312_455 . 312_455 N
O1 OII* Dg2 146.8(9) 312_456 . 107_555 N
O1 OII* Dg2 59.24(32) 312_456 . 208_465 N
O1 OII* Dg2 60.22(30) 312_456 . 312_456 N
O1 OII* Oh 143.1(10) 312_455 . 107_554 N
O1 OII* Oh 40.4(7) 312_455 . 208_464 N
O1 OII* Oh 89.4(7) 312_455 . 312_455 N
O1 OII* O3 34.07(13) -309_445 . -105_444 N
O1 OII* O3 73.6(4) -309_445 . -206_444 N
O1 OII* O3 95.6(6) -309_445 . -304_444 N
O1 OII* O4 33.94(17) -309_445 . 1_555 N
O1 OII* O4 109.7(7) -309_445 . 2_555 N
O1 OII* O4 69.8(4) -309_445 . 3_555 N
O1 OII* SII 65.2(4) -309_567 . 1_555 N
O1 OII* Og 132.7(4) -309_557 . 107_545 N
O1 OII* Og 105.18(30) -309_557 . 208_455 N
O1 OII* Og 32.99(21) -309_557 . 312_446 N
O1 OII* Dg1 142.2(5) -309_566 . 107_554 N
O1 OII* Dg1 93.46(29) -309_566 . 208_464 N
O1 OII* Dg1 38.88(24) -309_566 . 312_455 N
O1 OII* Dg2 122.2(5) -309_567 . 107_555 N
O1 OII* Dg2 103.9(4) -309_567 . 208_465 N
O1 OII* Dg2 20.05(20) -309_567 . 312_456 N
O1 OII* Oh 148.9(11) -309_566 . 107_554 N
O1 OII* Oh 82.4(7) -309_566 . 208_464 N
O1 OII* Oh 45.9(6) -309_566 . 312_455 N
O3 OII* O3 61.7(5) -105_444 . -206_444 N
O3 OII* O3 61.7(5) -105_444 . -304_444 N
O3 OII* O4 40.55(31) -105_444 . 1_555 N
O3 OII* O4 84.5(7) -105_444 . 2_555 N
O3 OII* O4 40.91(32) -105_444 . 3_555 N
O3 OII* SII 36.30(33) -105_566 . 1_555 N
O3 OII* Og 128.2(8) -105_556 . 107_545 N
O3 OII* Og 88.1(4) -105_556 . 208_455 N
O3 OII* Og 67.03(29) -105_556 . 312_446 N
O3 OII* Dg1 129.2(8) -105_565 . 107_554 N
O3 OII* Dg1 80.0(4) -105_565 . 208_464 N
O3 OII* Dg1 71.40(34) -105_565 . 312_455 N
O3 OII* Dg2 115.2(8) -105_566 . 107_555 N
O3 OII* Dg2 81.0(5) -105_566 . 208_465 N
O3 OII* Dg2 54.01(28) -105_566 . 312_456 N
O3 OII* Oh 127.5(13) -105_565 . 107_554 N
O3 OII* Oh 72.2(8) -105_565 . 208_464 N
O3 OII* Oh 75.5(8) -105_565 . 312_455 N
O3 OII* O3 61.7(5) -206_444 . -304_444 N
O3 OII* O4 40.91(32) -206_444 . 1_555 N
O3 OII* O4 40.55(31) -206_444 . 2_555 N
O3 OII* O4 84.5(7) -206_444 . 3_555 N
O3 OII* SII 36.30(33) -206_566 . 1_555 N
O3 OII* Og 67.03(29) -206_556 . 107_545 N
O3 OII* Og 128.2(8) -206_556 . 208_455 N
O3 OII* Og 88.1(4) -206_556 . 312_446 N
O3 OII* Dg1 71.40(34) -206_565 . 107_554 N
O3 OII* Dg1 129.2(8) -206_565 . 208_464 N
O3 OII* Dg1 80.0(4) -206_565 . 312_455 N
O3 OII* Dg2 54.01(28) -206_566 . 107_555 N
O3 OII* Dg2 115.2(8) -206_566 . 208_465 N
O3 OII* Dg2 81.0(5) -206_566 . 312_456 N
O3 OII* Oh 75.5(8) -206_565 . 107_554 N
O3 OII* Oh 127.5(13) -206_565 . 208_464 N
O3 OII* Oh 72.2(8) -206_565 . 312_455 N
O3 OII* O4 84.5(7) -304_444 . 1_555 N
O3 OII* O4 40.91(32) -304_444 . 2_555 N
O3 OII* O4 40.55(31) -304_444 . 3_555 N
O3 OII* SII 36.30(33) -304_566 . 1_555 N
O3 OII* Og 88.1(4) -304_556 . 107_545 N
O3 OII* Og 67.03(29) -304_556 . 208_455 N
O3 OII* Og 128.2(8) -304_556 . 312_446 N
O3 OII* Dg1 80.0(4) -304_565 . 107_554 N
O3 OII* Dg1 71.40(34) -304_565 . 208_464 N
O3 OII* Dg1 129.2(8) -304_565 . 312_455 N
O3 OII* Dg2 81.0(5) -304_566 . 107_555 N
O3 OII* Dg2 54.01(28) -304_566 . 208_465 N
O3 OII* Dg2 115.2(8) -304_566 . 312_456 N
O3 OII* Oh 72.2(8) -304_565 . 107_554 N
O3 OII* Oh 75.5(8) -304_565 . 208_464 N
O3 OII* Oh 127.5(13) -304_565 . 312_455 N
O4 OII* O4 80.4(6) 1_555 . 2_555 N
O4 OII* O4 80.4(6) 1_555 . 3_555 N
O4 OII* SII 48.2(4) 1_555 . 1_555 N
O4 OII* Og 100.4(4) 1_555 . 107_545 N
O4 OII* Og 128.7(6) 1_555 . 208_455 N
O4 OII* Og 49.93(21) 1_555 . 312_446 N
O4 OII* Dg1 108.6(5) 1_555 . 107_554 N
O4 OII* Dg1 119.7(6) 1_555 . 208_464 N
O4 OII* Dg1 45.66(29) 1_555 . 312_455 N
O4 OII* Dg2 88.8(4) 1_555 . 107_555 N
O4 OII* Dg2 121.0(8) 1_555 . 208_465 N
O4 OII* Dg2 40.60(28) 1_555 . 312_456 N
O4 OII* Oh 115.1(9) 1_555 . 107_554 N
O4 OII* Oh 110.4(9) 1_555 . 208_464 N
O4 OII* Oh 43.1(7) 1_555 . 312_455 N
O4 OII* O4 80.4(6) 2_555 . 3_555 N
O4 OII* SII 48.2(4) 2_555 . 1_555 N
O4 OII* Og 49.93(21) 2_555 . 107_545 N
O4 OII* Og 100.4(4) 2_555 . 208_455 N
O4 OII* Og 128.7(6) 2_555 . 312_446 N
O4 OII* Dg1 45.66(29) 2_555 . 107_554 N
O4 OII* Dg1 108.6(5) 2_555 . 208_464 N
O4 OII* Dg1 119.7(6) 2_555 . 312_455 N
O4 OII* Dg2 40.60(28) 2_555 . 107_555 N
O4 OII* Dg2 88.8(4) 2_555 . 208_465 N
O4 OII* Dg2 121.0(8) 2_555 . 312_456 N
O4 OII* Oh 43.1(7) 2_555 . 107_554 N
O4 OII* Oh 115.1(9) 2_555 . 208_464 N
O4 OII* Oh 110.4(9) 2_555 . 312_455 N
O4 OII* SII 48.2(4) 3_555 . 1_555 N
O4 OII* Og 128.7(6) 3_555 . 107_545 N
O4 OII* Og 49.93(21) 3_555 . 208_455 N
O4 OII* Og 100.4(4) 3_555 . 312_446 N
O4 OII* Dg1 119.7(6) 3_555 . 107_554 N
O4 OII* Dg1 45.66(29) 3_555 . 208_464 N
O4 OII* Dg1 108.6(5) 3_555 . 312_455 N
O4 OII* Dg2 121.0(8) 3_555 . 107_555 N
O4 OII* Dg2 40.60(28) 3_555 . 208_465 N
O4 OII* Dg2 88.8(4) 3_555 . 312_456 N
O4 OII* Oh 110.4(9) 3_555 . 107_554 N
O4 OII* Oh 43.1(7) 3_555 . 208_464 N
O4 OII* Oh 115.1(9) 3_555 . 312_455 N
SII OII* Og 94.6(5) 1_555 . 107_545 N
SII OII* Og 94.6(5) 1_555 . 208_455 N
SII OII* Og 94.6(5) 1_555 . 312_446 N
SII OII* Dg1 93.3(5) 1_555 . 107_554 N
SII OII* Dg1 93.3(5) 1_555 . 208_464 N
SII OII* Dg1 93.3(5) 1_555 . 312_455 N
SII OII* Dg2 82.4(5) 1_555 . 107_555 N
SII OII* Dg2 82.4(5) 1_555 . 208_465 N
SII OII* Dg2 82.4(5) 1_555 . 312_456 N
SII OII* Oh 91.2(10) 1_555 . 107_554 N
SII OII* Oh 91.2(10) 1_555 . 208_464 N
SII OII* Oh 91.2(10) 1_555 . 312_455 N
Og OII* Og 119.36(14) 107_545 . 208_455 N
Og OII* Og 119.36(14) 107_545 . 312_446 N
Og OII* Dg1 12.34(11) 107_554 . 107_554 N
Og OII* Dg1 131.69(19) 107_554 . 208_464 N
Og OII* Dg1 107.33(16) 107_554 . 312_455 N
Og OII* Dg2 13.05(5) 107_555 . 107_555 N
Og OII* Dg2 115.79(24) 107_555 . 208_465 N
Og OII* Dg2 124.83(24) 107_555 . 312_456 N
Og OII* Oh 23.8(6) 107_554 . 107_554 N
Og OII* Oh 143.2(7) 107_554 . 208_464 N
Og OII* Oh 96.3(6) 107_554 . 312_455 N
Og OII* Og 119.36(14) 208_455 . 312_446 N
Og OII* Dg1 107.33(16) 208_464 . 107_554 N
Og OII* Dg1 12.34(11) 208_464 . 208_464 N
Og OII* Dg1 131.69(19) 208_464 . 312_455 N
Og OII* Dg2 124.83(24) 208_465 . 107_555 N
Og OII* Dg2 13.05(5) 208_465 . 208_465 N
Og OII* Dg2 115.79(24) 208_465 . 312_456 N
Og OII* Oh 96.3(6) 208_464 . 107_554 N
Og OII* Oh 23.8(6) 208_464 . 208_464 N
Og OII* Oh 143.2(7) 208_464 . 312_455 N
Og OII* Dg1 131.69(19) 312_455 . 107_554 N
Og OII* Dg1 107.33(16) 312_455 . 208_464 N
Og OII* Dg1 12.34(11) 312_455 . 312_455 N
Og OII* Dg2 115.79(24) 312_456 . 107_555 N
Og OII* Dg2 124.83(24) 312_456 . 208_465 N
Og OII* Dg2 13.05(5) 312_456 . 312_456 N
Og OII* Oh 143.2(7) 312_455 . 107_554 N
Og OII* Oh 96.3(6) 312_455 . 208_464 N
Og OII* Oh 23.8(6) 312_455 . 312_455 N
Dg1 OII* Dg1 119.67(11) 107_554 . 208_464 N
Dg1 OII* Dg1 119.67(11) 107_554 . 312_455 N
Dg1 OII* Dg2 20.05(8) 107_555 . 107_555 N
Dg1 OII* Dg2 103.44(28) 107_555 . 208_465 N
Dg1 OII* Dg2 136.87(24) 107_555 . 312_456 N
Dg1 OII* Oh 11.5(6) 107_554 . 107_554 N
Dg1 OII* Oh 131.1(6) 107_554 . 208_464 N
Dg1 OII* Oh 108.6(6) 107_554 . 312_455 N
Dg1 OII* Dg1 119.67(11) 208_464 . 312_455 N
Dg1 OII* Dg2 136.87(24) 208_465 . 107_555 N
Dg1 OII* Dg2 20.05(8) 208_465 . 208_465 N
Dg1 OII* Dg2 103.44(28) 208_465 . 312_456 N
Dg1 OII* Oh 108.6(6) 208_464 . 107_554 N
Dg1 OII* Oh 11.5(6) 208_464 . 208_464 N
Dg1 OII* Oh 131.1(6) 208_464 . 312_455 N
Dg1 OII* Dg2 103.44(28) 312_456 . 107_555 N
Dg1 OII* Dg2 136.87(24) 312_456 . 208_465 N
Dg1 OII* Dg2 20.05(8) 312_456 . 312_456 N
Dg1 OII* Oh 131.1(6) 312_455 . 107_554 N
Dg1 OII* Oh 108.6(6) 312_455 . 208_464 N
Dg1 OII* Oh 11.5(6) 312_455 . 312_455 N
Dg2 OII* Dg2 118.28(23) 107_555 . 208_465 N
Dg2 OII* Dg2 118.28(23) 107_555 . 312_456 N
Dg2 OII* Oh 29.4(6) 107_554 . 107_554 N
Dg2 OII* Oh 147.6(7) 107_554 . 208_464 N
Dg2 OII* Oh 92.0(7) 107_554 . 312_455 N
Dg2 OII* Dg2 118.28(23) 208_465 . 312_456 N
Dg2 OII* Oh 92.0(7) 208_464 . 107_554 N
Dg2 OII* Oh 29.4(6) 208_464 . 208_464 N
Dg2 OII* Oh 147.6(7) 208_464 . 312_455 N
Dg2 OII* Oh 147.6(7) 312_455 . 107_554 N
Dg2 OII* Oh 92.0(7) 312_455 . 208_464 N
Dg2 OII* Oh 29.4(6) 312_455 . 312_455 N
Oh OII* Oh 119.95(7) 107_554 . 208_464 N
Oh OII* Oh 119.95(7) 107_554 . 312_455 N
Oh OII* Oh 119.95(7) 208_464 . 312_455 N
O1 DII*1 O3 40.8(7) 312_334 . -105_444 N
O1 DII*1 O3 96.5(15) 312_334 . -206_444 N
O1 DII*1 O3 78.4(14) 312_334 . -304_444 N
O1 DII*1 O4 75.7(11) 312_334 . 1_555 N
O1 DII*1 O4 39.3(6) 312_334 . 3_555 N
O1 DII*1 Og 38.3(4) 312_446 . 5_555 N
O1 DII*1 Og 73.1(10) 312_446 . 208_455 N
O1 DII*1 Og 80.1(8) 312_446 . 312_446 N
O1 DII*1 Dg1 60.5(8) 312_455 . 208_464 N
O1 DII*1 Dg2 25.17(34) 312_456 . 5_555 N
O1 DII*1 Dg2 69.4(11) 312_456 . 208_465 N
O1 DII*1 Oh 140.3(23) 312_455 . 107_554 N
O1 DII*1 Oh 52.3(18) 312_455 . 208_464 N
O1 DII*1 Oh 102.8(15) 312_455 . 312_455 N
O1 DII*1 Dh1 149.3(20) 312_434 . 107_533 N
O1 DII*1 Dh1 69.9(13) 312_434 . 208_443 N
O1 DII*1 Dh1 94.2(12) 312_434 . 312_434 N
O1 DII*1 Dh2 126.8(21) 312_434 . 107_533 N
O1 DII*1 Dh2 40.4(12) 312_434 . 208_443 N
O1 DII*1 Dh2 90.2(15) 312_434 . 312_434 N
O1 DII*1 OII* 134(6) 312_334 . 1_555 N
O1 DII*1 DII*1 131.4(25) 312_333 . 2_555 N
O1 DII*1 DII*1 140.2(23) 312_333 . 3_555 N
O1 DII*1 DII*2 151(5) 312_334 . 1_555 N
O3 DII*1 O3 56.1(8) -105_444 . -206_444 N
O3 DII*1 O3 60.9(12) -105_444 . -304_444 N
O3 DII*1 O4 39.3(6) -105_444 . 1_555 N
O3 DII*1 O4 44.6(10) -105_444 . 3_555 N
O3 DII*1 Og 77.3(11) -105_556 . 5_555 N
O3 DII*1 Og 100.9(18) -105_556 . 208_455 N
O3 DII*1 Og 71.4(9) -105_556 . 312_446 N
O3 DII*1 Dg1 93.6(16) -105_565 . 208_464 N
O3 DII*1 Dg2 65.0(10) -105_566 . 5_555 N
O3 DII*1 Dg2 90.2(17) -105_566 . 208_465 N
O3 DII*1 Oh 110.0(17) -105_565 . 107_554 N
O3 DII*1 Oh 85.9(29) -105_565 . 208_464 N
O3 DII*1 Oh 76.7(14) -105_565 . 312_455 N
O3 DII*1 Dh1 114.3(13) -105_544 . 107_533 N
O3 DII*1 Dh1 101.8(23) -105_544 . 208_443 N
O3 DII*1 Dh1 78.6(13) -105_544 . 312_434 N
O3 DII*1 Dh2 95.5(15) -105_544 . 107_533 N
O3 DII*1 Dh2 63.8(19) -105_544 . 208_443 N
O3 DII*1 Dh2 59.6(12) -105_544 . 312_434 N
O3 DII*1 OII* 95(5) -105_444 . 1_555 N
O3 DII*1 DII*1 93.9(18) -105_443 . 2_555 N
O3 DII*1 DII*1 113.21(29) -105_443 . 3_555 N
O3 DII*1 DII*2 126(5) -105_444 . 1_555 N
O3 DII*1 O3 53.7(7) -206_444 . -304_444 N
O3 DII*1 O4 36.1(4) -206_444 . 1_555 N
O3 DII*1 O4 79.6(14) -206_444 . 3_555 N
O3 DII*1 Og 128.4(19) -206_556 . 5_555 N
O3 DII*1 Og 123.8(18) -206_556 . 208_455 N
O3 DII*1 Og 81.8(8) -206_556 . 312_446 N
O3 DII*1 Dg1 129.7(20) -206_565 . 208_464 N
O3 DII*1 Dg2 118.6(18) -206_566 . 5_555 N
O3 DII*1 Dg2 109.6(16) -206_566 . 208_465 N
O3 DII*1 Oh 58.9(7) -206_565 . 107_554 N
O3 DII*1 Oh 126(4) -206_565 . 208_464 N
O3 DII*1 Oh 58.4(9) -206_565 . 312_455 N
O3 DII*1 Dh1 59.6(5) -206_544 . 107_533 N
O3 DII*1 Dh1 131.4(26) -206_544 . 208_443 N
O3 DII*1 Dh1 74.4(9) -206_544 . 312_434 N
O3 DII*1 Dh2 47.0(6) -206_544 . 107_533 N
O3 DII*1 Dh2 102.1(24) -206_544 . 208_443 N
O3 DII*1 Dh2 46.6(8) -206_544 . 312_434 N
O3 DII*1 OII* 39(4) -206_444 . 1_555 N
O3 DII*1 DII*1 46.9(8) -206_443 . 2_555 N
O3 DII*1 DII*1 63.6(16) -206_443 . 3_555 N
O3 DII*1 DII*2 73.7(34) -206_444 . 1_555 N
O3 DII*1 O4 78.2(12) -304_444 . 1_555 N
O3 DII*1 O4 40.8(8) -304_444 . 3_555 N
O3 DII*1 Og 86.4(13) -304_556 . 5_555 N
O3 DII*1 Og 70.2(12) -304_556 . 208_455 N
O3 DII*1 Og 127.1(16) -304_556 . 312_446 N
O3 DII*1 Dg1 77.0(13) -304_565 . 208_464 N
O3 DII*1 Dg2 84.7(14) -304_566 . 5_555 N
O3 DII*1 Dg2 55.9(10) -304_566 . 208_465 N
O3 DII*1 Oh 61.9(10) -304_565 . 107_554 N
O3 DII*1 Oh 75.8(27) -304_565 . 208_464 N
O3 DII*1 Oh 111.6(17) -304_565 . 312_455 N
O3 DII*1 Dh1 71.8(8) -304_544 . 107_533 N
O3 DII*1 Dh1 77.7(20) -304_544 . 208_443 N
O3 DII*1 Dh1 125.7(16) -304_544 . 312_434 N
O3 DII*1 Dh2 49.6(8) -304_544 . 107_533 N
O3 DII*1 Dh2 56.1(17) -304_544 . 208_443 N
O3 DII*1 Dh2 97.1(16) -304_544 . 312_434 N
O3 DII*1 OII* 68(5) -304_444 . 1_555 N
O3 DII*1 DII*1 94.8(15) -304_443 . 2_555 N
O3 DII*1 DII*1 61.9(14) -304_443 . 3_555 N
O3 DII*1 DII*2 74(4) -304_444 . 1_555 N
O4 DII*1 O4 81.8(14) 1_555 . 3_555 N
O4 DII*1 Og 114.0(14) 1_555 . 5_555 N
O4 DII*1 Og 139.0(22) 1_555 . 208_455 N
O4 DII*1 Og 49.8(6) 1_555 . 312_446 N
O4 DII*1 Dg1 132.9(20) 1_555 . 208_464 N
O4 DII*1 Dg2 100.8(14) 1_555 . 5_555 N
O4 DII*1 Dg2 126.2(21) 1_555 . 208_465 N
O4 DII*1 Oh 93.0(8) 1_555 . 107_554 N
O4 DII*1 Oh 125.1(33) 1_555 . 208_464 N
O4 DII*1 Oh 39.7(10) 1_555 . 312_455 N
O4 DII*1 Dh1 90.7(6) 1_555 . 107_533 N
O4 DII*1 Dh1 141.1(28) 1_555 . 208_443 N
O4 DII*1 Dh1 48.3(8) 1_555 . 312_434 N
O4 DII*1 Dh2 82.6(9) 1_555 . 107_533 N
O4 DII*1 Dh2 102.8(24) 1_555 . 208_443 N
O4 DII*1 Dh2 22.0(7) 1_555 . 312_434 N
O4 DII*1 OII* 68.3(32) 1_555 . 1_555 N
O4 DII*1 DII*1 56.0(22) 1_555 . 2_555 N
O4 DII*1 DII*1 98.1(20) 1_555 . 3_555 N
O4 DII*1 DII*2 106.1(30) 1_555 . 1_555 N
O4 DII*1 Og 50.1(6) 3_555 . 5_555 N
O4 DII*1 Og 57.3(10) 3_555 . 208_455 N
O4 DII*1 Og 112.3(15) 3_555 . 312_446 N
O4 DII*1 Dg1 53.8(9) 3_555 . 208_464 N
O4 DII*1 Dg2 44.9(7) 3_555 . 5_555 N
O4 DII*1 Dg2 45.6(9) 3_555 . 208_465 N
O4 DII*1 Oh 102.1(18) 3_555 . 107_554 N
O4 DII*1 Oh 48.0(23) 3_555 . 208_464 N
O4 DII*1 Oh 120.9(23) 3_555 . 312_455 N
O4 DII*1 Dh1 112.4(15) 3_555 . 107_533 N
O4 DII*1 Dh1 60.1(17) 3_555 . 208_443 N
O4 DII*1 Dh1 122.5(20) 3_555 . 312_434 N
O4 DII*1 Dh2 90.3(16) 3_555 . 107_533 N
O4 DII*1 Dh2 23.1(12) 3_555 . 208_443 N
O4 DII*1 Dh2 103.4(20) 3_555 . 312_434 N
O4 DII*1 OII* 107(6) 3_555 . 1_555 N
O4 DII*1 DII*1 126.5(6) 3_555 . 2_555 N
O4 DII*1 DII*1 101.2(23) 3_555 . 3_555 N
O4 DII*1 DII*2 112(5) 3_555 . 1_555 N
Og DII*1 Og 40.6(5) 5_555 . 208_455 N
Og DII*1 Og 104.8(6) 5_555 . 312_446 N
Og DII*1 Dg1 25.7(4) 5_555 . 208_464 N
Og DII*1 Dg2 13.28(11) 5_555 . 5_555 N
Og DII*1 Dg2 44.6(6) 5_555 . 208_465 N
Og DII*1 Oh 133.6(17) 5_555 . 107_554 N
Og DII*1 Oh 18.8(11) 5_555 . 208_464 N
Og DII*1 Oh 134.7(13) 5_555 . 312_455 N
Og DII*1 Dh1 143.2(15) 5_555 . 107_533 N
Og DII*1 Dh1 34.5(9) 5_555 . 208_443 N
Og DII*1 Dh1 119.9(10) 5_555 . 312_434 N
Og DII*1 Dh2 130.0(18) 5_555 . 107_533 N
Og DII*1 Dh2 30.3(8) 5_555 . 208_443 N
Og DII*1 Dh2 126.8(16) 5_555 . 312_434 N
Og DII*1 OII* 153(6) 5_555 . 1_555 N
Og DII*1 DII*1 169.2(31) 5_555 . 2_555 N
Og DII*1 DII*1 129(4) 5_555 . 3_555 N
Og DII*1 DII*2 130.2(30) 5_555 . 1_555 N
Og DII*1 Og 144.27(32) 208_455 . 312_446 N
Og DII*1 Dg1 15.03(19) 208_464 . 208_464 N
Og DII*1 Dg2 52.0(6) 208_465 . 5_555 N
Og DII*1 Dg2 14.52(26) 208_465 . 208_465 N
Og DII*1 Oh 94.4(13) 208_464 . 107_554 N
Og DII*1 Oh 22.1(13) 208_464 . 208_464 N
Og DII*1 Oh 175.3(12) 208_464 . 312_455 N
Og DII*1 Dh1 103.0(12) 208_443 . 107_533 N
Og DII*1 Dh1 8.7(9) 208_443 . 208_443 N
Og DII*1 Dh1 158.2(9) 208_443 . 312_434 N
Og DII*1 Dh2 95.4(13) 208_443 . 107_533 N
Og DII*1 Dh2 37.4(10) 208_443 . 208_443 N
Og DII*1 Dh2 160.5(27) 208_443 . 312_434 N
Og DII*1 OII* 119(4) 208_343 . 1_555 N
Og DII*1 DII*1 149.4(34) 208_342 . 2_555 N
Og DII*1 DII*1 89.5(34) 208_342 . 3_555 N
Og DII*1 DII*2 89.7(27) 208_343 . 1_555 N
Og DII*1 Dg1 129.5(5) 312_455 . 208_464 N
Og DII*1 Dg2 95.3(8) 312_456 . 5_555 N
Og DII*1 Dg2 148.2(11) 312_456 . 208_465 N
Og DII*1 Oh 121.2(11) 312_455 . 107_554 N
Og DII*1 Oh 123.6(15) 312_455 . 208_464 N
Og DII*1 Oh 31.2(8) 312_455 . 312_455 N
Og DII*1 Dh1 112.0(11) 312_434 . 107_533 N
Og DII*1 Dh1 136.2(11) 312_434 . 208_443 N
Og DII*1 Dh1 15.2(6) 312_434 . 312_434 N
Og DII*1 Dh2 119.7(10) 312_434 . 107_533 N
Og DII*1 Dh2 120.5(17) 312_434 . 208_443 N
Og DII*1 Dh2 35.5(9) 312_434 . 312_434 N
Og DII*1 OII* 96.3(32) 312_334 . 1_555 N
Og DII*1 DII*1 66.0(32) 312_333 . 2_555 N
Og DII*1 DII*1 125.9(33) 312_333 . 3_555 N
Og DII*1 DII*2 123.7(32) 312_334 . 1_555 N
Dg1 DII*1 Dg2 37.7(5) 208_465 . 5_555 N
Dg1 DII*1 Dg2 23.27(33) 208_465 . 208_465 N
Dg1 DII*1 Oh 109.3(14) 208_464 . 107_554 N
Dg1 DII*1 Oh 8.2(14) 208_464 . 208_464 N
Dg1 DII*1 Oh 160.3(12) 208_464 . 312_455 N
Dg1 DII*1 Dh1 118.0(13) 208_443 . 107_533 N
Dg1 DII*1 Dh1 9.4(9) 208_443 . 208_443 N
Dg1 DII*1 Dh1 144.0(9) 208_443 . 312_434 N
Dg1 DII*1 Dh2 109.3(15) 208_443 . 107_533 N
Dg1 DII*1 Dh2 31.0(9) 208_443 . 208_443 N
Dg1 DII*1 Dh2 150.7(21) 208_443 . 312_434 N
Dg1 DII*1 OII* 134(4) 208_343 . 1_555 N
Dg1 DII*1 DII*1 164(4) 208_342 . 2_555 N
Dg1 DII*1 DII*1 104(4) 208_342 . 3_555 N
Dg1 DII*1 DII*2 104.6(28) 208_343 . 1_555 N
Dg2 DII*1 Dg2 53.0(7) 5_555 . 208_465 N
Dg2 DII*1 Oh 140.4(20) 5_555 . 107_554 N
Dg2 DII*1 Oh 29.9(13) 5_555 . 208_464 N
Dg2 DII*1 Oh 123.4(15) 5_555 . 312_455 N
Dg2 DII*1 Dh1 151.2(18) 5_555 . 107_533 N
Dg2 DII*1 Dh1 46.9(10) 5_555 . 208_443 N
Dg2 DII*1 Dh1 110.5(11) 5_555 . 312_434 N
Dg2 DII*1 Dh2 132.8(21) 5_555 . 107_533 N
Dg2 DII*1 Dh2 30.8(9) 5_555 . 208_443 N
Dg2 DII*1 Dh2 113.8(16) 5_555 . 312_434 N
Dg2 DII*1 OII* 152(6) 5_555 . 1_555 N
Dg2 DII*1 DII*1 156.1(29) 5_555 . 2_555 N
Dg2 DII*1 DII*1 137(4) 5_555 . 3_555 N
Dg2 DII*1 DII*2 140.9(33) 5_555 . 1_555 N
Dg2 DII*1 Oh 89.0(13) 208_464 . 107_554 N
Dg2 DII*1 Oh 26.4(15) 208_464 . 208_464 N
Dg2 DII*1 Oh 165.8(28) 208_464 . 312_455 N
Dg2 DII*1 Dh1 99.0(11) 208_443 . 107_533 N
Dg2 DII*1 Dh1 21.8(11) 208_443 . 208_443 N
Dg2 DII*1 Dh1 163.3(15) 208_443 . 312_434 N
Dg2 DII*1 Dh2 86.8(13) 208_443 . 107_533 N
Dg2 DII*1 Dh2 29.6(11) 208_443 . 208_443 N
Dg2 DII*1 Dh2 148.1(26) 208_443 . 312_434 N
Dg2 DII*1 OII* 111(4) 208_343 . 1_555 N
Dg2 DII*1 DII*1 143.1(32) 208_342 . 2_555 N
Dg2 DII*1 DII*1 84.8(33) 208_342 . 3_555 N
Dg2 DII*1 DII*2 88.1(29) 208_343 . 1_555 N
Oh DII*1 Oh 115.0(22) 107_554 . 208_464 N
Oh DII*1 Oh 90.3(5) 107_554 . 312_455 N
Oh DII*1 Dh1 11.0(5) 107_533 . 107_533 N
Oh DII*1 Dh1 102.0(17) 107_533 . 208_443 N
Oh DII*1 Dh1 106.4(10) 107_533 . 312_434 N
Oh DII*1 Dh2 14.64(35) 107_533 . 107_533 N
Oh DII*1 Dh2 110.0(22) 107_533 . 208_443 N
Oh DII*1 Dh2 92.2(6) 107_533 . 312_434 N
Oh DII*1 OII* 26.5(21) 107_433 . 1_555 N
Oh DII*1 DII*1 55.2(23) 107_432 . 2_555 N
Oh DII*1 DII*1 5.4(23) 107_432 . 3_555 N
Oh DII*1 DII*2 15.7(35) 107_433 . 1_555 N
Oh DII*1 Oh 153.3(22) 208_464 . 312_455 N
Oh DII*1 Dh1 124.3(21) 208_443 . 107_533 N
Oh DII*1 Dh1 17.6(12) 208_443 . 208_443 N
Oh DII*1 Dh1 138.7(15) 208_443 . 312_434 N
Oh DII*1 Dh2 113.1(25) 208_443 . 107_533 N
Oh DII*1 Dh2 24.9(14) 208_443 . 208_443 N
Oh DII*1 Dh2 142.5(32) 208_443 . 312_434 N
Oh DII*1 OII* 138(5) 208_343 . 1_555 N
Oh DII*1 DII*1 169(4) 208_342 . 2_555 N
Oh DII*1 DII*1 110(4) 208_342 . 3_555 N
Oh DII*1 DII*2 112(4) 208_343 . 1_555 N
Oh DII*1 Dh1 81.7(7) 312_434 . 107_533 N
Oh DII*1 Dh1 167.3(16) 312_434 . 208_443 N
Oh DII*1 Dh1 17.8(5) 312_434 . 312_434 N
Oh DII*1 Dh2 88.9(5) 312_434 . 107_533 N
Oh DII*1 Dh2 139.7(29) 312_434 . 208_443 N
Oh DII*1 Dh2 17.7(5) 312_434 . 312_434 N
Oh DII*1 OII* 65.1(27) 312_334 . 1_555 N
Oh DII*1 DII*1 35.3(28) 312_333 . 2_555 N
Oh DII*1 DII*1 95.2(28) 312_333 . 3_555 N
Oh DII*1 DII*2 95.0(23) 312_334 . 1_555 N
Dh1 DII*1 Dh1 110.0(14) 107_533 . 208_443 N
Dh1 DII*1 Dh1 96.9(9) 107_533 . 312_434 N
Dh1 DII*1 Dh2 22.57(23) 107_533 . 107_533 N
Dh1 DII*1 Dh2 120.9(21) 107_533 . 208_443 N
Dh1 DII*1 Dh2 86.1(7) 107_533 . 312_434 N
Dh1 DII*1 OII* 22.4(29) 107_433 . 1_555 N
Dh1 DII*1 DII*1 46.4(24) 107_432 . 2_555 N
Dh1 DII*1 DII*1 14.3(22) 107_432 . 3_555 N
Dh1 DII*1 DII*2 15.5(23) 107_433 . 1_555 N
Dh1 DII*1 Dh1 149.6(14) 208_443 . 312_434 N
Dh1 DII*1 Dh2 103.8(18) 208_443 . 107_533 N
Dh1 DII*1 Dh2 38.3(8) 208_443 . 208_443 N
Dh1 DII*1 Dh2 160.0(26) 208_443 . 312_434 N
Dh1 DII*1 OII* 128(4) 208_343 . 1_555 N
Dh1 DII*1 DII*1 156(4) 208_342 . 2_555 N
Dh1 DII*1 DII*1 97(4) 208_342 . 3_555 N
Dh1 DII*1 DII*2 96.0(31) 208_343 . 1_555 N
Dh1 DII*1 Dh2 106.4(8) 312_434 . 107_533 N
Dh1 DII*1 Dh2 134.4(22) 312_434 . 208_443 N
Dh1 DII*1 Dh2 28.6(5) 312_434 . 312_434 N
Dh1 DII*1 OII* 82.3(32) 312_334 . 1_555 N
Dh1 DII*1 DII*1 51.2(30) 312_333 . 2_555 N
Dh1 DII*1 DII*1 110.9(31) 312_333 . 3_555 N
Dh1 DII*1 DII*2 108.5(31) 312_334 . 1_555 N
Dh2 DII*1 Dh2 102.2(22) 107_533 . 208_443 N
Dh2 DII*1 Dh2 86.5(6) 107_533 . 312_434 N
Dh2 DII*1 OII* 24.4(29) 107_433 . 1_555 N
Dh2 DII*1 DII*1 56.3(22) 107_432 . 2_555 N
Dh2 DII*1 DII*1 17.8(15) 107_432 . 3_555 N
Dh2 DII*1 DII*2 30(4) 107_433 . 1_555 N
Dh2 DII*1 Dh2 123.3(28) 208_443 . 312_434 N
Dh2 DII*1 OII* 124(6) 208_343 . 1_555 N
Dh2 DII*1 DII*1 148.9(20) 208_342 . 2_555 N
Dh2 DII*1 DII*1 107(4) 208_342 . 3_555 N
Dh2 DII*1 DII*2 114(4) 208_343 . 1_555 N
Dh2 DII*1 OII* 65.6(24) 312_334 . 1_555 N
Dh2 DII*1 DII*1 42.4(29) 312_333 . 2_555 N
Dh2 DII*1 DII*1 97.5(26) 312_333 . 3_555 N
Dh2 DII*1 DII*2 101.1(21) 312_334 . 1_555 N
OII* DII*1 DII*1 31.9(17) 1_555 . 2_555 N
OII* DII*1 DII*1 31.9(17) 1_555 . 3_555 N
OII* DII*1 DII*2 37.8(9) 1_555 . 1_555 N
DII*1 DII*1 DII*1 60.0 2_555 . 3_555 N
DII*1 DII*1 DII*2 60.1(14) 2_555 . 1_555 N
DII*1 DII*1 DII*2 13(5) 3_555 . 1_555 N
O1 DII*2 O3 72.3(11) 208_343 . -206_444 N
O1 DII*2 O3 37.6(6) 208_343 . -304_444 N
O1 DII*2 O4 36.2(6) 208_343 . 2_555 N
O1 DII*2 O4 71.0(9) 208_343 . 3_555 N
O1 DII*2 Og 36.1(6) 208_455 . 4_555 N
O1 DII*2 Og 68.5(11) 208_455 . 107_545 N
O1 DII*2 Og 76.9(9) 208_455 . 208_455 N
O1 DII*2 Dg1 56.7(9) 208_464 . 107_554 N
O1 DII*2 Dg2 64.8(10) 208_465 . 107_555 N
O1 DII*2 Oh 45.0(16) 208_464 . 107_554 N
O1 DII*2 Oh 96.8(15) 208_464 . 208_464 N
O1 DII*2 Oh 131.1(17) 208_464 . 312_455 N
O1 DII*2 Dh1 63.5(16) 208_443 . 107_533 N
O1 DII*2 Dh1 89.6(13) 208_443 . 208_443 N
O1 DII*2 Dh1 141.3(15) 208_443 . 312_434 N
O1 DII*2 Dh2 36.4(11) 208_443 . 107_533 N
O1 DII*2 Dh2 84.4(14) 208_443 . 208_443 N
O1 DII*2 Dh2 118.2(16) 208_443 . 312_434 N
O1 DII*2 OII* 111(5) 208_343 . 1_555 N
O1 DII*2 DII*1 120(5) 208_342 . 1_555 N
O1 DII*2 DII*1 125(5) 208_342 . 2_555 N
O1 DII*2 DII*1 34(4) 208_342 . 3_555 N
O1 DII*2 DII*2 133.1(19) 208_343 . 2_555 N
O1 DII*2 DII*2 135.4(20) 208_343 . 3_555 N
O3 DII*2 O3 56.0(9) -206_444 . -304_444 N
O3 DII*2 O4 37.6(6) -206_444 . 2_555 N
O3 DII*2 O4 73.5(8) -206_444 . 3_555 N
O3 DII*2 Og 80.6(12) -206_556 . 4_555 N
O3 DII*2 Og 66.0(10) -206_556 . 107_545 N
O3 DII*2 Og 120.7(12) -206_556 . 208_455 N
O3 DII*2 Dg1 72.2(11) -206_565 . 107_554 N
O3 DII*2 Dg2 52.4(8) -206_566 . 107_555 N
O3 DII*2 Oh 66.9(16) -206_565 . 107_554 N
O3 DII*2 Oh 105.6(11) -206_565 . 208_464 N
O3 DII*2 Oh 58.9(8) -206_565 . 312_455 N
O3 DII*2 Dh1 71.2(14) -206_544 . 107_533 N
O3 DII*2 Dh1 119.5(13) -206_544 . 208_443 N
O3 DII*2 Dh1 70.0(6) -206_544 . 312_434 N
O3 DII*2 Dh2 50.7(11) -206_544 . 107_533 N
O3 DII*2 Dh2 91.1(11) -206_544 . 208_443 N
O3 DII*2 Dh2 47.1(7) -206_544 . 312_434 N
O3 DII*2 OII* 51(4) -206_444 . 1_555 N
O3 DII*2 DII*1 86(4) -206_443 . 1_555 N
O3 DII*2 DII*1 52(4) -206_443 . 2_555 N
O3 DII*2 DII*1 39(5) -206_443 . 3_555 N
O3 DII*2 DII*2 94.2(12) -206_444 . 2_555 N
O3 DII*2 DII*2 63.6(12) -206_444 . 3_555 N
O3 DII*2 O4 40.5(8) -304_444 . 2_555 N
O3 DII*2 O4 37.3(4) -304_444 . 3_555 N
O3 DII*2 Og 71.7(12) -304_556 . 4_555 N
O3 DII*2 Og 93.0(16) -304_556 . 107_545 N
O3 DII*2 Og 68.6(8) -304_556 . 208_455 N
O3 DII*2 Dg1 86.3(15) -304_565 . 107_554 N
O3 DII*2 Dg2 82.9(14) -304_566 . 107_555 N
O3 DII*2 Oh 74.1(22) -304_565 . 107_554 N
O3 DII*2 Oh 71.6(12) -304_565 . 208_464 N
O3 DII*2 Oh 103.9(10) -304_565 . 312_455 N
O3 DII*2 Dh1 91.5(22) -304_544 . 107_533 N
O3 DII*2 Dh1 74.5(11) -304_544 . 208_443 N
O3 DII*2 Dh1 109.9(8) -304_544 . 312_434 N
O3 DII*2 Dh2 56.3(15) -304_544 . 107_533 N
O3 DII*2 Dh2 55.4(10) -304_544 . 208_443 N
O3 DII*2 Dh2 89.9(10) -304_544 . 312_434 N
O3 DII*2 OII* 76(4) -304_444 . 1_555 N
O3 DII*2 DII*1 84(4) -304_443 . 1_555 N
O3 DII*2 DII*1 101(4) -304_443 . 2_555 N
O3 DII*2 DII*1 26(6) -304_443 . 3_555 N
O3 DII*2 DII*2 97.4(15) -304_444 . 2_555 N
O3 DII*2 DII*2 113.01(15) -304_444 . 3_555 N
O4 DII*2 O4 75.8(11) 2_555 . 3_555 N
O4 DII*2 Og 46.9(8) 2_555 . 4_555 N
O4 DII*2 Og 53.4(9) 2_555 . 107_545 N
O4 DII*2 Og 105.8(14) 2_555 . 208_455 N
O4 DII*2 Dg1 50.1(9) 2_555 . 107_554 N
O4 DII*2 Dg2 42.5(7) 2_555 . 107_555 N
O4 DII*2 Oh 39.4(15) 2_555 . 107_554 N
O4 DII*2 Oh 111.7(18) 2_555 . 208_464 N
O4 DII*2 Oh 96.1(13) 2_555 . 312_455 N
O4 DII*2 Dh1 53.5(15) 2_555 . 107_533 N
O4 DII*2 Dh1 114.3(18) 2_555 . 208_443 N
O4 DII*2 Dh1 107.6(11) 2_555 . 312_434 N
O4 DII*2 Dh2 19.3(8) 2_555 . 107_533 N
O4 DII*2 Dh2 95.1(16) 2_555 . 208_443 N
O4 DII*2 Dh2 84.7(11) 2_555 . 312_434 N
O4 DII*2 OII* 85(4) 2_555 . 1_555 N
O4 DII*2 DII*1 113(5) 2_555 . 1_555 N
O4 DII*2 DII*1 89(5) 2_555 . 2_555 N
O4 DII*2 DII*1 15(5) 2_555 . 3_555 N
O4 DII*2 DII*2 124.7(4) 2_555 . 2_555 N
O4 DII*2 DII*2 99.2(18) 2_555 . 3_555 N
O4 DII*2 Og 107.0(15) 3_555 . 4_555 N
O4 DII*2 Og 129.1(19) 3_555 . 107_545 N
O4 DII*2 Og 48.7(4) 3_555 . 208_455 N
O4 DII*2 Dg1 123.6(18) 3_555 . 107_554 N
O4 DII*2 Dg2 117.3(16) 3_555 . 107_555 N
O4 DII*2 Oh 111.4(26) 3_555 . 107_554 N
O4 DII*2 Oh 36.5(8) 3_555 . 208_464 N
O4 DII*2 Oh 90.9(5) 3_555 . 312_455 N
O4 DII*2 Dh1 128.6(25) 3_555 . 107_533 N
O4 DII*2 Dh1 46.2(7) 3_555 . 208_443 N
O4 DII*2 Dh1 90.0(5) 3_555 . 312_434 N
O4 DII*2 Dh2 93.3(18) 3_555 . 107_533 N
O4 DII*2 Dh2 19.7(6) 3_555 . 208_443 N
O4 DII*2 Dh2 80.2(6) 3_555 . 312_434 N
O4 DII*2 OII* 58.5(25) 3_555 . 1_555 N
O4 DII*2 DII*1 49(4) 3_555 . 1_555 N
O4 DII*2 DII*1 92.9(29) 3_555 . 2_555 N
O4 DII*2 DII*1 61(5) 3_555 . 3_555 N
O4 DII*2 DII*2 62.1(21) 3_555 . 2_555 N
O4 DII*2 DII*2 101.8(18) 3_555 . 3_555 N
Og DII*2 Og 38.7(5) 4_555 . 107_545 N
Og DII*2 Og 102.0(10) 4_555 . 208_455 N
Og DII*2 Dg1 24.4(4) 4_555 . 107_554 N
Og DII*2 Dg2 42.4(6) 4_555 . 107_555 N
Og DII*2 Oh 17.7(9) 4_555 . 107_554 N
Og DII*2 Oh 129.4(17) 4_555 . 208_464 N
Og DII*2 Oh 129.0(15) 4_555 . 312_455 N
Og DII*2 Dh1 31.5(11) 4_555 . 107_533 N
Og DII*2 Dh1 116.6(13) 4_555 . 208_443 N
Og DII*2 Dh1 140.3(13) 4_555 . 312_434 N
Og DII*2 Dh2 30.0(7) 4_555 . 107_533 N
Og DII*2 Dh2 119.7(17) 4_555 . 208_443 N
Og DII*2 Dh2 123.7(16) 4_555 . 312_434 N
Og DII*2 OII* 131(5) 4_555 . 1_555 N
Og DII*2 DII*1 155(5) 4_555 . 1_555 N
Og DII*2 DII*1 121(4) 4_555 . 2_555 N
Og DII*2 DII*1 56.2(5) 4_555 . 3_555 N
Og DII*2 DII*2 169.1(14) 4_555 . 2_555 N
Og DII*2 DII*2 124.5(31) 4_555 . 3_555 N
Og DII*2 Og 140.6(13) 107_545 . 208_455 N
Og DII*2 Dg1 14.44(21) 107_554 . 107_554 N
Og DII*2 Dg2 13.66(24) 107_555 . 107_555 N
Og DII*2 Oh 23.7(10) 107_554 . 107_554 N
Og DII*2 Oh 164.4(26) 107_554 . 208_464 N
Og DII*2 Oh 93.2(11) 107_554 . 312_455 N
Og DII*2 Dh1 8.0(8) 107_533 . 107_533 N
Og DII*2 Dh1 155.3(16) 107_533 . 208_443 N
Og DII*2 Dh1 103.1(10) 107_533 . 312_434 N
Og DII*2 Dh2 36.9(8) 107_533 . 107_533 N
Og DII*2 Dh2 148.3(24) 107_533 . 208_443 N
Og DII*2 Dh2 93.0(11) 107_533 . 312_434 N
Og DII*2 OII* 110.4(32) 107_433 . 1_555 N
Og DII*2 DII*1 147.7(29) 107_432 . 1_555 N
Og DII*2 DII*1 85.9(30) 107_432 . 2_555 N
Og DII*2 DII*1 68(4) 107_432 . 3_555 N
Og DII*2 DII*2 146.6(29) 107_433 . 2_555 N
Og DII*2 DII*2 86.7(29) 107_433 . 3_555 N
Og DII*2 Dg1 126.2(11) 208_464 . 107_554 N
Og DII*2 Dg2 141.4(17) 208_465 . 107_555 N
Og DII*2 Oh 118.2(20) 208_464 . 107_554 N
Og DII*2 Oh 31.3(7) 208_464 . 208_464 N
Og DII*2 Oh 124.3(12) 208_464 . 312_455 N
Og DII*2 Dh1 133.0(17) 208_443 . 107_533 N
Og DII*2 Dh1 14.7(6) 208_443 . 208_443 N
Og DII*2 Dh1 115.7(13) 208_443 . 312_434 N
Og DII*2 Dh2 113.2(19) 208_443 . 107_533 N
Og DII*2 Dh2 35.9(7) 208_443 . 208_443 N
Og DII*2 Dh2 120.3(9) 208_443 . 312_434 N
Og DII*2 OII* 98.7(22) 208_343 . 1_555 N
Og DII*2 DII*1 67.3(25) 208_342 . 1_555 N
Og DII*2 DII*1 130.5(26) 208_342 . 2_555 N
Og DII*2 DII*1 93(7) 208_342 . 3_555 N
Og DII*2 DII*2 72.3(32) 208_343 . 2_555 N
Og DII*2 DII*2 132.2(31) 208_343 . 3_555 N
Dg1 DII*2 Dg2 22.21(31) 107_555 . 107_555 N
Dg1 DII*2 Oh 12.3(11) 107_554 . 107_554 N
Dg1 DII*2 Oh 153.2(21) 107_554 . 208_464 N
Dg1 DII*2 Oh 107.3(12) 107_554 . 312_455 N
Dg1 DII*2 Dh1 7.2(9) 107_533 . 107_533 N
Dg1 DII*2 Dh1 140.9(14) 107_533 . 208_443 N
Dg1 DII*2 Dh1 117.5(11) 107_533 . 312_434 N
Dg1 DII*2 Dh2 31.1(8) 107_533 . 107_533 N
Dg1 DII*2 Dh2 140.5(22) 107_533 . 208_443 N
Dg1 DII*2 Dh2 105.8(13) 107_533 . 312_434 N
Dg1 DII*2 OII* 121(4) 107_433 . 1_555 N
Dg1 DII*2 DII*1 158(4) 107_432 . 1_555 N
Dg1 DII*2 DII*1 99.7(33) 107_432 . 2_555 N
Dg1 DII*2 DII*1 63.7(30) 107_432 . 3_555 N
Dg1 DII*2 DII*2 160.7(30) 107_433 . 2_555 N
Dg1 DII*2 DII*2 101.1(30) 107_433 . 3_555 N
Dg2 DII*2 Oh 24.8(10) 107_554 . 107_554 N
Dg2 DII*2 Oh 153.7(23) 107_554 . 208_464 N
Dg2 DII*2 Oh 86.7(11) 107_554 . 312_455 N
Dg2 DII*2 Dh1 19.1(8) 107_533 . 107_533 N
Dg2 DII*2 Dh1 154.3(22) 107_533 . 208_443 N
Dg2 DII*2 Dh1 97.9(9) 107_533 . 312_434 N
Dg2 DII*2 Dh2 29.3(9) 107_533 . 107_533 N
Dg2 DII*2 Dh2 136.9(21) 107_533 . 208_443 N
Dg2 DII*2 Dh2 83.8(10) 107_533 . 312_434 N
Dg2 DII*2 OII* 98.8(34) 107_433 . 1_555 N
Dg2 DII*2 DII*1 136.6(34) 107_432 . 1_555 N
Dg2 DII*2 DII*1 78.9(33) 107_432 . 2_555 N
Dg2 DII*2 DII*1 57(5) 107_432 . 3_555 N
Dg2 DII*2 DII*2 139.3(26) 107_433 . 2_555 N
Dg2 DII*2 DII*2 82.3(27) 107_433 . 3_555 N
Oh DII*2 Oh 141.8(29) 107_554 . 208_464 N
Oh DII*2 Oh 111.2(15) 107_554 . 312_455 N
Oh DII*2 Dh1 18.6(9) 107_533 . 107_533 N
Oh DII*2 Dh1 132.5(22) 107_533 . 208_443 N
Oh DII*2 Dh1 122.6(15) 107_533 . 312_434 N
Oh DII*2 Dh2 20.1(10) 107_533 . 107_533 N
Oh DII*2 Dh2 128.2(29) 107_533 . 208_443 N
Oh DII*2 Dh2 106.7(17) 107_533 . 312_434 N
Oh DII*2 OII* 118(5) 107_433 . 1_555 N
Oh DII*2 DII*1 152(6) 107_432 . 1_555 N
Oh DII*2 DII*1 103(4) 107_432 . 2_555 N
Oh DII*2 DII*1 52.3(24) 107_432 . 3_555 N
Oh DII*2 DII*2 161.0(26) 107_433 . 2_555 N
Oh DII*2 DII*2 107.0(33) 107_433 . 3_555 N
Oh DII*2 Oh 93.0(9) 208_464 . 312_455 N
Oh DII*2 Dh1 160.2(28) 208_443 . 107_533 N
Oh DII*2 Dh1 18.4(5) 208_443 . 208_443 N
Oh DII*2 Dh1 85.1(11) 208_443 . 312_434 N
Oh DII*2 Dh2 127.6(25) 208_443 . 107_533 N
Oh DII*2 Dh2 16.8(5) 208_443 . 208_443 N
Oh DII*2 Dh2 89.6(7) 208_443 . 312_434 N
Oh DII*2 OII* 69.1(21) 208_343 . 1_555 N
Oh DII*2 DII*1 36.0(23) 208_342 . 1_555 N
Oh DII*2 DII*1 99.2(24) 208_342 . 2_555 N
Oh DII*2 DII*1 97(6) 208_342 . 3_555 N
Oh DII*2 DII*2 42.6(30) 208_343 . 2_555 N
Oh DII*2 DII*2 101.4(28) 208_343 . 3_555 N
Oh DII*2 Dh1 101.2(13) 312_434 . 107_533 N
Oh DII*2 Dh1 110.3(12) 312_434 . 208_443 N
Oh DII*2 Dh1 12.1(5) 312_434 . 312_434 N
Oh DII*2 Dh2 104.2(15) 312_434 . 107_533 N
Oh DII*2 Dh2 92.7(6) 312_434 . 208_443 N
Oh DII*2 Dh2 14.06(34) 312_434 . 312_434 N
Oh DII*2 OII* 32.6(25) 312_334 . 1_555 N
Oh DII*2 DII*1 57.0(21) 312_333 . 1_555 N
Oh DII*2 DII*1 8.1(29) 312_333 . 2_555 N
Oh DII*2 DII*1 97(4) 312_333 . 3_555 N
Oh DII*2 DII*2 53.5(20) 312_334 . 2_555 N
Oh DII*2 DII*2 10.9(17) 312_334 . 3_555 N
Dh1 DII*2 Dh1 147.7(16) 107_533 . 208_443 N
Dh1 DII*2 Dh1 111.0(10) 107_533 . 312_434 N
Dh1 DII*2 Dh2 35.4(8) 107_533 . 107_533 N
Dh1 DII*2 Dh2 146.5(29) 107_533 . 208_443 N
Dh1 DII*2 Dh2 100.9(14) 107_533 . 312_434 N
Dh1 DII*2 OII* 118(4) 107_433 . 1_555 N
Dh1 DII*2 DII*1 155.2(35) 107_432 . 1_555 N
Dh1 DII*2 DII*1 93.9(32) 107_432 . 2_555 N
Dh1 DII*2 DII*1 67.7(35) 107_432 . 3_555 N
Dh1 DII*2 DII*2 154.5(31) 107_433 . 2_555 N
Dh1 DII*2 DII*2 94.5(31) 107_433 . 3_555 N
Dh1 DII*2 Dh1 101.2(12) 208_443 . 312_434 N
Dh1 DII*2 Dh2 125.1(23) 208_443 . 107_533 N
Dh1 DII*2 Dh2 28.8(4) 208_443 . 208_443 N
Dh1 DII*2 Dh2 107.9(9) 208_443 . 312_434 N
Dh1 DII*2 OII* 87.5(23) 208_343 . 1_555 N
Dh1 DII*2 DII*1 53.6(25) 208_342 . 1_555 N
Dh1 DII*2 DII*1 117.0(28) 208_342 . 2_555 N
Dh1 DII*2 DII*1 101(7) 208_342 . 3_555 N
Dh1 DII*2 DII*2 57.7(31) 208_343 . 2_555 N
Dh1 DII*2 DII*2 117.7(31) 208_343 . 3_555 N
Dh1 DII*2 Dh2 116.3(14) 312_434 . 107_533 N
Dh1 DII*2 Dh2 87.8(9) 312_434 . 208_443 N
Dh1 DII*2 Dh2 23.21(22) 312_434 . 312_434 N
Dh1 DII*2 OII* 34.7(33) 312_334 . 1_555 N
Dh1 DII*2 DII*1 49.4(26) 312_333 . 1_555 N
Dh1 DII*2 DII*1 20.2(33) 312_333 . 2_555 N
Dh1 DII*2 DII*1 107(4) 312_333 . 3_555 N
Dh1 DII*2 DII*2 43.5(22) 312_334 . 2_555 N
Dh1 DII*2 DII*2 16.5(22) 312_334 . 3_555 N
Dh2 DII*2 Dh2 111.7(23) 107_533 . 208_443 N
Dh2 DII*2 Dh2 95.7(15) 107_533 . 312_434 N
Dh2 DII*2 OII* 101(5) 107_433 . 1_555 N
Dh2 DII*2 DII*1 132(5) 107_432 . 1_555 N
Dh2 DII*2 DII*1 96(5) 107_432 . 2_555 N
Dh2 DII*2 DII*1 32.6(30) 107_432 . 3_555 N
Dh2 DII*2 DII*2 143.2(13) 107_433 . 2_555 N
Dh2 DII*2 DII*2 103.8(28) 107_433 . 3_555 N
Dh2 DII*2 Dh2 85.6(5) 208_443 . 312_434 N
Dh2 DII*2 OII* 63.4(19) 208_343 . 1_555 N
Dh2 DII*2 DII*1 39.6(30) 208_342 . 1_555 N
Dh2 DII*2 DII*1 97.2(23) 208_342 . 2_555 N
Dh2 DII*2 DII*1 81(6) 208_342 . 3_555 N
Dh2 DII*2 DII*2 50.4(28) 208_343 . 2_555 N
Dh2 DII*2 DII*2 102.8(25) 208_343 . 3_555 N
Dh2 DII*2 OII* 22.3(19) 312_334 . 1_555 N
Dh2 DII*2 DII*1 55.0(19) 312_333 . 1_555 N
Dh2 DII*2 DII*1 12.8(28) 312_333 . 2_555 N
Dh2 DII*2 DII*1 84(4) 312_333 . 3_555 N
Dh2 DII*2 DII*2 55.5(18) 312_334 . 2_555 N
Dh2 DII*2 DII*2 23.7(14) 312_334 . 3_555 N
OII* DII*2 DII*1 37.7(5) 1_555 . 1_555 N
OII* DII*2 DII*1 34.6(25) 1_555 . 2_555 N
OII* DII*2 DII*1 79(4) 1_555 . 3_555 N
OII* DII*2 DII*2 43.5(31) 1_555 . 2_555 N
OII* DII*2 DII*2 43.5(31) 1_555 . 3_555 N
DII*1 DII*2 DII*1 63.4(7) 1_555 . 2_555 N
DII*1 DII*2 DII*1 101(5) 1_555 . 3_555 N
DII*1 DII*2 DII*2 14(5) 1_555 . 2_555 N
DII*1 DII*2 DII*2 65.5(26) 1_555 . 3_555 N
DII*1 DII*2 DII*1 91(6) 2_555 . 3_555 N
DII*1 DII*2 DII*2 61.0(16) 2_555 . 2_555 N
DII*1 DII*2 DII*2 12(5) 2_555 . 3_555 N
DII*1 DII*2 DII*2 114.1(10) 3_555 . 2_555 N
DII*1 DII*2 DII*2 103(5) 3_555 . 3_555 N
DII*2 DII*2 DII*2 60.0000(6) 2_555 . 3_555 N
O1 Oi O1 44.63(25) 2_555 . -3_555 N
O1 Oi O1 94.9(6) 2_555 . 111_433 N
O1 Oi O1 74.2(5) 2_555 . -108_544 N
O1 Oi O2 66.0(4) 2_555 . 1_555 N
O1 Oi O3 116.3(6) 2_555 . 4_555 N
O1 Oi O4 32.53(23) 2_555 . 310_334 N
O1 Oi O4 61.0(4) 2_555 . 312_334 N
O1 Oi O4 106.9(5) 2_555 . -302_444 N
O1 Oi O4 135.1(6) 2_555 . -303_444 N
O1 Oi Og 76.6(4) 2_555 . 1_555 N
O1 Oi Og 32.57(34) 2_555 . -3_555 N
O1 Oi Og 104.0(7) 2_555 . -108_656 N
O1 Oi Og 94.9(5) 2_555 . -207_566 N
O1 Oi Og 63.2(4) 2_555 . -304_556 N
O1 Oi Dg1 84.1(5) 2_555 . 1_555 N
O1 Oi Dg1 39.92(34) 2_555 . -3_555 N
O1 Oi Dg1 113.1(7) 2_555 . -108_665 N
O1 Oi Dg1 83.7(5) 2_555 . -207_575 N
O1 Oi Dg1 53.6(5) 2_555 . -304_565 N
O1 Oi Dg2 19.10(26) 2_555 . -3_555 N
O1 Oi Dg2 102.8(8) 2_555 . -108_666 N
O1 Oi Dg2 63.7(5) 2_555 . -304_566 N
O1 Oi Oh 47.0(4) 2_555 . -3_555 N
O1 Oi Oh 70.1(5) 2_555 . 105_544 N
O1 Oi O1 71.4(4) -3_555 . 111_433 N
O1 Oi O1 97.7(6) -3_555 . -108_544 N
O1 Oi O2 65.64(35) -3_555 . 1_555 N
O1 Oi O3 115.2(6) -3_555 . 4_555 N
O1 Oi O4 60.5(4) -3_555 . 310_334 N
O1 Oi O4 34.25(22) -3_555 . 312_334 N
O1 Oi O4 137.4(6) -3_555 . -302_444 N
O1 Oi O4 104.4(5) -3_555 . -303_444 N
O1 Oi Og 32.42(23) -3_555 . 1_555 N
O1 Oi Og 73.6(5) -3_555 . -3_555 N
O1 Oi Og 60.0(5) -3_555 . -108_656 N
O1 Oi Og 138.9(6) -3_555 . -207_566 N
O1 Oi Og 106.7(6) -3_555 . -304_556 N
O1 Oi Dg1 39.72(33) -3_555 . 1_555 N
O1 Oi Dg1 80.2(5) -3_555 . -3_555 N
O1 Oi Dg1 68.7(5) -3_555 . -108_665 N
O1 Oi Dg1 128.3(6) -3_555 . -207_575 N
O1 Oi Dg1 98.3(7) -3_555 . -304_565 N
O1 Oi Dg2 61.1(4) -3_555 . -3_555 N
O1 Oi Dg2 63.8(6) -3_555 . -108_666 N
O1 Oi Dg2 103.4(7) -3_555 . -304_566 N
O1 Oi Oh 70.5(5) -3_555 . -3_555 N
O1 Oi Oh 42.0(4) -3_555 . 105_544 N
O1 Oi O1 64.7(4) 111_433 . -108_544 N
O1 Oi O2 35.94(26) 111_433 . 1_555 N
O1 Oi O3 46.32(31) 111_433 . 4_555 N
O1 Oi O4 74.0(5) 111_433 . 310_334 N
O1 Oi O4 38.35(27) 111_433 . 312_334 N
O1 Oi O4 83.6(5) 111_433 . -302_444 N
O1 Oi O4 40.25(29) 111_433 . -303_444 N
O1 Oi Og 65.5(4) 111_545 . 1_555 N
O1 Oi Og 124.1(8) 111_545 . -3_555 N
O1 Oi Og 47.9(4) 111_545 . -108_656 N
O1 Oi Og 130.3(6) 111_545 . -207_566 N
O1 Oi Og 109.1(6) 111_545 . -304_556 N
O1 Oi Dg1 62.8(5) 111_554 . 1_555 N
O1 Oi Dg1 130.6(7) 111_554 . -3_555 N
O1 Oi Dg1 51.8(4) 111_554 . -108_665 N
O1 Oi Dg1 126.4(7) 111_554 . -207_575 N
O1 Oi Dg1 118.2(8) 111_554 . -304_565 N
O1 Oi Dg2 112.4(7) 111_555 . -3_555 N
O1 Oi Dg2 28.90(33) 111_555 . -108_666 N
O1 Oi Dg2 94.8(6) 111_555 . -304_566 N
O1 Oi Oh 139.4(8) 111_554 . -3_555 N
O1 Oi Oh 99.0(6) 111_554 . 105_544 N
O1 Oi O2 38.45(29) -108_544 . 1_555 N
O1 Oi O3 46.01(32) -108_544 . 4_555 N
O1 Oi O4 42.69(32) -108_544 . 310_334 N
O1 Oi O4 74.4(5) -108_544 . 312_334 N
O1 Oi O4 39.68(29) -108_544 . -302_444 N
O1 Oi O4 81.6(5) -108_544 . -303_444 N
O1 Oi Og 118.6(6) -108_656 . 1_555 N
O1 Oi Og 78.7(5) -108_656 . -3_555 N
O1 Oi Og 112.4(8) -108_656 . -108_656 N
O1 Oi Og 71.5(4) -108_656 . -207_566 N
O1 Oi Og 44.9(4) -108_656 . -304_556 N
O1 Oi Dg1 120.5(7) -108_665 . 1_555 N
O1 Oi Dg1 80.7(6) -108_665 . -3_555 N
O1 Oi Dg1 116.3(7) -108_665 . -108_665 N
O1 Oi Dg1 63.5(5) -108_665 . -207_575 N
O1 Oi Dg1 56.6(5) -108_665 . -304_565 N
O1 Oi Dg2 76.8(5) -108_666 . -3_555 N
O1 Oi Dg2 93.6(7) -108_666 . -108_666 N
O1 Oi Dg2 30.67(32) -108_666 . -304_566 N
O1 Oi Oh 107.5(7) -108_665 . -3_555 N
O1 Oi Oh 139.2(8) -108_665 . 105_544 N
O2 Oi O3 54.36(33) 1_555 . 4_555 N
O2 Oi O4 38.88(24) 1_555 . 310_334 N
O2 Oi O4 36.48(22) 1_555 . 312_334 N
O2 Oi O4 73.8(4) 1_555 . -302_444 N
O2 Oi O4 71.5(4) 1_555 . -303_444 N
O2 Oi Og 80.4(4) 1_555 . 1_555 N
O2 Oi Og 89.9(6) 1_555 . -3_555 N
O2 Oi Og 77.9(6) 1_555 . -108_656 N
O2 Oi Og 109.6(5) 1_555 . -207_566 N
O2 Oi Og 77.0(5) 1_555 . -304_556 N
O2 Oi Dg1 82.0(5) 1_555 . 1_555 N
O2 Oi Dg1 95.6(6) 1_555 . -3_555 N
O2 Oi Dg1 84.5(5) 1_555 . -108_665 N
O2 Oi Dg1 100.3(5) 1_555 . -207_575 N
O2 Oi Dg1 83.4(6) 1_555 . -304_565 N
O2 Oi Dg2 80.1(5) 1_555 . -3_555 N
O2 Oi Dg2 61.2(5) 1_555 . -108_666 N
O2 Oi Dg2 63.5(5) 1_555 . -304_566 N
O2 Oi Oh 112.7(7) 1_555 . -3_555 N
O2 Oi Oh 106.7(6) 1_555 . 105_544 N
O3 Oi O4 84.0(5) 4_555 . 310_334 N
O3 Oi O4 81.0(5) 4_555 . 312_334 N
O3 Oi O4 39.81(26) 4_555 . -302_444 N
O3 Oi O4 37.75(26) 4_555 . -303_444 N
O3 Oi Og 110.4(6) 4_555 . 1_555 N
O3 Oi Og 124.1(7) 4_555 . -3_555 N
O3 Oi Og 84.5(6) 4_555 . -108_656 N
O3 Oi Og 86.2(5) 4_555 . -207_566 N
O3 Oi Og 82.8(5) 4_555 . -304_556 N
O3 Oi Dg1 106.0(7) 4_555 . 1_555 N
O3 Oi Dg1 124.6(7) 4_555 . -3_555 N
O3 Oi Dg1 82.8(6) 4_555 . -108_665 N
O3 Oi Dg1 86.7(6) 4_555 . -207_575 N
O3 Oi Dg1 97.1(6) 4_555 . -304_565 N
O3 Oi Dg2 122.7(7) 4_555 . -3_555 N
O3 Oi Dg2 67.6(6) 4_555 . -108_666 N
O3 Oi Dg2 71.3(5) 4_555 . -304_566 N
O3 Oi Oh 152.2(7) 4_555 . -3_555 N
O3 Oi Oh 143.5(7) 4_555 . 105_544 N
O4 Oi O4 54.34(34) 310_334 . 312_334 N
O4 Oi O4 79.9(4) 310_334 . -302_444 N
O4 Oi O4 110.0(6) 310_334 . -303_444 N
O4 Oi Og 90.5(5) 310_446 . 1_555 N
O4 Oi Og 51.0(4) 310_446 . -3_555 N
O4 Oi Og 105.7(7) 310_446 . -108_656 N
O4 Oi Og 89.7(5) 310_446 . -207_566 N
O4 Oi Og 51.4(4) 310_446 . -304_556 N
O4 Oi Dg1 96.3(6) 310_455 . 1_555 N
O4 Oi Dg1 56.9(4) 310_455 . -3_555 N
O4 Oi Dg1 114.5(7) 310_455 . -108_665 N
O4 Oi Dg1 77.5(5) 310_455 . -207_575 N
O4 Oi Dg1 50.8(5) 310_455 . -304_565 N
O4 Oi Dg2 42.0(4) 310_456 . -3_555 N
O4 Oi Dg2 94.3(7) 310_456 . -108_666 N
O4 Oi Dg2 43.7(4) 310_456 . -304_566 N
O4 Oi Oh 75.6(5) 310_455 . -3_555 N
O4 Oi Oh 98.0(6) 310_455 . 105_544 N
O4 Oi O4 109.6(5) 312_334 . -302_444 N
O4 Oi O4 76.4(4) 312_334 . -303_444 N
O4 Oi Og 44.20(27) 312_446 . 1_555 N
O4 Oi Og 93.4(6) 312_446 . -3_555 N
O4 Oi Og 51.4(5) 312_446 . -108_656 N
O4 Oi Og 142.7(6) 312_446 . -207_566 N
O4 Oi Og 105.0(6) 312_446 . -304_556 N
O4 Oi Dg1 46.9(4) 312_455 . 1_555 N
O4 Oi Dg1 100.8(6) 312_455 . -3_555 N
O4 Oi Dg1 60.3(4) 312_455 . -108_665 N
O4 Oi Dg1 131.2(7) 312_455 . -207_575 N
O4 Oi Dg1 104.8(7) 312_455 . -304_565 N
O4 Oi Dg2 80.1(5) 312_456 . -3_555 N
O4 Oi Dg2 42.8(5) 312_456 . -108_666 N
O4 Oi Dg2 94.3(6) 312_456 . -304_566 N
O4 Oi Oh 101.4(6) 312_455 . -3_555 N
O4 Oi Oh 71.3(5) 312_455 . 105_544 N
O4 Oi O4 73.2(4) -302_444 . -303_444 N
O4 Oi Og 149.2(6) -302_556 . 1_555 N
O4 Oi Og 94.4(5) -302_556 . -3_555 N
O4 Oi Og 123.9(8) -302_556 . -108_656 N
O4 Oi Og 46.96(31) -302_556 . -207_566 N
O4 Oi Og 49.6(4) -302_556 . -304_556 N
O4 Oi Dg1 145.7(7) -302_565 . 1_555 N
O4 Oi Dg1 91.6(5) -302_565 . -3_555 N
O4 Oi Dg1 120.7(7) -302_565 . -108_665 N
O4 Oi Dg1 47.0(4) -302_565 . -207_575 N
O4 Oi Dg1 63.7(5) -302_565 . -304_565 N
O4 Oi Dg2 100.4(5) -302_566 . -3_555 N
O4 Oi Dg2 107.4(7) -302_566 . -108_666 N
O4 Oi Dg2 43.9(4) -302_566 . -304_566 N
O4 Oi Oh 116.6(6) -302_565 . -3_555 N
O4 Oi Oh 176.1(7) -302_565 . 105_544 N
O4 Oi Og 82.9(4) -303_556 . 1_555 N
O4 Oi Og 159.8(7) -303_556 . -3_555 N
O4 Oi Og 52.1(5) -303_556 . -108_656 N
O4 Oi Og 112.7(6) -303_556 . -207_566 N
O4 Oi Og 120.3(6) -303_556 . -304_556 N
O4 Oi Dg1 76.3(5) -303_565 . 1_555 N
O4 Oi Dg1 162.2(7) -303_565 . -3_555 N
O4 Oi Dg1 47.5(5) -303_565 . -108_665 N
O4 Oi Dg1 118.2(6) -303_565 . -207_575 N
O4 Oi Dg1 134.7(7) -303_565 . -304_565 N
O4 Oi Dg2 151.6(7) -303_566 . -3_555 N
O4 Oi Dg2 41.1(5) -303_566 . -108_666 N
O4 Oi Dg2 109.0(7) -303_566 . -304_566 N
O4 Oi Oh 169.9(6) -303_565 . -3_555 N
O4 Oi Oh 110.6(6) -303_565 . 105_544 N
Og Oi Og 102.2(7) 1_555 . -3_555 N
Og Oi Og 31.5(4) 1_555 . -108_656 N
Og Oi Og 163.3(6) 1_555 . -207_566 N
Og Oi Og 139.1(7) 1_555 . -304_556 N
Og Oi Dg1 7.65(20) 1_555 . 1_555 N
Og Oi Dg1 107.6(6) 1_555 . -3_555 N
Og Oi Dg1 38.6(4) 1_555 . -108_665 N
Og Oi Dg1 158.1(7) 1_555 . -207_575 N
Og Oi Dg1 130.0(8) 1_555 . -304_565 N
Og Oi Dg2 91.3(6) 1_555 . -3_555 N
Og Oi Dg2 43.7(4) 1_555 . -108_666 N
Og Oi Dg2 134.2(8) 1_555 . -304_566 N
Og Oi Oh 88.7(5) 1_555 . -3_555 N
Og Oi Oh 33.5(4) 1_555 . 105_544 N
Og Oi Og 133.1(9) -3_555 . -108_656 N
Og Oi Og 65.4(5) -3_555 . -207_566 N
Og Oi Og 44.9(4) -3_555 . -304_556 N
Og Oi Dg1 109.7(7) -3_555 . 1_555 N
Og Oi Dg1 7.36(27) -3_555 . -3_555 N
Og Oi Dg1 140.8(9) -3_555 . -108_665 N
Og Oi Dg1 56.1(5) -3_555 . -207_575 N
Og Oi Dg1 30.8(4) -3_555 . -304_565 N
Og Oi Dg2 13.48(20) -3_555 . -3_555 N
Og Oi Dg2 135.3(10) -3_555 . -108_666 N
Og Oi Dg2 53.6(4) -3_555 . -304_566 N
Og Oi Oh 28.7(4) -3_555 . -3_555 N
Og Oi Oh 81.8(6) -3_555 . 105_544 N
Og Oi Og 161.1(9) -108_656 . -207_566 N
Og Oi Og 154.8(9) -108_656 . -304_556 N
Og Oi Dg1 24.4(4) -108_665 . 1_555 N
Og Oi Dg1 138.9(9) -108_665 . -3_555 N
Og Oi Dg1 9.4(4) -108_665 . -108_665 N
Og Oi Dg1 170.3(10) -108_665 . -207_575 N
Og Oi Dg1 155.8(10) -108_665 . -304_565 N
Og Oi Dg2 121.1(9) -108_666 . -3_555 N
Og Oi Dg2 19.13(19) -108_666 . -108_666 N
Og Oi Dg2 141.4(10) -108_666 . -304_566 N
Og Oi Oh 118.8(8) -108_665 . -3_555 N
Og Oi Oh 59.7(6) -108_665 . 105_544 N
Og Oi Og 38.30(33) -207_566 . -304_556 N
Og Oi Dg1 166.9(7) -207_575 . 1_555 N
Og Oi Dg1 59.1(4) -207_575 . -3_555 N
Og Oi Dg1 152.0(8) -207_575 . -108_665 N
Og Oi Dg1 12.26(12) -207_575 . -207_575 N
Og Oi Dg1 42.2(4) -207_575 . -304_565 N
Og Oi Dg2 77.8(5) -207_576 . -3_555 N
Og Oi Dg2 152.9(9) -207_576 . -108_666 N
Og Oi Dg2 48.4(4) -207_576 . -304_566 N
Og Oi Oh 75.2(5) -207_575 . -3_555 N
Og Oi Oh 130.1(6) -207_575 . 105_544 N
Og Oi Dg1 146.2(8) -304_565 . 1_555 N
Og Oi Dg1 42.8(5) -304_565 . -3_555 N
Og Oi Dg1 160.9(8) -304_565 . -108_665 N
Og Oi Dg1 26.24(32) -304_565 . -207_575 N
Og Oi Dg1 14.50(14) -304_565 . -304_565 N
Og Oi Dg2 51.7(4) -304_566 . -3_555 N
Og Oi Dg2 137.6(9) -304_566 . -108_666 N
Og Oi Dg2 14.29(15) -304_566 . -304_566 N
Og Oi Oh 69.8(5) -304_565 . -3_555 N
Og Oi Oh 126.6(8) -304_565 . 105_544 N
Dg1 Oi Dg1 115.0(7) 1_555 . -3_555 N
Dg1 Oi Dg1 31.1(4) 1_555 . -108_665 N
Dg1 Oi Dg1 165.4(8) 1_555 . -207_575 N
Dg1 Oi Dg1 137.6(9) 1_555 . -304_565 N
Dg1 Oi Dg2 98.9(7) 1_555 . -3_555 N
Dg1 Oi Dg2 38.5(5) 1_555 . -108_666 N
Dg1 Oi Dg2 139.7(8) 1_555 . -304_566 N
Dg1 Oi Oh 94.9(6) 1_555 . -3_555 N
Dg1 Oi Oh 37.5(5) 1_555 . 105_544 N
Dg1 Oi Dg1 145.9(7) -3_555 . -108_665 N
Dg1 Oi Dg1 50.6(6) -3_555 . -207_575 N
Dg1 Oi Dg1 28.3(4) -3_555 . -304_565 N
Dg1 Oi Dg2 20.83(17) -3_555 . -3_555 N
Dg1 Oi Dg2 142.6(10) -3_555 . -108_666 N
Dg1 Oi Dg2 53.3(6) -3_555 . -304_566 N
Dg1 Oi Oh 27.6(4) -3_555 . -3_555 N
Dg1 Oi Oh 84.5(6) -3_555 . 105_544 N
Dg1 Oi Dg1 162.9(9) -108_665 . -207_575 N
Dg1 Oi Dg1 165.1(9) -108_665 . -304_565 N
Dg1 Oi Dg2 129.5(8) -108_666 . -3_555 N
Dg1 Oi Dg2 23.42(31) -108_666 . -108_666 N
Dg1 Oi Dg2 146.7(9) -108_666 . -304_566 N
Dg1 Oi Oh 122.7(7) -108_665 . -3_555 N
Dg1 Oi Oh 63.1(6) -108_665 . 105_544 N
Dg1 Oi Dg1 30.3(5) -207_575 . -304_565 N
Dg1 Oi Dg2 67.6(5) -207_576 . -3_555 N
Dg1 Oi Dg2 153.9(9) -207_576 . -108_666 N
Dg1 Oi Dg2 37.4(4) -207_576 . -304_566 N
Dg1 Oi Oh 70.8(5) -207_575 . -3_555 N
Dg1 Oi Oh 129.5(7) -207_575 . 105_544 N
Dg1 Oi Dg2 39.2(5) -304_566 . -3_555 N
Dg1 Oi Dg2 144.2(11) -304_566 . -108_666 N
Dg1 Oi Dg2 26.47(21) -304_566 . -304_566 N
Dg1 Oi Oh 55.4(5) -304_565 . -3_555 N
Dg1 Oi Oh 112.5(7) -304_565 . 105_544 N
Dg2 Oi Dg2 121.8(9) -3_555 . -108_666 N
Dg2 Oi Dg2 57.0(5) -3_555 . -304_566 N
Dg2 Oi Oh 33.7(4) -3_555 . -3_555 N
Dg2 Oi Oh 76.0(6) -3_555 . 105_544 N
Dg2 Oi Dg2 123.4(9) -108_666 . -304_566 N
Dg2 Oi Oh 131.7(9) -108_665 . -3_555 N
Dg2 Oi Oh 75.9(6) -108_665 . 105_544 N
Dg2 Oi Oh 80.9(6) -304_565 . -3_555 N
Dg2 Oi Oh 132.7(9) -304_565 . 105_544 N
Oh Oi Oh 59.6(6) -3_555 . 105_544 N
O1 Di1 O1 58.8(5) 111_433 . -108_544 N
O1 Di1 O3 42.00(32) 111_433 . 4_555 N
O1 Di1 O4 65.4(5) 111_433 . 310_334 N
O1 Di1 O4 84.6(7) 111_433 . -302_444 N
O1 Di1 O4 37.36(26) 111_433 . -303_444 N
O1 Di1 Og 108.4(8) 111_545 . -3_555 N
O1 Di1 Og 39.74(31) 111_545 . -108_656 N
O1 Di1 Og 141.9(12) 111_545 . -207_566 N
O1 Di1 Og 106.4(10) 111_545 . -304_556 N
O1 Di1 Dg1 133.4(12) 111_554 . -207_575 N
O1 Di1 Dg1 111.7(11) 111_554 . -304_565 N
O1 Di1 Dg2 24.80(26) 111_555 . -108_666 N
O1 Di1 Dg2 129.9(10) 111_555 . -207_576 N
O1 Di1 Dg2 89.5(9) 111_555 . -304_566 N
O1 Di1 Oh 119.1(6) 111_554 . -3_555 N
O1 Di1 Oh 58.5(6) 111_554 . -108_665 N
O1 Di1 Oh 132.3(20) 111_554 . -207_575 N
O1 Di1 Dh1 118.6(8) 111_533 . -3_555 N
O1 Di1 Dh1 52.5(6) 111_533 . -108_644 N
O1 Di1 Dh1 146.2(16) 111_533 . -207_554 N
O1 Di1 Dh2 47.1(6) 111_533 . -108_644 N
O1 Di1 Dh2 105.5(14) 111_533 . -207_554 N
O1 Di1 OII* 96.8(10) 111_433 . -301_444 N
O1 Di1 DII*1 84.9(16) 111_432 . -301_443 N
O1 Di1 O3 47.8(5) -108_544 . 4_555 N
O1 Di1 O4 39.3(4) -108_544 . 310_334 N
O1 Di1 O4 46.3(6) -108_544 . -302_444 N
O1 Di1 O4 79.9(6) -108_544 . -303_444 N
O1 Di1 Og 79.9(9) -108_656 . -3_555 N
O1 Di1 Og 96.9(7) -108_656 . -108_656 N
O1 Di1 Og 86.2(9) -108_656 . -207_566 N
O1 Di1 Og 49.7(7) -108_656 . -304_556 N
O1 Di1 Dg1 74.9(9) -108_665 . -207_575 N
O1 Di1 Dg1 61.3(8) -108_665 . -304_565 N
O1 Di1 Dg2 82.9(7) -108_666 . -108_666 N
O1 Di1 Dg2 78.6(9) -108_666 . -207_576 N
O1 Di1 Dg2 32.7(5) -108_666 . -304_566 N
O1 Di1 Oh 107.0(8) -108_665 . -3_555 N
O1 Di1 Oh 113.8(9) -108_665 . -108_665 N
O1 Di1 Oh 82.3(20) -108_665 . -207_575 N
O1 Di1 Dh1 99.6(10) -108_644 . -3_555 N
O1 Di1 Dh1 111.2(9) -108_644 . -108_644 N
O1 Di1 Dh1 91.1(14) -108_644 . -207_554 N
O1 Di1 Dh2 98.9(8) -108_644 . -108_644 N
O1 Di1 Dh2 60.1(14) -108_644 . -207_554 N
O1 Di1 OII* 122.3(15) -108_544 . -301_444 N
O1 Di1 DII*1 126.9(20) -108_543 . -301_443 N
O3 Di1 O4 80.8(8) 4_555 . 310_334 N
O3 Di1 O4 45.5(5) 4_555 . -302_444 N
O3 Di1 O4 35.81(28) 4_555 . -303_444 N
O3 Di1 Og 126.9(12) 4_555 . -3_555 N
O3 Di1 Og 75.4(5) 4_555 . -108_656 N
O3 Di1 Og 104.0(9) 4_555 . -207_566 N
O3 Di1 Og 92.3(11) 4_555 . -304_556 N
O3 Di1 Dg1 103.0(11) 4_555 . -207_575 N
O3 Di1 Dg1 107.3(13) 4_555 . -304_565 N
O3 Di1 Dg2 61.5(5) 4_555 . -108_666 N
O3 Di1 Dg2 90.4(8) 4_555 . -207_576 N
O3 Di1 Dg2 77.5(10) 4_555 . -304_566 N
O3 Di1 Oh 152.0(10) 4_555 . -3_555 N
O3 Di1 Oh 71.8(7) 4_555 . -108_665 N
O3 Di1 Oh 91.9(17) 4_555 . -207_575 N
O3 Di1 Dh1 146.1(12) 4_555 . -3_555 N
O3 Di1 Dh1 77.9(7) 4_555 . -108_644 N
O3 Di1 Dh1 107.1(13) 4_555 . -207_554 N
O3 Di1 Dh2 56.4(5) 4_555 . -108_644 N
O3 Di1 Dh2 66.1(12) 4_555 . -207_554 N
O3 Di1 OII* 78.2(11) 4_555 . -301_444 N
O3 Di1 DII*1 79.1(19) 4_555 . -301_443 N
O4 Di1 O4 83.4(8) 310_334 . -302_444 N
O4 Di1 O4 101.1(6) 310_334 . -303_444 N
O4 Di1 Og 47.6(5) 310_446 . -3_555 N
O4 Di1 Og 87.1(6) 310_446 . -108_656 N
O4 Di1 Og 97.8(9) 310_446 . -207_566 N
O4 Di1 Og 50.0(6) 310_446 . -304_556 N
O4 Di1 Dg1 82.1(8) 310_455 . -207_575 N
O4 Di1 Dg1 47.7(6) 310_455 . -304_565 N
O4 Di1 Dg2 79.6(6) 310_456 . -108_666 N
O4 Di1 Dg2 98.6(9) 310_456 . -207_576 N
O4 Di1 Dg2 39.5(6) 310_456 . -304_566 N
O4 Di1 Oh 71.3(5) 310_455 . -3_555 N
O4 Di1 Oh 120.2(8) 310_455 . -108_665 N
O4 Di1 Oh 102.4(20) 310_455 . -207_575 N
O4 Di1 Dh1 65.4(7) 310_434 . -3_555 N
O4 Di1 Dh1 106.7(8) 310_434 . -108_644 N
O4 Di1 Dh1 102.1(14) 310_434 . -207_554 N
O4 Di1 Dh2 112.1(8) 310_434 . -108_644 N
O4 Di1 Dh2 90.7(16) 310_434 . -207_554 N
O4 Di1 OII* 158.8(14) 310_334 . -301_444 N
O4 Di1 DII*1 150.1(16) 310_333 . -301_443 N
O4 Di1 O4 77.2(5) -302_444 . -303_444 N
O4 Di1 Og 107.2(11) -302_556 . -3_555 N
O4 Di1 Og 120.9(8) -302_556 . -108_656 N
O4 Di1 Og 58.8(6) -302_556 . -207_566 N
O4 Di1 Og 59.4(7) -302_556 . -304_556 N
O4 Di1 Dg1 58.2(7) -302_565 . -207_575 N
O4 Di1 Dg1 76.6(9) -302_565 . -304_565 N
O4 Di1 Dg2 106.8(8) -302_566 . -108_666 N
O4 Di1 Dg2 45.5(5) -302_566 . -207_576 N
O4 Di1 Dg2 52.9(7) -302_566 . -304_566 N
O4 Di1 Oh 130.7(9) -302_565 . -3_555 N
O4 Di1 Oh 109.3(8) -302_565 . -108_665 N
O4 Di1 Oh 47.7(15) -302_565 . -207_575 N
O4 Di1 Dh1 123.0(11) -302_544 . -3_555 N
O4 Di1 Dh1 120.8(9) -302_544 . -108_644 N
O4 Di1 Dh1 62.2(10) -302_544 . -207_554 N
O4 Di1 Dh2 95.9(8) -302_544 . -108_644 N
O4 Di1 Dh2 21.0(9) -302_544 . -207_554 N
O4 Di1 OII* 83.5(11) -302_444 . -301_444 N
O4 Di1 DII*1 97.8(15) -302_443 . -301_443 N
O4 Di1 Og 145.7(8) -303_556 . -3_555 N
O4 Di1 Og 47.9(4) -303_556 . -108_656 N
O4 Di1 Og 129.3(7) -303_556 . -207_566 N
O4 Di1 Og 127.8(11) -303_556 . -304_556 N
O4 Di1 Dg1 134.9(9) -303_565 . -207_575 N
O4 Di1 Dg1 141.1(12) -303_565 . -304_565 N
O4 Di1 Dg2 39.2(4) -303_566 . -108_666 N
O4 Di1 Dg2 115.9(7) -303_566 . -207_576 N
O4 Di1 Dg2 111.9(10) -303_566 . -304_566 N
O4 Di1 Oh 147.7(7) -303_565 . -3_555 N
O4 Di1 Oh 36.0(5) -303_565 . -108_665 N
O4 Di1 Oh 115.6(15) -303_565 . -207_575 N
O4 Di1 Dh1 151.5(8) -303_544 . -3_555 N
O4 Di1 Dh1 43.6(5) -303_544 . -108_644 N
O4 Di1 Dh1 129.9(11) -303_544 . -207_554 N
O4 Di1 Dh2 20.5(4) -303_544 . -108_644 N
O4 Di1 Dh2 95.1(12) -303_544 . -207_554 N
O4 Di1 OII* 59.7(8) -303_444 . -301_444 N
O4 Di1 DII*1 50.9(17) -303_443 . -301_443 N
Og Di1 Og 108.1(7) -3_555 . -108_656 N
Og Di1 Og 76.4(7) -3_555 . -207_566 N
Og Di1 Og 48.1(6) -3_555 . -304_556 N
Og Di1 Dg1 64.0(7) -3_555 . -207_575 N
Og Di1 Dg1 31.3(5) -3_555 . -304_565 N
Og Di1 Dg2 110.7(7) -3_555 . -108_666 N
Og Di1 Dg2 86.7(8) -3_555 . -207_576 N
Og Di1 Dg2 55.9(7) -3_555 . -304_566 N
Og Di1 Oh 27.5(4) -3_555 . -3_555 N
Og Di1 Oh 139.2(10) -3_555 . -108_665 N
Og Di1 Oh 88.7(15) -3_555 . -207_575 N
Og Di1 Dh1 19.8(5) -3_555 . -3_555 N
Og Di1 Dh1 122.6(9) -3_555 . -108_644 N
Og Di1 Dh1 77.9(10) -3_555 . -207_554 N
Og Di1 Dh2 145.0(9) -3_555 . -108_644 N
Og Di1 Dh2 98.5(15) -3_555 . -207_554 N
Og Di1 OII* 153.3(15) -3_555 . -301_444 N
Og Di1 DII*1 152.5(22) -3_555 . -301_443 N
Og Di1 Og 174.9(11) -108_656 . -207_566 N
Og Di1 Og 137.0(10) -108_656 . -304_556 N
Og Di1 Dg1 169.2(12) -108_665 . -207_575 N
Og Di1 Dg1 131.5(9) -108_665 . -304_565 N
Og Di1 Dg2 15.04(12) -108_666 . -108_666 N
Og Di1 Dg2 163.7(9) -108_666 . -207_576 N
Og Di1 Dg2 123.2(10) -108_666 . -304_566 N
Og Di1 Oh 99.9(7) -108_665 . -3_555 N
Og Di1 Oh 35.4(6) -108_665 . -108_665 N
Og Di1 Oh 162.9(16) -108_665 . -207_575 N
Og Di1 Dh1 104.6(8) -108_644 . -3_555 N
Og Di1 Dh1 19.7(6) -108_644 . -108_644 N
Og Di1 Dh1 170.7(18) -108_644 . -207_554 N
Og Di1 Dh2 37.0(6) -108_644 . -108_644 N
Og Di1 Dh2 141.3(14) -108_644 . -207_554 N
Og Di1 OII* 85.4(10) -108_544 . -301_444 N
Og Di1 DII*1 66.5(10) -108_543 . -301_443 N
Og Di1 Og 47.9(5) -207_566 . -304_556 N
Og Di1 Dg1 15.85(14) -207_575 . -207_575 N
Og Di1 Dg1 53.6(6) -207_575 . -304_565 N
Og Di1 Dg2 165.5(12) -207_576 . -108_666 N
Og Di1 Dg2 13.94(14) -207_576 . -207_576 N
Og Di1 Dg2 61.2(7) -207_576 . -304_566 N
Og Di1 Oh 83.0(6) -207_575 . -3_555 N
Og Di1 Oh 139.5(10) -207_575 . -108_665 N
Og Di1 Oh 13.6(11) -207_575 . -207_575 N
Og Di1 Dh1 78.8(7) -207_554 . -3_555 N
Og Di1 Dh1 155.3(12) -207_554 . -108_644 N
Og Di1 Dh1 5.0(9) -207_554 . -207_554 N
Og Di1 Dh2 138.6(9) -207_554 . -108_644 N
Og Di1 Dh2 37.9(9) -207_554 . -207_554 N
Og Di1 OII* 89.5(7) -207_454 . -301_444 N
Og Di1 DII*1 108.4(11) -207_453 . -301_443 N
Og Di1 Dg1 32.2(5) -304_565 . -207_575 N
Og Di1 Dg1 17.27(24) -304_565 . -304_565 N
Og Di1 Dg2 127.3(11) -304_566 . -108_666 N
Og Di1 Dg2 49.8(5) -304_566 . -207_576 N
Og Di1 Dg2 17.17(22) -304_566 . -304_566 N
Og Di1 Oh 72.1(6) -304_565 . -3_555 N
Og Di1 Oh 163.4(13) -304_565 . -108_665 N
Og Di1 Oh 53.4(15) -304_565 . -207_575 N
Og Di1 Dh1 64.1(7) -304_544 . -3_555 N
Og Di1 Dh1 156.4(12) -304_544 . -108_644 N
Og Di1 Dh1 52.3(11) -304_544 . -207_554 N
Og Di1 Dh2 148.1(13) -304_544 . -108_644 N
Og Di1 Dh2 51.9(13) -304_544 . -207_554 N
Og Di1 OII* 133.0(11) -304_444 . -301_444 N
Og Di1 DII*1 152.3(12) -304_443 . -301_443 N
Dg1 Di1 Dg1 38.3(6) -207_575 . -304_565 N
Dg1 Di1 Dg2 157.6(14) -207_576 . -108_666 N
Dg1 Di1 Dg2 22.75(25) -207_576 . -207_576 N
Dg1 Di1 Dg2 46.7(6) -207_576 . -304_566 N
Dg1 Di1 Oh 76.4(6) -207_575 . -3_555 N
Dg1 Di1 Oh 154.7(10) -207_575 . -108_665 N
Dg1 Di1 Oh 25.0(11) -207_575 . -207_575 N
Dg1 Di1 Dh1 70.6(7) -207_554 . -3_555 N
Dg1 Di1 Dh1 171.2(13) -207_554 . -108_644 N
Dg1 Di1 Dh1 20.0(10) -207_554 . -207_554 N
Dg1 Di1 Dh2 150.0(10) -207_554 . -108_644 N
Dg1 Di1 Dh2 39.8(10) -207_554 . -207_554 N
Dg1 Di1 OII* 104.9(8) -207_454 . -301_444 N
Dg1 Di1 DII*1 124.0(11) -207_453 . -301_443 N
Dg1 Di1 Dg2 127.0(11) -304_566 . -108_666 N
Dg1 Di1 Dg2 60.0(7) -304_566 . -207_576 N
Dg1 Di1 Dg2 29.9(4) -304_566 . -304_566 N
Dg1 Di1 Oh 54.9(6) -304_565 . -3_555 N
Dg1 Di1 Oh 166.9(10) -304_565 . -108_665 N
Dg1 Di1 Oh 62.9(15) -304_565 . -207_575 N
Dg1 Di1 Dh1 46.9(7) -304_544 . -3_555 N
Dg1 Di1 Dh1 150.1(10) -304_544 . -108_644 N
Dg1 Di1 Dh1 56.9(11) -304_544 . -207_554 N
Dg1 Di1 Dh2 158.6(13) -304_544 . -108_644 N
Dg1 Di1 Dh2 67.5(14) -304_544 . -207_554 N
Dg1 Di1 OII* 143.1(11) -304_444 . -301_444 N
Dg1 Di1 DII*1 161.6(15) -304_443 . -301_443 N
Dg2 Di1 Dg2 151.9(11) -108_666 . -207_576 N
Dg2 Di1 Dg2 111.5(10) -108_666 . -304_566 N
Dg2 Di1 Oh 109.2(7) -108_665 . -3_555 N
Dg2 Di1 Oh 40.7(6) -108_665 . -108_665 N
Dg2 Di1 Oh 153.0(19) -108_665 . -207_575 N
Dg2 Di1 Dh1 112.3(8) -108_644 . -3_555 N
Dg2 Di1 Dh1 29.5(6) -108_644 . -108_644 N
Dg2 Di1 Dh1 168.3(14) -108_644 . -207_554 N
Dg2 Di1 Dh2 35.6(7) -108_644 . -108_644 N
Dg2 Di1 Dh2 127.6(15) -108_644 . -207_554 N
Dg2 Di1 OII* 88.4(9) -108_544 . -301_444 N
Dg2 Di1 DII*1 71.4(13) -108_543 . -301_443 N
Dg2 Di1 Dg2 59.4(6) -207_576 . -304_566 N
Dg2 Di1 Oh 96.4(6) -207_575 . -3_555 N
Dg2 Di1 Oh 132.5(9) -207_575 . -108_665 N
Dg2 Di1 Oh 3.9(14) -207_575 . -207_575 N
Dg2 Di1 Dh1 91.6(7) -207_554 . -3_555 N
Dg2 Di1 Dh1 149.8(10) -207_554 . -108_644 N
Dg2 Di1 Dh1 16.8(8) -207_554 . -207_554 N
Dg2 Di1 Dh2 127.7(9) -207_554 . -108_644 N
Dg2 Di1 Dh2 24.5(9) -207_554 . -207_554 N
Dg2 Di1 OII* 83.9(7) -207_454 . -301_444 N
Dg2 Di1 DII*1 103.5(10) -207_453 . -301_443 N
Dg2 Di1 Oh 82.7(7) -304_565 . -3_555 N
Dg2 Di1 Oh 146.4(12) -304_565 . -108_665 N
Dg2 Di1 Oh 63.3(17) -304_565 . -207_575 N
Dg2 Di1 Dh1 74.6(8) -304_544 . -3_555 N
Dg2 Di1 Dh1 141.1(12) -304_544 . -108_644 N
Dg2 Di1 Dh1 66.0(12) -304_544 . -207_554 N
Dg2 Di1 Dh2 131.6(12) -304_544 . -108_644 N
Dg2 Di1 Dh2 52.9(14) -304_544 . -207_554 N
Dg2 Di1 OII* 135.3(14) -304_444 . -301_444 N
Dg2 Di1 DII*1 150.6(19) -304_443 . -301_443 N
Oh Di1 Oh 120.1(10) -3_555 . -108_665 N
Oh Di1 Oh 96.7(15) -3_555 . -207_575 N
Oh Di1 Dh1 8.2(5) -3_555 . -3_555 N
Oh Di1 Dh1 107.0(9) -3_555 . -108_644 N
Oh Di1 Dh1 82.1(10) -3_555 . -207_554 N
Oh Di1 Dh2 132.6(10) -3_555 . -108_644 N
Oh Di1 Dh2 115.9(13) -3_555 . -207_554 N
Oh Di1 OII* 129.5(16) -3_555 . -301_444 N
Oh Di1 DII*1 125.0(21) -3_555 . -301_443 N
Oh Di1 Oh 129.9(18) -108_665 . -207_575 N
Oh Di1 Dh1 127.5(11) -108_644 . -3_555 N
Oh Di1 Dh1 17.24(22) -108_644 . -108_644 N
Oh Di1 Dh1 136.2(15) -108_644 . -207_554 N
Oh Di1 Dh2 15.53(27) -108_644 . -108_644 N
Oh Di1 Dh2 121.9(14) -108_644 . -207_554 N
Oh Di1 OII* 50.0(8) -108_544 . -301_444 N
Oh Di1 DII*1 31.4(10) -108_543 . -301_443 N
Oh Di1 Dh1 92.3(15) -207_554 . -3_555 N
Oh Di1 Dh1 147.0(19) -207_554 . -108_644 N
Oh Di1 Dh1 15.3(10) -207_554 . -207_554 N
Oh Di1 Dh2 126.1(16) -207_554 . -108_644 N
Oh Di1 Dh2 26.8(10) -207_554 . -207_554 N
Oh Di1 OII* 80.7(14) -207_454 . -301_444 N
Oh Di1 DII*1 100.2(17) -207_453 . -301_443 N
Dh1 Di1 Dh1 113.6(10) -3_555 . -108_644 N
Dh1 Di1 Dh1 78.5(13) -3_555 . -207_554 N
Dh1 Di1 Dh2 139.1(11) -3_555 . -108_644 N
Dh1 Di1 Dh2 109.5(13) -3_555 . -207_554 N
Dh1 Di1 OII* 135.7(17) -3_555 . -301_444 N
Dh1 Di1 DII*1 132.9(22) -3_555 . -301_443 N
Dh1 Di1 Dh1 151.2(18) -108_644 . -207_554 N
Dh1 Di1 Dh2 25.54(34) -108_644 . -108_644 N
Dh1 Di1 Dh2 136.9(16) -108_644 . -207_554 N
Dh1 Di1 OII* 66.5(10) -108_544 . -301_444 N
Dh1 Di1 DII*1 47.3(10) -108_543 . -301_443 N
Dh1 Di1 Dh2 137.0(13) -207_554 . -108_644 N
Dh1 Di1 Dh2 41.2(7) -207_554 . -207_554 N
Dh1 Di1 OII* 86.4(12) -207_454 . -301_444 N
Dh1 Di1 DII*1 104.9(16) -207_453 . -301_443 N
Dh2 Di1 Dh2 111.4(16) -108_644 . -207_554 N
Dh2 Di1 OII* 53.0(9) -108_544 . -301_444 N
Dh2 Di1 DII*1 38.0(15) -108_543 . -301_443 N
Dh2 Di1 OII* 83.0(14) -207_454 . -301_444 N
Dh2 Di1 DII*1 101.1(16) -207_453 . -301_443 N
OII* Di1 DII*1 19.6(7) -301_443 . -301_443 N
O1 Di2 O1 52.47(33) 2_555 . -3_555 N
O1 Di2 O1 108.1(7) 2_555 . 111_433 N
O1 Di2 O1 91.9(8) 2_555 . -108_544 N
O1 Di2 O2 77.9(6) 2_555 . 1_555 N
O1 Di2 O3 129.5(10) 2_555 . 4_555 N
O1 Di2 O4 41.43(33) 2_555 . 310_334 N
O1 Di2 O4 72.5(5) 2_555 . 312_334 N
O1 Di2 O4 121.3(9) 2_555 . -302_444 N
O1 Di2 Og 43.4(5) 2_555 . -3_555 N
O1 Di2 Og 117.4(8) 2_555 . -108_656 N
O1 Di2 Og 109.4(7) 2_555 . -207_566 N
O1 Di2 Og 79.3(7) 2_555 . -304_556 N
O1 Di2 Dg1 50.1(5) 2_555 . -3_555 N
O1 Di2 Dg1 99.4(7) 2_555 . -207_575 N
O1 Di2 Dg1 70.1(7) 2_555 . -304_565 N
O1 Di2 Dg2 24.74(35) 2_555 . -3_555 N
O1 Di2 Dg2 116.7(8) 2_555 . -108_666 N
O1 Di2 Dg2 81.8(8) 2_555 . -304_566 N
O1 Di2 Oh 57.6(5) 2_555 . -3_555 N
O1 Di2 Oh 81.3(7) 2_555 . 105_544 N
O1 Di2 Oh 150.8(9) 2_555 . -108_665 N
O1 Di2 Oh 128.5(11) 2_555 . -207_575 N
O1 Di2 Oh 49.1(5) 2_555 . -304_565 N
O1 Di2 Dh1 56.4(7) 2_555 . -3_555 N
O1 Di2 O1 75.6(5) -3_555 . 111_433 N
O1 Di2 O1 112.5(8) -3_555 . -108_544 N
O1 Di2 O2 72.8(4) -3_555 . 1_555 N
O1 Di2 O3 116.9(7) -3_555 . 4_555 N
O1 Di2 O4 71.6(5) -3_555 . 310_334 N
O1 Di2 O4 38.30(27) -3_555 . 312_334 N
O1 Di2 O4 147.0(9) -3_555 . -302_444 N
O1 Di2 Og 90.3(7) -3_555 . -3_555 N
O1 Di2 Og 65.4(5) -3_555 . -108_656 N
O1 Di2 Og 160.1(7) -3_555 . -207_566 N
O1 Di2 Og 130.1(8) -3_555 . -304_556 N
O1 Di2 Dg1 96.3(6) -3_555 . -3_555 N
O1 Di2 Dg1 151.7(8) -3_555 . -207_575 N
O1 Di2 Dg1 122.5(8) -3_555 . -304_565 N
O1 Di2 Dg2 73.4(6) -3_555 . -3_555 N
O1 Di2 Dg2 68.9(6) -3_555 . -108_666 N
O1 Di2 Dg2 126.1(9) -3_555 . -304_566 N
O1 Di2 Oh 81.7(7) -3_555 . -3_555 N
O1 Di2 Oh 46.0(5) -3_555 . 105_544 N
O1 Di2 Oh 98.3(7) -3_555 . -108_665 N
O1 Di2 Oh 177.3(15) -3_555 . -207_575 N
O1 Di2 Oh 99.9(6) -3_555 . -304_565 N
O1 Di2 Dh1 88.4(9) -3_555 . -3_555 N
O1 Di2 O1 63.5(6) 111_433 . -108_544 N
O1 Di2 O2 37.83(33) 111_433 . 1_555 N
O1 Di2 O3 41.8(4) 111_433 . 4_555 N
O1 Di2 O4 80.7(7) 111_433 . 310_334 N
O1 Di2 O4 39.39(31) 111_433 . 312_334 N
O1 Di2 O4 77.4(6) 111_433 . -302_444 N
O1 Di2 Og 147.2(12) 111_545 . -3_555 N
O1 Di2 Og 43.5(4) 111_545 . -108_656 N
O1 Di2 Og 122.0(8) 111_545 . -207_566 N
O1 Di2 Og 113.8(11) 111_545 . -304_556 N
O1 Di2 Dg1 152.2(11) 111_554 . -3_555 N
O1 Di2 Dg1 123.2(10) 111_554 . -207_575 N
O1 Di2 Dg1 128.3(14) 111_554 . -304_565 N
O1 Di2 Dg2 131.3(10) 111_555 . -3_555 N
O1 Di2 Dg2 27.10(32) 111_555 . -108_666 N
O1 Di2 Dg2 97.2(11) 111_555 . -304_566 N
O1 Di2 Oh 157.2(9) 111_554 . -3_555 N
O1 Di2 Oh 96.5(7) 111_554 . 105_544 N
O1 Di2 Oh 58.0(5) 111_554 . -108_665 N
O1 Di2 Oh 105.9(10) 111_554 . -207_575 N
O1 Di2 Oh 115.1(10) 111_554 . -304_565 N
O1 Di2 Dh1 163.0(10) 111_533 . -3_555 N
O1 Di2 O2 41.8(5) -108_544 . 1_555 N
O1 Di2 O3 42.2(4) -108_544 . 4_555 N
O1 Di2 O4 51.5(6) -108_544 . 310_334 N
O1 Di2 O4 80.9(8) -108_544 . 312_334 N
O1 Di2 O4 36.7(4) -108_544 . -302_444 N
O1 Di2 Og 96.6(11) -108_656 . -3_555 N
O1 Di2 Og 106.0(9) -108_656 . -108_656 N
O1 Di2 Og 72.6(6) -108_656 . -207_566 N
O1 Di2 Og 50.3(6) -108_656 . -304_556 N
O1 Di2 Dg1 96.9(9) -108_665 . -3_555 N
O1 Di2 Dg1 66.9(7) -108_665 . -207_575 N
O1 Di2 Dg1 64.9(9) -108_665 . -304_565 N
O1 Di2 Dg2 95.5(10) -108_666 . -3_555 N
O1 Di2 Dg2 89.7(9) -108_666 . -108_666 N
O1 Di2 Dg2 33.7(5) -108_666 . -304_566 N
O1 Di2 Oh 129.5(10) -108_665 . -3_555 N
O1 Di2 Oh 156.0(9) -108_665 . 105_544 N
O1 Di2 Oh 101.9(8) -108_665 . -108_665 N
O1 Di2 Oh 70.3(10) -108_665 . -207_575 N
O1 Di2 Oh 59.3(7) -108_665 . -304_565 N
O1 Di2 Dh1 119.7(12) -108_644 . -3_555 N
O2 Di2 O3 54.4(5) 1_555 . 4_555 N
O2 Di2 O4 43.2(4) 1_555 . 310_334 N
O2 Di2 O4 39.17(32) 1_555 . 312_334 N
O2 Di2 O4 74.3(6) 1_555 . -302_444 N
O2 Di2 Og 109.9(10) 1_555 . -3_555 N
O2 Di2 Og 78.0(6) 1_555 . -108_656 N
O2 Di2 Og 114.4(9) 1_555 . -207_566 N
O2 Di2 Og 86.4(9) 1_555 . -304_556 N
O2 Di2 Dg1 114.5(9) 1_555 . -3_555 N
O2 Di2 Dg1 108.0(10) 1_555 . -207_575 N
O2 Di2 Dg1 96.8(11) 1_555 . -304_565 N
O2 Di2 Dg2 96.7(9) 1_555 . -3_555 N
O2 Di2 Dg2 62.9(6) 1_555 . -108_666 N
O2 Di2 Dg2 70.7(8) 1_555 . -304_566 N
O2 Di2 Oh 135.4(8) 1_555 . -3_555 N
O2 Di2 Oh 114.2(7) 1_555 . 105_544 N
O2 Di2 Oh 95.4(7) 1_555 . -108_665 N
O2 Di2 Oh 109.8(12) 1_555 . -207_575 N
O2 Di2 Oh 78.2(7) 1_555 . -304_565 N
O2 Di2 Dh1 132.0(11) 1_555 . -3_555 N
O3 Di2 O4 88.5(9) 4_555 . 310_334 N
O3 Di2 O4 79.0(6) 4_555 . 312_334 N
O3 Di2 O4 36.68(30) 4_555 . -302_444 N
O3 Di2 Og 135.7(12) 4_555 . -3_555 N
O3 Di2 Og 71.6(6) 4_555 . -108_656 N
O3 Di2 Og 80.2(6) 4_555 . -207_566 N
O3 Di2 Og 81.9(8) 4_555 . -304_556 N
O3 Di2 Dg1 133.6(10) 4_555 . -3_555 N
O3 Di2 Dg1 82.5(7) 4_555 . -207_575 N
O3 Di2 Dg1 97.7(11) 4_555 . -304_565 N
O3 Di2 Dg2 137.7(12) 4_555 . -3_555 N
O3 Di2 Dg2 58.2(5) 4_555 . -108_666 N
O3 Di2 Dg2 68.6(8) 4_555 . -304_566 N
O3 Di2 Oh 161.0(9) 4_555 . -3_555 N
O3 Di2 Oh 130.0(8) 4_555 . 105_544 N
O3 Di2 Oh 59.8(5) 4_555 . -108_665 N
O3 Di2 Oh 64.8(8) 4_555 . -207_575 N
O3 Di2 Oh 100.4(9) 4_555 . -304_565 N
O3 Di2 Dh1 152.3(12) 4_555 . -3_555 N
O4 Di2 O4 62.6(5) 310_334 . 312_334 N
O4 Di2 O4 85.8(8) 310_334 . -302_444 N
O4 Di2 Og 66.7(7) 310_446 . -3_555 N
O4 Di2 Og 114.9(9) 310_446 . -108_656 N
O4 Di2 Og 100.5(8) 310_446 . -207_566 N
O4 Di2 Og 62.7(7) 310_446 . -304_556 N
O4 Di2 Dg1 71.6(7) 310_455 . -3_555 N
O4 Di2 Dg1 89.6(8) 310_455 . -207_575 N
O4 Di2 Dg1 64.7(9) 310_455 . -304_565 N
O4 Di2 Dg2 54.3(6) 310_456 . -3_555 N
O4 Di2 Dg2 102.9(9) 310_456 . -108_666 N
O4 Di2 Dg2 54.6(7) 310_456 . -304_566 N
O4 Di2 Oh 94.4(7) 310_455 . -3_555 N
O4 Di2 Oh 115.1(8) 310_455 . 105_544 N
O4 Di2 Oh 138.6(10) 310_455 . -108_665 N
O4 Di2 Oh 110.9(13) 310_455 . -207_575 N
O4 Di2 Oh 40.1(5) 310_455 . -304_565 N
O4 Di2 Dh1 89.2(10) 310_434 . -3_555 N
O4 Di2 O4 110.0(8) 312_334 . -302_444 N
O4 Di2 Og 115.8(9) 312_446 . -3_555 N
O4 Di2 Og 53.1(5) 312_446 . -108_656 N
O4 Di2 Og 153.4(11) 312_446 . -207_566 N
O4 Di2 Og 122.1(11) 312_446 . -304_556 N
O4 Di2 Dg1 122.5(8) 312_455 . -3_555 N
O4 Di2 Dg1 146.7(11) 312_455 . -207_575 N
O4 Di2 Dg1 127.3(12) 312_455 . -304_565 N
O4 Di2 Dg2 97.2(7) 312_456 . -3_555 N
O4 Di2 Dg2 45.4(4) 312_456 . -108_666 N
O4 Di2 Dg2 108.2(11) 312_456 . -304_566 N
O4 Di2 Oh 118.9(8) 312_455 . -3_555 N
O4 Di2 Oh 75.1(6) 312_455 . 105_544 N
O4 Di2 Oh 84.3(6) 312_455 . -108_665 N
O4 Di2 Oh 143.7(13) 312_455 . -207_575 N
O4 Di2 Oh 102.4(8) 312_455 . -304_565 N
O4 Di2 Dh1 123.7(9) 312_434 . -3_555 N
O4 Di2 Og 102.6(9) -302_556 . -3_555 N
O4 Di2 Og 105.8(7) -302_556 . -108_656 N
O4 Di2 Og 45.40(35) -302_556 . -207_566 N
O4 Di2 Og 48.7(5) -302_556 . -304_556 N
O4 Di2 Dg1 98.9(8) -302_565 . -3_555 N
O4 Di2 Dg1 45.9(5) -302_565 . -207_575 N
O4 Di2 Dg1 63.5(7) -302_565 . -304_565 N
O4 Di2 Dg2 112.6(9) -302_566 . -3_555 N
O4 Di2 Dg2 94.3(7) -302_566 . -108_666 N
O4 Di2 Dg2 40.5(6) -302_566 . -304_566 N
O4 Di2 Oh 124.7(8) -302_565 . -3_555 N
O4 Di2 Oh 157.3(8) -302_565 . 105_544 N
O4 Di2 Oh 82.9(6) -302_565 . -108_665 N
O4 Di2 Oh 35.5(7) -302_565 . -207_575 N
O4 Di2 Oh 75.0(7) -302_565 . -304_565 N
O4 Di2 Dh1 115.6(10) -302_544 . -3_555 N
Og Di2 Og 151.6(13) -3_555 . -108_656 N
Og Di2 Og 69.9(7) -3_555 . -207_566 N
Og Di2 Og 54.5(6) -3_555 . -304_556 N
Og Di2 Dg1 6.7(4) -3_555 . -3_555 N
Og Di2 Dg1 62.4(7) -3_555 . -207_575 N
Og Di2 Dg1 39.2(6) -3_555 . -304_565 N
Og Di2 Dg2 18.66(28) -3_555 . -3_555 N
Og Di2 Dg2 159.0(10) -3_555 . -108_666 N
Og Di2 Dg2 67.2(8) -3_555 . -304_566 N
Og Di2 Oh 33.2(6) -3_555 . -3_555 N
Og Di2 Oh 94.2(10) -3_555 . 105_544 N
Og Di2 Oh 154.7(14) -3_555 . -108_665 N
Og Di2 Oh 89.6(10) -3_555 . -207_575 N
Og Di2 Oh 37.6(6) -3_555 . -304_565 N
Og Di2 Dh1 24.5(7) -3_555 . -3_555 N
Og Di2 Og 133.2(8) -108_656 . -207_566 N
Og Di2 Og 153.5(12) -108_656 . -304_556 N
Og Di2 Dg1 154.8(12) -108_665 . -3_555 N
Og Di2 Dg1 143.0(8) -108_665 . -207_575 N
Og Di2 Dg1 169.2(13) -108_665 . -304_565 N
Og Di2 Dg2 138.2(10) -108_666 . -3_555 N
Og Di2 Dg2 16.48(16) -108_666 . -108_666 N
Og Di2 Dg2 138.8(13) -108_666 . -304_566 N
Og Di2 Oh 123.3(12) -108_665 . -3_555 N
Og Di2 Oh 58.6(6) -108_665 . 105_544 N
Og Di2 Oh 34.0(4) -108_665 . -108_665 N
Og Di2 Oh 114.0(10) -108_665 . -207_575 N
Og Di2 Oh 154.9(10) -108_665 . -304_565 N
Og Di2 Dh1 133.5(15) -108_644 . -3_555 N
Og Di2 Og 37.8(4) -207_566 . -304_556 N
Og Di2 Dg1 63.8(6) -207_575 . -3_555 N
Og Di2 Dg1 11.19(18) -207_575 . -207_575 N
Og Di2 Dg1 40.5(6) -207_575 . -304_565 N
Og Di2 Dg2 87.1(7) -207_576 . -3_555 N
Og Di2 Dg2 131.0(8) -207_576 . -108_666 N
Og Di2 Dg2 48.1(5) -207_576 . -304_566 N
Og Di2 Oh 80.8(6) -207_575 . -3_555 N
Og Di2 Oh 131.4(9) -207_575 . 105_544 N
Og Di2 Oh 99.3(7) -207_575 . -108_665 N
Og Di2 Oh 19.8(6) -207_575 . -207_575 N
Og Di2 Oh 65.3(6) -207_575 . -304_565 N
Og Di2 Dh1 73.1(7) -207_554 . -3_555 N
Og Di2 Dg1 51.7(6) -304_565 . -3_555 N
Og Di2 Dg1 26.9(4) -304_565 . -207_575 N
Og Di2 Dg1 15.85(29) -304_565 . -304_565 N
Og Di2 Dg2 64.4(6) -304_566 . -3_555 N
Og Di2 Dg2 138.7(13) -304_566 . -108_666 N
Og Di2 Dg2 16.67(22) -304_566 . -304_566 N
Og Di2 Oh 82.7(7) -304_565 . -3_555 N
Og Di2 Oh 147.9(10) -304_565 . 105_544 N
Og Di2 Oh 129.1(9) -304_565 . -108_665 N
Og Di2 Oh 51.7(7) -304_565 . -207_575 N
Og Di2 Oh 30.4(5) -304_565 . -304_565 N
Og Di2 Dh1 72.5(9) -304_544 . -3_555 N
Dg1 Di2 Dg1 56.8(7) -3_555 . -207_575 N
Dg1 Di2 Dg1 36.0(5) -3_555 . -304_565 N
Dg1 Di2 Dg2 25.38(30) -3_555 . -3_555 N
Dg1 Di2 Dg2 165.2(10) -3_555 . -108_666 N
Dg1 Di2 Dg2 65.7(8) -3_555 . -304_566 N
Dg1 Di2 Oh 32.6(5) -3_555 . -3_555 N
Dg1 Di2 Oh 96.3(9) -3_555 . 105_544 N
Dg1 Di2 Oh 149.5(11) -3_555 . -108_665 N
Dg1 Di2 Oh 83.4(9) -3_555 . -207_575 N
Dg1 Di2 Oh 39.2(5) -3_555 . -304_565 N
Dg1 Di2 Dh1 22.9(7) -3_555 . -3_555 N
Dg1 Di2 Dg1 29.7(6) -207_575 . -304_565 N
Dg1 Di2 Dg2 78.4(7) -207_576 . -3_555 N
Dg1 Di2 Dg2 137.8(10) -207_576 . -108_666 N
Dg1 Di2 Dg2 38.8(5) -207_576 . -304_566 N
Dg1 Di2 Oh 78.8(7) -207_575 . -3_555 N
Dg1 Di2 Oh 136.8(10) -207_575 . 105_544 N
Dg1 Di2 Oh 109.6(8) -207_575 . -108_665 N
Dg1 Di2 Oh 29.0(6) -207_575 . -207_575 N
Dg1 Di2 Oh 54.2(6) -207_575 . -304_565 N
Dg1 Di2 Dh1 69.9(8) -207_554 . -3_555 N
Dg1 Di2 Dg2 51.3(7) -304_566 . -3_555 N
Dg1 Di2 Dg2 154.3(15) -304_566 . -108_666 N
Dg1 Di2 Dg2 31.4(4) -304_566 . -304_566 N
Dg1 Di2 Oh 66.9(7) -304_565 . -3_555 N
Dg1 Di2 Oh 132.0(12) -304_565 . 105_544 N
Dg1 Di2 Oh 139.1(10) -304_565 . -108_665 N
Dg1 Di2 Oh 58.5(9) -304_565 . -207_575 N
Dg1 Di2 Oh 25.6(7) -304_565 . -304_565 N
Dg1 Di2 Dh1 56.7(8) -304_544 . -3_555 N
Dg2 Di2 Dg2 140.9(10) -3_555 . -108_666 N
Dg2 Di2 Dg2 73.0(7) -3_555 . -304_566 N
Dg2 Di2 Oh 40.1(6) -3_555 . -3_555 N
Dg2 Di2 Oh 88.0(9) -3_555 . 105_544 N
Dg2 Di2 Oh 162.5(14) -3_555 . -108_665 N
Dg2 Di2 Oh 106.8(10) -3_555 . -207_575 N
Dg2 Di2 Oh 38.6(6) -3_555 . -304_565 N
Dg2 Di2 Dh1 35.3(7) -3_555 . -3_555 N
Dg2 Di2 Dg2 122.9(13) -108_666 . -304_566 N
Dg2 Di2 Oh 138.5(12) -108_665 . -3_555 N
Dg2 Di2 Oh 73.2(7) -108_665 . 105_544 N
Dg2 Di2 Oh 39.1(5) -108_665 . -108_665 N
Dg2 Di2 Oh 111.3(10) -108_665 . -207_575 N
Dg2 Di2 Oh 141.0(11) -108_665 . -304_565 N
Dg2 Di2 Dh1 148.6(15) -108_644 . -3_555 N
Dg2 Di2 Oh 97.9(8) -304_565 . -3_555 N
Dg2 Di2 Oh 160.9(10) -304_565 . 105_544 N
Dg2 Di2 Oh 123.2(10) -304_565 . -108_665 N
Dg2 Di2 Oh 56.3(9) -304_565 . -207_575 N
Dg2 Di2 Oh 34.7(6) -304_565 . -304_565 N
Dg2 Di2 Dh1 87.7(10) -304_544 . -3_555 N
Oh Di2 Oh 65.2(9) -3_555 . 105_544 N
Oh Di2 Oh 124.6(12) -3_555 . -108_665 N
Oh Di2 Oh 96.7(11) -3_555 . -207_575 N
Oh Di2 Oh 70.8(6) -3_555 . -304_565 N
Oh Di2 Dh1 10.2(6) -3_555 . -3_555 N
Oh Di2 Oh 75.6(9) 105_544 . -108_665 N
Oh Di2 Oh 131.3(14) 105_544 . -207_575 N
Oh Di2 Oh 126.4(9) 105_544 . -304_565 N
Oh Di2 Dh1 75.4(11) 105_544 . -3_555 N
Oh Di2 Oh 80.7(10) -108_665 . -207_575 N
Oh Di2 Oh 157.9(10) -108_665 . -304_565 N
Oh Di2 Dh1 131.5(15) -108_644 . -3_555 N
Oh Di2 Oh 81.7(10) -207_575 . -304_565 N
Oh Di2 Dh1 90.4(11) -207_554 . -3_555 N
Oh Di2 Dh1 61.7(9) -304_544 . -3_555 N
O1 Ok O1 102.0(6) 4_555 . -12_554 N
O1 Ok O1 57.4(7) 4_555 . 111_433 N
O1 Ok O2 59.5(5) 4_555 . 1_555 N
O1 Ok O2 68.8(4) 4_555 . -108_544 N
O1 Ok O2 35.83(28) 4_555 . -109_544 N
O1 Ok O3 73.4(5) 4_555 . 4_555 N
O1 Ok O3 93.0(5) 4_555 . 205_554 N
O1 Ok O3 38.52(34) 4_555 . 208_343 N
O1 Ok O4 34.03(24) 4_555 . 106_554 N
O1 Ok O4 78.1(7) 4_555 . 312_334 N
O1 Ok O4 78.8(7) 4_555 . -303_444 N
O1 Ok SJ 137.5(16) 4_555 . -108_656 N
O1 Ok Og 124.1(10) 4_555 . 1_555 N
O1 Ok Og 34.80(27) 4_555 . 111_545 N
O1 Ok Og 136.5(15) 4_555 . -108_656 N
O1 Ok Og 156.9(7) 4_555 . -201_555 N
O1 Ok Og 138.6(10) 4_555 . -305_556 N
O1 Ok Dg1 131.6(12) 4_555 . 1_555 N
O1 Ok Dg1 166.4(17) 4_555 . -108_665 N
O1 Ok Dg1 151.5(9) 4_555 . -305_565 N
O1 Ok Dg2 115.4(9) 4_555 . 1_555 N
O1 Ok Dg2 22.90(23) 4_555 . 111_555 N
O1 Ok Dg2 107.7(17) 4_555 . -108_666 N
O1 Ok Dg2 123.6(8) 4_555 . -305_566 N
O1 Ok O1 117.3(9) -12_554 . 111_433 N
O1 Ok O2 128.0(7) -12_554 . 1_555 N
O1 Ok O2 34.77(28) -12_554 . -108_544 N
O1 Ok O2 83.9(6) -12_554 . -109_544 N
O1 Ok O3 80.4(5) -12_554 . 4_555 N
O1 Ok O3 32.51(26) -12_554 . 205_554 N
O1 Ok O3 138.1(8) -12_554 . 208_343 N
O1 Ok O4 68.2(4) -12_554 . 106_554 N
O1 Ok O4 158.8(8) -12_554 . 312_334 N
O1 Ok O4 45.8(6) -12_554 . -303_444 N
O1 Ok SJ 56.6(15) -12_666 . -108_656 N
O1 Ok Og 133.3(10) -12_666 . 1_555 N
O1 Ok Og 96.7(6) -12_666 . 111_545 N
O1 Ok Og 107.7(14) -12_666 . -108_656 N
O1 Ok Og 60.6(6) -12_666 . -201_555 N
O1 Ok Og 47.4(7) -12_666 . -305_556 N
O1 Ok Dg1 126.3(12) -12_675 . 1_555 N
O1 Ok Dg1 89.0(16) -12_675 . -108_665 N
O1 Ok Dg1 56.2(7) -12_675 . -305_565 N
O1 Ok Dg2 142.5(10) -12_676 . 1_555 N
O1 Ok Dg2 99.7(6) -12_676 . 111_555 N
O1 Ok Dg2 116.3(16) -12_676 . -108_666 N
O1 Ok Dg2 25.8(4) -12_676 . -305_566 N
O1 Ok O2 10.8(4) 111_433 . 1_555 N
O1 Ok O2 90.1(7) 111_433 . -108_544 N
O1 Ok O2 43.2(5) 111_433 . -109_544 N
O1 Ok O3 38.4(5) 111_433 . 4_555 N
O1 Ok O3 86.0(7) 111_433 . 205_554 N
O1 Ok O3 39.4(6) 111_433 . 208_343 N
O1 Ok O4 77.9(7) 111_433 . 106_554 N
O1 Ok O4 44.8(6) 111_433 . 312_334 N
O1 Ok O4 71.5(8) 111_433 . -303_444 N
O1 Ok SJ 97.3(16) 111_545 . -108_656 N
O1 Ok Og 95.8(9) 111_545 . 1_555 N
O1 Ok Og 90.7(10) 111_545 . 111_545 N
O1 Ok Og 80.7(11) 111_545 . -108_656 N
O1 Ok Og 142.3(9) 111_545 . -201_555 N
O1 Ok Og 153.1(15) 111_545 . -305_556 N
O1 Ok Dg1 94.7(10) 111_554 . 1_555 N
O1 Ok Dg1 110.5(15) 111_554 . -108_665 N
O1 Ok Dg1 145.8(12) 111_554 . -305_565 N
O1 Ok Dg2 83.2(8) 111_555 . 1_555 N
O1 Ok Dg2 79.0(9) 111_555 . 111_555 N
O1 Ok Dg2 50.8(11) 111_555 . -108_666 N
O1 Ok Dg2 138.8(13) 111_555 . -305_566 N
O2 Ok O2 100.4(5) 1_555 . -108_544 N
O2 Ok O2 52.0(4) 1_555 . -109_544 N
O2 Ok O3 48.54(34) 1_555 . 4_555 N
O2 Ok O3 96.5(5) 1_555 . 205_554 N
O2 Ok O3 33.42(28) 1_555 . 208_343 N
O2 Ok O4 84.6(6) 1_555 . 106_554 N
O2 Ok O4 34.21(31) 1_555 . 312_334 N
O2 Ok O4 82.3(8) 1_555 . -303_444 N
O2 Ok SJ 102.5(16) 1_555 . -108_656 N
O2 Ok Og 86.3(6) 1_555 . 1_555 N
O2 Ok Og 90.1(7) 1_555 . 111_545 N
O2 Ok Og 77.2(11) 1_555 . -108_656 N
O2 Ok Og 142.7(5) 1_555 . -201_555 N
O2 Ok Og 158.1(10) 1_555 . -305_556 N
O2 Ok Dg1 86.4(8) 1_555 . 1_555 N
O2 Ok Dg1 107.4(13) 1_555 . -108_665 N
O2 Ok Dg1 147.3(8) 1_555 . -305_565 N
O2 Ok Dg2 73.7(6) 1_555 . 1_555 N
O2 Ok Dg2 79.1(6) 1_555 . 111_555 N
O2 Ok Dg2 48.4(13) 1_555 . -108_666 N
O2 Ok Dg2 148.5(10) 1_555 . -305_566 N
O2 Ok O2 50.37(32) -108_544 . -109_544 N
O2 Ok O3 62.0(4) -108_544 . 4_555 N
O2 Ok O3 31.96(21) -108_544 . 205_554 N
O2 Ok O3 103.4(6) -108_544 . 208_343 N
O2 Ok O4 36.65(23) -108_544 . 106_554 N
O2 Ok O4 134.3(8) -108_544 . 312_334 N
O2 Ok O4 29.9(4) -108_544 . -303_444 N
O2 Ok SJ 78.7(15) -108_656 . -108_656 N
O2 Ok Og 167.0(10) -108_656 . 1_555 N
O2 Ok Og 75.2(4) -108_656 . 111_545 N
O2 Ok Og 127.2(12) -108_656 . -108_656 N
O2 Ok Og 95.4(7) -108_656 . -201_555 N
O2 Ok Og 81.3(9) -108_656 . -305_556 N
O2 Ok Dg1 157.4(11) -108_665 . 1_555 N
O2 Ok Dg1 120.1(17) -108_665 . -108_665 N
O2 Ok Dg1 90.9(8) -108_665 . -305_565 N
O2 Ok Dg2 167.6(7) -108_666 . 1_555 N
O2 Ok Dg2 73.1(4) -108_666 . 111_555 N
O2 Ok Dg2 116.8(13) -108_666 . -108_666 N
O2 Ok Dg2 60.1(6) -108_666 . -305_566 N
O2 Ok O3 39.31(28) -109_544 . 4_555 N
O2 Ok O3 62.3(4) -109_544 . 205_554 N
O2 Ok O3 55.8(5) -109_544 . 208_343 N
O2 Ok O4 36.65(24) -109_544 . 106_554 N
O2 Ok O4 84.5(7) -109_544 . 312_334 N
O2 Ok O4 46.2(5) -109_544 . -303_444 N
O2 Ok SJ 101.9(15) -109_656 . -108_656 N
O2 Ok Og 138.2(10) -109_656 . 1_555 N
O2 Ok Og 67.0(5) -109_656 . 111_545 N
O2 Ok Og 117.3(12) -109_656 . -108_656 N
O2 Ok Og 141.7(8) -109_656 . -201_555 N
O2 Ok Og 131.2(11) -109_656 . -305_556 N
O2 Ok Dg1 137.9(11) -109_665 . 1_555 N
O2 Ok Dg1 140.3(14) -109_665 . -108_665 N
O2 Ok Dg1 138.8(10) -109_665 . -305_565 N
O2 Ok Dg2 125.6(9) -109_666 . 1_555 N
O2 Ok Dg2 56.3(4) -109_666 . 111_555 N
O2 Ok Dg2 88.9(13) -109_666 . -108_666 N
O2 Ok Dg2 109.7(9) -109_666 . -305_566 N
O3 Ok O3 48.14(30) 4_555 . 205_554 N
O3 Ok O3 75.0(6) 4_555 . 208_343 N
O3 Ok O4 71.5(4) 4_555 . 106_554 N
O3 Ok O4 79.3(6) 4_555 . 312_334 N
O3 Ok O4 35.7(4) 4_555 . -303_444 N
O3 Ok SJ 67.3(13) 4_555 . -108_656 N
O3 Ok Og 117.2(7) 4_555 . 1_555 N
O3 Ok Og 106.3(6) 4_555 . 111_545 N
O3 Ok Og 80.9(9) 4_555 . -108_656 N
O3 Ok Og 114.9(7) 4_555 . -201_555 N
O3 Ok Og 117.1(11) 4_555 . -305_556 N
O3 Ok Dg1 110.4(8) 4_555 . 1_555 N
O3 Ok Dg1 101.0(13) 4_555 . -108_665 N
O3 Ok Dg1 115.4(10) 4_555 . -305_565 N
O3 Ok Dg2 107.1(6) 4_555 . 1_555 N
O3 Ok Dg2 95.3(6) 4_555 . 111_555 N
O3 Ok Dg2 57.4(10) 4_555 . -108_666 N
O3 Ok Dg2 100.4(9) 4_555 . -305_566 N
O3 Ok O3 116.8(6) 205_554 . 208_343 N
O3 Ok O4 66.2(4) 205_554 . 106_554 N
O3 Ok O4 126.6(7) 205_554 . 312_334 N
O3 Ok O4 16.4(5) 205_554 . -303_444 N
O3 Ok SJ 48.2(13) 205_554 . -108_656 N
O3 Ok Og 136.8(8) 205_554 . 1_555 N
O3 Ok Og 107.0(5) 205_554 . 111_545 N
O3 Ok Og 95.3(10) 205_554 . -108_656 N
O3 Ok Og 79.6(6) 205_554 . -201_555 N
O3 Ok Og 73.3(9) 205_554 . -305_556 N
O3 Ok Dg1 126.4(9) 205_554 . 1_555 N
O3 Ok Dg1 92.1(14) 205_554 . -108_665 N
O3 Ok Dg1 77.2(8) 205_554 . -305_565 N
O3 Ok Dg2 136.5(6) 205_554 . 1_555 N
O3 Ok Dg2 103.4(5) 205_554 . 111_555 N
O3 Ok Dg2 90.3(13) 205_554 . -108_666 N
O3 Ok Dg2 53.4(6) 205_554 . -305_566 N
O3 Ok O4 72.1(5) 208_343 . 106_554 N
O3 Ok O4 39.8(4) 208_343 . 312_334 N
O3 Ok O4 100.4(10) 208_343 . -303_444 N
O3 Ok SJ 135.9(18) 208_455 . -108_656 N
O3 Ok Og 88.4(7) 208_455 . 1_555 N
O3 Ok Og 59.7(5) 208_455 . 111_545 N
O3 Ok Og 101.4(13) 208_455 . -108_656 N
O3 Ok Og 161.3(7) 208_455 . -201_555 N
O3 Ok Og 167.4(11) 208_455 . -305_556 N
O3 Ok Dg1 94.2(10) 208_464 . 1_555 N
O3 Ok Dg1 128.5(16) 208_464 . -108_665 N
O3 Ok Dg1 165.3(9) 208_464 . -305_565 N
O3 Ok Dg2 78.0(7) 208_465 . 1_555 N
O3 Ok Dg2 50.6(5) 208_465 . 111_555 N
O3 Ok Dg2 77.4(15) 208_465 . -108_666 N
O3 Ok Dg2 162.1(9) 208_465 . -305_566 N
O4 Ok O4 110.8(8) 106_554 . 312_334 N
O4 Ok O4 56.7(5) 106_554 . -303_444 N
O4 Ok SJ 114.4(16) 106_554 . -108_656 N
O4 Ok Og 156.2(10) 106_554 . 1_555 N
O4 Ok Og 42.11(27) 106_554 . 111_545 N
O4 Ok Og 152.5(12) 106_554 . -108_656 N
O4 Ok Og 125.4(7) 106_554 . -201_555 N
O4 Ok Og 107.7(9) 106_554 . -305_556 N
O4 Ok Dg1 165.4(12) 106_554 . 1_555 N
O4 Ok Dg1 156.6(18) 106_554 . -108_665 N
O4 Ok Dg1 120.1(9) 106_554 . -305_565 N
O4 Ok Dg2 149.3(10) 106_554 . 1_555 N
O4 Ok Dg2 37.16(29) 106_554 . 111_555 N
O4 Ok Dg2 125.6(15) 106_554 . -108_666 N
O4 Ok Dg2 90.0(7) 106_554 . -305_566 N
O4 Ok O4 114.8(10) 312_334 . -303_444 N
O4 Ok SJ 109.0(16) 312_446 . -108_656 N
O4 Ok Og 54.0(5) 312_446 . 1_555 N
O4 Ok Og 95.0(8) 312_446 . 111_545 N
O4 Ok Og 62.8(10) 312_446 . -108_656 N
O4 Ok Og 123.8(6) 312_446 . -201_555 N
O4 Ok Og 141.3(10) 312_446 . -305_556 N
O4 Ok Dg1 56.8(7) 312_455 . 1_555 N
O4 Ok Dg1 88.7(13) 312_455 . -108_665 N
O4 Ok Dg1 129.1(8) 312_455 . -305_565 N
O4 Ok Dg2 41.7(4) 312_456 . 1_555 N
O4 Ok Dg2 88.4(8) 312_456 . 111_555 N
O4 Ok Dg2 45.8(12) 312_456 . -108_666 N
O4 Ok Dg2 157.6(10) 312_456 . -305_566 N
O4 Ok SJ 60.0(13) -303_556 . -108_656 N
O4 Ok Og 143.2(9) -303_556 . 1_555 N
O4 Ok Og 98.8(7) -303_556 . 111_545 N
O4 Ok Og 100.0(11) -303_556 . -108_656 N
O4 Ok Og 95.9(10) -303_556 . -201_555 N
O4 Ok Og 89.4(12) -303_556 . -305_556 N
O4 Ok Dg1 133.2(11) -303_565 . 1_555 N
O4 Ok Dg1 104.2(17) -303_565 . -108_665 N
O4 Ok Dg1 93.6(12) -303_565 . -305_565 N
O4 Ok Dg2 137.8(9) -303_566 . 1_555 N
O4 Ok Dg2 92.6(7) -303_566 . 111_555 N
O4 Ok Dg2 87.0(13) -303_566 . -108_666 N
O4 Ok Dg2 69.0(9) -303_566 . -305_566 N
SJ Ok Og 89.0(14) -108_656 . 1_555 N
SJ Ok Og 152.8(18) -108_656 . 111_545 N
SJ Ok Og 51.6(12) -108_656 . -108_656 N
SJ Ok Og 47.9(15) -108_656 . -201_555 N
SJ Ok Og 56.1(16) -108_656 . -305_556 N
SJ Ok Dg1 78.8(14) -108_665 . 1_555 N
SJ Ok Dg1 44.3(14) -108_665 . -108_665 N
SJ Ok Dg1 49.6(15) -108_665 . -305_565 N
SJ Ok Dg2 91.7(14) -108_666 . 1_555 N
SJ Ok Dg2 151.6(17) -108_666 . 111_555 N
SJ Ok Dg2 63.5(14) -108_666 . -108_666 N
SJ Ok Dg2 52.2(16) -108_666 . -305_566 N
Og Ok Og 116.1(8) 1_555 . 111_545 N
Og Ok Og 43.2(7) 1_555 . -108_656 N
Og Ok Og 73.0(6) 1_555 . -201_555 N
Og Ok Og 88.3(10) 1_555 . -305_556 N
Og Ok Dg1 10.47(34) 1_555 . 1_555 N
Og Ok Dg1 46.9(11) 1_555 . -108_665 N
Og Ok Dg1 77.7(7) 1_555 . -305_565 N
Og Ok Dg2 12.60(15) 1_555 . 1_555 N
Og Ok Dg2 119.3(9) 1_555 . 111_555 N
Og Ok Dg2 59.9(10) 1_555 . -108_666 N
Og Ok Dg2 108.8(10) 1_555 . -305_566 N
Og Ok Og 155.5(15) 111_545 . -108_656 N
Og Ok Og 126.8(6) 111_545 . -201_555 N
Og Ok Og 111.3(9) 111_545 . -305_556 N
Og Ok Dg1 126.6(10) 111_554 . 1_555 N
Og Ok Dg1 152.6(15) 111_554 . -108_665 N
Og Ok Dg1 122.5(9) 111_554 . -305_565 N
Og Ok Dg2 115.2(8) 111_555 . 1_555 N
Og Ok Dg2 11.94(9) 111_555 . 111_555 N
Og Ok Dg2 137.1(19) 111_555 . -108_666 N
Og Ok Dg2 106.4(8) 111_555 . -305_566 N
Og Ok Og 66.4(11) -108_656 . -201_555 N
Og Ok Og 84.4(15) -108_656 . -305_556 N
Og Ok Dg1 33.2(7) -108_665 . 1_555 N
Og Ok Dg1 30.2(5) -108_665 . -108_665 N
Og Ok Dg1 71.6(12) -108_665 . -305_565 N
Og Ok Dg2 41.4(8) -108_666 . 1_555 N
Og Ok Dg2 151.2(16) -108_666 . 111_555 N
Og Ok Dg2 29.9(5) -108_666 . -108_666 N
Og Ok Dg2 94.9(15) -108_666 . -305_566 N
Og Ok Og 18.3(5) -201_555 . -305_556 N
Og Ok Dg1 67.7(7) -201_564 . 1_555 N
Og Ok Dg1 36.7(12) -201_564 . -108_665 N
Og Ok Dg1 5.4(4) -201_564 . -305_565 N
Og Ok Dg2 83.8(6) -201_565 . 1_555 N
Og Ok Dg2 138.1(7) -201_565 . 111_555 N
Og Ok Dg2 94.3(15) -201_565 . -108_666 N
Og Ok Dg2 36.0(5) -201_565 . -305_566 N
Og Ok Dg1 84.6(10) -305_565 . 1_555 N
Og Ok Dg1 55.0(14) -305_565 . -108_665 N
Og Ok Dg1 12.9(5) -305_565 . -305_565 N
Og Ok Dg2 100.0(10) -305_566 . 1_555 N
Og Ok Dg2 121.8(9) -305_566 . 111_555 N
Og Ok Dg2 111.2(18) -305_566 . -108_666 N
Og Ok Dg2 21.6(4) -305_566 . -305_566 N
Dg1 Ok Dg1 37.9(12) 1_555 . -108_665 N
Dg1 Ok Dg1 72.8(10) 1_555 . -305_565 N
Dg1 Ok Dg2 16.3(5) 1_555 . 1_555 N
Dg1 Ok Dg2 129.4(10) 1_555 . 111_555 N
Dg1 Ok Dg2 53.2(10) 1_555 . -108_666 N
Dg1 Ok Dg2 103.6(12) 1_555 . -305_566 N
Dg1 Ok Dg1 42.0(12) -108_665 . -305_565 N
Dg1 Ok Dg2 53.7(11) -108_666 . 1_555 N
Dg1 Ok Dg2 162.6(15) -108_666 . 111_555 N
Dg1 Ok Dg2 59.7(10) -108_666 . -108_666 N
Dg1 Ok Dg2 69.2(16) -108_666 . -305_566 N
Dg1 Ok Dg2 88.8(7) -305_566 . 1_555 N
Dg1 Ok Dg2 133.6(9) -305_566 . 111_555 N
Dg1 Ok Dg2 99.2(16) -305_566 . -108_666 N
Dg1 Ok Dg2 31.1(5) -305_566 . -305_566 N
Dg2 Ok Dg2 115.6(9) 1_555 . 111_555 N
Dg2 Ok Dg2 51.1(10) 1_555 . -108_666 N
Dg2 Ok Dg2 119.7(10) 1_555 . -305_566 N
Dg2 Ok Dg2 127.1(19) 111_555 . -108_666 N
Dg2 Ok Dg2 113.8(8) 111_555 . -305_566 N
Dg2 Ok Dg2 115.2(18) -108_666 . -305_566 N
O1 Dk1 O1 110.6(12) -12_554 . 111_433 N
O1 Dk1 O2 38.0(5) -12_554 . -108_544 N
O1 Dk1 O2 85.3(9) -12_554 . -109_544 N
O1 Dk1 O4 75.8(8) -12_554 . 106_554 N
O1 Dk1 O4 53.7(8) -12_554 . -303_444 N
O1 Dk1 SJ 75.8(17) -12_666 . -108_656 N
O1 Dk1 Og 135.8(12) -12_666 . 1_555 N
O1 Dk1 Og 112.2(9) -12_666 . 111_545 N
O1 Dk1 Og 107.7(14) -12_666 . -108_656 N
O1 Dk1 Og 68.8(7) -12_666 . -201_555 N
O1 Dk1 Og 61.2(13) -12_666 . -305_556 N
O1 Dk1 Dg1 127.6(13) -12_675 . 1_555 N
O1 Dk1 Dg1 101.1(17) -12_675 . -108_665 N
O1 Dk1 Dg1 67.8(10) -12_675 . -305_565 N
O1 Dk1 Dg2 110.4(15) -12_676 . -108_666 N
O1 Dk1 Dg2 31.3(7) -12_676 . -305_566 N
O1 Dk1 Oh 162.6(15) -12_675 . 1_555 N
O1 Dk1 Oh 65.4(10) -12_675 . -108_665 N
O1 Dk1 Oh 72.2(9) -12_675 . -305_565 N
O1 Dk1 Dh1 148.3(14) -12_654 . 1_555 N
O1 Dk1 Dh1 82.7(12) -12_654 . -108_644 N
O1 Dk1 Dh1 75.3(12) -12_654 . -305_544 N
O1 Dk1 Dh2 154.3(15) -12_654 . 1_555 N
O1 Dk1 Dh2 58.8(11) -12_654 . -108_644 N
O1 Dk1 O2 86.8(8) 111_433 . -108_544 N
O1 Dk1 O2 40.0(4) 111_433 . -109_544 N
O1 Dk1 O4 75.0(7) 111_433 . 106_554 N
O1 Dk1 O4 57.1(6) 111_433 . -303_444 N
O1 Dk1 SJ 62.0(12) 111_545 . -108_656 N
O1 Dk1 Og 75.2(7) 111_545 . 1_555 N
O1 Dk1 Og 85.9(9) 111_545 . 111_545 N
O1 Dk1 Og 55.6(7) 111_545 . -108_656 N
O1 Dk1 Og 125.2(10) 111_545 . -201_555 N
O1 Dk1 Og 127.7(19) 111_545 . -305_556 N
O1 Dk1 Dg1 71.8(8) 111_554 . 1_555 N
O1 Dk1 Dg1 73.3(11) 111_554 . -108_665 N
O1 Dk1 Dg1 122.8(14) 111_554 . -305_565 N
O1 Dk1 Dg2 34.0(5) 111_555 . -108_666 N
O1 Dk1 Dg2 124.6(18) 111_555 . -305_566 N
O1 Dk1 Oh 67.2(8) 111_554 . 1_555 N
O1 Dk1 Oh 72.7(9) 111_554 . -108_665 N
O1 Dk1 Oh 161.3(13) 111_554 . -305_565 N
O1 Dk1 Dh1 75.9(9) 111_533 . 1_555 N
O1 Dk1 Dh1 67.6(9) 111_533 . -108_644 N
O1 Dk1 Dh1 152.2(16) 111_533 . -305_544 N
O1 Dk1 Dh2 51.7(7) 111_533 . 1_555 N
O1 Dk1 Dh2 65.5(10) 111_533 . -108_644 N
O2 Dk1 O2 51.0(4) -108_544 . -109_544 N
O2 Dk1 O4 39.20(35) -108_544 . 106_554 N
O2 Dk1 O4 38.6(5) -108_544 . -303_444 N
O2 Dk1 SJ 88.8(17) -108_656 . -108_656 N
O2 Dk1 Og 156.1(10) -108_656 . 1_555 N
O2 Dk1 Og 81.8(6) -108_656 . 111_545 N
O2 Dk1 Og 118.4(12) -108_656 . -108_656 N
O2 Dk1 Og 106.7(9) -108_656 . -201_555 N
O2 Dk1 Og 99.1(16) -108_656 . -305_556 N
O2 Dk1 Dg1 146.9(11) -108_665 . 1_555 N
O2 Dk1 Dg1 123.1(18) -108_665 . -108_665 N
O2 Dk1 Dg1 105.5(13) -108_665 . -305_565 N
O2 Dk1 Dg2 106.5(12) -108_666 . -108_666 N
O2 Dk1 Dg2 69.3(11) -108_666 . -305_566 N
O2 Dk1 Oh 151.7(12) -108_665 . 1_555 N
O2 Dk1 Oh 83.8(10) -108_665 . -108_665 N
O2 Dk1 Oh 103.8(10) -108_665 . -305_565 N
O2 Dk1 Dh1 162.5(10) -108_644 . 1_555 N
O2 Dk1 Dh1 100.4(12) -108_644 . -108_644 N
O2 Dk1 Dh1 109.6(13) -108_644 . -305_544 N
O2 Dk1 Dh2 137.7(10) -108_644 . 1_555 N
O2 Dk1 Dh2 69.4(10) -108_644 . -108_644 N
O2 Dk1 O4 36.82(31) -109_544 . 106_554 N
O2 Dk1 O4 40.4(5) -109_544 . -303_444 N
O2 Dk1 SJ 82.7(14) -109_656 . -108_656 N
O2 Dk1 Og 114.9(7) -109_656 . 1_555 N
O2 Dk1 Og 66.7(6) -109_656 . 111_545 N
O2 Dk1 Og 92.0(9) -109_656 . -108_656 N
O2 Dk1 Og 142.6(11) -109_656 . -201_555 N
O2 Dk1 Og 138.2(20) -109_656 . -305_556 N
O2 Dk1 Dg1 111.7(8) -109_665 . 1_555 N
O2 Dk1 Dg1 108.3(13) -109_665 . -108_665 N
O2 Dk1 Dg1 139.9(15) -109_665 . -305_565 N
O2 Dk1 Dg2 71.1(8) -109_666 . -108_666 N
O2 Dk1 Dg2 113.5(15) -109_666 . -305_566 N
O2 Dk1 Oh 100.7(10) -109_665 . 1_555 N
O2 Dk1 Oh 88.1(9) -109_665 . -108_665 N
O2 Dk1 Oh 154.6(12) -109_665 . -305_565 N
O2 Dk1 Dh1 113.1(9) -109_644 . 1_555 N
O2 Dk1 Dh1 93.6(10) -109_644 . -108_644 N
O2 Dk1 Dh1 160.4(16) -109_644 . -305_544 N
O2 Dk1 Dh2 87.1(8) -109_644 . 1_555 N
O2 Dk1 Dh2 73.2(9) -109_644 . -108_644 N
O4 Dk1 O4 60.5(7) 106_554 . -303_444 N
O4 Dk1 SJ 114.0(17) 106_554 . -108_656 N
O4 Dk1 Og 143.2(10) 106_554 . 1_555 N
O4 Dk1 Og 44.6(4) 106_554 . 111_545 N
O4 Dk1 Og 128.9(11) 106_554 . -108_656 N
O4 Dk1 Og 143.5(10) 106_554 . -201_555 N
O4 Dk1 Og 135.8(18) 106_554 . -305_556 N
O4 Dk1 Dg1 144.6(10) 106_554 . 1_555 N
O4 Dk1 Dg1 144.6(15) 106_554 . -108_665 N
O4 Dk1 Dg1 143.2(14) 106_554 . -305_565 N
O4 Dk1 Dg2 107.8(11) 106_554 . -108_666 N
O4 Dk1 Dg2 106.6(14) 106_554 . -305_566 N
O4 Dk1 Oh 118.6(12) 106_554 . 1_555 N
O4 Dk1 Oh 114.7(11) 106_554 . -108_665 N
O4 Dk1 Oh 122.8(10) 106_554 . -305_565 N
O4 Dk1 Dh1 134.4(12) 106_554 . 1_555 N
O4 Dk1 Dh1 126.3(12) 106_554 . -108_644 N
O4 Dk1 Dh1 131.7(13) 106_554 . -305_544 N
O4 Dk1 Dh2 111.1(11) 106_554 . 1_555 N
O4 Dk1 Dh2 98.4(11) 106_554 . -108_644 N
O4 Dk1 SJ 54.6(13) -303_556 . -108_656 N
O4 Dk1 Og 117.6(10) -303_556 . 1_555 N
O4 Dk1 Og 102.9(10) -303_556 . 111_545 N
O4 Dk1 Og 80.5(11) -303_556 . -108_656 N
O4 Dk1 Og 102.5(12) -303_556 . -201_555 N
O4 Dk1 Og 97.8(20) -303_556 . -305_556 N
O4 Dk1 Dg1 108.8(11) -303_565 . 1_555 N
O4 Dk1 Dg1 88.9(15) -303_565 . -108_665 N
O4 Dk1 Dg1 100.0(15) -303_565 . -305_565 N
O4 Dk1 Dg2 68.4(10) -303_566 . -108_666 N
O4 Dk1 Dg2 75.4(14) -303_566 . -305_566 N
O4 Dk1 Oh 122.6(12) -303_565 . 1_555 N
O4 Dk1 Oh 54.3(9) -303_565 . -108_665 N
O4 Dk1 Oh 123.9(15) -303_565 . -305_565 N
O4 Dk1 Dh1 125.5(12) -303_544 . 1_555 N
O4 Dk1 Dh1 67.0(10) -303_544 . -108_644 N
O4 Dk1 Dh1 124.0(18) -303_544 . -305_544 N
O4 Dk1 Dh2 106.9(10) -303_544 . 1_555 N
O4 Dk1 Dh2 38.0(7) -303_544 . -108_644 N
SJ Dk1 Og 69.0(14) -108_656 . 1_555 N
SJ Dk1 Og 147.0(17) -108_656 . 111_545 N
SJ Dk1 Og 32.7(10) -108_656 . -108_656 N
SJ Dk1 Og 65.5(13) -108_656 . -201_555 N
SJ Dk1 Og 66.3(17) -108_656 . -305_556 N
SJ Dk1 Dg1 59.1(13) -108_665 . 1_555 N
SJ Dk1 Dg1 34.8(10) -108_665 . -108_665 N
SJ Dk1 Dg1 62.7(15) -108_665 . -305_565 N
SJ Dk1 Dg2 38.0(10) -108_666 . -108_666 N
SJ Dk1 Dg2 68.1(18) -108_666 . -305_566 N
SJ Dk1 Oh 88.7(16) -108_665 . 1_555 N
SJ Dk1 Oh 12.0(11) -108_665 . -108_665 N
SJ Dk1 Oh 102.3(17) -108_665 . -305_565 N
SJ Dk1 Dh1 81.0(15) -108_644 . 1_555 N
SJ Dk1 Dh1 12.5(10) -108_644 . -108_644 N
SJ Dk1 Dh1 95.1(19) -108_644 . -305_544 N
SJ Dk1 Dh2 79.0(15) -108_644 . 1_555 N
SJ Dk1 Dh2 19.5(12) -108_644 . -108_644 N
Og Dk1 Og 112.0(10) 1_555 . 111_545 N
Og Dk1 Og 37.9(6) 1_555 . -108_656 N
Og Dk1 Og 72.8(6) 1_555 . -201_555 N
Og Dk1 Og 80.3(14) 1_555 . -305_556 N
Og Dk1 Dg1 9.87(27) 1_555 . 1_555 N
Og Dk1 Dg1 36.6(11) 1_555 . -108_665 N
Og Dk1 Dg1 72.7(10) 1_555 . -305_565 N
Og Dk1 Dg2 50.3(7) 1_555 . -108_666 N
Og Dk1 Dg2 108.1(14) 1_555 . -305_566 N
Og Dk1 Oh 27.2(6) 1_555 . 1_555 N
Og Dk1 Oh 75.9(9) 1_555 . -108_665 N
Og Dk1 Oh 89.9(9) 1_555 . -305_565 N
Og Dk1 Dh1 13.1(6) 1_555 . 1_555 N
Og Dk1 Dh1 58.4(8) 1_555 . -108_644 N
Og Dk1 Dh1 82.0(11) 1_555 . -305_544 N
Og Dk1 Dh2 32.0(6) 1_555 . 1_555 N
Og Dk1 Dh2 88.5(11) 1_555 . -108_644 N
Og Dk1 Og 132.2(13) 111_545 . -108_656 N
Og Dk1 Og 147.5(8) 111_545 . -201_555 N
Og Dk1 Og 146.4(16) 111_545 . -305_556 N
Og Dk1 Dg1 120.1(11) 111_554 . 1_555 N
Og Dk1 Dg1 145.4(17) 111_554 . -108_665 N
Og Dk1 Dg1 150.3(12) 111_554 . -305_565 N
Og Dk1 Dg2 115.5(13) 111_555 . -108_666 N
Og Dk1 Dg2 134.8(14) 111_555 . -305_566 N
Og Dk1 Oh 85.2(11) 111_554 . 1_555 N
Og Dk1 Oh 154.7(11) 111_554 . -108_665 N
Og Dk1 Oh 110.7(10) 111_554 . -305_565 N
Og Dk1 Dh1 99.1(11) 111_533 . 1_555 N
Og Dk1 Dh1 153.1(12) 111_533 . -108_644 N
Og Dk1 Dh1 117.9(14) 111_533 . -305_544 N
Og Dk1 Dh2 87.0(12) 111_533 . 1_555 N
Og Dk1 Dh2 139.6(12) 111_533 . -108_644 N
Og Dk1 Og 72.0(9) -108_656 . -201_555 N
Og Dk1 Og 77.0(15) -108_656 . -305_556 N
Og Dk1 Dg1 28.5(6) -108_665 . 1_555 N
Og Dk1 Dg1 17.8(5) -108_665 . -108_665 N
Og Dk1 Dg1 70.1(12) -108_665 . -305_565 N
Og Dk1 Dg2 21.67(32) -108_666 . -108_666 N
Og Dk1 Dg2 92.5(16) -108_666 . -305_566 N
Og Dk1 Oh 56.1(8) -108_665 . 1_555 N
Og Dk1 Oh 42.4(8) -108_665 . -108_665 N
Og Dk1 Oh 105.7(13) -108_665 . -305_565 N
Og Dk1 Dh1 48.9(9) -108_644 . 1_555 N
Og Dk1 Dh1 25.3(7) -108_644 . -108_644 N
Og Dk1 Dh1 96.6(14) -108_644 . -305_544 N
Og Dk1 Dh2 48.1(8) -108_644 . 1_555 N
Og Dk1 Dh2 51.7(10) -108_644 . -108_644 N
Og Dk1 Og 7.7(9) -201_555 . -305_556 N
Og Dk1 Dg1 69.1(7) -201_564 . 1_555 N
Og Dk1 Dg1 54.6(10) -201_564 . -108_665 N
Og Dk1 Dg1 2.9(6) -201_564 . -305_565 N
Og Dk1 Dg2 92.6(11) -201_565 . -108_666 N
Og Dk1 Dg2 37.5(8) -201_565 . -305_566 N
Og Dk1 Oh 97.9(10) -201_564 . 1_555 N
Og Dk1 Oh 57.1(7) -201_564 . -108_665 N
Og Dk1 Oh 37.2(6) -201_564 . -305_565 N
Og Dk1 Dh1 82.1(8) -201_543 . 1_555 N
Og Dk1 Dh1 57.9(8) -201_543 . -108_644 N
Og Dk1 Dh1 29.6(10) -201_543 . -305_544 N
Og Dk1 Dh2 104.6(10) -201_543 . 1_555 N
Og Dk1 Dh2 70.4(10) -201_543 . -108_644 N
Og Dk1 Dg1 76.4(14) -305_565 . 1_555 N
Og Dk1 Dg1 60.0(14) -305_565 . -108_665 N
Og Dk1 Dg1 7.8(7) -305_565 . -305_565 N
Og Dk1 Dg2 96.6(18) -305_566 . -108_666 N
Og Dk1 Dg2 29.9(8) -305_566 . -305_566 N
Og Dk1 Oh 105.6(17) -305_565 . 1_555 N
Og Dk1 Oh 56.7(13) -305_565 . -108_665 N
Og Dk1 Oh 36.2(10) -305_565 . -305_565 N
Og Dk1 Dh1 89.8(15) -305_544 . 1_555 N
Og Dk1 Dh1 60.2(14) -305_544 . -108_644 N
Og Dk1 Dh1 30.2(11) -305_544 . -305_544 N
Og Dk1 Dh2 112.0(17) -305_544 . 1_555 N
Og Dk1 Dh2 68.4(16) -305_544 . -108_644 N
Dg1 Dk1 Dg1 27.1(11) 1_555 . -108_665 N
Dg1 Dk1 Dg1 68.6(11) 1_555 . -305_565 N
Dg1 Dk1 Dg2 43.3(7) 1_555 . -108_666 N
Dg1 Dk1 Dg2 102.1(15) 1_555 . -305_566 N
Dg1 Dk1 Oh 35.0(6) 1_555 . 1_555 N
Dg1 Dk1 Oh 66.2(9) 1_555 . -108_665 N
Dg1 Dk1 Oh 91.7(10) 1_555 . -305_565 N
Dg1 Dk1 Dh1 22.6(7) 1_555 . 1_555 N
Dg1 Dk1 Dh1 48.5(8) 1_555 . -108_644 N
Dg1 Dk1 Dh1 83.1(12) 1_555 . -305_544 N
Dg1 Dk1 Dh2 35.9(7) 1_555 . 1_555 N
Dg1 Dk1 Dh2 78.6(11) 1_555 . -108_644 N
Dg1 Dk1 Dg1 52.9(12) -108_665 . -305_565 N
Dg1 Dk1 Dg2 39.4(7) -108_666 . -108_666 N
Dg1 Dk1 Dg2 79.5(17) -108_666 . -305_566 N
Dg1 Dk1 Oh 61.5(13) -108_665 . 1_555 N
Dg1 Dk1 Oh 39.7(11) -108_665 . -108_665 N
Dg1 Dk1 Oh 87.9(13) -108_665 . -305_565 N
Dg1 Dk1 Dh1 49.6(13) -108_644 . 1_555 N
Dg1 Dk1 Dh1 22.8(10) -108_644 . -108_644 N
Dg1 Dk1 Dh1 78.9(15) -108_644 . -305_544 N
Dg1 Dk1 Dh2 58.4(12) -108_644 . 1_555 N
Dg1 Dk1 Dh2 53.8(13) -108_644 . -108_644 N
Dg1 Dk1 Dg2 90.4(14) -305_566 . -108_666 N
Dg1 Dk1 Dg2 36.7(7) -305_566 . -305_566 N
Dg1 Dk1 Oh 98.3(13) -305_565 . 1_555 N
Dg1 Dk1 Oh 54.3(10) -305_565 . -108_665 N
Dg1 Dk1 Oh 39.9(7) -305_565 . -305_565 N
Dg1 Dk1 Dh1 82.4(11) -305_544 . 1_555 N
Dg1 Dk1 Dh1 55.3(11) -305_544 . -108_644 N
Dg1 Dk1 Dh1 32.5(10) -305_544 . -305_544 N
Dg1 Dk1 Dh2 104.3(13) -305_544 . 1_555 N
Dg1 Dk1 Dh2 67.6(13) -305_544 . -108_644 N
Dg2 Dk1 Dg2 105.8(18) -108_666 . -305_566 N
Dg2 Dk1 Oh 57.5(9) -108_665 . 1_555 N
Dg2 Dk1 Oh 49.9(9) -108_665 . -108_665 N
Dg2 Dk1 Oh 127.3(15) -108_665 . -305_565 N
Dg2 Dk1 Dh1 57.1(10) -108_644 . 1_555 N
Dg2 Dk1 Dh1 37.9(9) -108_644 . -108_644 N
Dg2 Dk1 Dh1 118.2(16) -108_644 . -305_544 N
Dg2 Dk1 Dh2 44.1(8) -108_644 . 1_555 N
Dg2 Dk1 Dh2 51.9(11) -108_644 . -108_644 N
Dg2 Dk1 Oh 134.7(18) -305_565 . 1_555 N
Dg2 Dk1 Oh 56.1(12) -305_565 . -108_665 N
Dg2 Dk1 Oh 49.0(9) -305_565 . -305_565 N
Dg2 Dk1 Dh1 118.8(16) -305_544 . 1_555 N
Dg2 Dk1 Dh1 68.8(14) -305_544 . -108_644 N
Dg2 Dk1 Dh1 48.7(11) -305_544 . -305_544 N
Dg2 Dk1 Dh2 137.5(18) -305_544 . 1_555 N
Dg2 Dk1 Dh2 59.5(14) -305_544 . -108_644 N
Oh Dk1 Oh 98.3(12) 1_555 . -108_665 N
Oh Dk1 Oh 104.3(14) 1_555 . -305_565 N
Oh Dk1 Dh1 15.8(4) 1_555 . 1_555 N
Oh Dk1 Dh1 80.6(11) 1_555 . -108_644 N
Oh Dk1 Dh1 98.7(15) 1_555 . -305_544 N
Oh Dk1 Dh2 15.76(33) 1_555 . 1_555 N
Oh Dk1 Dh2 107.0(13) 1_555 . -108_644 N
Oh Dk1 Oh 92.9(12) -108_665 . -305_565 N
Oh Dk1 Dh1 88.7(12) -108_644 . 1_555 N
Oh Dk1 Dh1 17.79(27) -108_644 . -108_644 N
Oh Dk1 Dh1 86.5(14) -108_644 . -305_544 N
Oh Dk1 Dh2 89.9(11) -108_644 . 1_555 N
Oh Dk1 Dh2 16.3(4) -108_644 . -108_644 N
Oh Dk1 Dh1 92.3(11) -305_544 . 1_555 N
Oh Dk1 Dh1 95.0(12) -305_544 . -108_644 N
Oh Dk1 Dh1 9.1(8) -305_544 . -305_544 N
Oh Dk1 Dh2 118.3(13) -305_544 . 1_555 N
Oh Dk1 Dh2 103.4(14) -305_544 . -108_644 N
Dh1 Dk1 Dh1 71.0(12) 1_555 . -108_644 N
Dh1 Dk1 Dh1 85.6(14) 1_555 . -305_544 N
Dh1 Dk1 Dh2 26.11(34) 1_555 . 1_555 N
Dh1 Dk1 Dh2 100.4(13) 1_555 . -108_644 N
Dh1 Dk1 Dh1 86.9(16) -108_644 . -305_544 N
Dh1 Dk1 Dh2 73.4(11) -108_644 . 1_555 N
Dh1 Dk1 Dh2 31.0(6) -108_644 . -108_644 N
Dh1 Dk1 Dh2 111.7(16) -305_544 . 1_555 N
Dh1 Dk1 Dh2 98.6(17) -305_544 . -108_644 N
Dh2 Dk1 Dh2 95.5(13) 1_555 . -108_644 N
O1 Dk2 O1 108.4(11) 4_555 . -12_554 N
O1 Dk2 O1 80.8(12) 4_555 . 111_433 N
O1 Dk2 O2 70.9(6) 4_555 . 1_555 N
O1 Dk2 O2 44.2(5) 4_555 . -109_544 N
O1 Dk2 O3 83.4(9) 4_555 . 4_555 N
O1 Dk2 O3 49.2(5) 4_555 . 208_343 N
O1 Dk2 O4 40.1(5) 4_555 . 106_554 N
O1 Dk2 O4 96.5(9) 4_555 . 312_334 N
O1 Dk2 O4 94.2(12) 4_555 . -303_444 N
O1 Dk2 Og 141.9(12) 4_555 . 1_555 N
O1 Dk2 Og 42.5(5) 4_555 . 111_545 N
O1 Dk2 Og 153.6(16) 4_555 . -108_656 N
O1 Dk2 Og 143.0(13) 4_555 . -305_556 N
O1 Dk2 Dg1 150.7(13) 4_555 . 1_555 N
O1 Dk2 Dg1 170.6(20) 4_555 . -108_665 N
O1 Dk2 Dg1 151.2(12) 4_555 . -305_565 N
O1 Dk2 Dg2 28.5(4) 4_555 . 111_555 N
O1 Dk2 Dg2 135.8(19) 4_555 . -108_666 N
O1 Dk2 Dg2 129.5(13) 4_555 . -305_566 N
O1 Dk2 Oh 122.3(16) 4_555 . 1_555 N
O1 Dk2 Oh 56.5(6) 4_555 . 111_554 N
O1 Dk2 Oh 139.0(15) 4_555 . -108_665 N
O1 Dk2 Dh1 135.3(15) 4_555 . 1_555 N
O1 Dk2 Dh1 53.3(8) 4_555 . 111_533 N
O1 Dk2 O1 107.0(18) -12_554 . 111_433 N
O1 Dk2 O2 126.8(12) -12_554 . 1_555 N
O1 Dk2 O2 82.8(10) -12_554 . -109_544 N
O1 Dk2 O3 74.6(8) -12_554 . 4_555 N
O1 Dk2 O3 151.7(14) -12_554 . 208_343 N
O1 Dk2 O4 68.6(7) -12_554 . 106_554 N
O1 Dk2 O4 144.0(13) -12_554 . 312_334 N
O1 Dk2 O4 37.2(5) -12_554 . -303_444 N
O1 Dk2 Og 109.5(8) -12_666 . 1_555 N
O1 Dk2 Og 99.9(9) -12_666 . 111_545 N
O1 Dk2 Og 81.3(10) -12_666 . -108_656 N
O1 Dk2 Og 39.8(5) -12_666 . -305_556 N
O1 Dk2 Dg1 100.7(9) -12_675 . 1_555 N
O1 Dk2 Dg1 66.6(9) -12_675 . -108_665 N
O1 Dk2 Dg1 46.0(5) -12_675 . -305_565 N
O1 Dk2 Dg2 104.7(10) -12_676 . 111_555 N
O1 Dk2 Dg2 86.1(14) -12_676 . -108_666 N
O1 Dk2 Dg2 23.3(4) -12_676 . -305_566 N
O1 Dk2 Oh 125.0(13) -12_675 . 1_555 N
O1 Dk2 Oh 124.9(10) -12_675 . 111_554 N
O1 Dk2 Oh 49.7(6) -12_675 . -108_665 N
O1 Dk2 Dh1 113.4(11) -12_654 . 1_555 N
O1 Dk2 Dh1 112.5(10) -12_654 . 111_533 N
O1 Dk2 O2 20.6(7) 111_433 . 1_555 N
O1 Dk2 O2 54.2(11) 111_433 . -109_544 N
O1 Dk2 O3 33.4(10) 111_433 . 4_555 N
O1 Dk2 O3 57.7(9) 111_433 . 208_343 N
O1 Dk2 O4 96.2(16) 111_433 . 106_554 N
O1 Dk2 O4 51.0(9) 111_433 . 312_334 N
O1 Dk2 O4 70.8(16) 111_433 . -303_444 N
O1 Dk2 Og 91.6(14) 111_545 . 1_555 N
O1 Dk2 Og 122.6(14) 111_545 . 111_545 N
O1 Dk2 Og 72.9(14) 111_545 . -108_656 N
O1 Dk2 Og 120.7(19) 111_545 . -305_556 N
O1 Dk2 Dg1 87.6(14) 111_554 . 1_555 N
O1 Dk2 Dg1 93.0(17) 111_554 . -108_665 N
O1 Dk2 Dg1 116.0(16) 111_554 . -305_565 N
O1 Dk2 Dg2 108.7(14) 111_555 . 111_555 N
O1 Dk2 Dg2 55.0(13) 111_555 . -108_666 N
O1 Dk2 Dg2 116.2(19) 111_555 . -305_566 N
O1 Dk2 Oh 101.1(17) 111_554 . 1_555 N
O1 Dk2 Oh 119.5(14) 111_554 . 111_554 N
O1 Dk2 Oh 76.0(14) 111_554 . -108_665 N
O1 Dk2 Dh1 101.1(16) 111_533 . 1_555 N
O1 Dk2 Dh1 126.3(15) 111_533 . 111_533 N
O2 Dk2 O2 59.6(6) 1_555 . -109_544 N
O2 Dk2 O3 52.3(5) 1_555 . 4_555 N
O2 Dk2 O3 37.8(4) 1_555 . 208_343 N
O2 Dk2 O4 98.1(9) 1_555 . 106_554 N
O2 Dk2 O4 39.1(4) 1_555 . 312_334 N
O2 Dk2 O4 89.9(11) 1_555 . -303_444 N
O2 Dk2 Og 89.1(8) 1_555 . 1_555 N
O2 Dk2 Og 108.8(8) 1_555 . 111_545 N
O2 Dk2 Og 83.6(11) 1_555 . -108_656 N
O2 Dk2 Og 138.3(13) 1_555 . -305_556 N
O2 Dk2 Dg1 89.1(9) 1_555 . 1_555 N
O2 Dk2 Dg1 105.3(13) 1_555 . -108_665 N
O2 Dk2 Dg1 132.0(11) 1_555 . -305_565 N
O2 Dk2 Dg2 95.8(8) 1_555 . 111_555 N
O2 Dk2 Dg2 67.3(12) 1_555 . -108_666 N
O2 Dk2 Dg2 136.5(14) 1_555 . -305_566 N
O2 Dk2 Oh 91.0(11) 1_555 . 1_555 N
O2 Dk2 Oh 99.7(8) 1_555 . 111_554 N
O2 Dk2 Oh 94.7(10) 1_555 . -108_665 N
O2 Dk2 Dh1 95.3(10) 1_555 . 1_555 N
O2 Dk2 Dh1 108.0(9) 1_555 . 111_533 N
O2 Dk2 O3 40.9(6) -109_544 . 4_555 N
O2 Dk2 O3 68.9(7) -109_544 . 208_343 N
O2 Dk2 O4 42.0(5) -109_544 . 106_554 N
O2 Dk2 O4 98.6(10) -109_544 . 312_334 N
O2 Dk2 O4 54.0(8) -109_544 . -303_444 N
O2 Dk2 Og 145.7(12) -109_656 . 1_555 N
O2 Dk2 Og 81.0(8) -109_656 . 111_545 N
O2 Dk2 Og 116.4(16) -109_656 . -108_656 N
O2 Dk2 Og 121.5(15) -109_656 . -305_556 N
O2 Dk2 Dg1 140.3(15) -109_665 . 1_555 N
O2 Dk2 Dg1 126.5(18) -109_665 . -108_665 N
O2 Dk2 Dg1 125.5(14) -109_665 . -305_565 N
O2 Dk2 Dg2 69.0(7) -109_666 . 111_555 N
O2 Dk2 Dg2 100.1(19) -109_666 . -108_666 N
O2 Dk2 Dg2 105.5(13) -109_666 . -305_566 N
O2 Dk2 Oh 149.5(15) -109_665 . 1_555 N
O2 Dk2 Oh 100.7(9) -109_665 . 111_554 N
O2 Dk2 Oh 95.1(12) -109_665 . -108_665 N
O2 Dk2 Dh1 154.6(14) -109_644 . 1_555 N
O2 Dk2 Dh1 96.0(10) -109_644 . 111_533 N
O3 Dk2 O3 84.6(9) 4_555 . 208_343 N
O3 Dk2 O4 77.1(8) 4_555 . 106_554 N
O3 Dk2 O4 83.2(9) 4_555 . 312_334 N
O3 Dk2 O4 37.7(6) 4_555 . -303_444 N
O3 Dk2 Og 110.0(10) 4_555 . 1_555 N
O3 Dk2 Og 121.8(11) 4_555 . 111_545 N
O3 Dk2 Og 75.5(11) 4_555 . -108_656 N
O3 Dk2 Og 99.1(12) 4_555 . -305_556 N
O3 Dk2 Dg1 101.4(11) 4_555 . 1_555 N
O3 Dk2 Dg1 87.6(14) 4_555 . -108_665 N
O3 Dk2 Dg1 98.2(10) 4_555 . -305_565 N
O3 Dk2 Dg2 109.8(10) 4_555 . 111_555 N
O3 Dk2 Dg2 59.9(14) 4_555 . -108_666 N
O3 Dk2 Dg2 88.7(11) 4_555 . -305_566 N
O3 Dk2 Oh 127.7(14) 4_555 . 1_555 N
O3 Dk2 Oh 138.5(10) 4_555 . 111_554 N
O3 Dk2 Oh 58.9(8) 4_555 . -108_665 N
O3 Dk2 Dh1 122.2(13) 4_555 . 1_555 N
O3 Dk2 Dh1 136.5(11) 4_555 . 111_533 N
O3 Dk2 O4 88.5(9) 208_343 . 106_554 N
O3 Dk2 O4 47.6(5) 208_343 . 312_334 N
O3 Dk2 O4 118.6(15) 208_343 . -303_444 N
O3 Dk2 Og 95.4(10) 208_455 . 1_555 N
O3 Dk2 Og 74.9(8) 208_455 . 111_545 N
O3 Dk2 Og 112.1(14) 208_455 . -108_656 N
O3 Dk2 Og 167.3(16) 208_455 . -305_556 N
O3 Dk2 Dg1 102.1(12) 208_464 . 1_555 N
O3 Dk2 Dg1 132.4(16) 208_464 . -108_665 N
O3 Dk2 Dg1 159.5(13) 208_464 . -305_565 N
O3 Dk2 Dg2 64.4(7) 208_465 . 111_555 N
O3 Dk2 Dg2 100.0(15) 208_465 . -108_666 N
O3 Dk2 Dg2 173.4(18) 208_465 . -305_566 N
O3 Dk2 Oh 82.9(12) 208_464 . 1_555 N
O3 Dk2 Oh 61.9(8) 208_464 . 111_554 N
O3 Dk2 Oh 132.0(13) 208_464 . -108_665 N
O3 Dk2 Dh1 93.7(12) 208_443 . 1_555 N
O3 Dk2 Dh1 70.5(9) 208_443 . 111_533 N
O4 Dk2 O4 133.5(10) 106_554 . 312_334 N
O4 Dk2 O4 64.9(9) 106_554 . -303_444 N
O4 Dk2 Og 172.2(12) 106_554 . 1_555 N
O4 Dk2 Og 49.1(5) 106_554 . 111_545 N
O4 Dk2 Og 143.6(17) 106_554 . -108_656 N
O4 Dk2 Og 104.2(10) 106_554 . -305_556 N
O4 Dk2 Dg1 169.2(12) 106_554 . 1_555 N
O4 Dk2 Dg1 135.0(15) 106_554 . -108_665 N
O4 Dk2 Dg1 112.0(9) 106_554 . -305_565 N
O4 Dk2 Dg2 43.7(5) 106_554 . 111_555 N
O4 Dk2 Dg2 134.8(21) 106_554 . -108_666 N
O4 Dk2 Dg2 89.5(9) 106_554 . -305_566 N
O4 Dk2 Oh 152.4(18) 106_554 . 1_555 N
O4 Dk2 Oh 78.1(8) 106_554 . 111_554 N
O4 Dk2 Oh 109.8(12) 106_554 . -108_665 N
O4 Dk2 Dh1 160.8(16) 106_554 . 1_555 N
O4 Dk2 Dh1 67.5(8) 106_554 . 111_533 N
O4 Dk2 O4 117.7(15) 312_334 . -303_444 N
O4 Dk2 Og 52.5(6) 312_446 . 1_555 N
O4 Dk2 Og 116.0(11) 312_446 . 111_545 N
O4 Dk2 Og 65.7(9) 312_446 . -108_656 N
O4 Dk2 Og 120.5(12) 312_446 . -305_556 N
O4 Dk2 Dg1 56.1(8) 312_455 . 1_555 N
O4 Dk2 Dg1 84.8(12) 312_455 . -108_665 N
O4 Dk2 Dg1 112.2(10) 312_455 . -305_565 N
O4 Dk2 Dg2 109.4(10) 312_456 . 111_555 N
O4 Dk2 Dg2 58.1(12) 312_456 . -108_666 N
O4 Dk2 Dg2 132.1(12) 312_456 . -305_566 N
O4 Dk2 Oh 52.0(9) 312_455 . 1_555 N
O4 Dk2 Oh 90.4(10) 312_455 . 111_554 N
O4 Dk2 Oh 94.5(11) 312_455 . -108_665 N
O4 Dk2 Dh1 56.6(8) 312_434 . 1_555 N
O4 Dk2 Dh1 103.2(11) 312_434 . 111_533 N
O4 Dk2 Og 118.5(12) -303_556 . 1_555 N
O4 Dk2 Og 112.7(13) -303_556 . 111_545 N
O4 Dk2 Og 78.8(12) -303_556 . -108_656 N
O4 Dk2 Og 69.2(9) -303_556 . -305_556 N
O4 Dk2 Dg1 107.3(12) -303_565 . 1_555 N
O4 Dk2 Dg1 77.1(13) -303_565 . -108_665 N
O4 Dk2 Dg1 71.8(9) -303_565 . -305_565 N
O4 Dk2 Dg2 108.5(13) -303_566 . 111_555 N
O4 Dk2 Dg2 72.3(15) -303_566 . -108_666 N
O4 Dk2 Dg2 55.0(7) -303_566 . -305_566 N
O4 Dk2 Oh 141.5(17) -303_565 . 1_555 N
O4 Dk2 Oh 142.8(14) -303_565 . 111_554 N
O4 Dk2 Oh 46.4(7) -303_565 . -108_665 N
O4 Dk2 Dh1 129.1(15) -303_544 . 1_555 N
O4 Dk2 Dh1 130.9(14) -303_544 . 111_533 N
Og Dk2 Og 125.5(13) 1_555 . 111_545 N
Og Dk2 Og 40.0(7) 1_555 . -108_656 N
Og Dk2 Og 71.9(9) 1_555 . -305_556 N
Og Dk2 Dg1 11.22(30) 1_555 . 1_555 N
Og Dk2 Dg1 44.5(8) 1_555 . -108_665 N
Og Dk2 Dg1 64.5(7) 1_555 . -305_565 N
Og Dk2 Dg2 132.8(14) 1_555 . 111_555 N
Og Dk2 Dg2 51.2(11) 1_555 . -108_666 N
Og Dk2 Dg2 87.4(9) 1_555 . -305_566 N
Og Dk2 Oh 23.1(7) 1_555 . 1_555 N
Og Dk2 Oh 97.7(11) 1_555 . 111_554 N
Og Dk2 Oh 72.5(8) 1_555 . -108_665 N
Og Dk2 Dh1 12.4(7) 1_555 . 1_555 N
Og Dk2 Dh1 107.4(13) 1_555 . 111_533 N
Og Dk2 Og 162.5(17) 111_545 . -108_656 N
Og Dk2 Og 112.5(12) 111_545 . -305_556 N
Og Dk2 Dg1 135.7(15) 111_554 . 1_555 N
Og Dk2 Dg1 144.4(16) 111_554 . -108_665 N
Og Dk2 Dg1 119.2(11) 111_554 . -305_565 N
Og Dk2 Dg2 14.03(19) 111_555 . 111_555 N
Og Dk2 Dg2 174.0(18) 111_555 . -108_666 N
Og Dk2 Dg2 108.4(10) 111_555 . -305_566 N
Og Dk2 Oh 103.3(16) 111_554 . 1_555 N
Og Dk2 Oh 30.2(5) 111_554 . 111_554 N
Og Dk2 Oh 149.5(12) 111_554 . -108_665 N
Og Dk2 Dh1 113.2(16) 111_533 . 1_555 N
Og Dk2 Dh1 18.4(5) 111_533 . 111_533 N
Og Dk2 Og 57.8(9) -108_656 . -305_556 N
Og Dk2 Dg1 29.0(6) -108_665 . 1_555 N
Og Dk2 Dg1 21.8(4) -108_665 . -108_665 N
Og Dk2 Dg1 50.1(8) -108_665 . -305_565 N
Og Dk2 Dg2 172.7(18) -108_666 . 111_555 N
Og Dk2 Dg2 18.0(5) -108_666 . -108_666 N
Og Dk2 Dg2 66.5(9) -108_666 . -305_566 N
Og Dk2 Oh 63.1(11) -108_665 . 1_555 N
Og Dk2 Oh 137.7(17) -108_665 . 111_554 N
Og Dk2 Oh 34.4(7) -108_665 . -108_665 N
Og Dk2 Dh1 51.8(10) -108_644 . 1_555 N
Og Dk2 Dh1 146.6(18) -108_644 . 111_533 N
Og Dk2 Dg1 65.3(8) -305_565 . 1_555 N
Og Dk2 Dg1 36.6(7) -305_565 . -108_665 N
Og Dk2 Dg1 8.2(4) -305_565 . -305_565 N
Og Dk2 Dg2 124.5(12) -305_566 . 111_555 N
Og Dk2 Dg2 72.0(12) -305_566 . -108_666 N
Og Dk2 Dg2 16.43(25) -305_566 . -305_566 N
Og Dk2 Oh 85.3(13) -305_565 . 1_555 N
Og Dk2 Oh 119.0(13) -305_565 . 111_554 N
Og Dk2 Oh 44.7(7) -305_565 . -108_665 N
Og Dk2 Dh1 74.0(10) -305_544 . 1_555 N
Og Dk2 Dh1 113.0(13) -305_544 . 111_533 N
Dg1 Dk2 Dg1 34.4(8) 1_555 . -108_665 N
Dg1 Dk2 Dg1 57.4(8) 1_555 . -305_565 N
Dg1 Dk2 Dg2 143.9(16) 1_555 . 111_555 N
Dg1 Dk2 Dg2 41.6(10) 1_555 . -108_666 N
Dg1 Dk2 Dg2 79.7(9) 1_555 . -305_566 N
Dg1 Dk2 Oh 34.3(8) 1_555 . 1_555 N
Dg1 Dk2 Oh 108.8(13) 1_555 . 111_554 N
Dg1 Dk2 Oh 61.3(8) 1_555 . -108_665 N
Dg1 Dk2 Dh1 22.8(8) 1_555 . 1_555 N
Dg1 Dk2 Dh1 118.0(15) 1_555 . 111_533 N
Dg1 Dk2 Dg1 28.5(7) -108_665 . -305_565 N
Dg1 Dk2 Dg2 158.3(17) -108_666 . 111_555 N
Dg1 Dk2 Dg2 38.4(8) -108_666 . -108_666 N
Dg1 Dk2 Dg2 47.6(8) -108_666 . -305_566 N
Dg1 Dk2 Oh 65.6(12) -108_665 . 1_555 N
Dg1 Dk2 Oh 132.8(17) -108_665 . 111_554 N
Dg1 Dk2 Oh 31.8(9) -108_665 . -108_665 N
Dg1 Dk2 Dh1 52.6(11) -108_644 . 1_555 N
Dg1 Dk2 Dh1 135.5(18) -108_644 . 111_533 N
Dg1 Dk2 Dg2 131.8(12) -305_566 . 111_555 N
Dg1 Dk2 Dg2 64.9(12) -305_566 . -108_666 N
Dg1 Dk2 Dg2 23.02(28) -305_566 . -305_566 N
Dg1 Dk2 Oh 79.3(11) -305_565 . 1_555 N
Dg1 Dk2 Oh 121.9(12) -305_565 . 111_554 N
Dg1 Dk2 Oh 41.0(6) -305_565 . -108_665 N
Dg1 Dk2 Dh1 67.4(9) -305_544 . 1_555 N
Dg1 Dk2 Dh1 117.6(12) -305_544 . 111_533 N
Dg2 Dk2 Dg2 163.1(18) 111_555 . -108_666 N
Dg2 Dk2 Dg2 117.7(11) 111_555 . -305_566 N
Dg2 Dk2 Oh 109.7(17) 111_554 . 1_555 N
Dg2 Dk2 Oh 35.2(5) 111_554 . 111_554 N
Dg2 Dk2 Oh 152.7(14) 111_554 . -108_665 N
Dg2 Dk2 Dh1 121.2(17) 111_533 . 1_555 N
Dg2 Dk2 Dh1 27.2(6) 111_533 . 111_533 N
Dg2 Dk2 Dg2 77.0(13) -108_666 . -305_566 N
Dg2 Dk2 Oh 72.7(14) -108_665 . 1_555 N
Dg2 Dk2 Oh 144.4(20) -108_665 . 111_554 N
Dg2 Dk2 Oh 36.4(10) -108_665 . -108_665 N
Dg2 Dk2 Dh1 63.6(14) -108_644 . 1_555 N
Dg2 Dk2 Dh1 156.8(21) -108_644 . 111_533 N
Dg2 Dk2 Oh 101.7(13) -305_565 . 1_555 N
Dg2 Dk2 Oh 123.8(12) -305_565 . 111_554 N
Dg2 Dk2 Oh 43.3(7) -305_565 . -108_665 N
Dg2 Dk2 Dh1 90.2(11) -305_544 . 1_555 N
Dg2 Dk2 Dh1 114.4(11) -305_544 . 111_533 N
Oh Dk2 Oh 74.7(14) 1_555 . 111_554 N
Oh Dk2 Oh 95.3(14) 1_555 . -108_665 N
Oh Dk2 Dh1 13.0(6) 1_555 . 1_555 N
Oh Dk2 Dh1 84.9(16) 1_555 . 111_533 N
Oh Dk2 Oh 162.5(13) 111_554 . -108_665 N
Oh Dk2 Dh1 86.1(14) 111_533 . 1_555 N
Oh Dk2 Dh1 13.03(20) 111_533 . 111_533 N
Oh Dk2 Dh1 82.7(12) -108_644 . 1_555 N
Oh Dk2 Dh1 157.4(12) -108_644 . 111_533 N
Dh1 Dk2 Dh1 95.3(16) 1_555 . 111_533 N
O4 SIII O4 101.4(30) -10_554 . -12_554 N
O4 SIII Oi 125.6(10) -10_553 . 4_555 N
O4 SIII Oi 119.9(9) -10_553 . -301_443 N
O4 SIII Di2 147.0(20) -10_544 . 4_555 N
O4 SIII Di2 105.2(12) -10_544 . -301_434 N
O4 SIII Ok 64.7(9) -10_544 . 107_423 N
O4 SIII Ok 152.6(25) -10_544 . -205_444 N
O4 SIII Dk1 74.6(14) -10_666 . 107_545 N
O4 SIII Dk1 176(4) -10_666 . -205_566 N
O4 SIII Dk2 77.4(16) -10_766 . 107_645 N
O4 SIII Dk2 132.6(19) -10_766 . -205_666 N
O4 SIII Oi 119.9(9) -12_553 . 4_555 N
O4 SIII Oi 125.6(10) -12_553 . -301_443 N
O4 SIII Di2 105.2(12) -12_544 . 4_555 N
O4 SIII Di2 147.0(20) -12_544 . -301_434 N
O4 SIII Ok 152.6(25) -12_544 . 107_423 N
O4 SIII Ok 64.7(9) -12_544 . -205_444 N
O4 SIII Dk1 176(4) -12_666 . 107_545 N
O4 SIII Dk1 74.6(14) -12_666 . -205_566 N
O4 SIII Dk2 132.6(19) -12_766 . 107_645 N
O4 SIII Dk2 77.4(16) -12_766 . -205_666 N
Oi SIII Oi 63.0(25) 4_555 . -301_443 N
Oi SIII Di2 21.5(10) 4_555 . 4_555 N
Oi SIII Di2 56.5(28) 4_555 . -301_434 N
Oi SIII Ok 86.2(27) 4_555 . 107_423 N
Oi SIII Ok 56.4(17) 4_555 . -205_444 N
Oi SIII Dk1 63.3(25) 4_555 . 107_545 N
Oi SIII Dk1 57.5(24) 4_555 . -205_566 N
Oi SIII Dk2 96(4) 4_555 . 107_645 N
Oi SIII Dk2 44.0(21) 4_555 . -205_666 N
Oi SIII Di2 56.5(28) -301_434 . 4_555 N
Oi SIII Di2 21.5(10) -301_434 . -301_434 N
Oi SIII Ok 56.4(17) -301_434 . 107_423 N
Oi SIII Ok 86.2(27) -301_434 . -205_444 N
Oi SIII Dk1 57.5(24) -301_556 . 107_545 N
Oi SIII Dk1 63.3(25) -301_556 . -205_566 N
Oi SIII Dk2 44.0(21) -301_656 . 107_645 N
Oi SIII Dk2 96(4) -301_656 . -205_666 N
Di2 SIII Di2 59(4) 4_555 . -301_434 N
Di2 SIII Ok 97(4) 4_555 . 107_423 N
Di2 SIII Ok 40.9(16) 4_555 . -205_444 N
Di2 SIII Dk1 79(4) 4_555 . 107_545 N
Di2 SIII Dk1 36.3(19) 4_555 . -205_566 N
Di2 SIII Dk2 98(4) 4_555 . 107_645 N
Di2 SIII Dk2 39.9(21) 4_555 . -205_666 N
Di2 SIII Ok 40.9(16) -301_434 . 107_423 N
Di2 SIII Ok 97(4) -301_434 . -205_444 N
Di2 SIII Dk1 36.3(19) -301_556 . 107_545 N
Di2 SIII Dk1 79(4) -301_556 . -205_566 N
Di2 SIII Dk2 39.9(21) -301_656 . 107_645 N
Di2 SIII Dk2 98(4) -301_656 . -205_666 N
Ok SIII Ok 137(4) 107_423 . -205_444 N
Ok SIII Dk1 25.4(5) 107_545 . 107_545 N
Ok SIII Dk1 119(4) 107_545 . -205_566 N
Ok SIII Dk2 25.6(5) 107_645 . 107_645 N
Ok SIII Dk2 130(4) 107_645 . -205_666 N
Ok SIII Dk1 119(4) -205_566 . 107_545 N
Ok SIII Dk1 25.4(5) -205_566 . -205_566 N
Ok SIII Dk2 130(4) -205_666 . 107_645 N
Ok SIII Dk2 25.6(5) -205_666 . -205_666 N
Dk1 SIII Dk1 109(5) 107_545 . -205_566 N
Dk1 SIII Dk2 47.1(12) 107_645 . 107_645 N
Dk1 SIII Dk2 105.2(34) 107_645 . -205_666 N
Dk1 SIII Dk2 105.2(34) -205_666 . 107_645 N
Dk1 SIII Dk2 47.1(12) -205_666 . -205_666 N
Dk2 SIII Dk2 138(6) 107_645 . -205_666 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si1 O1 1.572(9) . 1_555 N
Si1 O2 1.568(8) . -206_454 N
Si1 O3 1.778(8) . 2_555 N
Si1 O4 1.630(8) . 209_555 N
Si2 O1 1.753(10) . -1_555 N
Si2 O2 1.780(9) . -105_544 N
Si2 O3 1.595(9) . 3_555 N
Si2 O4 1.682(9) . 107_555 N
Al1 O1 1.753(10) . -1_555 N
Al1 O2 1.780(9) . -105_544 N
Al1 O3 1.595(9) . 3_555 N
Al1 O4 1.682(9) . 107_555 N
O1 Si1 1.572(9) . 1_555 N
O1 Si2 1.753(10) . -1_555 N
O1 Al1 1.753(10) . -1_555 N
O1 O1 3.7404(32) . -2_555 N
O1 O1 3.7404(32) . -3_555 N
O1 O2 2.781(8) . 105_544 N
O1 O2 2.622(8) . -206_454 N
O1 O2 4.602(7) . 304_445 N
O1 O2 4.642(7) . -304_445 N
O1 O3 2.718(7) . 2_555 N
O1 O3 2.825(7) . -3_555 N
O1 O4 2.796(9) . -107_443 N
O1 O4 4.627(10) . -111_434 N
O1 O4 4.649(10) . 208_555 N
O1 O4 2.626(9) . 209_555 N
O1 Og 2.716(13) . -2_555 N
O1 Og 4.315(14) . 212_544 N
O1 Og 4.611(15) . -206_454 N
O1 Dg1 3.176(17) . -2_555 N
O1 Dg1 3.957(21) . -206_454 N
O1 Dg2 1.763(12) . -2_555 N
O1 Oh 3.718(23) . -2_555 N
O1 Oh 3.367(25) . -206_454 N
O1 Dh1 3.385(29) . -2_555 N
O1 Dh1 3.992(29) . -206_454 N
O1 Dh2 3.143(32) . -2_555 N
O1 Dh2 2.839(32) . -206_454 N
O1 OII* 4.840(17) . -105_544 N
O1 OII* 4.987(16) . -107_443 N
O1 DII*1 4.12(5) . 312_555 N
O1 DII*2 4.42(7) . -105_544 N
O1 Oi 4.884(28) . 3_555 N
O1 Oi 4.965(27) . -2_555 N
O1 Oi 3.366(24) . 105_544 N
O1 Oi 3.611(24) . -206_454 N
O1 Di1 3.25(4) . 105_544 N
O1 Di1 4.191(27) . -206_454 N
O1 Di2 3.937(26) . 3_555 N
O1 Di2 4.458(29) . -2_555 N
O1 Di2 3.15(4) . 105_544 N
O1 Di2 3.865(31) . -206_454 N
O1 Ok 3.665(34) . -112_534 N
O1 Ok 2.273(34) . -206_454 N
O1 Ok 4.436(33) . 304_445 N
O1 Dk1 3.10(4) . -112_534 N
O1 Dk1 3.132(31) . -206_454 N
O1 Dk2 4.23(4) . -112_534 N
O1 Dk2 1.90(4) . -206_454 N
O1 Dk2 3.54(4) . 304_445 N
O2 Si1 1.568(8) . 111_555 N
O2 Si2 1.780(9) . 208_555 N
O2 Al1 1.780(9) . 208_555 N
O2 O1 4.602(7) . 4_555 N
O2 O1 2.622(8) . 111_555 N
O2 O1 2.781(8) . -108_544 N
O2 O1 4.642(7) . -304_445 N
O2 O2 3.762(6) . 107_555 N
O2 O2 3.924(6) . -109_543 N
O2 O2 3.762(6) . 209_555 N
O2 O2 3.924(6) . -207_453 N
O2 O2 3.686(7) . -304_445 N
O2 O3 4.553(7) . 2_555 N
O2 O3 4.695(7) . 3_555 N
O2 O3 3.758(4) . 4_555 N
O2 O3 2.767(7) . 111_555 N
O2 O3 2.655(7) . 208_555 N
O2 O4 2.870(7) . 310_555 N
O2 O4 2.726(7) . 312_555 N
O2 SI' 2.303(4) . 111_555 N
O2 Og 4.773(15) . -108_544 N
O2 Dg2 3.991(16) . -108_544 N
O2 Dg2 4.207(15) . -304_445 N
O2 Oh 4.995(25) . 1_555 N
O2 Dh2 4.132(25) . 1_555 N
O2 Dh2 4.357(24) . -304_445 N
O2 OII' 4.939(10) . 1_555 N
O2 OII' 3.804(5) . 107_555 N
O2 OII' 3.746(5) . -105_544 N
O2 DII'1 4.163(24) . 2_555 N
O2 DII'1 4.460(32) . 107_555 N
O2 DII'1 3.51(5) . 209_555 N
O2 DII'1 2.897(13) . -206_454 N
O2 DII'1 4.27(4) . 310_555 N
O2 DII'1 3.30(5) . 312_555 N
O2 DII'2 4.239(18) . 3_555 N
O2 DII'2 3.96(5) . 107_555 N
O2 DII'2 3.690(29) . -105_544 N
O2 DII'2 4.251(29) . 209_555 N
O2 DII'2 4.366(22) . -206_454 N
O2 DII'2 3.811(33) . 310_555 N
O2 DII'2 4.11(4) . 312_555 N
O2 Oi 4.468(24) . 1_555 N
O2 Di2 4.17(4) . 1_555 N
O2 Ok 4.82(4) . 1_555 N
O2 Ok 4.594(27) . 105_544 N
O2 Ok 3.963(30) . -207_453 N
O2 Dk1 4.24(4) . 105_544 N
O2 Dk1 4.319(34) . -207_453 N
O2 Dk2 4.32(4) . 1_555 N
O2 Dk2 3.43(5) . -207_453 N
O3 Si1 1.778(8) . 3_555 N
O3 Si2 1.595(9) . 2_555 N
O3 Al1 1.595(9) . 2_555 N
O3 O1 2.718(7) . 3_555 N
O3 O1 2.825(7) . -2_555 N
O3 O2 4.695(7) . 2_555 N
O3 O2 4.553(7) . 3_555 N
O3 O2 2.655(7) . -105_544 N
O3 O2 2.767(7) . -206_454 N
O3 O2 3.758(4) . 304_445 N
O3 O3 3.809(5) . 107_555 N
O3 O3 3.809(5) . 209_555 N
O3 O4 2.658(7) . 111_555 N
O3 O4 2.636(7) . 208_555 N
O3 SII 2.328(4) . 111_555 N
O3 Og 4.354(14) . 3_555 N
O3 Og 4.810(13) . -1_555 N
O3 Dg2 3.650(16) . 3_555 N
O3 Dg2 4.007(14) . -1_555 N
O3 Oh 3.911(22) . 3_555 N
O3 Oh 3.778(25) . -105_544 N
O3 Dh1 4.182(27) . 3_555 N
O3 Dh2 3.292(28) . 3_555 N
O3 Dh2 3.210(29) . -105_544 N
O3 OII' 4.923(9) . 107_555 N
O3 OII' 3.185(14) . 111_555 N
O3 OII' 4.906(8) . -105_544 N
O3 DII'1 2.767(34) . 111_555 N
O3 DII'1 3.855(26) . 208_555 N
O3 DII'1 4.48(4) . 209_555 N
O3 DII'1 4.039(18) . 310_555 N
O3 DII'1 3.480(34) . -304_445 N
O3 DII'2 4.43(4) . 107_555 N
O3 DII'2 4.041(19) . 111_555 N
O3 DII'2 3.693(19) . 208_555 N
O3 DII'2 4.302(27) . 312_555 N
O3 DII'2 3.943(28) . -304_445 N
O3 OII* 3.714(29) . 111_555 N
O3 DII*1 4.41(4) . 111_555 N
O3 DII*1 3.51(7) . 208_555 N
O3 DII*1 3.97(7) . -304_445 N
O3 DII*2 4.25(5) . 111_555 N
O3 DII*2 3.84(6) . -304_445 N
O3 Oi 3.571(24) . 304_445 N
O3 Di1 3.449(31) . 304_445 N
O3 Di2 4.042(33) . 304_445 N
O3 Ok 4.06(4) . -105_544 N
O3 Ok 4.229(27) . 304_445 N
O3 Ok 4.963(30) . -308_345 N
O3 Dk2 3.206(34) . -105_544 N
O3 Dk2 4.21(5) . 304_445 N
O4 Si1 1.630(8) . 107_555 N
O4 Si2 1.682(9) . 209_555 N
O4 Al1 1.682(9) . 209_555 N
O4 O1 4.627(10) . 6_555 N
O4 O1 2.626(9) . 107_555 N
O4 O1 4.649(10) . -105_544 N
O4 O1 2.796(9) . -309_445 N
O4 O2 2.870(7) . 310_555 N
O4 O2 2.726(7) . 312_555 N
O4 O3 2.636(7) . -105_544 N
O4 O3 2.658(7) . -206_454 N
O4 O4 3.788(7) . -304_445 N
O4 SJ 2.167(18) . 312_555 N
O4 Og 3.291(14) . 6_555 N
O4 Og 3.395(13) . 312_555 N
O4 Dg1 3.977(16) . 6_555 N
O4 Dg1 3.258(22) . 312_555 N
O4 Dg2 2.862(18) . 6_555 N
O4 Dg2 2.844(18) . 312_555 N
O4 Oh 4.913(24) . -102_544 N
O4 Oh 2.678(22) . 312_555 N
O4 Dh1 4.430(29) . 6_555 N
O4 Dh1 3.101(25) . 312_555 N
O4 Dh2 1.720(21) . 312_555 N
O4 OII' 3.966(14) . 1_555 N
O4 DII'1 4.06(4) . 1_555 N
O4 DII'1 3.581(32) . 3_555 N
O4 DII'1 4.360(34) . 208_555 N
O4 DII'2 4.468(32) . 2_555 N
O4 OII* 3.879(24) . 1_555 N
O4 DII*1 4.13(5) . 1_555 N
O4 DII*1 3.49(8) . 2_555 N
O4 DII*2 4.29(4) . 2_555 N
O4 DII*2 3.84(7) . 3_555 N
O4 Oi 4.297(25) . -102_544 N
O4 Oi 4.100(24) . -203_454 N
O4 Oi 4.089(26) . 310_555 N
O4 Oi 4.203(25) . 312_555 N
O4 Di1 4.494(27) . -102_544 N
O4 Di1 3.42(4) . -203_454 N
O4 Di1 4.40(4) . 310_555 N
O4 Di2 4.354(34) . -203_454 N
O4 Di2 3.285(34) . 310_555 N
O4 Di2 3.927(28) . 312_555 N
O4 Ok 2.502(27) . -102_544 N
O4 Ok 3.692(34) . 312_555 N
O4 Ok 4.533(26) . -311_435 N
O4 Dk1 2.66(4) . -102_544 N
O4 Dk1 4.31(4) . -311_435 N
O4 Dk2 2.77(5) . -102_544 N
O4 Dk2 3.37(4) . 312_555 N
O4 Dk2 4.02(4) . -311_435 N
O4 SIII 2.45(5) . -112_534 N
SI' O2 2.303(4) . -105_544 N
SI' O2 2.303(4) . -206_454 N
SI' O2 2.303(4) . -304_445 N
SII O3 2.328(4) . -105_544 N
SII O3 2.328(4) . -206_454 N
SII O3 2.328(4) . -304_445 N
SII OII* 2.23(4) . 1_555 N
SJ O4 2.167(18) . 312_555 N
SJ Og 1.497(24) . 1_555 N
SJ Og 1.799(21) . -108_544 N
SJ Dg1 1.110(26) . 1_555 N
SJ Dg2 1.485(26) . 1_555 N
SJ Oh 1.541(26) . 1_555 N
SJ Dh1 1.36(4) . 1_555 N
SJ Dh2 1.19(4) . 1_555 N
SJ Ok 1.324(34) . 105_544 N
SJ Dk1 1.68(4) . 105_544 N
Og O1 2.716(13) . -3_555 N
Og O1 4.611(15) . 111_555 N
Og O1 4.315(14) . 212_544 N
Og O2 4.773(15) . 105_544 N
Og O3 4.354(14) . 2_555 N
Og O3 4.810(13) . -1_555 N
Og O4 3.291(14) . -111_434 N
Og O4 3.395(13) . 312_555 N
Og SJ 1.497(24) . 1_555 N
Og SJ 1.799(21) . 105_544 N
Og Og 2.735(17) . 105_544 N
Og Og 2.735(17) . -108_544 N
Og Og 4.308(23) . 308_544 N
Og Og 4.308(23) . -305_444 N
Og Dg1 0.959980(10) . 1_555 N
Og Dg1 1.800(19) . 105_544 N
Og Dg1 2.952(22) . -108_544 N
Og Dg1 3.574(23) . 308_544 N
Og Dg1 4.272(25) . -305_444 N
Og Dg2 0.960770(10) . 1_555 N
Og Dg2 3.035(18) . 105_544 N
Og Dg2 3.305(17) . -108_544 N
Og Oh 2.134(26) . 1_555 N
Og Oh 2.626(23) . 105_544 N
Og Oh 4.648(28) . -108_544 N
Og Oh 3.721(25) . 308_544 N
Og Dh1 1.259(29) . 1_555 N
Og Dh1 2.56(4) . 105_544 N
Og Dh1 3.706(29) . -108_544 N
Og Dh1 3.721(33) . 308_544 N
Og Dh2 2.282(33) . 1_555 N
Og Dh2 2.529(34) . 105_544 N
Og Dh2 4.245(30) . 308_544 N
Og OII* 4.144(12) . -105_544 N
Og DII*1 3.59(5) . -105_544 N
Og DII*1 4.152(34) . -208_344 N
Og DII*1 3.93(5) . 312_555 N
Og DII*2 3.89(4) . -105_544 N
Og DII*2 3.71(5) . 209_555 N
Og DII*2 4.34(5) . 304_445 N
Og Oi 4.729(26) . 1_555 N
Og Oi 3.435(28) . -2_555 N
Og Oi 2.855(27) . 105_544 N
Og Oi 4.394(26) . -109_543 N
Og Oi 3.703(26) . -304_445 N
Og Di1 3.468(31) . -2_555 N
Og Di1 3.665(31) . 105_544 N
Og Di1 3.497(29) . -109_543 N
Og Di1 3.22(4) . -304_445 N
Og Di2 2.614(30) . -2_555 N
Og Di2 3.340(34) . 105_544 N
Og Di2 4.441(30) . -109_543 N
Og Di2 3.24(4) . -304_445 N
Og Ok 3.789(30) . 1_555 N
Og Ok 1.899(27) . 105_544 N
Og Ok 4.70(4) . -201_453 N
Og Ok 4.626(31) . -206_454 N
Og Ok 2.16(4) . 308_544 N
Og Dk1 4.27(4) . 1_555 N
Og Dk1 2.60(4) . 105_544 N
Og Dk1 4.33(4) . -201_453 N
Og Dk1 4.36(4) . -206_454 N
Og Dk1 1.62(4) . 308_544 N
Og Dk2 4.15(4) . 1_555 N
Og Dk2 2.58(4) . 105_544 N
Og Dk2 3.90(4) . -206_454 N
Og Dk2 3.02(4) . 308_544 N
Dg1 O1 3.176(17) . -3_555 N
Dg1 O1 3.957(21) . 111_555 N
Dg1 O4 3.977(16) . -111_434 N
Dg1 O4 3.258(22) . 312_555 N
Dg1 SJ 1.110(26) . 1_555 N
Dg1 Og 0.959980(10) . 1_555 N
Dg1 Og 2.952(22) . 105_544 N
Dg1 Og 1.800(19) . -108_544 N
Dg1 Og 4.272(25) . 308_544 N
Dg1 Og 3.574(23) . -305_444 N
Dg1 Dg1 2.063(20) . 105_544 N
Dg1 Dg1 2.063(20) . -108_544 N
Dg1 Dg1 3.560(34) . 308_544 N
Dg1 Dg1 3.560(34) . -305_444 N
Dg1 Dg2 1.51866 . 1_555 N
Dg1 Dg2 3.497(27) . 105_544 N
Dg1 Dg2 2.471(24) . -108_544 N
Dg1 Oh 2.060(29) . 1_555 N
Dg1 Oh 2.643(29) . 105_544 N
Dg1 Oh 3.693(28) . -108_544 N
Dg1 Oh 4.154(29) . 308_544 N
Dg1 Dh1 1.38(4) . 1_555 N
Dg1 Dh1 2.57(4) . 105_544 N
Dg1 Dh1 2.750(30) . -108_544 N
Dg1 Dh1 3.93(4) . 308_544 N
Dg1 Dh2 2.15(4) . 1_555 N
Dg1 Dh2 2.873(35) . 105_544 N
Dg1 OII* 4.418(22) . -105_544 N
Dg1 DII*1 3.70(5) . -105_544 N
Dg1 DII*2 3.85(5) . 209_555 N
Dg1 Oi 3.962(30) . 1_555 N
Dg1 Oi 4.260(30) . -2_555 N
Dg1 Oi 3.657(29) . 105_544 N
Dg1 Oi 4.068(31) . -109_543 N
Dg1 Oi 3.337(31) . -304_445 N
Dg1 Di1 3.27(4) . -109_543 N
Dg1 Di1 2.97(4) . -304_445 N
Dg1 Di2 3.506(32) . -2_555 N
Dg1 Di2 3.934(34) . -109_543 N
Dg1 Di2 2.74(4) . -304_445 N
Dg1 Ok 3.057(31) . 1_555 N
Dg1 Ok 1.562(35) . 105_544 N
Dg1 Ok 2.94(4) . 308_544 N
Dg1 Dk1 3.59(4) . 1_555 N
Dg1 Dk1 1.94(4) . 105_544 N
Dg1 Dk1 2.54(4) . 308_544 N
Dg1 Dk2 3.55(4) . 1_555 N
Dg1 Dk2 2.44(4) . 105_544 N
Dg1 Dk2 3.85(4) . 308_544 N
Dg2 O1 1.763(12) . -3_555 N
Dg2 O2 3.991(16) . 105_544 N
Dg2 O2 4.207(15) . -304_445 N
Dg2 O3 3.650(16) . 2_555 N
Dg2 O3 4.007(14) . -1_555 N
Dg2 O4 2.862(18) . -111_434 N
Dg2 O4 2.844(18) . 312_555 N
Dg2 SJ 1.485(26) . 1_555 N
Dg2 Og 0.96077 . 1_555 N
Dg2 Og 3.305(17) . 105_544 N
Dg2 Og 3.035(18) . -108_544 N
Dg2 Dg1 1.51866 . 1_555 N
Dg2 Dg1 2.471(24) . 105_544 N
Dg2 Dg1 3.497(27) . -108_544 N
Dg2 Dg2 3.454(15) . 105_544 N
Dg2 Dg2 3.454(15) . -108_544 N
Dg2 Oh 2.431(27) . 1_555 N
Dg2 Oh 2.612(26) . 105_544 N
Dg2 Dh1 1.811(31) . 1_555 N
Dg2 Dh1 2.88(4) . 105_544 N
Dg2 Dh2 2.20(4) . 1_555 N
Dg2 Dh2 2.34(4) . 105_544 N
Dg2 OII* 4.254(17) . -105_544 N
Dg2 DII*1 3.81(6) . -105_544 N
Dg2 DII*1 3.92(4) . -208_344 N
Dg2 DII*2 4.00(6) . 209_555 N
Dg2 Oi 3.871(32) . -2_555 N
Dg2 Oi 2.916(32) . 105_544 N
Dg2 Oi 3.293(31) . -304_445 N
Dg2 Di1 3.674(32) . 105_544 N
Dg2 Di1 3.856(31) . -109_543 N
Dg2 Di1 2.92(4) . -304_445 N
Dg2 Di2 2.950(33) . -2_555 N
Dg2 Di2 3.36(4) . 105_544 N
Dg2 Di2 2.86(5) . -304_445 N
Dg2 Ok 4.188(33) . 1_555 N
Dg2 Ok 1.486(34) . 105_544 N
Dg2 Ok 4.44(4) . -206_454 N
Dg2 Ok 2.55(4) . 308_544 N
Dg2 Dk1 2.39(4) . 105_544 N
Dg2 Dk1 1.93(5) . 308_544 N
Dg2 Dk2 1.91(5) . 105_544 N
Dg2 Dk2 3.61(5) . -206_454 N
Dg2 Dk2 3.34(4) . 308_544 N
Oh O1 3.718(23) . -3_555 N
Oh O1 3.367(25) . 111_555 N
Oh O2 4.995(25) . 1_555 N
Oh O3 3.911(22) . 2_555 N
Oh O3 3.778(25) . 208_555 N
Oh O4 2.678(22) . 312_555 N
Oh O4 4.913(24) . -303_445 N
Oh SJ 1.541(26) . 1_555 N
Oh Og 2.134(26) . 1_555 N
Oh Og 4.648(28) . 105_544 N
Oh Og 2.626(23) . -108_544 N
Oh Og 3.721(25) . -305_444 N
Oh Dg1 2.060(29) . 1_555 N
Oh Dg1 3.693(28) . 105_544 N
Oh Dg1 2.643(29) . -108_544 N
Oh Dg1 4.154(29) . -305_444 N
Oh Dg2 2.431(27) . 1_555 N
Oh Dg2 2.612(26) . -108_544 N
Oh Oh 4.603(33) . 105_544 N
Oh Oh 4.271(34) . 111_555 N
Oh Oh 4.603(33) . -108_544 N
Oh Oh 4.271(34) . -206_454 N
Oh Oh 4.87(4) . 308_544 N
Oh Oh 4.87(4) . -305_444 N
Oh Dh1 0.96 . 1_555 N
Oh Dh1 4.46(5) . 111_555 N
Oh Dh1 3.81(4) . -108_544 N
Oh Dh1 4.04(4) . -305_444 N
Oh Dh2 0.96077 . 1_555 N
Oh Dh2 4.48(4) . -108_544 N
Oh OII* 2.466(19) . -105_544 N
Oh DII*1 1.67(4) . -105_544 N
Oh DII*1 3.288(28) . 209_555 N
Oh DII*1 2.71(5) . 312_555 N
Oh DII*2 2.64(4) . -105_544 N
Oh DII*2 1.87(6) . 209_555 N
Oh DII*2 3.221(32) . 312_555 N
Oh Oi 4.36(4) . -2_555 N
Oh Oi 2.902(35) . 105_544 N
Oh Oi 4.226(33) . -108_544 N
Oh Oi 2.375(33) . -109_543 N
Oh Oi 4.949(31) . -304_445 N
Oh Di1 4.49(4) . -2_555 N
Oh Di1 3.21(4) . 105_544 N
Oh Di1 1.430(34) . -109_543 N
Oh Di2 3.77(4) . -2_555 N
Oh Di2 3.80(4) . 105_544 N
Oh Di2 4.13(4) . -108_544 N
Oh Di2 2.67(4) . -109_543 N
Oh Di2 4.16(4) . -304_445 N
Oh Ok 2.48(4) . 1_555 N
Oh Ok 2.85(4) . 105_544 N
Oh Ok 4.95(4) . -206_454 N
Oh Ok 3.99(4) . 308_544 N
Oh Dk1 2.94(4) . 1_555 N
Oh Dk1 3.14(4) . 105_544 N
Oh Dk1 3.21(4) . 308_544 N
Oh Dk2 2.44(5) . 1_555 N
Oh Dk2 3.69(4) . 105_544 N
Oh Dk2 4.21(5) . -206_454 N
Dh1 O1 3.385(29) . -3_555 N
Dh1 O1 3.992(29) . 111_555 N
Dh1 O3 4.182(27) . 2_555 N
Dh1 O4 4.430(29) . -111_434 N
Dh1 O4 3.101(25) . 312_555 N
Dh1 SJ 1.36(4) . 1_555 N
Dh1 Og 1.259(29) . 1_555 N
Dh1 Og 3.706(29) . 105_544 N
Dh1 Og 2.56(4) . -108_544 N
Dh1 Og 3.721(33) . -305_444 N
Dh1 Dg1 1.38(4) . 1_555 N
Dh1 Dg1 2.750(30) . 105_544 N
Dh1 Dg1 2.57(4) . -108_544 N
Dh1 Dg1 3.93(4) . -305_444 N
Dh1 Dg2 1.811(31) . 1_555 N
Dh1 Dg2 2.88(4) . -108_544 N
Dh1 Oh 0.96 . 1_555 N
Dh1 Oh 3.81(4) . 105_544 N
Dh1 Oh 4.46(5) . -206_454 N
Dh1 Oh 4.04(4) . 308_544 N
Dh1 Dh1 3.67(6) . 105_544 N
Dh1 Dh1 3.67(6) . -108_544 N
Dh1 Dh1 3.95(4) . 308_544 N
Dh1 Dh1 3.95(4) . -305_444 N
Dh1 Dh2 1.518660(10) . 1_555 N
Dh1 Dh2 3.78(4) . 105_544 N
Dh1 OII* 3.090(32) . -105_544 N
Dh1 DII*1 2.41(5) . -105_544 N
Dh1 DII*1 3.96(4) . 209_555 N
Dh1 DII*1 3.07(7) . 312_555 N
Dh1 DII*2 2.98(5) . -105_544 N
Dh1 DII*2 2.53(6) . 209_555 N
Dh1 DII*2 3.83(5) . 312_555 N
Dh1 Oi 3.67(4) . -2_555 N
Dh1 Oi 2.62(4) . 105_544 N
Dh1 Oi 3.17(4) . -109_543 N
Dh1 Di1 3.72(4) . -2_555 N
Dh1 Di1 3.19(5) . 105_544 N
Dh1 Di1 2.26(4) . -109_543 N
Dh1 Di2 3.02(4) . -2_555 N
Dh1 Di2 3.38(4) . 105_544 N
Dh1 Di2 3.32(4) . -109_543 N
Dh1 Di2 3.86(5) . -304_445 N
Dh1 Ok 2.94(4) . 1_555 N
Dh1 Ok 2.49(5) . 105_544 N
Dh1 Ok 3.07(4) . 308_544 N
Dh1 Dk1 3.36(5) . 1_555 N
Dh1 Dk1 2.94(5) . 105_544 N
Dh1 Dk1 2.36(4) . 308_544 N
Dh1 Dk2 3.16(5) . 1_555 N
Dh1 Dk2 3.33(5) . 105_544 N
Dh1 Dk2 3.96(5) . -206_454 N
Dh1 Dk2 3.79(4) . 308_544 N
Dh2 O1 3.143(32) . -3_555 N
Dh2 O1 2.839(32) . 111_555 N
Dh2 O2 4.132(25) . 1_555 N
Dh2 O2 4.357(24) . -304_445 N
Dh2 O3 3.292(28) . 2_555 N
Dh2 O3 3.210(29) . 208_555 N
Dh2 O4 1.720(21) . 312_555 N
Dh2 SJ 1.19(4) . 1_555 N
Dh2 Og 2.282(33) . 1_555 N
Dh2 Og 2.529(34) . -108_544 N
Dh2 Og 4.245(30) . -305_444 N
Dh2 Dg1 2.15(4) . 1_555 N
Dh2 Dg1 2.873(35) . -108_544 N
Dh2 Dg2 2.20(4) . 1_555 N
Dh2 Dg2 2.34(4) . -108_544 N
Dh2 Oh 0.96077 . 1_555 N
Dh2 Oh 4.48(4) . 105_544 N
Dh2 Dh1 1.518660(10) . 1_555 N
Dh2 Dh1 3.78(4) . -108_544 N
Dh2 OII* 2.82(4) . -105_544 N
Dh2 DII*1 2.17(7) . -105_544 N
Dh2 DII*1 3.66(4) . 209_555 N
Dh2 DII*1 3.07(6) . 312_555 N
Dh2 DII*2 3.11(5) . -105_544 N
Dh2 DII*2 2.47(7) . 209_555 N
Dh2 DII*2 3.68(4) . 312_555 N
Dh2 Oi 3.23(4) . 105_544 N
Dh2 Oi 2.85(4) . -109_543 N
Dh2 Oi 4.43(4) . -304_445 N
Dh2 Di1 3.52(4) . 105_544 N
Dh2 Di1 1.99(4) . -109_543 N
Dh2 Di2 3.12(4) . -109_543 N
Dh2 Di2 3.60(5) . -304_445 N
Dh2 Ok 2.66(5) . 1_555 N
Dh2 Ok 2.36(4) . 105_544 N
Dh2 Ok 4.30(5) . 308_544 N
Dh2 Dk1 3.37(5) . 1_555 N
Dh2 Dk1 2.63(5) . 105_544 N
Dh2 Dk1 3.50(4) . 308_544 N
Dh2 Dk2 2.50(5) . 1_555 N
Dh2 Dk2 3.09(5) . 105_544 N
OII' O2 4.939(10) . 1_555 N
OII' O2 4.939(10) . 2_555 N
OII' O2 4.939(10) . 3_555 N
OII' O2 3.746(5) . 107_555 N
OII' O2 3.804(5) . 111_555 N
OII' O2 3.746(5) . 208_555 N
OII' O2 3.804(5) . 209_555 N
OII' O2 3.804(5) . 310_555 N
OII' O2 3.746(5) . 312_555 N
OII' O3 4.906(8) . 107_555 N
OII' O3 4.923(9) . 111_555 N
OII' O3 3.185(14) . -105_544 N
OII' O3 4.906(8) . 208_555 N
OII' O3 4.923(9) . 209_555 N
OII' O3 3.185(14) . -206_454 N
OII' O3 4.923(9) . 310_555 N
OII' O3 4.906(8) . 312_555 N
OII' O3 3.185(14) . -304_445 N
OII' O4 3.966(14) . 1_555 N
OII' O4 3.966(14) . 2_555 N
OII' O4 3.966(14) . 3_555 N
OII' OII' 2.698(32) . 107_555 N
OII' OII' 2.698(32) . 111_555 N
OII' OII' 2.698(32) . -105_544 N
OII' DII'1 0.9600(14) . 1_555 N
OII' DII'1 0.9600(14) . 2_555 N
OII' DII'1 0.9600(14) . 3_555 N
OII' DII'1 2.32(4) . 107_555 N
OII' DII'1 3.237(32) . 111_555 N
OII' DII'1 2.72(4) . -105_544 N
OII' DII'1 2.32(4) . 208_555 N
OII' DII'1 3.237(32) . 209_555 N
OII' DII'1 2.72(4) . -206_454 N
OII' DII'1 3.237(32) . 310_555 N
OII' DII'1 2.32(4) . 312_555 N
OII' DII'1 2.72(4) . -304_445 N
OII' DII'2 0.961(12) . 1_555 N
OII' DII'2 0.961(12) . 2_555 N
OII' DII'2 0.961(12) . 3_555 N
OII' DII'2 2.317(32) . 107_555 N
OII' DII'2 1.864(31) . 111_555 N
OII' DII'2 2.00(5) . -105_544 N
OII' DII'2 2.317(32) . 208_555 N
OII' DII'2 1.864(31) . 209_555 N
OII' DII'2 2.00(5) . -206_454 N
OII' DII'2 1.864(31) . 310_555 N
OII' DII'2 2.317(32) . 312_555 N
OII' DII'2 2.00(5) . -304_445 N
DII'1 O2 4.163(24) . 3_555 N
DII'1 O2 3.51(5) . 107_555 N
DII'1 O2 2.897(13) . 111_555 N
DII'1 O2 4.460(32) . 209_555 N
DII'1 O2 4.27(4) . 310_555 N
DII'1 O2 3.30(5) . 312_555 N
DII'1 O3 4.48(4) . 107_555 N
DII'1 O3 3.855(26) . -105_544 N
DII'1 O3 2.767(34) . -206_454 N
DII'1 O3 4.039(18) . 310_555 N
DII'1 O3 3.480(34) . -304_445 N
DII'1 O4 4.06(4) . 1_555 N
DII'1 O4 3.581(32) . 2_555 N
DII'1 O4 4.360(34) . -105_544 N
DII'1 OII' 0.9600(14) . 1_555 N
DII'1 OII' 3.237(32) . 107_555 N
DII'1 OII' 2.72(4) . 111_555 N
DII'1 OII' 2.32(4) . -105_544 N
DII'1 DII'1 1.653(6) . 2_555 N
DII'1 DII'1 1.653(6) . 3_555 N
DII'1 DII'1 3.07(5) . 107_555 N
DII'1 DII'1 3.13(5) . 111_555 N
DII'1 DII'1 2.12(5) . -105_544 N
DII'1 DII'1 2.12(5) . 208_555 N
DII'1 DII'1 3.07(5) . 209_555 N
DII'1 DII'1 3.13(5) . -206_454 N
DII'1 DII'1 3.62(5) . 310_555 N
DII'1 DII'1 2.01(9) . 312_555 N
DII'1 DII'1 3.06(6) . -304_445 N
DII'1 DII'2 1.518680(10) . 1_555 N
DII'1 DII'2 1.059(32) . 2_555 N
DII'1 DII'2 1.25(6) . 3_555 N
DII'1 DII'2 2.611(27) . 107_555 N
DII'1 DII'2 2.09(6) . 111_555 N
DII'1 DII'2 1.95(4) . -105_544 N
DII'1 DII'2 2.424(12) . 208_555 N
DII'1 DII'2 1.59(6) . 209_555 N
DII'1 DII'2 2.475(17) . -206_454 N
DII'1 DII'2 2.297(34) . 310_555 N
DII'1 DII'2 2.19(4) . 312_555 N
DII'1 DII'2 1.926(28) . -304_445 N
DII'2 O2 4.239(18) . 2_555 N
DII'2 O2 4.251(29) . 107_555 N
DII'2 O2 4.366(22) . 111_555 N
DII'2 O2 3.690(29) . 208_555 N
DII'2 O2 3.96(5) . 209_555 N
DII'2 O2 3.811(33) . 310_555 N
DII'2 O2 4.11(4) . 312_555 N
DII'2 O3 3.693(19) . -105_544 N
DII'2 O3 4.43(4) . 209_555 N
DII'2 O3 4.041(19) . -206_454 N
DII'2 O3 4.302(27) . 312_555 N
DII'2 O3 3.943(28) . -304_445 N
DII'2 O4 4.468(32) . 3_555 N
DII'2 OII' 0.961(12) . 1_555 N
DII'2 OII' 1.864(31) . 107_555 N
DII'2 OII' 2.00(5) . 111_555 N
DII'2 OII' 2.317(32) . -105_544 N
DII'2 DII'1 1.518680(10) . 1_555 N
DII'2 DII'1 1.25(6) . 2_555 N
DII'2 DII'1 1.059(32) . 3_555 N
DII'2 DII'1 1.59(6) . 107_555 N
DII'2 DII'1 2.475(17) . 111_555 N
DII'2 DII'1 2.424(12) . -105_544 N
DII'2 DII'1 1.95(4) . 208_555 N
DII'2 DII'1 2.611(27) . 209_555 N
DII'2 DII'1 2.09(6) . -206_454 N
DII'2 DII'1 2.297(34) . 310_555 N
DII'2 DII'1 2.19(4) . 312_555 N
DII'2 DII'1 1.926(28) . -304_445 N
DII'2 DII'2 0.63(4) . 2_555 N
DII'2 DII'2 0.63(4) . 3_555 N
DII'2 DII'2 1.433(33) . 107_555 N
DII'2 DII'2 1.057(26) . 111_555 N
DII'2 DII'2 1.462(34) . -105_544 N
DII'2 DII'2 1.462(34) . 208_555 N
DII'2 DII'2 1.433(33) . 209_555 N
DII'2 DII'2 1.057(26) . -206_454 N
DII'2 DII'2 1.07(6) . 310_555 N
DII'2 DII'2 1.66(4) . 312_555 N
DII'2 DII'2 1.34(7) . -304_445 N
OII* O1 4.840(17) . 107_555 N
OII* O1 4.987(16) . -110_544 N
OII* O1 4.840(17) . 208_555 N
OII* O1 4.987(16) . -211_454 N
OII* O1 4.840(17) . 312_555 N
OII* O1 4.987(16) . -309_445 N
OII* O3 3.714(29) . -105_544 N
OII* O3 3.714(29) . -206_454 N
OII* O3 3.714(29) . -304_445 N
OII* O4 3.879(24) . 1_555 N
OII* O4 3.879(24) . 2_555 N
OII* O4 3.879(24) . 3_555 N
OII* SII 2.23(4) . 1_555 N
OII* Og 4.144(12) . 107_555 N
OII* Og 4.144(12) . 208_555 N
OII* Og 4.144(12) . 312_555 N
OII* Dg1 4.418(22) . 107_555 N
OII* Dg1 4.418(22) . 208_555 N
OII* Dg1 4.418(22) . 312_555 N
OII* Dg2 4.254(17) . 107_555 N
OII* Dg2 4.254(17) . 208_555 N
OII* Dg2 4.254(17) . 312_555 N
OII* Oh 2.466(19) . 107_555 N
OII* Oh 2.466(19) . 208_555 N
OII* Oh 2.466(19) . 312_555 N
OII* Dh1 3.090(32) . 107_555 N
OII* Dh1 3.090(32) . 208_555 N
OII* Dh1 3.090(32) . 312_555 N
OII* Dh2 2.82(4) . 107_555 N
OII* Dh2 2.82(4) . 208_555 N
OII* Dh2 2.82(4) . 312_555 N
OII* DII*1 0.960(5) . 1_555 N
OII* DII*1 0.960(5) . 2_555 N
OII* DII*1 0.960(5) . 3_555 N
OII* DII*2 0.961(13) . 1_555 N
OII* DII*2 0.961(13) . 2_555 N
OII* DII*2 0.961(13) . 3_555 N
OII* Oi 4.761(31) . 4_555 N
OII* Oi 4.761(31) . 5_555 N
OII* Oi 4.761(31) . 6_555 N
OII* Oi 2.765(27) . -102_544 N
OII* Oi 2.765(27) . -203_454 N
OII* Oi 2.765(27) . -301_445 N
OII* Di1 2.252(32) . -102_544 N
OII* Di1 2.252(32) . -203_454 N
OII* Di1 2.252(32) . -301_445 N
OII* Di2 4.47(4) . 4_555 N
OII* Di2 4.47(4) . 5_555 N
OII* Di2 4.47(4) . 6_555 N
OII* Di2 3.645(26) . -102_544 N
OII* Di2 3.645(26) . -203_454 N
OII* Di2 3.645(26) . -301_445 N
OII* Ok 4.292(32) . 107_555 N
OII* Ok 4.292(32) . 208_555 N
OII* Ok 4.292(32) . 312_555 N
OII* Dk1 4.50(4) . 107_555 N
OII* Dk1 4.465(32) . -104_544 N
OII* Dk1 4.50(4) . 208_555 N
OII* Dk1 4.465(32) . -205_454 N
OII* Dk1 4.50(4) . 312_555 N
OII* Dk1 4.465(32) . -306_445 N
OII* Dk2 3.79(5) . 107_555 N
OII* Dk2 3.79(5) . 208_555 N
OII* Dk2 3.79(5) . 312_555 N
DII*1 O1 4.12(5) . 312_555 N
DII*1 O3 3.51(7) . -105_544 N
DII*1 O3 4.41(4) . -206_454 N
DII*1 O3 3.97(7) . -304_445 N
DII*1 O4 4.13(5) . 1_555 N
DII*1 O4 3.49(8) . 3_555 N
DII*1 Og 4.152(34) . 5_555 N
DII*1 Og 3.59(5) . 208_555 N
DII*1 Og 3.93(5) . 312_555 N
DII*1 Dg1 3.70(5) . 208_555 N
DII*1 Dg2 3.92(4) . 5_555 N
DII*1 Dg2 3.81(6) . 208_555 N
DII*1 Oh 3.288(28) . 107_555 N
DII*1 Oh 1.67(4) . 208_555 N
DII*1 Oh 2.71(5) . 312_555 N
DII*1 Dh1 3.96(4) . 107_555 N
DII*1 Dh1 2.41(5) . 208_555 N
DII*1 Dh1 3.07(7) . 312_555 N
DII*1 Dh2 3.66(4) . 107_555 N
DII*1 Dh2 2.17(7) . 208_555 N
DII*1 Dh2 3.07(6) . 312_555 N
DII*1 OII* 0.960(5) . 1_555 N
DII*1 DII*1 1.630(27) . 2_555 N
DII*1 DII*1 1.630(27) . 3_555 N
DII*1 DII*2 1.518670(10) . 1_555 N
DII*1 DII*2 0.37(14) . 2_555 N
DII*1 DII*2 1.58(4) . 3_555 N
DII*1 Oi 4.02(5) . 5_555 N
DII*1 Oi 1.96(4) . -102_544 N
DII*1 Oi 3.56(4) . -203_454 N
DII*1 Oi 2.93(5) . -301_445 N
DII*1 Di1 1.313(34) . -102_544 N
DII*1 Di1 2.91(5) . -203_454 N
DII*1 Di1 2.72(5) . -301_445 N
DII*1 Di2 3.77(5) . 5_555 N
DII*1 Di2 2.764(34) . -102_544 N
DII*1 Di2 3.87(5) . -301_445 N
DII*1 Ok 3.350(34) . 208_555 N
DII*1 Ok 4.43(6) . -301_445 N
DII*1 Dk1 3.56(4) . 208_555 N
DII*1 Dk1 3.92(6) . -306_445 N
DII*1 Dk2 2.92(6) . 208_555 N
DII*2 O1 4.42(7) . 208_555 N
DII*2 O3 4.25(5) . -206_454 N
DII*2 O3 3.84(6) . -304_445 N
DII*2 O4 3.84(7) . 2_555 N
DII*2 O4 4.29(4) . 3_555 N
DII*2 Og 4.34(5) . 4_555 N
DII*2 Og 3.71(5) . 107_555 N
DII*2 Og 3.89(4) . 208_555 N
DII*2 Dg1 3.85(5) . 107_555 N
DII*2 Dg2 4.00(6) . 107_555 N
DII*2 Oh 1.87(6) . 107_555 N
DII*2 Oh 2.64(4) . 208_555 N
DII*2 Oh 3.221(32) . 312_555 N
DII*2 Dh1 2.53(6) . 107_555 N
DII*2 Dh1 2.98(5) . 208_555 N
DII*2 Dh1 3.83(5) . 312_555 N
DII*2 Dh2 2.47(7) . 107_555 N
DII*2 Dh2 3.11(5) . 208_555 N
DII*2 Dh2 3.68(4) . 312_555 N
DII*2 OII* 0.961(13) . 1_555 N
DII*2 DII*1 1.518670(10) . 1_555 N
DII*2 DII*1 1.58(4) . 2_555 N
DII*2 DII*1 0.37(14) . 3_555 N
DII*2 DII*2 1.39(7) . 2_555 N
DII*2 DII*2 1.39(7) . 3_555 N
DII*2 Oi 3.903(33) . 4_555 N
DII*2 Oi 3.39(5) . -102_544 N
DII*2 Oi 2.92(4) . -203_454 N
DII*2 Oi 2.00(4) . -301_445 N
DII*2 Di1 2.77(5) . -102_544 N
DII*2 Di1 2.68(5) . -203_454 N
DII*2 Di1 1.44(6) . -301_445 N
DII*2 Di2 3.70(5) . 4_555 N
DII*2 Di2 3.84(4) . -203_454 N
DII*2 Di2 2.81(4) . -301_445 N
DII*2 Ok 3.50(5) . 107_555 N
DII*2 Dk1 3.62(5) . 107_555 N
DII*2 Dk1 3.88(4) . -205_454 N
DII*2 Dk2 3.11(7) . 107_555 N
Oi O1 4.884(28) . 2_555 N
Oi O1 4.965(27) . -3_555 N
Oi O1 3.611(24) . 111_555 N
Oi O1 3.366(24) . -108_544 N
Oi O2 4.468(24) . 1_555 N
Oi O3 3.571(24) . 4_555 N
Oi O4 4.089(26) . 310_555 N
Oi O4 4.203(25) . 312_555 N
Oi O4 4.100(24) . -302_445 N
Oi O4 4.297(25) . -303_445 N
Oi Og 4.729(26) . 1_555 N
Oi Og 3.435(28) . -3_555 N
Oi Og 2.855(27) . -108_544 N
Oi Og 4.394(26) . -207_453 N
Oi Og 3.703(26) . -304_445 N
Oi Dg1 3.962(30) . 1_555 N
Oi Dg1 4.260(30) . -3_555 N
Oi Dg1 3.657(29) . -108_544 N
Oi Dg1 4.068(31) . -207_453 N
Oi Dg1 3.337(31) . -304_445 N
Oi Dg2 3.871(32) . -3_555 N
Oi Dg2 2.916(32) . -108_544 N
Oi Dg2 3.293(31) . -304_445 N
Oi Oh 4.36(4) . -3_555 N
Oi Oh 4.226(33) . 105_544 N
Oi Oh 2.902(35) . -108_544 N
Oi Oh 2.375(33) . -207_453 N
Oi Oh 4.949(31) . -304_445 N
Oi Dh1 3.67(4) . -3_555 N
Oi Dh1 2.62(4) . -108_544 N
Oi Dh1 3.17(4) . -207_453 N
Oi Dh2 3.23(4) . -108_544 N
Oi Dh2 2.85(4) . -207_453 N
Oi Dh2 4.43(4) . -304_445 N
Oi OII* 4.761(31) . -111_434 N
Oi OII* 2.765(27) . -301_445 N
Oi DII*1 4.02(5) . -208_344 N
Oi DII*1 2.93(5) . -301_445 N
Oi DII*1 3.56(4) . -302_445 N
Oi DII*1 1.96(4) . -303_445 N
Oi DII*2 3.903(33) . 304_445 N
Oi DII*2 2.00(4) . -301_445 N
Oi DII*2 2.92(4) . -302_445 N
Oi DII*2 3.39(5) . -303_445 N
Oi Oi 4.70(5) . 103_554 N
Oi Oi 4.70(5) . 202_554 N
Oi Oi 2.38(5) . -304_445 N
Oi Di1 0.959980(10) . 1_555 N
Oi Di1 3.83(4) . 202_554 N
Oi Di1 3.07(5) . -304_445 N
Oi Di2 0.96077 . 1_555 N
Oi Di2 1.94(5) . -304_445 N
Oi Ok 4.299(32) . 1_555 N
Oi Ok 4.88(4) . 103_554 N
Oi Ok 3.071(33) . 105_544 N
Oi Ok 2.12(4) . -207_453 N
Oi Dk1 2.20(4) . 105_544 N
Oi Dk1 2.03(5) . -207_453 N
Oi Dk2 3.13(5) . 105_544 N
Oi Dk2 1.61(5) . -207_453 N
Oi SIII 2.28(7) . 304_445 N
Di1 O1 4.191(27) . 111_555 N
Di1 O1 3.25(4) . -108_544 N
Di1 O3 3.449(31) . 4_555 N
Di1 O4 4.40(4) . 310_555 N
Di1 O4 3.42(4) . -302_445 N
Di1 O4 4.494(27) . -303_445 N
Di1 Og 3.468(31) . -3_555 N
Di1 Og 3.665(31) . -108_544 N
Di1 Og 3.497(29) . -207_453 N
Di1 Og 3.22(4) . -304_445 N
Di1 Dg1 3.27(4) . -207_453 N
Di1 Dg1 2.97(4) . -304_445 N
Di1 Dg2 3.674(32) . -108_544 N
Di1 Dg2 3.856(31) . -207_453 N
Di1 Dg2 2.92(4) . -304_445 N
Di1 Oh 4.49(4) . -3_555 N
Di1 Oh 3.21(4) . -108_544 N
Di1 Oh 1.430(34) . -207_453 N
Di1 Dh1 3.72(4) . -3_555 N
Di1 Dh1 3.19(5) . -108_544 N
Di1 Dh1 2.26(4) . -207_453 N
Di1 Dh2 3.52(4) . -108_544 N
Di1 Dh2 1.99(4) . -207_453 N
Di1 OII* 2.252(32) . -301_445 N
Di1 DII*1 2.72(5) . -301_445 N
Di1 DII*1 2.91(5) . -302_445 N
Di1 DII*1 1.313(34) . -303_445 N
Di1 DII*2 1.44(6) . -301_445 N
Di1 DII*2 2.68(5) . -302_445 N
Di1 DII*2 2.77(5) . -303_445 N
Di1 Oi 0.959980(10) . 1_555 N
Di1 Oi 3.83(4) . 103_554 N
Di1 Oi 3.07(5) . -304_445 N
Di1 Di1 3.86(6) . 103_554 N
Di1 Di1 3.86(6) . 202_554 N
Di1 Di1 3.80(6) . -304_445 N
Di1 Di2 1.518640(10) . 1_555 N
Di1 Di2 2.82(5) . -304_445 N
Di1 Ok 4.08(5) . 103_554 N
Di1 Ok 4.025(33) . 105_544 N
Di1 Ok 2.08(5) . -207_453 N
Di1 Dk1 3.16(4) . 105_544 N
Di1 Dk1 2.26(5) . -207_453 N
Di1 Dk2 1.71(6) . -207_453 N
Di2 O1 3.937(26) . 2_555 N
Di2 O1 4.458(29) . -3_555 N
Di2 O1 3.865(31) . 111_555 N
Di2 O1 3.15(4) . -108_544 N
Di2 O2 4.17(4) . 1_555 N
Di2 O3 4.042(33) . 4_555 N
Di2 O4 3.285(34) . 310_555 N
Di2 O4 3.927(28) . 312_555 N
Di2 O4 4.354(34) . -302_445 N
Di2 Og 2.614(30) . -3_555 N
Di2 Og 3.340(34) . -108_544 N
Di2 Og 4.441(30) . -207_453 N
Di2 Og 3.24(4) . -304_445 N
Di2 Dg1 3.506(32) . -3_555 N
Di2 Dg1 3.934(34) . -207_453 N
Di2 Dg1 2.74(4) . -304_445 N
Di2 Dg2 2.950(33) . -3_555 N
Di2 Dg2 3.36(4) . -108_544 N
Di2 Dg2 2.86(5) . -304_445 N
Di2 Oh 3.77(4) . -3_555 N
Di2 Oh 4.13(4) . 105_544 N
Di2 Oh 3.80(4) . -108_544 N
Di2 Oh 2.67(4) . -207_453 N
Di2 Oh 4.16(4) . -304_445 N
Di2 Dh1 3.02(4) . -3_555 N
Di2 Dh1 3.38(4) . -108_544 N
Di2 Dh1 3.32(4) . -207_453 N
Di2 Dh1 3.86(5) . -304_445 N
Di2 Dh2 3.12(4) . -207_453 N
Di2 Dh2 3.60(5) . -304_445 N
Di2 OII* 4.47(4) . -111_434 N
Di2 OII* 3.645(26) . -301_445 N
Di2 DII*1 3.77(5) . -208_344 N
Di2 DII*1 3.87(5) . -301_445 N
Di2 DII*1 2.764(34) . -303_445 N
Di2 DII*2 3.70(5) . 304_445 N
Di2 DII*2 2.81(4) . -301_445 N
Di2 DII*2 3.84(4) . -302_445 N
Di2 Oi 0.96077 . 1_555 N
Di2 Oi 1.94(5) . -304_445 N
Di2 Di1 1.518640(10) . 1_555 N
Di2 Di1 2.82(5) . -304_445 N
Di2 Di2 1.62(7) . -304_445 N
Di2 Ok 2.92(4) . 105_544 N
Di2 Ok 1.45(4) . -207_453 N
Di2 Ok 4.36(4) . -304_445 N
Di2 Dk1 2.23(5) . 105_544 N
Di2 Dk1 1.11(5) . -207_453 N
Di2 Dk2 2.70(5) . 105_544 N
Di2 Dk2 1.25(5) . -207_453 N
Di2 SIII 1.64(7) . 304_445 N
Ok O1 4.436(33) . 4_555 N
Ok O1 3.665(34) . -12_554 N
Ok O1 2.273(34) . 111_555 N
Ok O2 4.82(4) . 1_555 N
Ok O2 4.594(27) . -108_544 N
Ok O2 3.963(30) . -109_543 N
Ok O3 4.229(27) . 4_555 N
Ok O3 4.963(30) . 205_554 N
Ok O3 4.06(4) . 208_555 N
Ok O4 4.533(26) . 106_554 N
Ok O4 3.692(34) . 312_555 N
Ok O4 2.502(27) . -303_445 N
Ok SJ 1.324(34) . -108_544 N
Ok Og 3.789(30) . 1_555 N
Ok Og 4.626(31) . 111_555 N
Ok Og 1.899(27) . -108_544 N
Ok Og 4.70(4) . -201_453 N
Ok Og 2.16(4) . -305_444 N
Ok Dg1 3.057(31) . 1_555 N
Ok Dg1 1.562(35) . -108_544 N
Ok Dg1 2.94(4) . -305_444 N
Ok Dg2 4.188(33) . 1_555 N
Ok Dg2 4.44(4) . 111_555 N
Ok Dg2 1.486(34) . -108_544 N
Ok Dg2 2.55(4) . -305_444 N
Ok Oh 2.48(4) . 1_555 N
Ok Oh 4.95(4) . 111_555 N
Ok Oh 2.85(4) . -108_544 N
Ok Oh 3.99(4) . -305_444 N
Ok Dh1 2.94(4) . 1_555 N
Ok Dh1 2.49(5) . -108_544 N
Ok Dh1 3.07(4) . -305_444 N
Ok Dh2 2.66(5) . 1_555 N
Ok Dh2 2.36(4) . -108_544 N
Ok Dh2 4.30(5) . -305_444 N
Ok OII* 4.292(32) . -105_544 N
Ok DII*1 3.350(34) . -105_544 N
Ok DII*1 4.43(6) . -301_445 N
Ok DII*2 3.50(5) . 209_555 N
Ok Oi 4.299(32) . 1_555 N
Ok Oi 3.071(33) . -108_544 N
Ok Oi 2.12(4) . -109_543 N
Ok Oi 4.88(4) . 202_554 N
Ok Di1 4.025(33) . -108_544 N
Ok Di1 2.08(5) . -109_543 N
Ok Di1 4.08(5) . 202_554 N
Ok Di2 2.92(4) . -108_544 N
Ok Di2 1.45(4) . -109_543 N
Ok Di2 4.36(4) . -304_445 N
Ok Ok 3.71(4) . 105_544 N
Ok Ok 4.13(5) . 110_554 N
Ok Ok 3.71(4) . -108_544 N
Ok Dk1 0.960000(10) . 1_555 N
Ok Dk1 3.29(5) . 105_544 N
Ok Dk1 3.52(5) . 110_554 N
Ok Dk1 4.49(4) . -108_544 N
Ok Dk2 0.960760(10) . 1_555 N
Ok Dk2 3.76(6) . 110_554 N
Ok Dk2 4.02(6) . -108_544 N
Ok SIII 2.22(4) . 8_554 N
Dk1 O1 3.10(4) . -12_554 N
Dk1 O1 3.132(31) . 111_555 N
Dk1 O2 4.24(4) . -108_544 N
Dk1 O2 4.319(34) . -109_543 N
Dk1 O4 4.31(4) . 106_554 N
Dk1 O4 2.66(4) . -303_445 N
Dk1 SJ 1.68(4) . -108_544 N
Dk1 Og 4.27(4) . 1_555 N
Dk1 Og 4.36(4) . 111_555 N
Dk1 Og 2.60(4) . -108_544 N
Dk1 Og 4.33(4) . -201_453 N
Dk1 Og 1.62(4) . -305_444 N
Dk1 Dg1 3.59(4) . 1_555 N
Dk1 Dg1 1.94(4) . -108_544 N
Dk1 Dg1 2.54(4) . -305_444 N
Dk1 Dg2 2.39(4) . -108_544 N
Dk1 Dg2 1.93(5) . -305_444 N
Dk1 Oh 2.94(4) . 1_555 N
Dk1 Oh 3.14(4) . -108_544 N
Dk1 Oh 3.21(4) . -305_444 N
Dk1 Dh1 3.36(5) . 1_555 N
Dk1 Dh1 2.94(5) . -108_544 N
Dk1 Dh1 2.36(4) . -305_444 N
Dk1 Dh2 3.37(5) . 1_555 N
Dk1 Dh2 2.63(5) . -108_544 N
Dk1 Dh2 3.50(4) . -305_444 N
Dk1 OII* 4.465(32) . 8_554 N
Dk1 OII* 4.50(4) . -105_544 N
Dk1 DII*1 3.56(4) . -105_544 N
Dk1 DII*1 3.92(6) . 311_554 N
Dk1 DII*2 3.88(4) . 8_554 N
Dk1 DII*2 3.62(5) . 209_555 N
Dk1 Oi 2.20(4) . -108_544 N
Dk1 Oi 2.03(5) . -109_543 N
Dk1 Di1 3.16(4) . -108_544 N
Dk1 Di1 2.26(5) . -109_543 N
Dk1 Di2 2.23(5) . -108_544 N
Dk1 Di2 1.11(5) . -109_543 N
Dk1 Ok 0.960000(10) . 1_555 N
Dk1 Ok 4.49(4) . 105_544 N
Dk1 Ok 3.52(5) . 110_554 N
Dk1 Ok 3.29(5) . -108_544 N
Dk1 Dk1 3.04(8) . 110_554 N
Dk1 Dk2 1.518650(10) . 1_555 N
Dk1 Dk2 3.02(5) . 110_554 N
Dk1 Dk2 3.67(5) . -108_544 N
Dk1 SIII 1.87(6) . 8_554 N
Dk2 O1 3.54(4) . 4_555 N
Dk2 O1 4.23(4) . -12_554 N
Dk2 O1 1.90(4) . 111_555 N
Dk2 O2 4.32(4) . 1_555 N
Dk2 O2 3.43(5) . -109_543 N
Dk2 O3 4.21(5) . 4_555 N
Dk2 O3 3.206(34) . 208_555 N
Dk2 O4 4.02(4) . 106_554 N
Dk2 O4 3.37(4) . 312_555 N
Dk2 O4 2.77(5) . -303_445 N
Dk2 Og 4.15(4) . 1_555 N
Dk2 Og 3.90(4) . 111_555 N
Dk2 Og 2.58(4) . -108_544 N
Dk2 Og 3.02(4) . -305_444 N
Dk2 Dg1 3.55(4) . 1_555 N
Dk2 Dg1 2.44(4) . -108_544 N
Dk2 Dg1 3.85(4) . -305_444 N
Dk2 Dg2 3.61(5) . 111_555 N
Dk2 Dg2 1.91(5) . -108_544 N
Dk2 Dg2 3.34(4) . -305_444 N
Dk2 Oh 2.44(5) . 1_555 N
Dk2 Oh 4.21(5) . 111_555 N
Dk2 Oh 3.69(4) . -108_544 N
Dk2 Dh1 3.16(5) . 1_555 N
Dk2 Dh1 3.96(5) . 111_555 N
Dk2 Dh1 3.33(5) . -108_544 N
Dk2 Dh1 3.79(4) . -305_444 N
Dk2 Dh2 2.50(5) . 1_555 N
Dk2 Dh2 3.09(5) . -108_544 N
Dk2 OII* 3.79(5) . -105_544 N
Dk2 DII*1 2.92(6) . -105_544 N
Dk2 DII*2 3.11(7) . 209_555 N
Dk2 Oi 3.13(5) . -108_544 N
Dk2 Oi 1.61(5) . -109_543 N
Dk2 Di1 1.71(6) . -109_543 N
Dk2 Di2 2.70(5) . -108_544 N
Dk2 Di2 1.25(5) . -109_543 N
Dk2 Ok 0.960760(10) . 1_555 N
Dk2 Ok 4.02(6) . 105_544 N
Dk2 Ok 3.76(6) . 110_554 N
Dk2 Dk1 1.518650(10) . 1_555 N
Dk2 Dk1 3.67(5) . 105_544 N
Dk2 Dk1 3.02(5) . 110_554 N
Dk2 Dk2 3.60(8) . 110_554 N
Dk2 SIII 1.93(5) . 8_554 N
SIII O4 2.45(5) . -10_554 N
SIII O4 2.45(5) . -12_554 N
SIII Oi 2.28(7) . 4_555 N
SIII Oi 2.28(7) . -301_445 N
SIII Di2 1.64(7) . 4_555 N
SIII Di2 1.64(7) . -301_445 N
SIII Ok 2.22(4) . 107_555 N
SIII Ok 2.22(4) . -205_454 N
SIII Dk1 1.87(6) . 107_555 N
SIII Dk1 1.87(6) . -205_454 N
SIII Dk2 1.93(5) . 107_555 N
SIII Dk2 1.93(5) . -205_454 N
loop_
_pd_meas_intensity_total
_pd_proc_ls_weight
_pd_proc_intensity_bkg_calc
_pd_calc_intensity_total
0.0(20) 0.0 -10969.88 .
0.0(20) 0.0 -10611.84 .
0.0(20) 0.0 -10262.30 .
0.0(20) 0.0 -9921.07 .
0.0(20) 0.0 -9588.00 .
0.0(20) 0.0 -9262.95 .
0.0(20) 0.0 -8945.73 .
0.0(20) 0.0 -8636.21 .
0.0(20) 0.0 -8334.23 .
0.0(20) 0.0 -8039.63 .
0.0(20) 0.0 -7752.28 .
0.0(20) 0.0 -7472.03 .
0.0(20) 0.0 -7198.75 .
0.0(20) 0.0 -6932.28 .
0.0(20) 0.0 -6672.49 .
0.0(20) 0.0 -6419.25 .
0.0(20) 0.0 -6172.44 .
0.0(20) 0.0 -5931.90 .
0.0(20) 0.0 -5697.53 .
0.0(20) 0.0 -5469.19 .
0.0(20) 0.0 -5246.75 .
4.0(20) 0.0 -5030.10 .
4.0(20) 0.0 -4819.13 .
7.0(20) 0.0 -4613.70 .
5.0(20) 0.0 -4413.70 .
8.0(20) 0.0 -4219.04 .
11.0(20) 0.0 -4029.57 .
11.0(20) 0.0 -3845.22 .
15.0(20) 0.0 -3665.85 .
13.0(20) 0.0 -3491.37 .
19.0(20) 0.0 -3321.68 .
17.0(20) 0.0 -3156.68 .
23.0(20) 0.0 -2996.24 .
22.0(20) 0.0 -2840.30 .
27.0(20) 0.0 -2688.74 .
27.0(20) 0.0 -2541.48 .
31.0(20) 0.0 -2398.42 .
31.0(20) 0.0 -2259.46 .
34.0(20) 0.0 -2124.52 .
34.0(20) 0.0 -1993.51 .
41.0(20) 0.0 -1866.33 .
40.0(20) 0.0 -1742.92 .
40.0(20) 0.0 -1623.18 .
43.0(20) 0.0 -1507.03 .
42.0(20) 0.0 -1394.40 .
41.0(20) 0.0 -1285.19 .
42.0(20) 0.0 -1179.34 .
40.0(20) 0.0 -1076.76 .
40.0(20) 0.0 -977.39 .
41.0(20) 0.0 -881.15 .
41.0(20) 0.0 -787.96 .
42.0(20) 0.0 -697.77 .
39.0(20) 0.0 -610.48 .
42.0(20) 0.0 -526.05 .
44.0(20) 0.0 -444.39 .
46.0(20) 0.0 -365.46 .
46.0(20) 0.0 -289.17 .
49.0(20) 0.0 -215.47 .
48.0(20) 0.0 -144.30 .
49.0(30) 0.0 -75.60 .
47.0(20) 0.0 -9.30 .
50.0(30) 0.0 54.66 .
52.0(30) 0.0 116.32 .
53.0(30) 0.0 175.74 .
51.0(30) 0.0 232.99 .
57.0(30) 0.0 288.12 .
61.0(30) 0.0 341.17 .
62.0(30) 0.0 392.20 .
65.0(30) 0.0 441.27 .
72.0(30) 0.0 488.41 .
76(4) 0.0 533.7 .
89(4) 0.0 577.1 .
104(4) 0.0 618.8 .
108(4) 0.0 658.8 .
122(4) 0.0 697.0 .
135(5) 0.0 733.7 .
149(5) 0.0 768.7 .
164(5) 0.0 802.2 .
185(5) 0.0 834.1 .
190(5) 0.0 864.6 .
207(5) 0.0 893.7 .
226(6) 0.0 921.4 .
243(6) 0.0 947.7 .
260(6) 0.0 972.7 .
273(6) 0.0 996.4 .
286(6) 0.0 1018.9 .
304(6) 0.0 1040.2 .
316(6) 0.0 1060.3 .
327(6) 0.0 1079.2 .
350(7) 0.0 1097.1 .
364(7) 0.0 1113.9 .
383(7) 0.0 1129.6 .
405(7) 0.0 1144.3 .
410(7) 0.0 1158.1 .
430(7) 0.0 1170.8 .
438(7) 0.0 1182.7 .
443(7) 0.0 1193.7 .
441(7) 0.0 1203.8 .
458(7) 0.0 1213.0 .
473(7) 0.0 1221.5 .
465(7) 0.0 1229.1 .
477(7) 0.0 1236.0 .
486(8) 0.0 1242.2 .
495(8) 0.0 1247.6 .
503(7) 0.0 1252.4 .
503(7) 0.0 1256.4 .
504(7) 0.0 1259.9 .
504(7) 0.0 1262.7 .
495(7) 0.0 1264.9 .
479(7) 0.0 1266.5 .
496(7) 0.0 1267.6 .
502(7) 0.0 1268.1 .
499(7) 0.0 1268.1 .
489(7) 0.0 1267.6 .
485(7) 0.0 1266.7 .
484(7) 0.0 1265.2 .
484(7) 0.0 1263.3 .
490(7) 0.0 1261.0 .
479(7) 0.0 1258.3 .
475(7) 0.0 1255.2 .
459(7) 0.0 1251.7 .
475(7) 0.0 1247.8 .
479(7) 0.0 1243.6 .
466(7) 0.0 1239.0 .
471(7) 0.0 1234.1 .
478(7) 0.0 1229.0 .
479(7) 0.0 1223.5 .
475(7) 0.0 1217.7 .
470(7) 0.0 1211.7 .
468(7) 0.0 1205.4 .
467(7) 0.0 1198.9 .
473(7) 0.0 1192.2 .
474(7) 0.0 1185.2 .
473(7) 0.0 1178.0 .
473(7) 0.0 1170.7 .
473(7) 0.0 1163.1 .
459(7) 0.0 1155.4 .
463(7) 0.0 1147.5 .
479(7) 0.0 1139.5 .
481(7) 0.0 1131.3 .
479(7) 0.0 1123.0 .
467(7) 0.0 1114.6 .
483(7) 0.0 1106.0 .
474(7) 0.0 1097.3 .
476(7) 0.0 1088.6 .
467(7) 0.0 1079.7 .
477(7) 0.0 1070.8 .
467(7) 0.0 1061.7 .
473(7) 0.0 1052.6 .
487(7) 0.0 1043.5 .
469(7) 0.0 1034.3 .
471(7) 0.0 1025.0 .
478(7) 0.0 1015.7 .
486(7) 0.0 1006.4 .
472(7) 0.0 997.0 .
489(7) 0.0 987.6 .
502(8) 0.0 978.2 .
500(8) 0.0 968.8 .
510(7) 0.0 959.4 .
496(8) 0.0 949.9 .
504(8) 0.0 940.5 .
513(8) 0.0 931.1 .
526(8) 0.0 921.7 .
528(8) 0.0 912.3 .
543(8) 0.0 902.9 .
550(8) 0.0 893.5 .
553(8) 0.0 884.2 .
568(8) 0.0 874.9 .
585(9) 0.0 865.7 .
594(9) 0.0 856.4 .
626(9) 0.0 847.3 .
655(10) 0.0 838.1 .
710(10) 0.0 829.1 .
780(10) 0.0 820.0 .
838(11) 0.0 811.0 .
896(12) 0.0 802.1 .
1012(12) 0.0 793.3 .
1144(13) 0.0 784.5 .
1299(14) 0.0 775.7 .
1465(15) 0.0 767.1 .
1639(16) 0.0 758.4 .
1884(17) 0.0 749.9 .
2129(18) 0.0 741.5 .
2452(19) 0.0 733.1 .
2835(20) 0.0 724.8 .
3367(22) 0.0 716.5 .
3920(24) 0.0 708.4 .
4532(25) 0.0 700.3 .
5089(26) 0.0 692.3 .
5441(27) 0.0 684.4 .
5458(25) 0.0 676.6 .
5049(23) 0.0 668.8 .
4357(20) 0.0 661.2 .
3483(17) 0.0 653.6 .
2642(14) 0.0 646.1 .
1901(11) 0.0 638.7 .
1348(10) 0.0 631.4 .
1003(9) 0.0 624.2 .
792(8) 0.0 617.1 .
672(8) 0.0 610.1 .
591(8) 0.0 603.1 .
562(8) 0.0 596.3 .
548(8) 0.0 589.5 .
534(8) 0.0 582.9 .
518(9) 0.0 576.3 .
506(7) 0.0 569.8 .
507(8) 0.0 563.4 .
502(8) 0.0 557.1 .
490(8) 0.0 550.9 .
491(7) 0.0 544.8 .
495(8) 0.0 538.8 .
477(7) 0.0 532.9 .
482(8) 0.0 527.1 .
485(8) 0.0 521.3 .
487(8) 0.0 515.7 .
497(8) 0.0 510.1 .
493(7) 0.0 504.7 .
476(8) 0.0 499.3 .
470(8) 0.0 494.0 .
469(8) 0.0 488.8 .
469(7) 0.0 483.7 .
455(8) 0.0 478.7 .
446(7) 0.0 473.8 .
451(8) 0.0 469.0 .
454(7) 0.0 464.2 .
443(7) 0.0 459.5 .
429(7) 0.0 455.0 .
423(8) 0.0 450.5 .
430(7) 0.0 446.1 .
427(7) 0.0 441.8 .
417(7) 0.0 437.5 .
410(7) 0.0 433.4 .
421(8) 0.0 429.3 .
416(7) 0.0 425.3 .
402(7) 0.0 421.4 .
421(7) 0.0 417.6 .
409(7) 0.0 413.8 .
399(7) 0.0 410.1 .
389(7) 0.0 406.5 .
391(7) 0.0 403.0 .
397(7) 0.0 399.6 .
381(7) 0.0 396.2 .
382(7) 0.0 392.9 .
382(7) 0.0 389.7 .
386(7) 0.0 386.5 .
380(7) 0.0 383.5 .
386(7) 0.0 380.5 .
369(6) 0.0 377.5 .
366(7) 0.0 374.6 .
377(6) 0.0 371.8 .
368(6) 0.0 369.1 .
365(6) 0.0 366.4 .
362(6) 0.0 363.8 .
366(6) 0.0 361.3 .
368(7) 0.0 358.8 .
369(6) 0.0 356.4 .
355(6) 0.0 354.0 .
348(7) 0.0 351.7 .
346(6) 0.0 349.5 .
353(6) 0.0 347.3 .
349(6) 0.0 345.2 .
345(6) 0.0 343.1 .
351(6) 0.0 341.1 .
341(6) 0.0 339.2 .
342(6) 0.0 337.3 .
333(6) 0.0 335.4 .
330(6) 0.0 333.6 .
328(6) 0.0 331.9 .
322(6) 0.0 330.2 .
331(6) 0.0 328.5 .
330(6) 0.02778 326.9 333.1
330(6) 0.02778 325.4 331.6
319(6) 0.02778 323.9 330.2
323(6) 0.02778 322.4 328.9
325(6) 0.02778 321.0 327.6
328(6) 0.02778 319.6 326.4
325(6) 0.02778 318.3 325.3
322(6) 0.02778 317.0 324.2
328(6) 0.02778 315.7 323.2
323(6) 0.02778 314.5 322.3
326(6) 0.02778 313.3 321.4
314(6) 0.02778 312.2 320.7
321(6) 0.02778 311.1 320.0
318(6) 0.02778 310.0 319.3
325(6) 0.02778 309.0 318.8
315(6) 0.02778 308.0 318.4
322(6) 0.02778 307.1 318.1
320(6) 0.02778 306.1 317.9
324(6) 0.02778 305.2 317.9
316(6) 0.02778 304.4 318.0
323(6) 0.02778 303.6 318.3
322(6) 0.02778 302.8 318.9
318(6) 0.02778 302.0 319.7
311(6) 0.02778 301.2 320.8
328(6) 0.02778 300.5 322.3
324(6) 0.02778 299.8 324.3
318(6) 0.02778 299.2 327.0
331(6) 0.02778 298.5 330.9
359(7) 0.02041 297.9 336.7
378(6) 0.02778 297.3 346.1
384(7) 0.02041 296.8 362.3
408(7) 0.02041 296.2 390.0
459(8) 0.01563 295.7 436.1
520(8) 0.01563 295.2 508.4
613(9) 0.01235 294.7 614.8
735(10) 0.01000 294.3 761.4
902(10) 0.01000 293.8 948.7
1099(12) 0.00694 293.4 1168.2
1324(14) 0.00510 293.0 1404.8
1535(13) 0.00592 292.6 1628.9
1685(13) 0.00592 292.3 1780.3
1765(14) 0.00510 291.9 1787.4
1631(14) 0.00510 291.6 1631.0
1450(11) 0.00826 291.3 1365.8
1167(11) 0.00826 291.0 1072.6
897(8) 0.01563 290.7 813.5
673(7) 0.02041 290.4 618.5
505(7) 0.02041 290.1 489.6
405(6) 0.02778 289.9 412.9
371(7) 0.02041 289.6 370.5
348(6) 0.02778 289.4 347.6
322(6) 0.02778 289.2 334.7
312(6) 0.02778 289.0 326.5
317(6) 0.02778 288.8 320.8
306(6) 0.02778 288.6 316.3
307(6) 0.02778 288.4 312.8
306(6) 0.02778 288.2 309.8
296(6) 0.02778 288.1 307.3
292(6) 0.02778 287.9 305.2
284(6) 0.02778 287.8 303.4
297(6) 0.02778 287.6 301.9
299(6) 0.02778 287.5 300.5
287(6) 0.02778 287.4 299.4
287(6) 0.02778 287.2 298.3
302(6) 0.02778 287.1 297.4
294(6) 0.02778 287.0 296.5
296(6) 0.02778 286.9 295.8
282(6) 0.02778 286.8 295.1
288(6) 0.02778 286.7 294.5
288(6) 0.02778 286.6 294.0
289(6) 0.02778 286.5 293.5
287(6) 0.02778 286.4 293.0
282(6) 0.02778 286.3 292.6
282(6) 0.02778 286.2 292.2
281(6) 0.02778 286.2 291.8
279(6) 0.02778 286.1 291.5
277(6) 0.02778 286.0 291.2
283(6) 0.02778 285.9 290.9
286(6) 0.02778 285.8 290.6
281(6) 0.02778 285.8 290.3
280(5) 0.0400 285.7 290.1
277(6) 0.02778 285.6 289.9
284(6) 0.02778 285.5 289.6
287(6) 0.02778 285.4 289.5
287(6) 0.02778 285.4 289.3
292(6) 0.02778 285.3 289.1
285(6) 0.02778 285.2 289.1
287(6) 0.02778 285.1 289.1
302(6) 0.02778 285.0 289.2
297(6) 0.02778 285.0 289.4
297(6) 0.02778 284.9 289.9
288(5) 0.0400 284.8 290.5
302(6) 0.02778 284.7 291.3
295(6) 0.02778 284.6 292.0
291(6) 0.02778 284.5 292.5
305(6) 0.02778 284.4 292.6
306(6) 0.02778 284.3 292.0
306(6) 0.02778 284.2 291.0
304(6) 0.02778 284.1 289.9
296(6) 0.02778 284.0 288.8
294(5) 0.0400 283.9 287.9
294(6) 0.02778 283.8 287.3
282(6) 0.02778 283.7 286.9
296(6) 0.02778 283.5 286.8
300(6) 0.02778 283.4 286.9
288(5) 0.0400 283.3 287.3
290(6) 0.02778 283.2 288.0
294(6) 0.02778 283.0 289.0
296(5) 0.0400 282.9 290.3
287(6) 0.02778 282.8 291.6
300(6) 0.02778 282.6 292.7
309(6) 0.02778 282.5 293.3
297(6) 0.02778 282.3 293.0
305(6) 0.02778 282.2 291.6
304(6) 0.02778 282.0 289.8
296(5) 0.0400 281.8 287.9
288(6) 0.02778 281.7 286.2
296(6) 0.02778 281.5 285.0
297(5) 0.0400 281.3 284.1
290(6) 0.02778 281.1 283.6
287(6) 0.02778 280.9 283.1
292(6) 0.02778 280.8 282.8
291(6) 0.02778 280.6 282.5
294(6) 0.02778 280.4 282.3
290(6) 0.02778 280.2 282.0
282(6) 0.02778 280.0 281.8
290(6) 0.02778 279.7 281.6
281(6) 0.02778 279.5 281.3
274(6) 0.02778 279.3 281.1
284(6) 0.02778 279.1 280.8
280(6) 0.02778 278.9 280.6
278(6) 0.02778 278.6 280.3
279(6) 0.02778 278.4 280.1
284(6) 0.02778 278.2 279.8
278(6) 0.02778 277.9 279.6
281(6) 0.02778 277.7 279.3
276(6) 0.02778 277.4 279.0
273(6) 0.02778 277.2 278.8
273(6) 0.02778 276.9 278.5
282(6) 0.02778 276.6 278.2
274(6) 0.02778 276.4 278.0
275(6) 0.02778 276.1 277.7
266(6) 0.02778 275.8 277.4
275(6) 0.02778 275.5 277.1
278(6) 0.02778 275.3 276.9
276(6) 0.02778 275.0 276.6
277(6) 0.02778 274.7 276.3
276(6) 0.02778 274.4 276.0
274(6) 0.02778 274.1 275.7
272(6) 0.02778 273.8 275.4
272(6) 0.02778 273.5 275.1
266(6) 0.02778 273.2 274.8
275(6) 0.02778 272.9 274.5
278(6) 0.02778 272.6 274.2
270(5) 0.0400 272.3 273.9
267(5) 0.0400 272.0 273.6
265(5) 0.0400 271.6 273.3
266(6) 0.02778 271.3 273.0
269(6) 0.02778 271.0 272.7
274(6) 0.02778 270.7 272.4
275(5) 0.0400 270.3 272.1
259(5) 0.0400 270.0 271.8
264(5) 0.0400 269.7 271.5
266(5) 0.0400 269.3 271.2
265(5) 0.0400 269.0 270.9
272(5) 0.0400 268.7 270.6
276(6) 0.02778 268.3 270.3
272(5) 0.0400 268.0 270.0
266(5) 0.0400 267.6 269.6
276(6) 0.02778 267.3 269.3
266(5) 0.0400 266.9 269.0
266(5) 0.0400 266.6 268.8
271(5) 0.0400 266.2 268.5
263(5) 0.0400 265.9 268.2
260(5) 0.0400 265.5 267.9
259(5) 0.0400 265.2 267.6
260(5) 0.0400 264.8 267.3
262(5) 0.0400 264.5 267.0
264(6) 0.02778 264.1 266.8
258(5) 0.0400 263.8 266.5
264(5) 0.0400 263.4 266.3
268(5) 0.0400 263.0 266.1
263(5) 0.0400 262.7 265.8
266(5) 0.0400 262.3 265.6
260(5) 0.0400 262.0 265.4
262(5) 0.0400 261.6 265.3
248(5) 0.0400 261.2 265.1
260(6) 0.02778 260.9 265.0
271(5) 0.0400 260.5 264.9
261(5) 0.0400 260.2 264.9
247(5) 0.0400 259.8 264.9
260(5) 0.0400 259.4 264.9
268(5) 0.0400 259.1 265.0
253(5) 0.0400 258.7 265.2
257(5) 0.0400 258.4 265.5
256(5) 0.0400 258.0 265.9
266(6) 0.02778 257.6 266.5
268(5) 0.0400 257.3 267.2
273(6) 0.02778 256.9 268.2
275(6) 0.02778 256.6 269.6
272(6) 0.02778 256.2 271.6
278(6) 0.02778 255.9 274.6
280(6) 0.02778 255.5 279.8
299(6) 0.02778 255.2 289.0
316(6) 0.02778 254.8 305.6
336(6) 0.02778 254.5 334.6
382(7) 0.02041 254.1 381.9
462(7) 0.02041 253.8 452.2
533(8) 0.01563 253.4 544.8
634(9) 0.01235 253.1 649.6
741(9) 0.01235 252.7 746.5
795(9) 0.01235 252.4 809.4
800(9) 0.01235 252.1 811.8
757(9) 0.01235 251.7 747.8
659(8) 0.01563 251.4 642.6
531(7) 0.02041 251.1 530.3
429(7) 0.02041 250.7 434.5
355(6) 0.02778 250.4 364.5
303(6) 0.02778 250.1 319.5
285(6) 0.02778 249.8 293.3
276(6) 0.02778 249.4 279.0
275(5) 0.0400 249.1 271.1
267(5) 0.0400 248.8 266.4
263(5) 0.0400 248.5 263.3
263(5) 0.0400 248.2 260.9
263(5) 0.0400 247.9 259.0
265(5) 0.0400 247.6 257.4
258(5) 0.0400 247.3 256.1
257(5) 0.0400 247.0 254.9
252(5) 0.0400 246.7 253.9
253(5) 0.0400 246.4 253.0
251(5) 0.0400 246.1 252.2
254(5) 0.0400 245.8 251.5
262(5) 0.0400 245.5 250.8
262(5) 0.0400 245.2 250.2
253(5) 0.0400 245.0 249.7
262(5) 0.0400 244.7 249.1
262(5) 0.0400 244.4 248.7
252(5) 0.0400 244.2 248.2
253(5) 0.0400 243.9 247.8
249(5) 0.0400 243.6 247.4
253(5) 0.0400 243.4 247.0
249(5) 0.0400 243.1 246.7
248(5) 0.0400 242.9 246.3
252(5) 0.0400 242.6 246.0
256(5) 0.0400 242.4 245.7
249(5) 0.0400 242.2 245.5
244(5) 0.0400 241.9 245.2
250(5) 0.0400 241.7 245.0
244(5) 0.0400 241.5 244.8
251(5) 0.0400 241.2 244.6
256(5) 0.0400 241.0 244.4
256(5) 0.0400 240.8 244.3
244(5) 0.0400 240.6 244.2
252(5) 0.0400 240.4 244.1
246(5) 0.0400 240.2 244.0
249(5) 0.0400 240.0 244.0
240(5) 0.0400 239.8 244.1
246(5) 0.0400 239.6 244.2
260(5) 0.0400 239.4 244.4
250(5) 0.0400 239.2 244.7
255(5) 0.0400 239.0 245.2
252(5) 0.0400 238.8 246.0
252(5) 0.0400 238.7 247.4
254(5) 0.0400 238.5 249.9
259(5) 0.0400 238.3 254.6
265(6) 0.02778 238.2 263.0
282(6) 0.02778 238.0 277.1
303(6) 0.02778 237.9 298.3
330(6) 0.02778 237.7 326.7
370(7) 0.02041 237.6 359.1
392(7) 0.02041 237.4 388.7
412(7) 0.02041 237.3 406.9
416(7) 0.02041 237.2 405.7
389(7) 0.02041 237.0 384.4
362(6) 0.02778 236.9 351.7
324(6) 0.02778 236.8 318.1
297(6) 0.02778 236.7 290.1
263(5) 0.0400 236.5 270.2
256(5) 0.0400 236.4 257.6
241(5) 0.0400 236.3 250.4
247(5) 0.0400 236.2 246.5
250(5) 0.0400 236.1 244.4
251(5) 0.0400 236.0 243.1
242(5) 0.0400 235.9 242.2
247(5) 0.0400 235.9 241.6
244(5) 0.0400 235.8 241.2
245(5) 0.0400 235.7 240.8
236(5) 0.0400 235.6 240.5
241(5) 0.0400 235.6 240.4
240(5) 0.0400 235.5 240.3
236(5) 0.0400 235.4 240.2
236(5) 0.0400 235.4 240.3
237(5) 0.0400 235.3 240.4
244(5) 0.0400 235.3 240.6
245(5) 0.0400 235.2 241.0
244(5) 0.0400 235.2 241.7
237(5) 0.0400 235.1 242.8
254(5) 0.0400 235.1 244.9
248(5) 0.0400 235.1 248.8
255(5) 0.0400 235.0 255.7
265(5) 0.0400 235.0 267.0
280(6) 0.02778 235.0 283.7
307(6) 0.02778 235.0 305.1
319(6) 0.02778 234.9 328.3
334(6) 0.02778 234.9 347.7
346(6) 0.02778 234.9 356.8
352(6) 0.02778 234.9 351.0
323(6) 0.02778 234.9 332.3
308(6) 0.02778 234.9 308.3
284(6) 0.02778 234.9 285.6
256(5) 0.0400 234.9 267.9
254(5) 0.0400 234.9 255.9
246(5) 0.0400 235.0 248.6
241(5) 0.0400 235.0 244.6
243(5) 0.0400 235.0 242.5
243(5) 0.0400 235.0 241.3
240(5) 0.0400 235.0 240.6
233(5) 0.0400 235.1 240.1
243(5) 0.0400 235.1 239.8
239(5) 0.0400 235.1 239.6
240(5) 0.0400 235.2 239.4
240(5) 0.0400 235.2 239.3
236(5) 0.0400 235.3 239.3
235(5) 0.0400 235.3 239.3
237(5) 0.0400 235.4 239.3
232(5) 0.0400 235.4 239.3
230(5) 0.0400 235.5 239.4
240(5) 0.0400 235.5 239.5
236(5) 0.0400 235.6 239.6
229(5) 0.0400 235.7 239.7
228(5) 0.0400 235.7 239.9
234(5) 0.0400 235.8 240.1
235(5) 0.0400 235.9 240.3
235(5) 0.0400 235.9 240.6
232(5) 0.0400 236.0 240.9
242(5) 0.0400 236.1 241.2
239(5) 0.0400 236.2 241.6
242(5) 0.0400 236.3 242.0
232(5) 0.0400 236.4 242.5
236(5) 0.0400 236.4 243.1
241(5) 0.0400 236.5 243.7
239(5) 0.0400 236.6 244.5
243(5) 0.0400 236.7 245.4
249(5) 0.0400 236.8 246.5
245(5) 0.0400 236.9 247.8
245(5) 0.0400 237.0 249.3
241(5) 0.0400 237.1 251.4
254(5) 0.0400 237.2 254.1
263(5) 0.0400 237.3 258.3
255(5) 0.0400 237.4 265.1
278(6) 0.02778 237.5 277.4
307(6) 0.02778 237.6 299.4
339(6) 0.02778 237.7 337.2
394(7) 0.02041 237.9 396.2
491(7) 0.02041 238.0 478.2
608(8) 0.01563 238.1 576.1
696(9) 0.01235 238.2 670.7
753(9) 0.01235 238.3 733.9
763(9) 0.01235 238.4 738.8
699(9) 0.01235 238.6 680.5
596(7) 0.02041 238.7 584.6
472(7) 0.02041 238.8 483.8
366(6) 0.02778 238.9 399.3
311(6) 0.02778 239.0 338.7
273(5) 0.0400 239.2 300.6
258(6) 0.02778 239.3 278.8
248(5) 0.0400 239.4 267.2
248(5) 0.0400 239.6 260.9
255(5) 0.0400 239.7 257.2
247(5) 0.0400 239.8 254.9
245(5) 0.0400 239.9 253.3
246(5) 0.0400 240.1 252.1
252(5) 0.0400 240.2 251.2
252(5) 0.0400 240.3 250.5
254(5) 0.0400 240.5 250.1
246(5) 0.0400 240.6 249.8
250(6) 0.02778 240.7 249.8
251(5) 0.0400 240.9 250.0
256(5) 0.0400 241.0 250.6
256(5) 0.0400 241.1 251.8
255(5) 0.0400 241.3 254.2
257(5) 0.0400 241.4 258.7
265(5) 0.0400 241.5 266.3
278(6) 0.02778 241.7 278.0
292(6) 0.02778 241.8 293.7
313(6) 0.02778 241.9 311.3
320(6) 0.02778 242.1 327.0
330(6) 0.02778 242.2 335.2
324(6) 0.02778 242.3 332.2
313(6) 0.02778 242.5 319.1
301(6) 0.02778 242.6 301.8
279(6) 0.02778 242.7 285.7
268(5) 0.0400 242.9 273.9
266(5) 0.0400 243.0 267.0
258(5) 0.0400 243.1 264.3
267(6) 0.02778 243.3 264.2
266(5) 0.0400 243.4 264.9
269(5) 0.0400 243.5 264.8
257(5) 0.0400 243.6 263.0
254(5) 0.0400 243.8 260.1
256(5) 0.0400 243.9 257.0
263(5) 0.0400 244.0 254.2
263(5) 0.0400 244.2 252.2
257(5) 0.0400 244.3 250.9
251(5) 0.0400 244.4 250.2
247(5) 0.0400 244.5 249.8
253(5) 0.0400 244.6 249.7
251(5) 0.0400 244.8 249.7
249(5) 0.0400 244.9 249.7
256(5) 0.0400 245.0 249.8
257(5) 0.0400 245.1 250.0
253(5) 0.0400 245.3 250.1
253(5) 0.0400 245.4 250.3
252(5) 0.0400 245.5 250.5
254(5) 0.0400 245.6 250.7
247(5) 0.0400 245.7 251.0
248(5) 0.0400 245.8 251.3
250(5) 0.0400 245.9 251.6
251(5) 0.0400 246.0 252.0
252(5) 0.0400 246.2 252.4
261(5) 0.0400 246.3 252.8
259(5) 0.0400 246.4 253.4
261(5) 0.0400 246.5 254.0
257(5) 0.0400 246.6 254.8
262(6) 0.02778 246.7 255.8
254(5) 0.0400 246.8 257.3
257(5) 0.0400 246.9 259.6
262(5) 0.0400 247.0 263.6
271(6) 0.02778 247.1 270.5
300(6) 0.02778 247.2 281.9
308(6) 0.02778 247.3 299.3
319(6) 0.02778 247.3 322.4
346(7) 0.02041 247.4 348.5
367(6) 0.02778 247.5 371.6
383(7) 0.02041 247.6 383.5
380(6) 0.02778 247.7 378.6
365(6) 0.02778 247.8 359.2
339(6) 0.02778 247.8 333.9
302(6) 0.02778 247.9 310.2
291(5) 0.0400 248.0 292.0
277(6) 0.02778 248.1 280.1
275(5) 0.0400 248.1 273.4
276(6) 0.02778 248.2 270.4
280(6) 0.02778 248.3 269.6
277(6) 0.02778 248.4 269.9
285(5) 0.0400 248.4 271.1
272(5) 0.0400 248.5 272.9
280(6) 0.02778 248.5 275.4
287(5) 0.0400 248.6 278.6
279(6) 0.02778 248.7 282.7
287(6) 0.02778 248.7 288.1
301(6) 0.02778 248.8 295.9
316(6) 0.02778 248.8 307.9
330(6) 0.02778 248.9 328.8
382(7) 0.02041 248.9 366.6
463(7) 0.02041 248.9 434.6
585(9) 0.01235 249.0 549.0
768(10) 0.01000 249.0 722.4
1016(11) 0.00826 249.1 952.4
1264(12) 0.00694 249.1 1208.9
1454(13) 0.00592 249.1 1428.5
1552(13) 0.00592 249.2 1529.6
1458(13) 0.00592 249.2 1460.8
1249(11) 0.00826 249.2 1255.1
985(10) 0.01000 249.2 1001.0
721(8) 0.01563 249.3 771.6
541(8) 0.01563 249.3 602.9
466(7) 0.02041 249.3 499.5
453(7) 0.02041 249.3 446.6
438(7) 0.02041 249.3 422.0
441(7) 0.02041 249.3 405.3
408(7) 0.02041 249.3 384.6
373(6) 0.02778 249.3 359.1
343(6) 0.02778 249.3 333.5
317(6) 0.02778 249.3 311.6
305(6) 0.02778 249.3 295.2
295(6) 0.02778 249.3 284.0
287(5) 0.0400 249.3 276.7
266(6) 0.02778 249.3 272.1
260(5) 0.0400 249.3 269.0
275(6) 0.02778 249.3 266.8
275(6) 0.02778 249.3 265.0
268(6) 0.02778 249.3 263.6
266(5) 0.0400 249.3 262.4
275(5) 0.0400 249.2 261.3
269(5) 0.0400 249.2 260.4
265(6) 0.02778 249.2 259.7
274(5) 0.0400 249.1 259.0
275(6) 0.02778 249.1 258.5
274(5) 0.0400 249.1 258.0
271(5) 0.0400 249.0 257.6
257(5) 0.0400 249.0 257.2
257(5) 0.0400 249.0 257.0
255(6) 0.02778 248.9 256.8
258(5) 0.0400 248.9 256.7
259(5) 0.0400 248.8 256.8
266(5) 0.0400 248.8 257.3
269(6) 0.02778 248.7 258.3
261(5) 0.0400 248.7 260.4
274(5) 0.0400 248.6 264.2
268(5) 0.0400 248.6 270.2
274(6) 0.02778 248.5 278.4
295(6) 0.02778 248.4 287.7
310(6) 0.02778 248.4 295.9
308(6) 0.02778 248.3 299.8
306(6) 0.02778 248.2 297.3
289(6) 0.02778 248.1 289.5
272(6) 0.02778 248.1 279.8
269(5) 0.0400 248.0 270.7
262(5) 0.0400 247.9 263.7
258(5) 0.0400 247.8 259.0
260(6) 0.02778 247.8 256.2
256(5) 0.0400 247.7 254.6
263(5) 0.0400 247.6 253.7
265(5) 0.0400 247.5 253.1
252(6) 0.02778 247.4 252.7
242(5) 0.0400 247.3 252.4
251(5) 0.0400 247.2 252.2
254(5) 0.0400 247.1 252.0
248(5) 0.0400 247.0 251.9
249(5) 0.0400 246.9 251.9
248(5) 0.0400 246.8 252.0
252(5) 0.0400 246.7 252.4
252(6) 0.02778 246.6 253.2
259(5) 0.0400 246.5 254.6
265(5) 0.0400 246.4 256.8
259(5) 0.0400 246.2 259.9
258(5) 0.0400 246.1 263.3
257(5) 0.0400 246.0 266.1
265(5) 0.0400 245.9 267.3
261(5) 0.0400 245.8 266.1
253(5) 0.0400 245.6 263.1
253(5) 0.0400 245.5 259.6
249(5) 0.0400 245.4 256.4
252(5) 0.0400 245.3 253.9
255(6) 0.02778 245.1 252.3
252(5) 0.0400 245.0 251.4
250(5) 0.0400 244.9 250.9
250(5) 0.0400 244.7 250.7
255(5) 0.0400 244.6 250.6
251(5) 0.0400 244.4 250.6
236(5) 0.0400 244.3 250.6
249(5) 0.0400 244.1 250.7
254(5) 0.0400 244.0 250.9
250(5) 0.0400 243.9 251.1
254(5) 0.0400 243.7 251.3
251(6) 0.02778 243.6 251.6
256(5) 0.0400 243.4 252.0
251(5) 0.0400 243.3 252.5
259(5) 0.0400 243.1 253.0
251(5) 0.0400 242.9 253.7
250(5) 0.0400 242.8 254.5
241(5) 0.0400 242.6 255.5
248(5) 0.0400 242.5 256.7
262(5) 0.0400 242.3 258.2
266(5) 0.0400 242.1 260.0
260(6) 0.02778 242.0 262.3
254(5) 0.0400 241.8 265.2
267(5) 0.0400 241.6 269.0
280(5) 0.0400 241.5 274.2
284(6) 0.02778 241.3 282.2
299(6) 0.02778 241.1 295.8
329(6) 0.02778 240.9 320.3
371(7) 0.02041 240.8 364.9
458(7) 0.02041 240.6 441.1
599(8) 0.01563 240.4 559.0
752(10) 0.01000 240.2 719.0
935(10) 0.01000 240.1 902.3
1084(11) 0.00826 239.9 1064.6
1161(11) 0.00826 239.7 1143.7
1116(11) 0.00826 239.5 1098.0
953(10) 0.01000 239.3 950.2
749(9) 0.01235 239.2 764.8
557(8) 0.01563 239.0 594.4
409(6) 0.02778 238.8 464.1
333(6) 0.02778 238.6 377.5
289(6) 0.02778 238.4 325.9
286(6) 0.02778 238.2 297.3
273(5) 0.0400 238.0 281.6
257(5) 0.0400 237.8 272.4
258(5) 0.0400 237.6 266.4
263(5) 0.0400 237.5 262.1
255(5) 0.0400 237.3 258.8
247(5) 0.0400 237.1 256.2
243(5) 0.0400 236.9 254.2
251(5) 0.0400 236.7 252.7
247(5) 0.0400 236.5 252.0
246(5) 0.0400 236.3 252.1
248(5) 0.0400 236.1 253.4
239(5) 0.0400 235.9 255.9
247(5) 0.0400 235.7 259.3
253(5) 0.0400 235.5 262.7
254(5) 0.0400 235.3 264.7
246(5) 0.0400 235.1 263.9
245(5) 0.0400 234.9 260.3
251(5) 0.0400 234.7 255.3
250(5) 0.0400 234.5 250.5
243(5) 0.0400 234.3 246.4
243(5) 0.0400 234.1 243.5
247(5) 0.0400 233.9 241.6
240(5) 0.0400 233.7 240.3
237(5) 0.0400 233.5 239.5
239(5) 0.0400 233.3 238.8
230(5) 0.0400 233.1 238.3
234(5) 0.0400 232.9 237.8
237(5) 0.0400 232.7 237.4
233(5) 0.0400 232.5 237.0
228(5) 0.0400 232.3 236.7
231(5) 0.0400 232.1 236.3
234(5) 0.0400 231.8 236.0
233(5) 0.0400 231.6 235.7
229(5) 0.0400 231.4 235.4
237(5) 0.0400 231.2 235.1
233(5) 0.0400 231.0 234.9
236(5) 0.0400 230.8 234.6
235(5) 0.0400 230.6 234.4
247(5) 0.0400 230.4 234.1
233(5) 0.0400 230.2 233.9
227(5) 0.0400 230.0 233.7
229(5) 0.0400 229.8 233.5
227(5) 0.0400 229.6 233.3
236(5) 0.0400 229.4 233.1
239(5) 0.0400 229.2 232.9
233(5) 0.0400 229.0 232.7
234(5) 0.0400 228.8 232.6
231(5) 0.0400 228.6 232.5
237(5) 0.0400 228.4 232.4
231(5) 0.0400 228.2 232.3
232(5) 0.0400 228.0 232.2
232(5) 0.0400 227.8 232.2
231(5) 0.0400 227.6 232.1
237(5) 0.0400 227.4 232.1
228(5) 0.0400 227.2 232.0
230(5) 0.0400 227.0 232.0
234(5) 0.0400 226.8 232.1
234(5) 0.0400 226.6 232.1
227(5) 0.0400 226.4 232.3
229(5) 0.0400 226.2 232.5
228(5) 0.0400 226.0 232.9
227(5) 0.0400 225.8 233.3
237(5) 0.0400 225.6 233.9
244(5) 0.0400 225.4 234.8
246(5) 0.0400 225.2 236.0
238(5) 0.0400 225.0 237.8
243(5) 0.0400 224.8 240.8
254(5) 0.0400 224.6 246.3
261(5) 0.0400 224.4 256.5
276(5) 0.0400 224.2 274.2
307(6) 0.02778 224.0 302.6
350(6) 0.02778 223.8 342.8
401(6) 0.02778 223.6 391.4
440(7) 0.02041 223.4 438.0
454(7) 0.02041 223.2 466.3
454(6) 0.02778 223.0 461.6
418(6) 0.02778 222.9 426.2
371(6) 0.02778 222.7 377.1
322(6) 0.02778 222.5 329.9
289(5) 0.0400 222.3 292.8
263(5) 0.0400 222.1 267.6
251(5) 0.0400 221.9 252.3
243(5) 0.0400 221.7 243.7
243(5) 0.0400 221.6 238.7
238(5) 0.0400 221.4 235.7
238(5) 0.0400 221.2 233.6
239(5) 0.0400 221.0 232.1
237(5) 0.0400 220.8 231.0
241(5) 0.0400 220.7 230.2
241(5) 0.0400 220.5 229.6
236(5) 0.0400 220.3 229.1
234(5) 0.0400 220.1 228.8
230(5) 0.0400 220.0 228.6
234(5) 0.0400 219.8 228.4
239(5) 0.0400 219.6 228.4
241(5) 0.0400 219.4 228.5
231(5) 0.0400 219.3 228.6
232(5) 0.0400 219.1 228.9
238(5) 0.0400 218.9 229.4
230(5) 0.0400 218.8 230.0
229(5) 0.0400 218.6 230.9
240(5) 0.0400 218.4 232.3
241(5) 0.0400 218.3 234.6
245(5) 0.0400 218.1 238.7
250(5) 0.0400 218.0 246.0
269(5) 0.0400 217.8 258.7
288(5) 0.0400 217.6 278.8
316(6) 0.02778 217.5 307.0
348(6) 0.02778 217.3 340.8
374(6) 0.02778 217.2 373.0
379(6) 0.02778 217.0 391.9
378(6) 0.02778 216.9 388.0
350(6) 0.02778 216.7 363.6
329(6) 0.02778 216.6 330.8
300(5) 0.0400 216.4 300.0
272(5) 0.0400 216.3 276.5
259(5) 0.0400 216.1 261.4
247(5) 0.0400 216.0 253.3
246(5) 0.0400 215.8 250.2
259(5) 0.0400 215.7 250.2
256(5) 0.0400 215.5 252.5
255(5) 0.0400 215.4 256.8
267(5) 0.0400 215.3 264.0
278(5) 0.0400 215.1 276.1
308(6) 0.02778 215.0 298.2
349(6) 0.02778 214.9 338.7
420(7) 0.02041 214.7 409.9
531(8) 0.01563 214.6 524.4
701(9) 0.01235 214.5 687.2
896(10) 0.01000 214.3 885.8
1081(11) 0.00826 214.2 1079.5
1216(12) 0.00694 214.1 1199.6
1183(11) 0.00826 214.0 1184.1
1045(11) 0.00826 213.8 1040.7
849(9) 0.01235 213.7 839.5
623(8) 0.01563 213.6 645.8
451(7) 0.02041 213.5 493.3
362(6) 0.02778 213.4 389.4
305(6) 0.02778 213.2 326.2
269(5) 0.0400 213.1 290.3
258(5) 0.0400 213.0 270.1
248(5) 0.0400 212.9 258.0
243(5) 0.0400 212.8 250.0
241(5) 0.0400 212.7 244.3
232(5) 0.0400 212.6 240.0
235(5) 0.0400 212.5 236.6
235(5) 0.0400 212.3 234.0
231(5) 0.0400 212.2 231.9
231(5) 0.0400 212.1 230.1
231(5) 0.0400 212.0 228.8
242(5) 0.0400 211.9 227.7
229(5) 0.0400 211.8 226.8
231(5) 0.0400 211.7 226.2
232(5) 0.0400 211.6 225.9
224(5) 0.0400 211.5 225.7
224(5) 0.0400 211.5 225.8
226(5) 0.0400 211.4 226.4
237(5) 0.0400 211.3 227.6
240(5) 0.0400 211.2 230.1
251(5) 0.0400 211.1 235.0
247(5) 0.0400 211.0 244.1
256(5) 0.0400 210.9 259.7
278(6) 0.02778 210.8 283.3
313(6) 0.02778 210.8 314.2
348(6) 0.02778 210.7 347.9
377(7) 0.02041 210.6 374.6
389(7) 0.02041 210.5 381.9
365(6) 0.02778 210.4 365.4
333(6) 0.02778 210.4 334.0
314(6) 0.02778 210.3 300.1
274(5) 0.0400 210.2 271.3
239(5) 0.0400 210.1 250.7
240(5) 0.0400 210.1 237.6
236(5) 0.0400 210.0 230.2
222(5) 0.0400 209.9 226.1
229(5) 0.0400 209.9 224.0
227(5) 0.0400 209.8 222.9
229(5) 0.0400 209.7 222.5
235(5) 0.0400 209.7 222.8
232(5) 0.0400 209.6 224.0
232(5) 0.0400 209.6 226.6
239(5) 0.0400 209.5 231.6
245(5) 0.0400 209.4 239.4
255(5) 0.0400 209.4 250.3
262(5) 0.0400 209.3 263.1
279(6) 0.02778 209.3 275.2
286(6) 0.02778 209.2 282.9
294(6) 0.02778 209.2 284.4
287(6) 0.02778 209.1 283.3
285(6) 0.02778 209.1 284.8
288(6) 0.02778 209.0 291.8
291(6) 0.02778 209.0 302.9
305(6) 0.02778 208.9 312.3
305(6) 0.02778 208.9 312.5
304(6) 0.02778 208.8 300.6
284(6) 0.02778 208.8 281.6
265(5) 0.0400 208.8 261.9
245(5) 0.0400 208.7 245.6
238(5) 0.0400 208.7 234.1
229(5) 0.0400 208.6 226.8
225(5) 0.0400 208.6 222.6
220(5) 0.0400 208.6 220.4
221(5) 0.0400 208.5 219.2
226(5) 0.0400 208.5 218.6
220(5) 0.0400 208.5 218.3
227(5) 0.0400 208.5 218.3
232(5) 0.0400 208.4 218.5
226(5) 0.0400 208.4 218.9
234(5) 0.0400 208.4 219.6
233(5) 0.0400 208.3 220.7
233(5) 0.0400 208.3 222.5
236(5) 0.0400 208.3 225.5
236(5) 0.0400 208.3 230.9
245(5) 0.0400 208.3 240.8
272(6) 0.02778 208.2 257.8
289(6) 0.02778 208.2 284.6
333(6) 0.02778 208.2 321.9
364(6) 0.02778 208.2 365.8
400(7) 0.02041 208.2 406.3
420(7) 0.02041 208.1 427.4
415(7) 0.02041 208.1 417.2
378(6) 0.02778 208.1 381.8
334(6) 0.02778 208.1 337.4
299(6) 0.02778 208.1 297.1
261(5) 0.0400 208.1 266.5
234(5) 0.0400 208.1 246.3
230(5) 0.0400 208.1 234.4
227(5) 0.0400 208.1 227.9
223(5) 0.0400 208.0 224.6
225(5) 0.0400 208.0 223.1
227(5) 0.0400 208.0 222.7
229(5) 0.0400 208.0 223.5
233(5) 0.0400 208.0 226.1
235(5) 0.0400 208.0 231.6
233(5) 0.0400 208.0 241.3
250(5) 0.0400 208.0 256.1
275(6) 0.02778 208.0 275.5
293(6) 0.02778 208.0 296.3
304(6) 0.02778 208.0 312.3
289(6) 0.02778 208.0 315.6
295(6) 0.02778 208.0 304.0
284(6) 0.02778 208.0 283.7
259(5) 0.0400 208.0 262.5
244(5) 0.0400 208.0 244.9
225(5) 0.0400 208.0 232.4
230(5) 0.0400 208.0 224.5
227(5) 0.0400 208.1 219.9
215(5) 0.0400 208.1 217.3
210(5) 0.0400 208.1 215.8
218(5) 0.0400 208.1 214.8
217(5) 0.0400 208.1 214.1
209(5) 0.0400 208.1 213.6
203(5) 0.0400 208.1 213.2
208(5) 0.0400 208.1 212.9
215(5) 0.0400 208.1 212.6
216(5) 0.0400 208.1 212.4
210(5) 0.0400 208.2 212.2
220(5) 0.0400 208.2 212.1
211(5) 0.0400 208.2 212.0
210(5) 0.0400 208.2 211.9
206(5) 0.0400 208.2 211.8
200(5) 0.0400 208.2 211.7
212(5) 0.0400 208.2 211.7
214(5) 0.0400 208.3 211.7
213(5) 0.0400 208.3 211.7
211(5) 0.0400 208.3 211.7
212(5) 0.0400 208.3 211.8
211(5) 0.0400 208.3 211.9
219(5) 0.0400 208.3 212.1
217(5) 0.0400 208.4 212.3
211(5) 0.0400 208.4 212.4
214(5) 0.0400 208.4 212.5
216(5) 0.0400 208.4 212.6
215(5) 0.0400 208.4 212.6
212(5) 0.0400 208.5 212.6
211(5) 0.0400 208.5 212.6
216(5) 0.0400 208.5 212.8
210(5) 0.0400 208.5 213.0
217(5) 0.0400 208.5 213.3
207(5) 0.0400 208.6 213.7
209(5) 0.0400 208.6 214.3
213(5) 0.0400 208.6 215.2
213(5) 0.0400 208.6 216.6
228(5) 0.0400 208.6 219.1
221(5) 0.0400 208.7 223.5
226(5) 0.0400 208.7 230.7
239(5) 0.0400 208.7 241.5
257(5) 0.0400 208.7 255.4
262(5) 0.0400 208.8 270.3
269(5) 0.0400 208.8 281.7
282(6) 0.02778 208.8 284.2
271(5) 0.0400 208.8 276.2
255(5) 0.0400 208.8 262.1
248(5) 0.0400 208.9 247.5
233(5) 0.0400 208.9 235.4
231(5) 0.0400 208.9 226.9
216(5) 0.0400 208.9 221.5
223(5) 0.0400 209.0 218.5
212(5) 0.0400 209.0 216.8
215(5) 0.0400 209.0 215.9
220(5) 0.0400 209.0 215.4
222(5) 0.0400 209.1 215.1
215(5) 0.0400 209.1 214.9
216(5) 0.0400 209.1 214.8
214(5) 0.0400 209.1 214.8
215(5) 0.0400 209.2 214.8
215(5) 0.0400 209.2 214.9
215(5) 0.0400 209.2 215.1
225(5) 0.0400 209.2 215.2
217(5) 0.0400 209.2 215.5
213(5) 0.0400 209.3 215.8
213(5) 0.0400 209.3 216.2
222(5) 0.0400 209.3 216.8
228(5) 0.0400 209.3 217.7
220(5) 0.0400 209.4 219.2
219(5) 0.0400 209.4 221.6
220(5) 0.0400 209.4 225.5
231(5) 0.0400 209.4 231.3
241(5) 0.0400 209.5 238.8
256(5) 0.0400 209.5 247.2
253(5) 0.0400 209.5 254.2
251(5) 0.0400 209.5 256.7
254(5) 0.0400 209.5 253.5
242(5) 0.0400 209.6 246.8
233(5) 0.0400 209.6 239.6
230(5) 0.0400 209.6 233.8
232(5) 0.0400 209.6 229.9
229(5) 0.0400 209.6 227.9
228(5) 0.0400 209.7 227.4
221(5) 0.0400 209.7 228.0
225(5) 0.0400 209.7 229.3
228(5) 0.0400 209.7 231.2
230(5) 0.0400 209.7 233.8
235(5) 0.0400 209.7 237.2
236(5) 0.0400 209.8 241.8
251(5) 0.0400 209.8 248.2
274(6) 0.02778 209.8 257.2
279(6) 0.02778 209.8 270.7
299(6) 0.02778 209.8 292.6
338(6) 0.02778 209.8 329.3
386(7) 0.02041 209.9 390.8
482(7) 0.02041 209.9 487.9
621(8) 0.01563 209.9 626.2
782(9) 0.01235 209.9 796.3
960(10) 0.01000 209.9 964.3
1062(11) 0.00826 209.9 1068.3
1070(11) 0.00826 209.9 1050.9
962(10) 0.01000 210.0 921.9
781(9) 0.01235 210.0 746.5
580(8) 0.01563 210.0 580.7
445(7) 0.02041 210.0 451.2
355(6) 0.02778 210.0 363.2
307(6) 0.02778 210.0 309.4
272(5) 0.0400 210.0 278.7
254(5) 0.0400 210.0 261.3
247(5) 0.0400 210.0 251.0
235(5) 0.0400 210.0 244.2
231(5) 0.0400 210.1 239.3
232(5) 0.0400 210.1 235.5
233(5) 0.0400 210.1 232.6
222(5) 0.0400 210.1 230.2
224(5) 0.0400 210.1 228.3
223(5) 0.0400 210.1 226.7
220(5) 0.0400 210.1 225.4
222(5) 0.0400 210.1 224.3
216(5) 0.0400 210.1 223.5
221(5) 0.0400 210.1 222.8
226(5) 0.0400 210.1 222.2
218(5) 0.0400 210.1 221.8
219(5) 0.0400 210.1 221.4
224(5) 0.0400 210.1 221.2
223(5) 0.0400 210.1 221.1
219(5) 0.0400 210.1 221.2
218(5) 0.0400 210.1 221.3
224(5) 0.0400 210.1 221.6
229(5) 0.0400 210.1 222.1
220(5) 0.0400 210.1 222.7
218(5) 0.0400 210.1 223.7
224(5) 0.0400 210.1 225.1
225(5) 0.0400 210.1 227.4
230(5) 0.0400 210.1 231.3
239(5) 0.0400 210.0 238.1
253(5) 0.0400 210.0 249.9
274(5) 0.0400 210.0 269.1
296(5) 0.0400 210.0 297.2
338(6) 0.02778 210.0 333.1
382(6) 0.02778 210.0 371.1
411(6) 0.02778 210.0 399.7
409(6) 0.02778 210.0 406.1
410(6) 0.02778 210.0 389.6
380(6) 0.02778 210.0 363.3
357(6) 0.02778 209.9 339.6
337(6) 0.02778 209.9 323.2
325(6) 0.02778 209.9 311.8
301(5) 0.0400 209.9 299.5
289(5) 0.0400 209.9 283.9
275(5) 0.0400 209.9 267.1
253(5) 0.0400 209.8 252.2
240(5) 0.0400 209.8 240.7
234(5) 0.0400 209.8 232.7
226(5) 0.0400 209.8 227.6
217(5) 0.0400 209.8 224.6
221(5) 0.0400 209.7 222.8
220(5) 0.0400 209.7 221.7
217(5) 0.0400 209.7 221.1
220(5) 0.0400 209.7 220.7
216(5) 0.0400 209.6 220.6
218(5) 0.0400 209.6 220.7
211(5) 0.0400 209.6 221.1
215(5) 0.0400 209.6 222.1
219(5) 0.0400 209.5 224.0
221(5) 0.0400 209.5 227.5
227(5) 0.0400 209.5 233.8
250(5) 0.0400 209.4 243.7
261(5) 0.0400 209.4 257.6
278(5) 0.0400 209.4 274.2
293(5) 0.0400 209.3 290.0
312(6) 0.02778 209.3 298.7
304(6) 0.02778 209.3 295.3
291(5) 0.0400 209.2 281.9
277(5) 0.0400 209.2 265.1
262(5) 0.0400 209.2 249.8
245(5) 0.0400 209.1 238.2
225(5) 0.0400 209.1 230.6
225(5) 0.0400 209.1 226.2
222(5) 0.0400 209.0 223.9
217(5) 0.0400 209.0 223.1
215(5) 0.0400 208.9 223.2
221(5) 0.0400 208.9 224.5
223(5) 0.0400 208.9 227.4
230(5) 0.0400 208.8 232.4
226(5) 0.0400 208.8 240.2
235(5) 0.0400 208.7 250.5
249(5) 0.0400 208.7 262.0
258(5) 0.0400 208.6 271.4
264(5) 0.0400 208.6 274.4
270(5) 0.0400 208.5 269.2
248(5) 0.0400 208.5 258.9
248(5) 0.0400 208.4 247.9
233(5) 0.0400 208.4 238.8
238(5) 0.0400 208.3 232.4
233(5) 0.0400 208.3 228.5
222(5) 0.0400 208.2 226.6
222(5) 0.0400 208.2 226.0
228(5) 0.0400 208.1 226.1
228(5) 0.0400 208.1 226.6
223(5) 0.0400 208.0 227.6
217(5) 0.0400 208.0 228.9
225(5) 0.0400 207.9 230.6
231(5) 0.0400 207.9 232.7
230(5) 0.0400 207.8 235.3
237(5) 0.0400 207.7 238.6
233(5) 0.0400 207.7 242.7
235(5) 0.0400 207.6 248.1
249(5) 0.0400 207.6 255.4
262(5) 0.0400 207.5 266.2
279(6) 0.02778 207.4 283.5
294(6) 0.02778 207.4 313.5
346(6) 0.02778 207.3 365.6
422(7) 0.02041 207.3 451.6
546(8) 0.01563 207.2 580.9
722(9) 0.01235 207.1 752.3
924(10) 0.01000 207.1 944.4
1080(11) 0.00826 207.0 1104.8
1166(11) 0.00826 206.9 1159.2
1135(11) 0.00826 206.9 1074.5
972(10) 0.01000 206.8 900.9
766(9) 0.01235 206.7 711.4
574(8) 0.01563 206.7 550.4
433(7) 0.02041 206.6 433.5
364(6) 0.02778 206.5 358.7
314(6) 0.02778 206.4 315.5
291(6) 0.02778 206.4 292.7
270(5) 0.0400 206.3 282.5
273(6) 0.02778 206.2 281.3
295(6) 0.02778 206.1 289.3
296(6) 0.02778 206.1 308.9
328(6) 0.02778 206.0 342.9
382(7) 0.02041 205.9 391.9
433(7) 0.02041 205.8 451.4
497(7) 0.02041 205.8 508.0
549(8) 0.01563 205.7 539.6
550(8) 0.01563 205.6 530.4
510(8) 0.01563 205.5 491.0
451(7) 0.02041 205.4 445.0
412(7) 0.02041 205.4 407.3
377(6) 0.02778 205.3 380.1
343(6) 0.02778 205.2 356.9
314(6) 0.02778 205.1 331.5
293(6) 0.02778 205.0 304.9
270(5) 0.0400 205.0 280.9
260(5) 0.0400 204.9 261.9
252(5) 0.0400 204.8 248.1
229(5) 0.0400 204.7 239.0
237(5) 0.0400 204.6 233.3
230(5) 0.0400 204.5 229.7
235(5) 0.0400 204.4 227.5
231(5) 0.0400 204.3 226.0
221(5) 0.0400 204.3 225.0
227(5) 0.0400 204.2 224.4
229(5) 0.0400 204.1 224.1
232(5) 0.0400 204.0 224.2
232(5) 0.0400 203.9 224.7
227(5) 0.0400 203.8 226.0
224(5) 0.0400 203.7 228.3
236(5) 0.0400 203.6 232.2
238(5) 0.0400 203.5 237.9
244(5) 0.0400 203.4 245.3
250(5) 0.0400 203.4 253.5
257(5) 0.0400 203.3 260.2
262(5) 0.0400 203.2 262.7
261(5) 0.0400 203.1 260.6
264(5) 0.0400 203.0 256.1
257(5) 0.0400 202.9 252.0
266(5) 0.0400 202.8 250.0
268(5) 0.0400 202.7 250.6
277(6) 0.02778 202.6 254.2
284(6) 0.02778 202.5 261.3
302(6) 0.02778 202.4 273.3
331(6) 0.02778 202.3 293.9
358(6) 0.02778 202.2 329.9
404(7) 0.02041 202.1 391.9
495(7) 0.02041 202.0 492.1
626(8) 0.01563 201.9 638.7
805(10) 0.01000 201.8 827.4
999(11) 0.00826 201.7 1030.6
1137(12) 0.00694 201.6 1187.6
1204(12) 0.00694 201.5 1223.2
1161(12) 0.00694 201.4 1122.5
984(11) 0.00826 201.3 951.6
816(10) 0.01000 201.2 781.2
666(9) 0.01235 201.1 645.2
552(8) 0.01563 201.0 545.2
469(8) 0.01563 200.9 468.0
396(7) 0.02041 200.8 404.2
350(7) 0.02041 200.7 352.5
321(6) 0.02778 200.6 312.7
282(6) 0.02778 200.5 283.8
257(6) 0.02778 200.3 263.8
238(5) 0.0400 200.2 250.5
241(5) 0.0400 200.1 241.7
228(5) 0.0400 200.0 235.7
222(5) 0.0400 199.9 231.5
227(5) 0.0400 199.8 228.3
227(5) 0.0400 199.7 226.0
215(5) 0.0400 199.6 224.3
229(5) 0.0400 199.5 223.4
216(5) 0.0400 199.4 223.4
216(5) 0.0400 199.3 225.0
228(5) 0.0400 199.2 228.8
249(6) 0.02778 199.1 236.0
245(6) 0.02778 198.9 247.3
267(6) 0.02778 198.8 262.5
290(6) 0.02778 198.7 279.1
304(6) 0.02778 198.6 292.3
300(6) 0.02778 198.5 295.1
299(6) 0.02778 198.4 285.4
277(6) 0.02778 198.3 268.5
273(6) 0.02778 198.2 250.8
244(5) 0.0400 198.1 235.9
228(5) 0.0400 198.0 225.2
218(5) 0.0400 197.8 218.2
221(5) 0.0400 197.7 213.9
208(5) 0.0400 197.6 211.4
213(5) 0.0400 197.5 210.1
205(5) 0.0400 197.4 209.5
220(5) 0.0400 197.3 209.7
218(5) 0.0400 197.2 210.6
216(5) 0.0400 197.1 212.4
239(5) 0.0400 196.9 214.8
225(5) 0.0400 196.8 217.4
231(5) 0.0400 196.7 219.1
229(5) 0.0400 196.6 218.8
216(5) 0.0400 196.5 216.3
220(5) 0.0400 196.4 213.0
211(5) 0.0400 196.3 209.7
213(6) 0.02778 196.1 207.0
204(5) 0.0400 196.0 205.2
203(5) 0.0400 195.9 203.9
215(6) 0.02778 195.8 203.1
210(5) 0.0400 195.7 202.7
205(5) 0.0400 195.6 202.4
203(5) 0.0400 195.5 202.2
198(5) 0.0400 195.3 202.0
196(5) 0.0400 195.2 202.0
204(5) 0.0400 195.1 202.0
205(5) 0.0400 195.0 202.1
207(5) 0.0400 194.9 202.3
205(5) 0.0400 194.8 202.7
203(5) 0.0400 194.6 203.2
200(5) 0.0400 194.5 204.0
208(5) 0.0400 194.4 205.4
214(6) 0.02778 194.3 207.8
219(6) 0.02778 194.2 212.0
224(6) 0.02778 194.1 219.1
230(6) 0.02778 194.0 230.2
253(6) 0.02778 193.8 245.4
259(6) 0.02778 193.7 263.5
284(6) 0.02778 193.6 280.6
297(7) 0.02041 193.5 289.8
302(7) 0.02041 193.4 285.8
284(6) 0.02778 193.3 271.0
265(6) 0.02778 193.1 252.6
239(6) 0.02778 193.0 235.9
235(6) 0.02778 192.9 223.1
220(6) 0.02778 192.8 214.5
204(5) 0.0400 192.7 209.4
204(5) 0.0400 192.6 206.8
198(5) 0.0400 192.5 205.8
207(5) 0.0400 192.3 206.3
207(5) 0.0400 192.2 208.4
214(6) 0.02778 192.1 212.5
218(6) 0.02778 192.0 219.0
215(6) 0.02778 191.9 227.5
222(6) 0.02778 191.8 236.9
217(6) 0.02778 191.6 244.2
224(6) 0.02778 191.5 245.6
229(6) 0.02778 191.4 240.1
220(6) 0.02778 191.3 230.7
220(6) 0.02778 191.2 221.0
209(5) 0.0400 191.1 212.9
199(5) 0.0400 191.0 207.0
202(5) 0.0400 190.8 203.2
203(5) 0.0400 190.7 200.8
205(5) 0.0400 190.6 199.5
211(6) 0.02778 190.5 198.6
199(5) 0.0400 190.4 198.1
198(5) 0.0400 190.3 197.8
205(5) 0.0400 190.2 197.6
204(5) 0.0400 190.0 197.4
205(5) 0.0400 189.9 197.3
200(5) 0.0400 189.8 197.4
199(5) 0.0400 189.7 197.4
195(5) 0.0400 189.6 197.6
196(5) 0.0400 189.5 197.9
197(5) 0.0400 189.4 198.3
208(5) 0.0400 189.2 199.0
205(5) 0.0400 189.1 200.2
211(5) 0.0400 189.0 202.0
206(5) 0.0400 188.9 204.6
207(5) 0.0400 188.8 208.1
218(6) 0.02778 188.7 212.3
212(6) 0.02778 188.6 216.2
219(6) 0.02778 188.5 218.6
214(6) 0.02778 188.3 218.4
223(6) 0.02778 188.2 216.5
217(6) 0.02778 188.1 214.1
215(6) 0.02778 188.0 212.5
216(6) 0.02778 187.9 212.0
212(5) 0.0400 187.8 213.0
208(5) 0.0400 187.7 215.4
219(6) 0.02778 187.6 219.8
231(6) 0.02778 187.5 227.2
238(5) 0.0400 187.3 239.4
262(6) 0.02778 187.2 259.3
285(7) 0.02041 187.1 289.9
319(7) 0.02041 187.0 333.2
379(7) 0.02041 186.9 388.5
446(8) 0.01563 186.8 449.9
500(8) 0.01563 186.7 504.4
547(9) 0.01235 186.6 539.4
569(9) 0.01235 186.5 559.3
573(9) 0.01235 186.4 581.7
600(9) 0.01235 186.3 614.1
618(9) 0.01235 186.1 643.1
614(9) 0.01235 186.0 639.6
583(9) 0.01235 185.9 587.9
525(9) 0.01235 185.8 506.1
435(8) 0.01563 185.7 421.6
348(7) 0.02041 185.6 350.6
296(6) 0.02778 185.5 298.3
260(6) 0.02778 185.4 263.6
238(6) 0.02778 185.3 242.2
227(6) 0.02778 185.2 229.6
218(6) 0.02778 185.1 222.0
217(6) 0.02778 185.0 217.4
212(6) 0.02778 184.9 214.5
205(5) 0.0400 184.8 212.9
203(5) 0.0400 184.7 212.6
196(5) 0.0400 184.6 214.0
219(6) 0.02778 184.5 218.0
218(6) 0.02778 184.4 225.9
236(6) 0.02778 184.2 239.3
252(6) 0.02778 184.1 258.8
275(6) 0.02778 184.0 283.7
291(6) 0.02778 183.9 309.7
314(7) 0.02041 183.8 328.0
321(7) 0.02041 183.7 328.9
297(6) 0.02778 183.6 311.5
282(6) 0.02778 183.5 285.3
260(6) 0.02778 183.4 259.5
243(6) 0.02778 183.3 238.7
217(6) 0.02778 183.2 224.1
212(5) 0.0400 183.1 215.3
210(5) 0.0400 183.0 211.0
205(5) 0.0400 182.9 210.3
206(5) 0.0400 182.8 212.9
211(5) 0.0400 182.7 219.7
231(6) 0.02778 182.6 231.8
242(6) 0.02778 182.5 250.2
272(6) 0.02778 182.4 274.1
293(6) 0.02778 182.3 300.4
314(6) 0.02778 182.2 321.2
301(6) 0.02778 182.1 326.4
301(6) 0.02778 182.0 312.9
284(6) 0.02778 182.0 289.0
259(6) 0.02778 181.9 264.1
235(5) 0.0400 181.8 243.4
225(5) 0.0400 181.7 227.8
210(5) 0.0400 181.6 216.4
204(5) 0.0400 181.5 208.1
202(5) 0.0400 181.4 202.1
192(5) 0.0400 181.3 197.9
191(5) 0.0400 181.2 195.0
190(5) 0.0400 181.1 192.8
193(5) 0.0400 181.0 191.4
190(5) 0.0400 180.9 190.3
186(5) 0.0400 180.8 189.5
190(5) 0.0400 180.7 188.9
191(5) 0.0400 180.6 188.4
183(5) 0.0400 180.5 188.0
193(5) 0.0400 180.5 187.8
199(5) 0.0400 180.4 187.7
184(5) 0.0400 180.3 187.8
190(5) 0.0400 180.2 188.2
198(5) 0.0400 180.1 189.0
189(5) 0.0400 180.0 190.2
195(5) 0.0400 179.9 191.9
200(5) 0.0400 179.8 193.6
197(5) 0.0400 179.7 195.0
199(5) 0.0400 179.7 195.2
197(5) 0.0400 179.6 194.3
200(5) 0.0400 179.5 192.8
195(5) 0.0400 179.4 191.4
194(5) 0.0400 179.3 190.4
190(5) 0.0400 179.2 190.0
193(5) 0.0400 179.1 190.3
193(5) 0.0400 179.0 191.4
197(5) 0.0400 179.0 193.5
211(5) 0.0400 178.9 197.4
208(5) 0.0400 178.8 204.0
219(5) 0.0400 178.7 214.4
240(5) 0.0400 178.6 229.3
262(6) 0.02778 178.5 248.3
285(6) 0.02778 178.5 269.0
287(6) 0.02778 178.4 285.7
306(6) 0.02778 178.3 291.4
302(6) 0.02778 178.2 284.5
273(6) 0.02778 178.1 271.5
268(6) 0.02778 178.0 258.8
241(5) 0.0400 178.0 248.6
233(5) 0.0400 177.9 239.3
218(5) 0.0400 177.8 229.1
214(5) 0.0400 177.7 218.4
204(5) 0.0400 177.6 208.7
193(5) 0.0400 177.6 200.9
195(5) 0.0400 177.5 195.1
188(5) 0.0400 177.4 191.2
191(5) 0.0400 177.3 188.6
187(5) 0.0400 177.3 186.9
188(5) 0.0400 177.2 185.8
179(5) 0.0400 177.1 185.0
179(5) 0.0400 177.0 184.5
183(5) 0.0400 177.0 184.1
181(5) 0.0400 176.9 183.8
188(5) 0.0400 176.8 183.6
188(5) 0.0400 176.7 183.5
192(5) 0.0400 176.7 183.5
184(5) 0.0400 176.6 183.6
186(5) 0.0400 176.5 183.8
188(5) 0.0400 176.4 184.1
184(5) 0.0400 176.4 184.4
187(5) 0.0400 176.3 184.8
178(5) 0.0400 176.2 185.1
184(5) 0.0400 176.1 185.5
195(5) 0.0400 176.1 186.0
179(4) 0.0625 176.0 186.7
185(5) 0.0400 175.9 187.6
195(5) 0.0400 175.9 189.0
195(5) 0.0400 175.8 191.2
195(5) 0.0400 175.7 194.5
208(5) 0.0400 175.7 200.1
216(5) 0.0400 175.6 209.3
219(5) 0.0400 175.5 224.3
247(5) 0.0400 175.5 247.0
281(6) 0.02778 175.4 277.8
308(6) 0.02778 175.3 314.7
341(6) 0.02778 175.3 350.5
367(6) 0.02778 175.2 371.9
366(6) 0.02778 175.1 366.9
341(6) 0.02778 175.1 338.7
296(6) 0.02778 175.0 301.2
264(5) 0.0400 174.9 265.9
235(5) 0.0400 174.9 237.7
214(5) 0.0400 174.8 217.9
207(5) 0.0400 174.7 205.1
197(5) 0.0400 174.7 197.2
191(5) 0.0400 174.6 192.5
183(5) 0.0400 174.6 189.6
186(5) 0.0400 174.5 187.7
186(5) 0.0400 174.4 186.3
184(5) 0.0400 174.4 185.3
181(4) 0.0625 174.3 184.6
183(5) 0.0400 174.3 184.1
181(4) 0.0625 174.2 183.8
181(4) 0.0625 174.1 183.7
190(5) 0.0400 174.1 183.8
184(5) 0.0400 174.0 184.3
187(5) 0.0400 174.0 185.3
186(5) 0.0400 173.9 187.2
198(5) 0.0400 173.8 190.4
201(5) 0.0400 173.8 194.9
207(5) 0.0400 173.7 200.9
226(5) 0.0400 173.7 207.5
213(5) 0.0400 173.6 213.0
230(5) 0.0400 173.6 214.9
227(5) 0.0400 173.5 212.2
217(5) 0.0400 173.5 206.7
212(5) 0.0400 173.4 200.8
193(5) 0.0400 173.4 195.9
191(5) 0.0400 173.3 192.7
191(5) 0.0400 173.2 191.2
198(5) 0.0400 173.2 191.4
196(5) 0.0400 173.1 193.5
195(5) 0.0400 173.1 198.0
209(5) 0.0400 173.0 206.1
215(5) 0.0400 173.0 218.9
233(5) 0.0400 172.9 237.2
256(5) 0.0400 172.9 260.5
287(5) 0.0400 172.8 285.6
298(5) 0.0400 172.8 305.5
307(6) 0.02778 172.8 311.0
295(5) 0.0400 172.7 299.4
277(5) 0.0400 172.7 278.1
252(5) 0.0400 172.6 255.7
236(5) 0.0400 172.6 236.9
213(5) 0.0400 172.5 222.4
208(5) 0.0400 172.5 211.4
207(5) 0.0400 172.4 203.2
201(4) 0.0625 172.4 197.4
196(4) 0.0625 172.3 193.5
189(4) 0.0625 172.3 190.9
184(4) 0.0625 172.3 189.4
183(4) 0.0625 172.2 188.7
180(4) 0.0625 172.2 188.6
187(4) 0.0625 172.1 189.1
192(4) 0.0625 172.1 190.1
189(4) 0.0625 172.0 191.8
196(4) 0.0625 172.0 194.5
198(4) 0.0625 172.0 198.9
206(5) 0.0400 171.9 206.4
214(5) 0.0400 171.9 218.7
241(5) 0.0400 171.8 238.2
269(5) 0.0400 171.8 266.9
313(6) 0.02778 171.8 304.9
356(6) 0.02778 171.7 348.9
391(6) 0.02778 171.7 389.4
403(6) 0.02778 171.7 410.2
403(6) 0.02778 171.6 399.5
370(6) 0.02778 171.6 363.8
319(6) 0.02778 171.6 319.7
282(5) 0.0400 171.5 279.3
253(5) 0.0400 171.5 247.7
223(5) 0.0400 171.5 225.7
205(5) 0.0400 171.4 211.8
200(4) 0.0625 171.4 203.9
194(4) 0.0625 171.4 200.2
199(4) 0.0625 171.3 199.7
195(4) 0.0625 171.3 201.9
205(5) 0.0400 171.3 206.8
215(5) 0.0400 171.2 214.1
222(5) 0.0400 171.2 222.8
231(5) 0.0400 171.2 230.7
230(5) 0.0400 171.1 234.4
234(5) 0.0400 171.1 232.0
215(5) 0.0400 171.1 225.6
208(5) 0.0400 171.1 218.4
197(4) 0.0625 171.0 212.1
198(4) 0.0625 171.0 206.8
194(5) 0.0400 171.0 201.9
199(4) 0.0625 171.0 197.2
190(5) 0.0400 170.9 193.2
190(4) 0.0625 170.9 190.0
190(5) 0.0400 170.9 187.7
183(4) 0.0625 170.9 186.1
185(4) 0.0625 170.8 185.3
186(4) 0.0625 170.8 184.9
185(4) 0.0625 170.8 184.8
181(4) 0.0625 170.8 185.0
183(4) 0.0625 170.7 185.4
191(4) 0.0625 170.7 186.1
189(4) 0.0625 170.7 187.1
191(4) 0.0625 170.7 188.5
189(4) 0.0625 170.7 190.6
197(4) 0.0625 170.6 193.7
198(4) 0.0625 170.6 197.9
198(4) 0.0625 170.6 203.5
202(4) 0.0625 170.6 210.0
206(5) 0.0400 170.6 216.7
210(5) 0.0400 170.6 221.8
217(5) 0.0400 170.5 223.8
210(5) 0.0400 170.5 223.2
217(5) 0.0400 170.5 221.9
223(5) 0.0400 170.5 221.8
228(5) 0.0400 170.5 223.9
228(5) 0.0400 170.5 229.3
248(5) 0.0400 170.5 239.1
253(5) 0.0400 170.4 255.8
292(5) 0.0400 170.4 283.8
343(6) 0.02778 170.4 329.3
400(6) 0.02778 170.4 400.0
517(7) 0.02041 170.4 502.1
661(8) 0.01563 170.4 635.8
798(9) 0.01235 170.4 789.6
934(10) 0.01000 170.4 931.1
1001(10) 0.01000 170.4 1007.0
964(10) 0.01000 170.3 979.4
866(9) 0.01235 170.3 872.0
712(8) 0.01563 170.3 739.5
597(8) 0.01563 170.3 618.5
509(7) 0.02041 170.3 519.8
421(6) 0.02778 170.3 440.0
367(6) 0.02778 170.3 375.0
320(6) 0.02778 170.3 324.0
283(5) 0.0400 170.3 285.8
257(5) 0.0400 170.3 258.1
232(5) 0.0400 170.3 238.5
221(5) 0.0400 170.3 224.8
217(5) 0.0400 170.3 215.4
209(5) 0.0400 170.3 208.8
208(5) 0.0400 170.3 204.0
200(4) 0.0625 170.3 200.4
198(4) 0.0625 170.3 197.7
194(4) 0.0625 170.3 195.9
194(4) 0.0625 170.3 194.8
191(4) 0.0625 170.3 194.7
198(4) 0.0625 170.3 195.7
199(4) 0.0625 170.3 198.2
197(4) 0.0625 170.3 202.2
216(5) 0.0400 170.3 207.3
215(5) 0.0400 170.3 212.5
212(5) 0.0400 170.3 215.7
216(5) 0.0400 170.3 214.9
209(5) 0.0400 170.3 210.2
202(4) 0.0625 170.3 203.8
197(4) 0.0625 170.3 197.5
201(4) 0.0625 170.3 192.3
184(4) 0.0625 170.3 188.6
187(4) 0.0625 170.3 186.2
179(4) 0.0625 170.3 184.9
182(4) 0.0625 170.3 184.6
191(4) 0.0625 170.3 185.2
190(4) 0.0625 170.3 186.9
197(4) 0.0625 170.4 189.7
199(4) 0.0625 170.4 193.6
210(5) 0.0400 170.4 198.3
202(4) 0.0625 170.4 202.6
207(5) 0.0400 170.4 204.9
206(5) 0.0400 170.4 203.9
208(5) 0.0400 170.4 200.0
207(5) 0.0400 170.4 195.0
193(4) 0.0625 170.4 190.3
194(4) 0.0625 170.5 186.6
189(4) 0.0625 170.5 183.9
177(4) 0.0625 170.5 182.2
195(4) 0.0625 170.5 181.2
184(4) 0.0625 170.5 180.7
189(4) 0.0625 170.5 180.5
188(4) 0.0625 170.5 180.5
184(4) 0.0625 170.6 180.7
190(4) 0.0625 170.6 181.1
184(4) 0.0625 170.6 181.6
191(4) 0.0625 170.6 182.4
189(4) 0.0625 170.6 183.4
190(4) 0.0625 170.6 185.0
184(4) 0.0625 170.7 187.3
199(4) 0.0625 170.7 190.9
204(5) 0.0400 170.7 196.8
210(5) 0.0400 170.7 205.8
228(5) 0.0400 170.7 219.0
246(5) 0.0400 170.8 236.8
263(5) 0.0400 170.8 258.0
271(5) 0.0400 170.8 279.5
288(5) 0.0400 170.8 294.4
278(5) 0.0400 170.8 295.6
274(5) 0.0400 170.9 282.4
255(5) 0.0400 170.9 262.0
241(5) 0.0400 170.9 241.3
216(5) 0.0400 170.9 224.0
211(5) 0.0400 171.0 211.4
196(4) 0.0625 171.0 203.4
201(4) 0.0625 171.0 199.1
203(5) 0.0400 171.0 198.0
206(5) 0.0400 171.1 199.7
211(5) 0.0400 171.1 204.2
220(5) 0.0400 171.1 211.7
231(5) 0.0400 171.2 222.5
263(5) 0.0400 171.2 236.0
268(5) 0.0400 171.2 250.9
281(5) 0.0400 171.2 264.2
290(5) 0.0400 171.3 273.3
292(5) 0.0400 171.3 279.3
296(5) 0.0400 171.3 285.2
303(6) 0.02778 171.4 291.8
292(5) 0.0400 171.4 295.3
287(5) 0.0400 171.4 290.1
274(5) 0.0400 171.5 275.1
255(5) 0.0400 171.5 255.2
232(5) 0.0400 171.5 235.7
215(5) 0.0400 171.6 219.5
213(5) 0.0400 171.6 207.3
200(4) 0.0625 171.6 198.9
197(4) 0.0625 171.7 193.4
188(4) 0.0625 171.7 189.9
184(4) 0.0625 171.7 187.7
188(4) 0.0625 171.8 186.3
191(4) 0.0625 171.8 185.4
188(4) 0.0625 171.8 184.8
188(4) 0.0625 171.9 184.5
182(4) 0.0625 171.9 184.4
175(4) 0.0625 171.9 184.5
180(4) 0.0625 172.0 184.8
180(4) 0.0625 172.0 185.4
182(4) 0.0625 172.1 186.2
194(4) 0.0625 172.1 187.1
184(4) 0.0625 172.1 188.0
181(4) 0.0625 172.2 188.7
188(4) 0.0625 172.2 189.1
190(4) 0.0625 172.2 189.4
189(4) 0.0625 172.3 189.9
186(4) 0.0625 172.3 190.6
190(4) 0.0625 172.4 191.8
202(4) 0.0625 172.4 193.4
199(4) 0.0625 172.5 195.5
197(4) 0.0625 172.5 198.3
201(4) 0.0625 172.5 202.0
205(5) 0.0400 172.6 207.0
222(5) 0.0400 172.6 213.9
231(5) 0.0400 172.7 224.1
248(5) 0.0400 172.7 239.4
275(5) 0.0400 172.8 262.9
307(6) 0.02778 172.8 298.1
358(6) 0.02778 172.8 348.4
429(7) 0.02041 172.9 415.7
513(7) 0.02041 172.9 497.7
601(8) 0.01563 173.0 583.8
644(8) 0.01563 173.0 650.7
654(8) 0.01563 173.1 668.1
618(8) 0.01563 173.1 626.0
529(7) 0.02041 173.2 546.3
462(7) 0.02041 173.2 458.7
376(6) 0.02778 173.2 381.1
314(6) 0.02778 173.3 320.6
277(5) 0.0400 173.3 277.3
262(5) 0.0400 173.4 248.5
234(5) 0.0400 173.4 230.1
229(5) 0.0400 173.5 218.4
206(5) 0.0400 173.5 210.8
201(4) 0.0625 173.6 205.6
203(5) 0.0400 173.6 201.8
193(4) 0.0625 173.7 199.0
188(4) 0.0625 173.7 196.8
190(4) 0.0625 173.8 195.1
192(4) 0.0625 173.8 193.8
191(4) 0.0625 173.9 192.9
192(4) 0.0625 173.9 192.2
197(4) 0.0625 174.0 191.8
192(4) 0.0625 174.0 191.6
192(4) 0.0625 174.1 191.7
198(4) 0.0625 174.1 192.0
191(4) 0.0625 174.2 192.6
195(4) 0.0625 174.2 193.6
198(4) 0.0625 174.3 194.9
199(4) 0.0625 174.3 196.9
204(5) 0.0400 174.4 199.8
203(4) 0.0625 174.4 204.2
220(5) 0.0400 174.5 211.2
224(5) 0.0400 174.5 222.1
241(5) 0.0400 174.6 238.9
260(5) 0.0400 174.6 263.3
298(5) 0.0400 174.7 296.0
341(6) 0.02778 174.7 335.8
375(6) 0.02778 174.8 377.7
408(6) 0.02778 174.8 411.0
430(7) 0.02041 174.9 421.8
406(6) 0.02778 174.9 405.3
368(6) 0.02778 175.0 371.5
318(6) 0.02778 175.0 333.9
291(5) 0.0400 175.1 300.2
263(5) 0.0400 175.2 272.5
245(5) 0.0400 175.2 250.3
229(5) 0.0400 175.3 233.1
214(5) 0.0400 175.3 220.1
214(5) 0.0400 175.4 210.7
202(4) 0.0625 175.4 204.1
199(4) 0.0625 175.5 199.3
198(4) 0.0625 175.5 196.0
193(4) 0.0625 175.6 193.7
195(4) 0.0625 175.6 192.1
183(4) 0.0625 175.7 191.0
176(4) 0.0625 175.7 190.3
182(4) 0.0625 175.8 189.9
180(4) 0.0625 175.8 189.9
193(4) 0.0625 175.9 190.3
194(4) 0.0625 176.0 191.4
192(4) 0.0625 176.0 193.2
194(4) 0.0625 176.1 195.8
189(4) 0.0625 176.1 199.4
190(4) 0.0625 176.2 203.5
204(5) 0.0400 176.2 207.4
196(4) 0.0625 176.3 209.8
199(4) 0.0625 176.3 209.7
204(5) 0.0400 176.4 207.2
201(4) 0.0625 176.4 203.9
196(4) 0.0625 176.5 200.8
196(4) 0.0625 176.5 198.6
196(4) 0.0625 176.6 197.6
189(4) 0.0625 176.6 198.0
183(4) 0.0625 176.7 200.3
201(4) 0.0625 176.7 204.8
213(5) 0.0400 176.8 212.3
214(5) 0.0400 176.9 223.7
226(5) 0.0400 176.9 239.7
257(5) 0.0400 177.0 260.0
283(5) 0.0400 177.0 282.8
305(6) 0.02778 177.1 303.7
325(6) 0.02778 177.1 315.3
312(6) 0.02778 177.2 311.9
304(6) 0.02778 177.2 295.4
288(5) 0.0400 177.3 272.9
257(5) 0.0400 177.3 250.9
244(5) 0.0400 177.4 232.5
221(5) 0.0400 177.4 218.5
214(5) 0.0400 177.5 208.8
205(5) 0.0400 177.5 202.4
196(4) 0.0625 177.6 198.4
200(4) 0.0625 177.6 196.0
204(5) 0.0400 177.7 194.5
195(4) 0.0625 177.7 193.7
198(4) 0.0625 177.8 193.4
190(4) 0.0625 177.8 193.3
192(4) 0.0625 177.9 193.7
196(4) 0.0625 177.9 194.4
196(4) 0.0625 178.0 195.6
199(4) 0.0625 178.0 197.6
209(5) 0.0400 178.1 200.9
209(5) 0.0400 178.1 206.0
214(5) 0.0400 178.2 213.6
214(5) 0.0400 178.2 224.6
233(5) 0.0400 178.3 239.3
246(5) 0.0400 178.3 257.1
268(5) 0.0400 178.4 276.0
282(5) 0.0400 178.4 291.5
287(5) 0.0400 178.5 297.6
281(5) 0.0400 178.5 291.4
277(5) 0.0400 178.6 276.5
254(5) 0.0400 178.6 258.9
252(5) 0.0400 178.6 242.9
235(5) 0.0400 178.7 230.5
220(5) 0.0400 178.7 222.2
229(5) 0.0400 178.8 218.2
225(5) 0.0400 178.8 218.3
230(5) 0.0400 178.9 222.6
231(5) 0.0400 178.9 231.7
256(5) 0.0400 179.0 246.2
279(5) 0.0400 179.0 266.2
291(5) 0.0400 179.0 291.0
311(6) 0.02778 179.1 317.7
347(6) 0.02778 179.1 340.1
339(6) 0.02778 179.2 349.5
336(6) 0.02778 179.2 341.4
315(6) 0.02778 179.3 320.4
298(5) 0.0400 179.3 294.9
274(5) 0.0400 179.3 271.0
242(5) 0.0400 179.4 251.1
230(5) 0.0400 179.4 235.4
232(5) 0.0400 179.5 223.6
214(5) 0.0400 179.5 215.2
211(5) 0.0400 179.5 209.3
205(5) 0.0400 179.6 205.3
203(5) 0.0400 179.6 202.6
202(4) 0.0625 179.7 201.0
206(5) 0.0400 179.7 200.0
195(4) 0.0625 179.7 199.6
202(4) 0.0625 179.8 199.7
204(5) 0.0400 179.8 200.2
202(4) 0.0625 179.8 201.4
202(4) 0.0625 179.9 203.4
205(5) 0.0400 179.9 206.6
204(5) 0.0400 179.9 211.5
222(5) 0.0400 180.0 218.8
231(5) 0.0400 180.0 229.0
236(5) 0.0400 180.1 242.3
261(5) 0.0400 180.1 258.2
279(5) 0.0400 180.1 274.6
292(5) 0.0400 180.2 287.7
298(5) 0.0400 180.2 292.7
298(5) 0.0400 180.2 287.7
270(5) 0.0400 180.2 276.1
260(5) 0.0400 180.3 262.9
250(5) 0.0400 180.3 251.5
241(5) 0.0400 180.3 243.8
239(5) 0.0400 180.4 240.6
238(5) 0.0400 180.4 242.8
259(5) 0.0400 180.4 251.2
272(5) 0.0400 180.4 267.5
288(5) 0.0400 180.5 293.7
320(6) 0.02778 180.5 331.8
382(6) 0.02778 180.5 382.5
434(7) 0.02041 180.6 443.9
495(7) 0.02041 180.6 509.1
567(8) 0.01563 180.6 563.1
579(8) 0.01563 180.6 585.8
558(7) 0.02041 180.7 566.0
510(7) 0.02041 180.7 513.8
452(7) 0.02041 180.7 449.6
387(6) 0.02778 180.7 388.2
332(6) 0.02778 180.7 336.8
292(5) 0.0400 180.8 297.2
273(5) 0.0400 180.8 268.5
251(5) 0.0400 180.8 248.7
244(5) 0.0400 180.8 235.5
230(5) 0.0400 180.8 226.8
214(5) 0.0400 180.9 221.1
218(5) 0.0400 180.9 217.4
219(5) 0.0400 180.9 215.0
215(5) 0.0400 180.9 213.7
217(5) 0.0400 180.9 213.3
214(5) 0.0400 180.9 213.8
219(5) 0.0400 181.0 215.6
224(5) 0.0400 181.0 219.0
225(5) 0.0400 181.0 224.8
229(5) 0.0400 181.0 234.2
242(5) 0.0400 181.0 248.5
255(5) 0.0400 181.0 268.9
285(5) 0.0400 181.0 295.7
327(6) 0.02778 181.1 328.2
364(6) 0.02778 181.1 362.9
392(6) 0.02778 181.1 392.2
408(6) 0.02778 181.1 405.6
406(6) 0.02778 181.1 396.7
377(6) 0.02778 181.1 369.9
350(6) 0.02778 181.1 335.7
312(6) 0.02778 181.1 302.5
283(5) 0.0400 181.1 274.6
261(5) 0.0400 181.1 253.3
241(5) 0.0400 181.1 238.7
231(5) 0.0400 181.1 229.7
229(5) 0.0400 181.2 225.5
238(5) 0.0400 181.2 225.3
235(5) 0.0400 181.2 228.6
241(5) 0.0400 181.2 235.2
250(5) 0.0400 181.2 244.6
261(5) 0.0400 181.2 256.0
274(5) 0.0400 181.2 267.3
282(5) 0.0400 181.2 275.6
282(5) 0.0400 181.2 277.9
275(5) 0.0400 181.2 274.6
263(5) 0.0400 181.2 268.5
254(5) 0.0400 181.2 262.1
250(5) 0.0400 181.2 255.9
239(5) 0.0400 181.2 249.0
240(5) 0.0400 181.2 240.9
227(5) 0.0400 181.2 232.2
222(5) 0.0400 181.2 224.1
217(5) 0.0400 181.2 217.4
210(5) 0.0400 181.1 212.4
214(5) 0.0400 181.1 208.8
213(5) 0.0400 181.1 206.6
200(4) 0.0625 181.1 205.6
204(5) 0.0400 181.1 205.5
203(5) 0.0400 181.1 206.4
200(4) 0.0625 181.1 208.2
212(5) 0.0400 181.1 211.4
218(5) 0.0400 181.1 216.6
229(5) 0.0400 181.1 224.6
232(5) 0.0400 181.1 236.8
254(5) 0.0400 181.1 254.2
281(5) 0.0400 181.0 277.9
296(5) 0.0400 181.0 307.8
323(6) 0.02778 181.0 342.2
365(6) 0.02778 181.0 376.4
386(6) 0.02778 181.0 401.6
403(6) 0.02778 181.0 407.8
384(6) 0.02778 181.0 392.1
354(6) 0.02778 180.9 361.5
316(6) 0.02778 180.9 326.1
296(5) 0.0400 180.9 293.0
254(5) 0.0400 180.9 265.4
234(5) 0.0400 180.9 244.2
230(5) 0.0400 180.9 228.9
218(5) 0.0400 180.8 218.3
210(5) 0.0400 180.8 211.3
211(5) 0.0400 180.8 206.7
210(5) 0.0400 180.8 203.7
202(4) 0.0625 180.8 201.7
204(5) 0.0400 180.7 200.4
203(4) 0.0625 180.7 199.6
195(4) 0.0625 180.7 199.0
203(5) 0.0400 180.7 198.4
200(5) 0.0400 180.7 197.6
195(5) 0.0400 180.6 196.7
200(5) 0.0400 180.6 195.8
206(5) 0.0400 180.6 195.0
203(5) 0.0400 180.6 194.3
195(5) 0.0400 180.5 193.9
199(5) 0.0400 180.5 193.6
184(5) 0.0400 180.5 193.5
187(5) 0.0400 180.5 193.6
193(5) 0.0400 180.4 193.9
195(5) 0.0400 180.4 194.3
193(5) 0.0400 180.4 194.8
187(5) 0.0400 180.3 195.6
201(5) 0.0400 180.3 196.6
194(5) 0.0400 180.3 197.9
199(5) 0.0400 180.3 199.6
207(5) 0.0400 180.2 201.9
211(5) 0.0400 180.2 205.3
215(5) 0.0400 180.2 210.1
223(5) 0.0400 180.1 217.3
223(5) 0.0400 180.1 227.7
233(5) 0.0400 180.1 242.3
256(5) 0.0400 180.0 261.9
284(6) 0.02778 180.0 286.5
316(6) 0.02778 180.0 315.0
348(6) 0.02778 179.9 343.8
371(6) 0.02778 179.9 366.5
390(7) 0.02041 179.9 375.2
371(6) 0.02778 179.8 366.2
360(6) 0.02778 179.8 343.7
327(6) 0.02778 179.8 315.8
297(6) 0.02778 179.7 288.9
278(6) 0.02778 179.7 266.2
262(5) 0.0400 179.7 249.1
245(5) 0.0400 179.6 237.6
238(5) 0.0400 179.6 231.4
242(5) 0.0400 179.5 230.1
238(5) 0.0400 179.5 233.5
243(5) 0.0400 179.5 241.3
258(5) 0.0400 179.4 253.6
279(6) 0.02778 179.4 269.7
295(6) 0.02778 179.3 288.2
301(6) 0.02778 179.3 306.2
310(6) 0.02778 179.3 318.9
327(6) 0.02778 179.2 321.1
325(6) 0.02778 179.2 312.0
307(6) 0.02778 179.2 295.5
273(6) 0.02778 179.1 276.8
257(5) 0.0400 179.1 259.1
241(5) 0.0400 179.0 244.1
234(5) 0.0400 179.0 231.8
220(5) 0.0400 178.9 222.1
207(5) 0.0400 178.9 214.9
216(5) 0.0400 178.9 209.7
209(5) 0.0400 178.8 206.1
207(5) 0.0400 178.8 203.8
204(5) 0.0400 178.7 202.3
203(5) 0.0400 178.7 201.6
215(5) 0.0400 178.6 201.6
209(5) 0.0400 178.6 202.2
206(5) 0.0400 178.6 203.5
210(5) 0.0400 178.5 205.7
210(5) 0.0400 178.5 209.3
216(5) 0.0400 178.4 214.8
221(5) 0.0400 178.4 223.0
233(5) 0.0400 178.3 235.0
250(5) 0.0400 178.3 251.5
271(5) 0.0400 178.3 273.1
305(6) 0.02778 178.2 299.5
327(6) 0.02778 178.2 328.8
351(6) 0.02778 178.1 356.8
375(6) 0.02778 178.1 376.5
382(7) 0.02041 178.0 380.6
368(6) 0.02778 178.0 367.3
328(6) 0.02778 177.9 342.1
303(6) 0.02778 177.9 312.8
279(6) 0.02778 177.9 284.9
261(5) 0.0400 177.8 261.2
243(5) 0.0400 177.8 242.8
237(5) 0.0400 177.7 229.5
229(5) 0.0400 177.7 220.6
215(5) 0.0400 177.6 215.4
204(5) 0.0400 177.6 213.3
205(5) 0.0400 177.5 213.6
210(5) 0.0400 177.5 215.9
220(5) 0.0400 177.4 220.0
221(5) 0.0400 177.4 225.5
221(5) 0.0400 177.4 231.4
217(5) 0.0400 177.3 236.6
225(5) 0.0400 177.3 239.7
235(5) 0.0400 177.2 240.5
234(5) 0.0400 177.2 240.0
235(5) 0.0400 177.1 239.0
239(5) 0.0400 177.1 237.6
228(5) 0.0400 177.0 235.2
228(5) 0.0400 177.0 230.8
230(5) 0.0400 177.0 224.5
230(5) 0.0400 176.9 217.5
213(5) 0.0400 176.9 210.8
200(5) 0.0400 176.8 205.0
199(5) 0.0400 176.8 200.2
203(5) 0.0400 176.7 196.6
198(5) 0.0400 176.7 194.0
191(5) 0.0400 176.7 192.1
195(5) 0.0400 176.6 190.8
198(5) 0.0400 176.6 190.0
194(5) 0.0400 176.5 189.5
192(5) 0.0400 176.5 189.3
189(5) 0.0400 176.4 189.4
192(5) 0.0400 176.4 189.7
198(5) 0.0400 176.4 190.3
190(5) 0.0400 176.3 191.3
192(5) 0.0400 176.3 192.6
200(5) 0.0400 176.2 194.3
202(5) 0.0400 176.2 196.4
203(5) 0.0400 176.1 198.6
197(5) 0.0400 176.1 200.6
200(5) 0.0400 176.1 202.0
201(5) 0.0400 176.0 202.5
198(5) 0.0400 176.0 202.3
198(5) 0.0400 175.9 202.0
203(5) 0.0400 175.9 201.9
206(5) 0.0400 175.9 202.6
203(5) 0.0400 175.8 204.3
214(5) 0.0400 175.8 207.4
216(5) 0.0400 175.7 212.7
222(5) 0.0400 175.7 220.7
237(5) 0.0400 175.7 232.4
249(5) 0.0400 175.6 248.7
267(5) 0.0400 175.6 270.3
300(6) 0.02778 175.6 297.4
335(6) 0.02778 175.5 329.0
367(6) 0.02778 175.5 362.5
389(7) 0.02041 175.5 392.4
407(7) 0.02041 175.4 411.0
402(7) 0.02041 175.4 412.2
392(7) 0.02041 175.4 396.7
374(6) 0.02778 175.3 371.1
341(6) 0.02778 175.3 342.7
316(6) 0.02778 175.3 315.6
289(6) 0.02778 175.2 291.3
264(5) 0.0400 175.2 269.9
253(5) 0.0400 175.2 251.4
232(5) 0.0400 175.1 236.2
219(5) 0.0400 175.1 224.0
220(5) 0.0400 175.1 214.5
206(5) 0.0400 175.0 207.3
206(5) 0.0400 175.0 201.9
209(5) 0.0400 175.0 197.8
203(5) 0.0400 174.9 194.7
195(5) 0.0400 174.9 192.4
195(5) 0.0400 174.9 190.5
195(4) 0.0625 174.9 189.1
194(5) 0.0400 174.8 187.9
192(5) 0.0400 174.8 187.0
185(4) 0.0625 174.8 186.2
184(5) 0.0400 174.8 185.6
190(5) 0.0400 174.7 185.1
184(5) 0.0400 174.7 184.7
185(5) 0.0400 174.7 184.5
188(5) 0.0400 174.7 184.3
185(5) 0.0400 174.6 184.2
184(5) 0.0400 174.6 184.1
191(5) 0.0400 174.6 183.9
188(5) 0.0400 174.6 183.7
186(5) 0.0400 174.6 183.4
182(4) 0.0625 174.5 183.0
189(5) 0.0400 174.5 182.6
185(5) 0.0400 174.5 182.3
180(4) 0.0625 174.5 182.0
178(4) 0.0625 174.5 181.9
182(5) 0.0400 174.4 181.8
183(4) 0.0625 174.4 181.8
187(5) 0.0400 174.4 182.0
187(5) 0.0400 174.4 182.2
180(4) 0.0625 174.4 182.7
183(5) 0.0400 174.4 183.3
186(5) 0.0400 174.4 184.0
185(5) 0.0400 174.3 184.8
183(4) 0.0625 174.3 185.6
190(5) 0.0400 174.3 186.2
192(5) 0.0400 174.3 186.5
188(5) 0.0400 174.3 186.2
180(4) 0.0625 174.3 185.6
180(4) 0.0625 174.3 184.8
180(4) 0.0625 174.3 184.0
185(5) 0.0400 174.3 183.3
186(5) 0.0400 174.3 182.7
179(4) 0.0625 174.3 182.3
181(4) 0.0625 174.2 182.0
183(4) 0.0625 174.2 181.9
178(5) 0.0400 174.2 181.8
180(4) 0.0625 174.2 181.8
181(4) 0.0625 174.2 181.9
185(5) 0.0400 174.2 182.0
181(4) 0.0625 174.2 182.1
181(4) 0.0625 174.2 182.3
180(4) 0.0625 174.2 182.6
183(4) 0.0625 174.2 182.9
192(4) 0.0625 174.2 183.3
186(5) 0.0400 174.2 183.8
185(5) 0.0400 174.2 184.4
178(5) 0.0400 174.2 185.2
189(5) 0.0400 174.2 186.3
187(5) 0.0400 174.2 187.6
182(5) 0.0400 174.2 189.3
185(5) 0.0400 174.2 191.2
188(5) 0.0400 174.3 193.5
186(5) 0.0400 174.3 195.8
190(5) 0.0400 174.3 198.0
187(5) 0.0400 174.3 199.7
189(5) 0.0400 174.3 200.4
190(5) 0.0400 174.3 200.2
191(5) 0.0400 174.3 199.5
191(5) 0.0400 174.3 198.6
195(5) 0.0400 174.3 197.8
193(5) 0.0400 174.3 197.5
196(5) 0.0400 174.3 197.6
193(5) 0.0400 174.4 198.3
202(5) 0.0400 174.4 199.5
200(5) 0.0400 174.4 201.4
209(5) 0.0400 174.4 204.1
211(5) 0.0400 174.4 207.8
217(5) 0.0400 174.4 212.9
215(6) 0.02778 174.5 219.9
228(5) 0.0400 174.5 229.6
241(5) 0.0400 174.5 243.0
259(6) 0.02778 174.5 261.1
287(6) 0.02778 174.5 284.7
312(6) 0.02778 174.6 314.3
344(6) 0.02778 174.6 349.9
388(7) 0.02041 174.6 390.0
422(7) 0.02041 174.6 431.1
450(7) 0.02041 174.6 466.8
481(8) 0.01563 174.7 488.6
486(8) 0.01563 174.7 489.6
464(8) 0.01563 174.7 469.6
431(7) 0.02041 174.7 435.3
396(7) 0.02041 174.8 395.3
359(7) 0.02041 174.8 356.1
328(6) 0.02778 174.8 321.5
295(6) 0.02778 174.9 293.0
269(6) 0.02778 174.9 270.8
258(6) 0.02778 174.9 254.6
251(6) 0.02778 174.9 243.4
244(6) 0.02778 175.0 236.4
239(5) 0.0400 175.0 232.7
241(5) 0.0400 175.0 232.0
242(5) 0.0400 175.1 234.0
248(5) 0.0400 175.1 239.1
247(6) 0.02778 175.1 247.6
253(5) 0.0400 175.2 260.3
269(5) 0.0400 175.2 277.8
288(5) 0.0400 175.2 300.6
318(6) 0.02778 175.3 328.4
357(6) 0.02778 175.3 360.4
395(7) 0.02041 175.4 394.0
417(7) 0.02041 175.4 424.6
434(7) 0.02041 175.4 445.4
449(7) 0.02041 175.5 450.3
430(7) 0.02041 175.5 437.8
407(7) 0.02041 175.6 411.9
383(7) 0.02041 175.6 379.7
355(6) 0.02778 175.6 346.9
316(6) 0.02778 175.7 317.3
291(6) 0.02778 175.7 292.8
281(6) 0.02778 175.8 274.1
272(6) 0.02778 175.8 261.1
260(5) 0.0400 175.9 253.7
258(6) 0.02778 175.9 251.4
253(5) 0.0400 175.9 253.8
268(5) 0.0400 176.0 260.6
275(6) 0.02778 176.0 271.2
287(5) 0.0400 176.1 285.1
297(6) 0.02778 176.1 301.0
315(6) 0.02778 176.2 317.0
320(6) 0.02778 176.2 329.9
330(6) 0.02778 176.3 336.5
331(6) 0.02778 176.3 334.9
327(6) 0.02778 176.4 326.0
320(6) 0.02778 176.4 312.8
295(6) 0.02778 176.5 298.2
274(6) 0.02778 176.5 283.8
261(5) 0.0400 176.6 270.4
255(5) 0.0400 176.6 257.9
244(5) 0.0400 176.7 246.6
226(5) 0.0400 176.7 236.7
231(5) 0.0400 176.8 228.3
223(5) 0.0400 176.8 221.6
218(5) 0.0400 176.9 216.4
210(5) 0.0400 177.0 212.5
206(5) 0.0400 177.0 209.7
208(5) 0.0400 177.1 207.8
211(5) 0.0400 177.1 206.8
213(5) 0.0400 177.2 206.5
205(5) 0.0400 177.2 206.9
209(5) 0.0400 177.3 208.0
210(5) 0.0400 177.3 210.1
210(5) 0.0400 177.4 213.4
214(5) 0.0400 177.5 218.1
227(5) 0.0400 177.5 224.6
230(5) 0.0400 177.6 233.3
242(5) 0.0400 177.6 244.3
249(5) 0.0400 177.7 257.8
265(5) 0.0400 177.7 273.2
289(6) 0.02778 177.8 289.8
304(6) 0.02778 177.9 305.7
313(6) 0.02778 177.9 318.4
330(6) 0.02778 178.0 324.7
331(6) 0.02778 178.0 323.1
314(6) 0.02778 178.1 314.4
300(6) 0.02778 178.2 301.3
293(6) 0.02778 178.2 286.9
279(6) 0.02778 178.3 273.5
268(5) 0.0400 178.3 262.4
259(5) 0.0400 178.4 254.5
255(5) 0.0400 178.5 250.3
259(5) 0.0400 178.5 250.1
264(5) 0.0400 178.6 254.3
258(5) 0.0400 178.7 263.2
274(5) 0.0400 178.7 276.8
286(6) 0.02778 178.8 295.3
314(6) 0.02778 178.8 318.3
343(6) 0.02778 178.9 345.0
364(6) 0.02778 179.0 373.2
396(7) 0.02041 179.0 399.7
416(7) 0.02041 179.1 419.4
426(7) 0.02041 179.2 427.3
421(7) 0.02041 179.2 420.8
404(7) 0.02041 179.3 401.9
379(7) 0.02041 179.4 375.2
357(6) 0.02778 179.4 345.9
324(6) 0.02778 179.5 317.6
294(6) 0.02778 179.5 292.3
273(6) 0.02778 179.6 270.9
259(5) 0.0400 179.7 253.7
235(5) 0.0400 179.7 240.3
232(5) 0.0400 179.8 230.2
230(5) 0.0400 179.9 222.8
228(5) 0.0400 179.9 217.4
220(5) 0.0400 180.0 213.6
212(5) 0.0400 180.0 211.0
210(5) 0.0400 180.1 209.2
208(5) 0.0400 180.2 208.0
209(5) 0.0400 180.2 207.4
206(5) 0.0400 180.3 207.3
204(5) 0.0400 180.4 207.9
210(5) 0.0400 180.4 209.0
208(5) 0.0400 180.5 211.1
219(5) 0.0400 180.6 214.2
218(5) 0.0400 180.6 218.6
225(5) 0.0400 180.7 224.6
225(5) 0.0400 180.7 232.4
238(5) 0.0400 180.8 242.0
252(5) 0.0400 180.9 253.4
270(5) 0.0400 180.9 266.2
278(6) 0.02778 181.0 279.5
284(6) 0.02778 181.1 291.6
300(6) 0.02778 181.1 300.5
313(6) 0.02778 181.2 304.1
305(6) 0.02778 181.2 301.3
300(6) 0.02778 181.3 293.0
292(6) 0.02778 181.4 281.4
278(6) 0.02778 181.4 268.6
263(5) 0.0400 181.5 256.3
244(5) 0.0400 181.5 245.6
237(5) 0.0400 181.6 236.8
227(5) 0.0400 181.7 230.4
230(5) 0.0400 181.7 226.2
221(5) 0.0400 181.8 224.4
226(5) 0.0400 181.8 224.7
223(5) 0.0400 181.9 227.2
230(5) 0.0400 182.0 231.7
233(5) 0.0400 182.0 237.9
242(5) 0.0400 182.1 245.5
262(6) 0.02778 182.1 254.0
274(6) 0.02778 182.2 262.3
273(6) 0.02778 182.3 269.2
288(6) 0.02778 182.3 273.0
287(6) 0.02778 182.4 272.6
276(6) 0.02778 182.4 268.0
271(6) 0.02778 182.5 260.3
256(6) 0.02778 182.5 250.9
253(6) 0.02778 182.6 241.3
242(6) 0.02778 182.7 232.2
228(5) 0.0400 182.7 224.2
214(5) 0.0400 182.8 217.5
209(5) 0.0400 182.8 212.0
203(5) 0.0400 182.9 207.7
200(5) 0.0400 182.9 204.4
209(5) 0.0400 183.0 201.9
203(5) 0.0400 183.0 200.1
195(5) 0.0400 183.1 198.7
195(5) 0.0400 183.1 197.7
194(5) 0.0400 183.2 196.9
203(5) 0.0400 183.2 196.4
197(5) 0.0400 183.3 195.9
188(5) 0.0400 183.4 195.6
188(5) 0.0400 183.4 195.4
192(5) 0.0400 183.5 195.2
198(5) 0.0400 183.5 195.2
191(5) 0.0400 183.6 195.2
188(5) 0.0400 183.6 195.2
189(5) 0.0400 183.6 195.4
198(5) 0.0400 183.7 195.6
194(5) 0.0400 183.7 196.0
192(5) 0.0400 183.8 196.4
195(5) 0.0400 183.8 196.8
204(5) 0.0400 183.9 197.4
207(5) 0.0400 183.9 198.0
196(5) 0.0400 184.0 198.6
198(5) 0.0400 184.0 199.2
201(5) 0.0400 184.1 199.7
198(5) 0.0400 184.1 200.2
192(5) 0.0400 184.2 200.8
200(5) 0.0400 184.2 201.4
202(5) 0.0400 184.2 202.3
203(5) 0.0400 184.3 203.5
201(5) 0.0400 184.3 205.1
208(5) 0.0400 184.4 207.3
211(5) 0.0400 184.4 210.2
213(6) 0.02778 184.5 214.2
215(6) 0.02778 184.5 219.3
223(6) 0.02778 184.5 225.9
238(5) 0.0400 184.6 234.2
240(6) 0.02778 184.6 244.3
258(6) 0.02778 184.7 256.0
266(6) 0.02778 184.7 269.3
276(6) 0.02778 184.7 283.4
306(7) 0.02041 184.8 297.3
308(7) 0.02041 184.8 309.2
316(7) 0.02041 184.8 317.3
322(7) 0.02041 184.9 320.0
311(7) 0.02041 184.9 317.0
310(7) 0.02041 185.0 309.3
306(7) 0.02041 185.0 298.8
289(6) 0.02778 185.0 287.2
266(6) 0.02778 185.1 275.6
265(6) 0.02778 185.1 264.6
254(6) 0.02778 185.1 254.4
247(6) 0.02778 185.2 245.2
242(6) 0.02778 185.2 237.1
231(6) 0.02778 185.2 230.2
225(6) 0.02778 185.3 224.5
222(6) 0.02778 185.3 219.9
218(6) 0.02778 185.3 216.3
209(6) 0.02778 185.3 213.6
205(5) 0.0400 185.4 211.5
206(5) 0.0400 185.4 210.1
207(5) 0.0400 185.4 209.2
207(5) 0.0400 185.5 208.7
211(5) 0.0400 185.5 208.7
205(5) 0.0400 185.5 209.1
210(5) 0.0400 185.5 209.9
217(5) 0.0400 185.6 211.2
221(5) 0.0400 185.6 213.1
219(5) 0.0400 185.6 215.6
219(5) 0.0400 185.7 218.8
214(5) 0.0400 185.7 222.9
229(5) 0.0400 185.7 227.9
238(5) 0.0400 185.7 233.7
243(5) 0.0400 185.8 240.2
254(6) 0.02778 185.8 247.2
257(6) 0.02778 185.8 254.3
262(6) 0.02778 185.8 260.7
264(6) 0.02778 185.8 265.5
282(6) 0.02778 185.9 268.2
274(6) 0.02778 185.9 268.3
271(6) 0.02778 185.9 266.4
269(6) 0.02778 185.9 263.2
268(6) 0.02778 186.0 259.8
263(6) 0.02778 186.0 256.9
256(6) 0.02778 186.0 255.3
251(6) 0.02778 186.0 255.6
257(6) 0.02778 186.0 258.2
266(6) 0.02778 186.1 263.7
272(6) 0.02778 186.1 272.6
284(6) 0.02778 186.1 285.4
303(6) 0.02778 186.1 302.5
333(6) 0.02778 186.1 324.2
345(7) 0.02041 186.1 350.7
374(7) 0.02041 186.2 381.6
419(7) 0.02041 186.2 416.2
445(7) 0.02041 186.2 452.8
501(8) 0.01563 186.2 488.7
530(8) 0.01563 186.2 519.9
550(8) 0.01563 186.2 541.6
559(8) 0.01563 186.3 549.6
567(8) 0.01563 186.3 542.3
534(8) 0.01563 186.3 521.5
501(8) 0.01563 186.3 491.4
467(8) 0.01563 186.3 456.5
425(7) 0.02041 186.3 420.8
384(7) 0.02041 186.4 386.6
356(7) 0.02041 186.4 355.4
325(6) 0.02778 186.4 327.9
301(6) 0.02778 186.4 304.3
284(6) 0.02778 186.4 284.6
265(6) 0.02778 186.4 268.5
247(6) 0.02778 186.4 255.5
253(6) 0.02778 186.5 245.2
241(6) 0.02778 186.5 237.1
228(6) 0.02778 186.5 230.7
230(6) 0.02778 186.5 225.7
224(6) 0.02778 186.5 221.7
215(6) 0.02778 186.5 218.5
209(5) 0.0400 186.5 215.9
205(5) 0.0400 186.5 213.8
212(5) 0.0400 186.6 212.0
210(6) 0.02778 186.6 210.5
213(5) 0.0400 186.6 209.2
212(6) 0.02778 186.6 208.1
204(5) 0.0400 186.6 207.2
199(5) 0.0400 186.6 206.4
207(5) 0.0400 186.6 205.8
205(5) 0.0400 186.6 205.2
207(5) 0.0400 186.7 204.8
203(5) 0.0400 186.7 204.4
203(5) 0.0400 186.7 204.1
211(6) 0.02778 186.7 203.9
205(5) 0.0400 186.7 203.8
204(5) 0.0400 186.7 203.8
202(5) 0.0400 186.7 203.8
206(5) 0.0400 186.7 203.9
203(5) 0.0400 186.8 204.2
203(5) 0.0400 186.8 204.5
198(5) 0.0400 186.8 205.0
201(5) 0.0400 186.8 205.7
197(5) 0.0400 186.8 206.6
198(5) 0.0400 186.8 207.8
215(6) 0.02778 186.8 209.3
214(6) 0.02778 186.8 211.3
207(5) 0.0400 186.8 213.9
215(6) 0.02778 186.9 217.3
212(6) 0.02778 186.9 221.5
220(6) 0.02778 186.9 226.7
227(6) 0.02778 186.9 233.1
254(6) 0.02778 186.9 240.6
244(6) 0.02778 186.9 249.3
262(6) 0.02778 186.9 259.0
278(6) 0.02778 186.9 269.4
279(6) 0.02778 187.0 279.9
288(6) 0.02778 187.0 289.7
307(7) 0.02041 187.0 297.8
306(7) 0.02041 187.0 302.8
318(7) 0.02041 187.0 304.1
314(7) 0.02041 187.0 301.3
306(7) 0.02041 187.0 295.0
287(6) 0.02778 187.1 286.3
274(6) 0.02778 187.1 276.5
258(6) 0.02778 187.1 266.3
247(6) 0.02778 187.1 256.6
245(6) 0.02778 187.1 247.6
237(6) 0.02778 187.1 239.7
228(6) 0.02778 187.1 232.8
217(6) 0.02778 187.2 227.0
219(6) 0.02778 187.2 222.3
213(6) 0.02778 187.2 218.5
207(5) 0.0400 187.2 215.5
214(6) 0.02778 187.2 213.3
211(6) 0.02778 187.2 211.5
204(5) 0.0400 187.2 210.2
202(5) 0.0400 187.3 209.3
208(5) 0.0400 187.3 208.6
206(6) 0.02778 187.3 208.2
202(5) 0.0400 187.3 208.0
208(5) 0.0400 187.3 207.9
211(6) 0.02778 187.3 208.0
203(5) 0.0400 187.4 208.3
200(5) 0.0400 187.4 208.7
203(5) 0.0400 187.4 209.2
205(5) 0.0400 187.4 209.9
200(5) 0.0400 187.4 210.8
206(5) 0.0400 187.5 211.9
205(5) 0.0400 187.5 213.1
210(5) 0.0400 187.5 214.6
218(6) 0.02778 187.5 216.3
219(6) 0.02778 187.5 218.1
221(6) 0.02778 187.5 220.1
228(6) 0.02778 187.6 222.2
209(5) 0.0400 187.6 224.4
229(6) 0.02778 187.6 226.5
226(6) 0.02778 187.6 228.5
228(6) 0.02778 187.6 230.4
230(6) 0.02778 187.7 232.3
233(6) 0.02778 187.7 234.3
249(6) 0.02778 187.7 236.7
252(6) 0.02778 187.7 239.6
241(6) 0.02778 187.7 243.4
243(6) 0.02778 187.8 248.4
262(6) 0.02778 187.8 254.9
253(6) 0.02778 187.8 263.3
271(6) 0.02778 187.8 274.2
283(6) 0.02778 187.9 287.9
301(6) 0.02778 187.9 305.0
329(7) 0.02041 187.9 325.9
352(7) 0.02041 187.9 351.0
381(7) 0.02041 188.0 380.4
411(8) 0.01563 188.0 414.0
445(8) 0.01563 188.0 451.5
497(8) 0.01563 188.0 492.0
533(9) 0.01235 188.0 533.8
585(9) 0.01235 188.1 574.6
623(9) 0.01235 188.1 610.9
647(10) 0.01000 188.1 638.8
662(10) 0.01000 188.1 654.4
644(10) 0.01000 188.2 655.2
645(10) 0.01000 188.2 641.2
609(9) 0.01235 188.2 614.6
582(9) 0.01235 188.2 579.2
544(9) 0.01235 188.3 538.9
497(9) 0.01235 188.3 497.3
461(8) 0.01563 188.3 456.9
420(8) 0.01563 188.3 419.2
380(8) 0.01563 188.4 385.3
343(7) 0.02041 188.4 355.5
330(7) 0.02041 188.4 330.1
302(7) 0.02041 188.4 308.8
291(6) 0.02778 188.5 291.3
293(6) 0.02778 188.5 277.1
281(6) 0.02778 188.5 265.8
275(6) 0.02778 188.5 256.9
264(6) 0.02778 188.6 250.0
248(6) 0.02778 188.6 244.6
250(6) 0.02778 188.6 240.4
249(6) 0.02778 188.7 237.3
240(6) 0.02778 188.7 235.1
233(5) 0.0400 188.7 233.5
239(5) 0.0400 188.7 232.7
233(5) 0.0400 188.8 232.5
231(5) 0.0400 188.8 233.0
232(5) 0.0400 188.8 234.2
237(5) 0.0400 188.8 236.2
249(6) 0.02778 188.9 239.0
250(6) 0.02778 188.9 242.9
253(6) 0.02778 188.9 247.7
253(6) 0.02778 188.9 253.6
271(6) 0.02778 189.0 260.5
273(6) 0.02778 189.0 268.5
275(6) 0.02778 189.0 277.3
299(6) 0.02778 189.1 286.6
305(6) 0.02778 189.1 296.2
306(6) 0.02778 189.1 305.2
325(6) 0.02778 189.1 313.1
340(7) 0.02041 189.2 318.9
329(6) 0.02778 189.2 321.7
327(6) 0.02778 189.2 321.3
326(6) 0.02778 189.2 317.6
329(6) 0.02778 189.3 311.1
323(6) 0.02778 189.3 302.7
303(6) 0.02778 189.3 293.3
284(6) 0.02778 189.3 283.5
272(6) 0.02778 189.4 274.0
261(6) 0.02778 189.4 265.2
256(6) 0.02778 189.4 257.3
246(6) 0.02778 189.4 250.5
234(5) 0.0400 189.5 244.8
247(6) 0.02778 189.5 240.2
237(5) 0.0400 189.5 236.8
229(5) 0.0400 189.5 234.4
226(5) 0.0400 189.6 233.1
239(5) 0.0400 189.6 232.7
233(5) 0.0400 189.6 233.1
235(5) 0.0400 189.6 234.3
237(5) 0.0400 189.7 236.1
237(5) 0.0400 189.7 238.6
241(6) 0.02778 189.7 241.4
242(5) 0.0400 189.7 244.6
242(5) 0.0400 189.7 247.9
250(6) 0.02778 189.8 251.1
257(6) 0.02778 189.8 254.0
258(6) 0.02778 189.8 256.6
261(6) 0.02778 189.8 258.9
260(6) 0.02778 189.9 260.8
250(6) 0.02778 189.9 262.3
261(6) 0.02778 189.9 263.5
277(6) 0.02778 189.9 264.2
277(6) 0.02778 189.9 264.3
259(6) 0.02778 190.0 263.5
250(6) 0.02778 190.0 261.8
258(6) 0.02778 190.0 259.1
254(6) 0.02778 190.0 255.7
254(6) 0.02778 190.0 251.7
251(6) 0.02778 190.1 247.6
245(6) 0.02778 190.1 243.4
232(6) 0.02778 190.1 239.4
235(6) 0.02778 190.1 235.8
226(6) 0.02778 190.1 232.6
223(6) 0.02778 190.2 229.9
226(6) 0.02778 190.2 227.6
227(6) 0.02778 190.2 225.9
224(6) 0.02778 190.2 224.7
222(6) 0.02778 190.2 223.9
218(6) 0.02778 190.3 223.7
230(6) 0.02778 190.3 223.9
228(6) 0.02778 190.3 224.6
228(6) 0.02778 190.3 225.9
234(6) 0.02778 190.3 227.8
233(6) 0.02778 190.4 230.2
220(6) 0.02778 190.4 233.3
229(6) 0.02778 190.4 237.2
240(6) 0.02778 190.4 241.7
242(6) 0.02778 190.4 247.1
247(6) 0.02778 190.4 253.3
250(6) 0.02778 190.5 260.2
257(7) 0.02041 190.5 267.9
269(7) 0.02041 190.5 276.1
276(7) 0.02041 190.5 284.8
296(7) 0.02041 190.5 293.6
291(7) 0.02041 190.6 302.1
297(7) 0.02041 190.6 309.8
310(7) 0.02041 190.6 316.2
308(7) 0.02041 190.6 320.7
324(7) 0.02041 190.6 323.0
308(7) 0.02041 190.6 322.9
327(7) 0.02041 190.7 320.8
302(7) 0.02041 190.7 317.1
313(7) 0.02041 190.7 312.4
304(7) 0.02041 190.7 307.5
296(7) 0.02041 190.7 302.9
305(7) 0.02041 190.8 299.1
295(7) 0.02041 190.8 296.5
286(7) 0.02041 190.8 295.6
301(7) 0.02041 190.8 296.5
295(7) 0.02041 190.9 299.6
303(8) 0.01563 190.9 305.1
309(8) 0.01563 190.9 313.1
328(8) 0.01563 190.9 323.8
342(8) 0.01563 191.0 337.3
351(8) 0.01563 191.0 353.6
371(8) 0.01563 191.0 372.7
399(9) 0.01235 191.0 394.2
427(9) 0.01235 191.1 417.9
450(9) 0.01235 191.1 443.3
477(10) 0.01000 191.1 469.5
499(10) 0.01000 191.1 495.4
514(10) 0.01000 191.2 519.8
543(10) 0.01000 191.2 540.8
564(11) 0.00826 191.2 556.8
577(11) 0.00826 191.3 566.2
577(11) 0.00826 191.3 568.1
567(11) 0.00826 191.3 562.5
547(10) 0.01000 191.4 550.1
529(10) 0.01000 191.4 532.3
521(10) 0.01000 191.5 510.7
490(10) 0.01000 191.5 486.9
461(10) 0.01000 191.5 462.1
424(9) 0.01235 191.6 437.4
389(9) 0.01235 191.6 413.2
371(9) 0.01235 191.7 390.2
369(9) 0.01235 191.7 368.6
338(8) 0.01563 191.8 348.6
335(8) 0.01563 191.8 330.4
325(8) 0.01563 191.8 314.1
289(8) 0.01563 191.9 299.6
288(8) 0.01563 192.0 286.9
284(7) 0.02041 192.0 275.9
280(7) 0.02041 192.1 266.5
270(7) 0.02041 192.1 258.4
259(7) 0.02041 192.2 251.6
264(7) 0.02041 192.2 245.8
261(7) 0.02041 192.3 240.9
255(7) 0.02041 192.4 236.8
246(7) 0.02041 192.4 233.3
234(7) 0.02041 192.5 230.3
242(7) 0.02041 192.6 227.8
218(7) 0.02041 192.6 225.6
211(6) 0.02778 192.7 223.8
218(7) 0.02041 192.8 222.3
217(6) 0.02778 192.9 220.9
223(7) 0.02041 192.9 219.8
222(7) 0.02041 193.0 218.8
226(7) 0.02041 193.1 218.0
223(7) 0.02041 193.2 217.3
213(7) 0.02041 193.3 216.7
206(7) 0.02041 193.4 216.3
217(7) 0.02041 193.4 215.9
215(7) 0.02041 193.5 215.6
216(7) 0.02041 193.6 215.4
219(7) 0.02041 193.7 215.2
211(7) 0.02041 193.8 215.1
216(7) 0.02041 193.9 215.1
218(7) 0.02041 194.0 215.1
207(7) 0.02041 194.1 215.1
224(7) 0.02041 194.2 215.1
211(7) 0.02041 194.4 215.1
203(7) 0.02041 194.5 215.2
220(7) 0.02041 194.6 215.2
205(7) 0.02041 194.7 215.2
203(7) 0.02041 194.8 215.2
216(7) 0.02041 194.9 215.2
218(7) 0.02041 195.0 215.2
215(7) 0.02041 195.2 215.3
216(8) 0.01563 195.3 215.5
199(7) 0.02041 195.4 215.7
218(7) 0.02041 195.5 216.0
217(7) 0.02041 195.7 216.4
221(7) 0.02041 195.8 216.9
224(7) 0.02041 195.9 217.6
227(8) 0.01563 196.1 218.4
211(8) 0.01563 196.2 219.4
216(8) 0.01563 196.3 220.6
216(9) 0.01235 196.5 222.1
218(9) 0.01235 196.6 223.8
231(9) 0.01235 196.7 225.8
236(9) 0.01235 196.9 228.1
228(9) 0.01235 197.0 230.7
222(9) 0.01235 197.2 233.8
242(9) 0.01235 197.3 237.3
248(9) 0.01235 197.4 241.3
260(9) 0.01235 197.6 245.7
247(9) 0.01235 197.7 250.6
252(9) 0.01235 197.9 255.9
261(9) 0.01235 198.0 261.7
274(10) 0.01000 198.1 267.9
279(10) 0.01000 198.3 274.4
291(10) 0.01000 198.4 281.2
295(10) 0.01000 198.5 288.2
283(10) 0.01000 198.7 295.3
280(10) 0.01000 198.8 302.3
302(10) 0.01000 198.9 309.1
333(11) 0.00826 199.1 315.4
335(11) 0.00826 199.2 320.9
340(10) 0.01000 199.3 325.3
331(11) 0.00826 199.4 328.3
317(13) 0.00592 199.5 329.5
335(13) 0.00592 199.6 328.9
346(13) 0.00592 199.7 326.5
313(13) 0.00592 199.8 322.3
332(13) 0.00592 199.9 316.8
326(13) 0.00592 200.0 310.2
303(12) 0.00694 200.1 303.0
307(12) 0.00694 200.2 295.4
281(12) 0.00694 200.3 287.7
278(12) 0.00694 200.3 280.1
250(12) 0.00694 200.4 272.9
247(11) 0.00826 200.4 266.1
263(11) 0.00826 200.5 259.8
244(11) 0.00826 200.5 254.0
250(11) 0.00826 200.5 248.9
230(11) 0.00826 200.5 244.2
223(11) 0.00826 200.5 240.2
246(11) 0.00826 200.5 236.6
228(11) 0.00826 200.4 233.6
236(11) 0.00826 200.4 231.0
239(11) 0.00826 200.3 228.8
217(10) 0.01000 200.3 226.9
234(11) 0.00826 200.2 225.4
223(11) 0.00826 200.1 224.1
233(10) 0.01000 199.9 223.1
244(16) . . .
212(15) . . .
217(15) . . .
227(14) . . .
206(15) . . .
234(15) . . .
226(16) . . .
221(14) . . .
221(16) . . .
214(14) . . .
232(15) . . .
234(15) . . .
215(15) . . .
211(14) . . .
219(15) . . .
230(15) . . .
233(16) . . .
224(15) . . .
219(15) . . .
221(15) . . .
241(15) . . .
220(15) . . .
233(16) . . .
175(15) . . .
0(15) . . .
